Home >
Documents >
arXiv:1511.06706v2 [cond-mat.mes-hall] 23 Oct 2016 · 2016-10-25 · graphene systems. Three types...

Share this document with a friend

Embed Size (px)

of 132
/132

Transcript

Electronic properties of graphene-based bilayer systems

A.V. Rozhkova,b,c, A.O. Sboychakova,b, A.L. Rakhmanova,b,c,d, Franco Noria,e

aCEMS, RIKEN, Saitama 351-0198, JapanbInstitute for Theoretical and Applied Electrodynamics, Russian Academy of Sciences, 125412 Moscow, Russia

cMoscow Institute of Physics and Technology, Dolgoprudny, Moscow Region, 141700 RussiadAll-Russia Research Institute of Automatics, Moscow, 127055 Russia

ePhysics Department, The University of Michigan, Ann Arbor, Michigan 48109-1040, USA

Abstract

This article reviews the theoretical and experimental work related to the electronic properties of bilayergraphene systems. Three types of bilayer stackings are discussed: the AA, AB, and twisted bilayer graphene.This review covers single-electron properties, effects of static electric and magnetic fields, bilayer-basedmesoscopic systems, spin-orbit coupling, dc transport and optical response, as well as spontaneous symmetryviolation and other interaction effects. The selection of the material aims to introduce the reader to themost commonly studied topics of theoretical and experimental research in bilayer graphene.

Contents

1 Introduction 5

2 AA and AB graphene bilayers: available samples 72.1 AA-stacked bilayer graphene . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 72.2 AB-stacked bilayer graphene . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7

3 Electron spectra: free electron approximation 73.1 Single-layer graphene . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8

3.1.1 Single-electron tight-binding description . . . . . . . . . . . . . . . . . . . . . . . . . . 83.1.2 Effective Dirac equation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 113.1.3 Density of states . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11

3.2 AA bilayer graphene . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 123.2.1 Single-electron tight-binding description . . . . . . . . . . . . . . . . . . . . . . . . . . 123.2.2 Density of states . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 153.2.3 Effect of the bias voltage . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16

3.3 AB bilayer graphene . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 173.3.1 Single-electron tight-binding description . . . . . . . . . . . . . . . . . . . . . . . . . . 173.3.2 Effect of the bias voltage . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 203.3.3 Density of states . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 213.3.4 Immediate consequences of the single-electron band theory . . . . . . . . . . . . . . . 21

4 Dirac electrons: chirality and Klein paradox 234.1 Chiral electrons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 23

4.1.1 AA bilayer graphene . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 234.1.2 AB bilayer graphene . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 25

Email address: [email protected] (Franco Nori)

Preprint submitted to Elsevier October 25, 2016

arX

iv:1

511.

0670

6v2

[co

nd-m

at.m

es-h

all]

23

Oct

201

6

4.2 Klein tunneling and chiral scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 254.2.1 Klein scattering in AA-stacked bilayer graphene . . . . . . . . . . . . . . . . . . . . . 274.2.2 Klein scattering in AB-stacked bilayer graphene . . . . . . . . . . . . . . . . . . . . . . 27

5 Bilayer graphene in a magnetic field: Landau levels and quantum Hall effect 285.1 Landau levels and integer quantum Hall effect in AA-stacked bilayer graphene . . . . . . . . . 29

5.1.1 Landau levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 295.1.2 Conductivity in the magnetic field and integer quantum Hall effect . . . . . . . . . . . 30

5.2 Landau levels and integer quantum Hall effect in AB-stacked bilayer graphene . . . . . . . . . 325.2.1 Landau levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 325.2.2 Conductivity in a magnetic field and magneto-optic phenomena . . . . . . . . . . . . . 365.2.3 Integer quantum Hall effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 365.2.4 Fractional quantum Hall effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 38

6 Spin-orbit coupling 40

7 Bilayer-based mesoscopic systems 427.1 AB bilayer graphene quantum dots . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 427.2 Bilayer graphene nanoribbons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 43

7.2.1 AA bilayer nanoribbons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 437.2.2 AB bilayer nanoribbons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 44

7.3 Topologically-protected conducting channels in AB bilayer samples . . . . . . . . . . . . . . . 467.4 pn-junctions and similar structures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 48

8 Electronic transport through an AB bilayer sample 518.1 Transport through doped bilayer . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 518.2 Minimum conductivity of a bilayer . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 548.3 Transport through an AB bilayer in a transverse electric field . . . . . . . . . . . . . . . . . . 57

9 Dynamic conductivity and optical spectra 589.1 Dynamic conductivity in AA-stacked bilayer graphene . . . . . . . . . . . . . . . . . . . . . . 589.2 Dynamic conductivity in AB-stacked bilayer graphene . . . . . . . . . . . . . . . . . . . . . . 60

10 Broken symmetry phases 6210.1 Low-temperature broken symmetry phases of AA bilayer graphene . . . . . . . . . . . . . . . 63

10.1.1 Electron correlations: symmetry analysis . . . . . . . . . . . . . . . . . . . . . . . . . 6310.1.2 Electron correlations and antiferromagnetic order . . . . . . . . . . . . . . . . . . . . . 6410.1.3 Incommensurate antiferromagnetic order . . . . . . . . . . . . . . . . . . . . . . . . . . 6610.1.4 Phase separation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6710.1.5 Nearest-neighbor Coulomb repulsion, bias voltage, and exciton order parameter . . . . 6810.1.6 Long-range Coulomb interaction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 69

10.2 Low-temperature broken symmetry phases of AB bilayer graphene . . . . . . . . . . . . . . . 6910.2.1 Ferromagnetic and antiferromagnetic states . . . . . . . . . . . . . . . . . . . . . . . . 6910.2.2 “Pseudospin magnetic” states . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7010.2.3 Antiferromagnetic state . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7210.2.4 Nematic phase . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7310.2.5 Other types of order . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 74

11 Many-body and non-Fermi liquid effects in bilayer graphene 75

12 Dielectric function and plasmonics in AB bilayer 76

2

13 Twisted bilayer graphene 7713.1 Geometrical properties: Moire pattern and superstructure. . . . . . . . . . . . . . . . . . . . . 7713.2 Effective low-energy theories of twisted bilayer graphene electronic spectrum . . . . . . . . . . 82

13.2.1 Low-energy Hamiltonians . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8213.2.2 Fermi velocity reduction and low-energy van Hove singularities . . . . . . . . . . . . . 8613.2.3 Low-energy spectrum at very small angles . . . . . . . . . . . . . . . . . . . . . . . . . 8813.2.4 Fine structure of the low-energy bands: band splitting and band gap . . . . . . . . . . 89

13.3 Tight-binding calculations of the twisted bilayer graphene spectrum . . . . . . . . . . . . . . 9113.4 Twisted bilayer graphene in a magnetic field . . . . . . . . . . . . . . . . . . . . . . . . . . . . 100

13.4.1 Landau levels and quantum Hall effect . . . . . . . . . . . . . . . . . . . . . . . . . . . 10013.4.2 Fine structure of the Landau levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10413.4.3 The Hofstadter butterfly spectrum . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 106

13.5 Electronic transport in twisted bilayer graphene . . . . . . . . . . . . . . . . . . . . . . . . . . 11113.5.1 Dynamical conductivity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11113.5.2 Plasmons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11513.5.3 Interlayer conductivity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11613.5.4 Klein tunneling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 117

14 Conclusions 118

Notation used in the text

Section 1c0: interlayer distance

Section 2σ, σαβ : conductivityn: electron density

Section 3a1,2: elementary lattice vectorsa0: distance between nearest carbon atoms in the layert: hoping amplitude between in-plane nearest-neighbor carbon atomst0: hoping amplitude between inter-plane nearest-neighbor carbon atomst′: hoping amplitude between in-plane next-nearest-neighbor carbon atomstg: hoping amplitude between inter-plane next-nearest-neighbor carbon atomst3: hoping amplitude between nearest-neighbor non-dimer carbon atomst4: hoping amplitude between nearest-neighbor non-dimer to dimer carbon atomsσ: spin projectionN : number of unit cellsf(k) =

∑3j=1 exp(ikδj)

F (k) = 2 cos (√

3kya0) + 4 cos (√

3kya0/2) cos (3kxa0/2)b1,2: elementary reciprocal-lattice vectorsδj : three vectors (j = 1, 2, 3) connecting nearest-neighbor sites in honeycomb latticeK,K′: locations of the Dirac points in the reciprocal space

ε(s)k : electronic bandsσ = (σx, σy, σz): Pauli matricesρ(ε): density of statesµ: chemical potentialVBZ : volume of Brillouin zoneV : bias voltage

3

njασ: the electron number operatorξ = ±1: valley indexm0: free electron massm = t0/2v

2F : effective charge carrier mass

pL: shift of the cones from Brillouin zone corner due to trigonal warpingεL: energy of saddle points due to trigonal warping

Section 4χ1,2: chirality operatorsη1,2: band indicesγ5: 5th Dirac matrixc = η1η2: cone indexχ = η1: chirality indexπ = ξ∂/∂x+ i∂/∂yJ : winding number

Section 5Φ0 = 2π~c/e: magnetic flux quantumωc: cyclotron frequencylb: magnetic lengthELL(n): nth Landau level energyNf : degeneracy factorN : electron numberν: filling factorΘF : Faraday rotation angle

Section 6tR: Rashba spin-orbit strengthdij: lattice vector from site i to site jM : magnetization

Section 8ε0 = 4εL: energy scale characterizing the trigonal warpingΣ(ε): self-energyni: impurity concentrationu: energy characterizing the impurity strengthx: dopingx: local dopingx2

rms = 〈x2〉 − x2

ρ∞: density of states asymptotic at high energyW = niu

2ρ∞/2ε0: dimensionless disorder strengthΓ = πWε0/2: scattering rate due to disorderµc: mobility

Section 9G(z): Green’s functionωn: Matsubara frequencyf(ε): Fermi functionµ: chemical potentialAij : amplitudes of the spectral representation of Green’s functionΓ: phenomenological broadening constant

Section 10U0: on-site Coulomb repulsion

4

U01: nearest-neighbor in-plane Coulomb repulsionU02: next-nearest-neighbor in-plane Coulomb repulsionU11: nearest-neighbor inter-plane Coulomb repulsion∆xykσ: order parameters

Ω: grand potentialµ′ = µ− U0x/2: shifted chemical potentialq: vector characterizing incommensurability of the antiferromagnetic stateSnαa: average electron spin at site nV (q): Coulomb potential in the momentum space

Section 11ε(k, ω): dielectric functionΠ(k, ω): irreducible polarization

Section 13A: in this section means the complex conjugate Aθ: twist angle between two graphene layersL: Moire periodm0, r: mutually prime positive integers defining a particular “commensurate” twist angleN(m0, r) or N : number of sites in the elementary unit cell of the superlatticeR1,2: superlattice vectorsLSC = |R1,2|: supercell linear sizeG1,2: basis vectors of the reciprocal superlatticeKθ,K

′θ: Dirac points of the top (rotated) layer

∆K = Kθ −KK1,2: non-equivalent Dirac points of the reciprocal superlattice

t⊥(r) and tαβ⊥ (G): interlayer hoping amplitude and its Fourier transform

Tαβ⊥ : interlayer hoping Hamiltonian%: relative shift between the layersv∗F : renormalized Fermi velocityθc: twist angle at which v∗F (θc) = 0∆EvHs: energy difference between two van Hove singularitiesVppπ(r) and Vppσ(r): Slater-Koster parameters∆s: band splittingω∗c : twist-dependent cyclotron frequency

1. Introduction

Systems with only carbon atoms show a number of different structures with a variety of physical proper-ties because of the flexibility of its chemical bonding. Among these systems there are allotropes of differentdimensionality from three-dimensional (3D) graphite and diamond to low-dimensional structures, such asfullerene and carbon nanotubes, which could be thought as zero-dimensional and one-dimensional objectsrespectively. A two-dimensional (2D) carbon allotrope graphene was the first produced stable 2D crystal [1].Graphene is composed of carbon atoms forming a honeycomb lattice. This 2D system has a number of in-triguing physical properties that are of interest for fundamental physics and important applications. It isalso important and interesting to increase the family of 2D solids. A possible approach in this direction is toproduce 2D structures of different chemical compositions such as silicene, nitrogen boride, etc. A differentmethod is to manufacture few-layer carbon systems, of which the simplest and the most obvious is thegraphene bilayer. The electronic properties of the graphene bilayer is the subject of the present review.

The graphene bilayer can exist in three modifications: AA, AB (or Bernal phase), and twisted bilayer.The simplest form is the AA bilayer [2], in which each carbon atom of the second layer is placed exactly

5

above the corresponding atom of the first carbon sheet. However, this structure is likely to be metastable,and only few authors reported manufacturing AA samples. In the AB bilayer, or Bernal phase, half of thecarbon atoms of the top layer are above the carbon atoms of the lower layer, while other atoms locatedabove the centers of the lower-layer hexagons (in naturally-occurring graphite the carbon atoms are orderedin similar manner). The Bernal (or AB) bilayer graphene is the most stable, and its high-quality samplesare produced and studied in many experiments. In the third type of bilayer graphene structure, the topcarbon layer is rotated with respect to the lower layer by some angle θ [3]. Such a structure is also stable,and the twisted samples are produced using some special technological processes. The electronic propertiesof the bilayer structures listed above are rather different. Thus, in the chapters of this review we usuallyconsider each of them separately.

The theories of electronic properties of the bilayer systems are built upon the knowledge of the electronicstructure of single-layer graphene [4]. It is established that, for single-layer graphene, the sp2 hybridizationbetween the carbon s orbital and two p orbitals enables the formation of a σ bond between neighboringatoms. The σ bond is responsible for the robustness of the lattice structure in all carbon allotropes. Becauseof the Pauli principle, these bands have a filled shell. As a result, a valence band appears. The pz orbital,which is perpendicular to the graphene plane, binds covalently with carbon atoms nearby. This leads to theformation of a π band. Since every p orbital hosts one extra electron, the π band is half-filled.

In the equilibrium configuration, the interlayer spacing in the AB bilayer is estimated [5] as c0 = 3.35 A.In the AA and twisted bilayer samples, the interlayer distance could be slightly different. Furthermore, intwisted bilayer graphene the interlayer distance is spatially modulated [6]. The nature of the interactionbetween graphene sheets in bilayer graphene was analyzed by many authors (see, e.g., Refs. [7, 8, 9, 10, 11]).The hybridization between the s orbital and the pz orbitals in the bilayers is more cumbersome than in thesingle-layer graphene. However, as in the case of the single layer, the π band is formed in bilayer grapheneand the π band is half-filled if the sample is not doped.

The charge carriers in single-layer graphene are massless chiral quasiparticles with a linear dispersion,as described by a Dirac-like effective Hamiltonian [4]. This was confirmed in a number of experimentalobservations, particularly, the Landau quantization in the magnetic field and the integer quantum Halleffect. The low-energy Hamiltonian of bilayer graphene may be viewed as a generalization of the Dirac-likeHamiltonian of monolayer graphene, resulting in a more complicated picture of electron and hole dispersion.For example, AB bilayer quasiparticles demonstrate parabolic dispersion at low energies and linear dispersionat higher energies. As we will see below, the electronic spectrum of bilayer graphene may be gapped orgapless. There are several mechanisms, which could induce a single-electron gap in a bilayer sample. Such amechanism may, or may not, rely on the electron-electron interaction. Depending on a particular situation,the gap in the spectrum can be controlled by doping, gate voltage, or some other parameter. The possibilityof having a graphene-based system with the gap in the spectrum is of interest for applications in electronicdevices.

Many macroscopic properties of bilayer graphene are similar to that of the monolayer samples. Inparticular, the well-prepared samples have high electric and thermal conductivity, high mechanical stiffness,high transparency with respect to white light, impermeability to gases, and the ability to be chemicallyfunctionalized (see, e.g., the review in Ref. [5] and the papers cited therein). For some applications, thegraphene bilayers may have definite advantages over the monolayer due to larger possibilities for tuningtheir physical properties. All this makes the study of bilayer graphene a timely and important endeavor.

Currently, in graphene-related reviews, it is an accepted marketing device to scare the readers withhuge numbers of published papers dedicated to the graphene research. Following this trend, let us remindthat in years 2014-2015 at least 1000 publications mentioned bilayer graphene. Clearly, for navigation insuch a sea of information a role of review papers must not be underestimated. While this review aims tooffer a more general and synergetic coverage of the field, a reader interested in more specialized areas mayconsider more topical works. For example, paper of Das Sarma et al. [12] is focused primarily on transportproperties of both single-layer and AB bilayer graphene. Bilayer photonics applications are discussed inRef. [13]. Publications regarding plasmons in graphene-based systems are reviewed by T. Stauber in Ref. [14].Nonlinear optical phenomena of single-layer and AB bilayer were subject of Ref. [15]. Mini-review of theworks on twisted bilayer is Ref. [16]. Finally, let us cite several reviews, Refs. [17, 18, 19], which might be

6

useful for understanding the subject.Regarding the organization of the presented material, we would like to comment that the AB and AA

bilayers are reviewed in parallel. Due to peculiar geometry of the twisted bilayer lattice, this type of thegraphene bilayer is discussed separately, in Section 13.

2. AA and AB graphene bilayers: available samples

2.1. AA-stacked bilayer graphene

We would like to start the review with a brief discussion of the available samples and their quality. To thisdate, both theoretical and experimental reasearch of AA-stacked bilayer lags behind the studies of AB bilayerby a significant margin. While several papers described preparation of AA bilayer samples [2, 20, 21, 22],most of the available data are gathered either by transmission electron microscopy (TEM) [2, 20, 22], or byscanning tunneling microscopy (STM) [21]. These are imaging methods. As a result, the lattice structure ofthe samples is visualized with high precision. Unfortunately, these techniques give virtually no informationabout the electronic properties. At present, we cannot say how good or bad the available samples are interms of mobility or other electronic characteristics. However, witnessing the growing theoretical interest inAA-stacked systems, we think that the situation with experiment will improve.

2.2. AB-stacked bilayer graphene

The study of AB bilayer graphene is a very active and diverse area of research. As a result, severalpublications reported the preparation of AB samples of excellent quality. In modern graphene literature itis common to characterize the quality of samples by their electron mobility (although, there is an exceptionto this rule [23]). Interpreting the relevant data one has to remember two points. First, it is well-knownthat single-layer graphene has large mobility: even in the earliest samples [24] the mobility was as high as104 cm2/Vs. This is about 10 times larger than that of silicon. For a suspended single-layer sample it iseven higher (e.g., K. Bolotin et al. [25] reported the value of 2× 105 cm2/Vs). Therefore, one should not besurprised by the extremely high mobility values of graphene-based systems. Second, since this property isnot directly accessible from experiments, it must be extracted from measurements of other quantities. Forexample, A. S. Mayorov et al. [26] estimated the mobility as c/B0, where c is the velocity of light, B0 is thethreshold magnetic field for the onset of quantum oscillations. Such quantity is called “quantum mobility”.In other papers, e.g., Refs. [26, 27], the mobility was equated with the expression (1/e)dσ/dn, where e is theelectron charge, σ is conductivity, and n is electron density. The discrepancy between two definitions canbe as small as 30% [26], or as large as 200% (see Supporting Information for Ref. [28]). Thus, comparingdata from different experimental groups one must keep in mind the possible ambiguity in the experimentaldefinition of this quantity.

The samples should be divided into two classes: suspended samples and samples on a substrate [e.g.,SiO2, boron nitride, polymethylmethacrylate (PMMA)]. The former usually have higher mobility becausethey are free from disorder introduced by the substrate. The experimental data is summarized in Table 1.

3. Electron spectra: free electron approximation

In this section we analyze the single-electron spectra of bilayer graphene. Two alternative approaches areusually applied to derive the electronic spectra of graphene systems, as well as many other materials. The firstis the “ab-initio” density functional theory (DFT) calculations. The second is a tight-binding approximation,using as input parameters appropriate hopping amplitudes. In many cases these amplitudes are calculatedby means of the DFT method. The results obtained in the framework of these two approaches are almostsimilar for the graphene-like systems. The tight-binding approach is more simple and physically transparent.Thus, in this review we will follow the tight-binding calculations, mentionning the DFT approach where itis possible.

Electronic spectra of different graphene systems can be classified as the so-called Dirac-type spectra.For example, in single-layer graphene the dispersion of the low-energy electronic states is linear, similar

7

Substrate Mobility, ×104 cm2/Vs Temperature References

SiO2 and PMMA0.7 from liquid He to room T [29]

SiO2 0.3 unspecified [30]

h-BN 4 room T [31]

substratematerial wasnot specified

0.05 – 0.2 1.5 K [28]

Suspended 0.6 – 35most data were taken at 1.5 K,

highest mobility data were taken at0.3 K

[28]

Suspended 1.0 – 1.5 some data were taken at 450 mK [27]

Suspended 50–150 unspecified [26]

Suspended 8–10 unspecified [32]

Suspended > 2 4.2 K [33]

Table 1: The quality of a bilayer sample is characterized by the mobility of its charge carriers. In this table the summary ofreported mobility data for AB-bilayer graphene samples is presented.

to the dispersion of relativistic massless Dirac electrons. Accordingly, relativistic effect, such as the Kleinparadox, is observed in graphene. Recently, a number of other systems of this type became a focus of intenseinvestigation, including topological insulators, and Weil semimetals. Note, however, that the physical reasonsgiving rise to the Dirac-like behavior of the electronic spectra may be quite different in different systems.For example, in topological insulators it arises due to a strong spin-orbital interaction, while in graphene itoccurs due to the specific symmetry of the crystalline lattice.

A graphene bilayer consists of two connected single layers of graphene. Thus, the tight-binding Hamil-tonian of the bilayer graphene can be written as a sum of the Hamiltonians of two single-layer graphenesheets and a term describing the electron hopping between these sheets. For readers’ convenience, we startwith a brief review of the electronic spectrum of single-layer graphene. Then, we consider bilayer graphenewith AA stacking, (Section 3.2) and with AB stacking (Section 3.3). The electronic spectrum of twistedbilayer graphene is analyzed separately, in Section 13. In this chapter we disregard the effects of electron-electron interaction, which, however, is not small in graphene systems. The applicability condition of suchan approach as well as the effects of electron-electron coupling will be discussed in detail in Section 10.

3.1. Single-layer graphene

3.1.1. Single-electron tight-binding description

The electronic spectrum of single-layer graphene was investigated in details in many papers (see, e.g.,the review [4]). The honeycomb lattice of graphene consists of two sublattices, A and B (see Fig. 1, leftpanel). The lattice vectors are

a1 =a0

2(3,√

3), a2 =a0

2(3,−

√3), (1)

8

Figure 1: (Color online) Honeycomb lattice of graphene and its Brillouin zone. Left panel: lattice structure of single-layergraphene, made out of two triangular sublattices, A (red circles) and B (black circles); a1,2 are the lattice unit vectors and δiare the nearest-neighbor vectors. Right panel: the Brillouin zone of graphene is a hexagon in momentum space. The reciprocallattice vectors are b1,2. The Brillouin zone corners are denoted by K and K′.

where a0 = 1.42 A is the distance between the nearest carbon atoms. The simplest tight-binding Hamiltonianof single-layer graphene can be written in the form

H = −t∑〈ij〉σ

a†iσbjσ + h.c. , (2)

where t is the nearest-neighbor hopping amplitude, a†iσ (b†iσ) is the creation operator of the electron on site iof the sublattice A (B). Index σ labels spin projection, the brackets 〈...〉 stand for nearest-neighbor hopping,and h.c. means the Hermitian conjugate term. Since elementary crystalline unit of graphene includes twocarbon atoms A and B, the single-electronic spectrum of the Hamiltonian Eq. (2) consists of two bands,both of which are doubly degenerate with respect to the spin projection σ.

To derive the spectrum we will follow the standard procedure. We rewrite Eq. (2) in k-space with thehelp of the Fourier transform of the electron operators,

akσ =1√N

∑n

eikrAn anσ, bkσ =

1√N

∑n

eikrBn bnσ, (3)

where the index n runs over all the unit cells of the honeycomb lattice, N is the number of unit cells inthe lattice, and rαn is the position of a carbon atom in the n-th unit cell for sublattice α (sublattice indexα = A,B). The quasimomentum k belongs to the Brillouin zone. For the honeycomb lattice, the Brillouinzone is a hexagon (see the right panel of Fig. 1). The corresponding reciprocal-lattice vectors are given by

b1 =2π

3a0(1,√

3), b2 =2π

3a0(1,−

√3). (4)

It is convenient to group two operators, introduced by Eq. (3), into a single spinor Ψkσ = (akσ, bkσ)T ,where superscript T means transposed matrix. In this representation the Hamiltonian Eq. (2) becomes

H =∑kσ

Ψ†kσHkΨk, where Hk = −t(

0 f(k)f∗(k) 0

). (5)

9

Figure 2: (Color online) Electronic dispersion of single-layer graphene. The single-layer graphene conductance band(top red-and-blue surface) touches the valence band (bottom yellow-and-green surface) at K,K′ points in the reciprocal space.

The function f(k) is very common in the theoretical description of the single-particle graphene spectrum. It

is defined as follows f(k) =∑3j=1 exp(ikδj), with δj being the nearest-neighbor vectors (see Fig. 1). These

vectors are equal to

δ1 =a0

2(1,√

3), δ2 =a0

2(1,−

√3), δ3 = −a0(1, 0). (6)

Thus,

f(k) = exp(−ia0kx)

[1 + 2 exp

(3ia0kx

2

)cos

√3a0ky

2

]. (7)

The function f∗ in Eq. (7) is the complex conjugate of f . The electron spectrum is obtained by diagonalizingthe matrix Hk. It is given by

ε(1,2)k = ±t|f(k)|. (8)

The functions ε(1,2)k are shown in Fig. 2.

As it follows from Eqs. (7) and (8), the energies ε(1,2)k become zero at the corners of the Brillouin zone.

It is important to remember that of six corners of the BZ only two non-equivalent points may be chosen.These points are conventionally denoted as K and K′ (see Fig. 1). A possible choice of two non-equivalentpoints is

K =2π

3a0

(1,

1√3

), K′ =

2π

3a0

(1,− 1√

3

). (9)

All other Brillouin zone corners are connected to either K, or K′ by a reciprocal lattice vector. Near thecorners, the electronic dispersion is linear with zero effective mass, similar to relativistic massless Diracparticles

ε(1,2)K+q = ±~vF |q|, vF =

3a0t

2~, (10)

where vF is the Fermi velocity, q = k−K (or q = k−K′), and |q| |K|.

10

Thus, at low energies the single-particle spectrum of graphene consists of two Dirac cones located at the Kand K′ points of the BZ. This feature of the electronic spectrum has numerous experimental confirmations [4],and the measured value of the Fermi velocity is vF ' 106 m/s.

The Hamiltonian Eq. (2) is symmetric with respect to electron-hole exchange. Thus, the Fermi level iszero if the sample is undoped, that is, there is one electron per carbon atom. In this regime, the single layergraphene is semimetal, because the energy gap in its electronic spectrum is zero, but the density of stateson the Fermi level is also zero. Graphene becomes a metal upon electron or hole doping. The electron-holesymmetry is an accidental symmetry, it breaks when the next-to-nearest neighbor hopping amplitude t′ istaken into account. However, near the Dirac points, a non-zero t′ only renormalizes the Fermi level. Thelinear dispersion and the expression for the Fermi velocity, Eq. (10), remain the same. The value of t′ isestimated as [4]

0.02t . t′ . 0.2t (11)

(see also the discussion in subsection 3.2.1).

3.1.2. Effective Dirac equation

At low energy, the electron states of the single-layer graphene obey massless Dirac equation. To obtainthe Dirac equation one can proceed as follows. Using the transformation of the electronic operators Eq. (3),the electronic fields can be expressed as a sum of two terms, each containing single-electron states withmomenta close to a particular Dirac point, either K or K′

an = e−iKRna1n + e−iK′Rna2n, bn = e−iKRnb1n + e−iK

′Rnb2n, (12)

where the index i = 1 (i = 2) refers to the K (K′) point, and the spin label σ is suppressed. These new fieldsare assumed to vary slowly over the unit cell. To derive the desired low-energy theory we substitute thisrepresentation in the tight-binding Hamiltonian and expand the operators up to linear order in the δ’s. Theresultant effective Hamiltonian splits into two copies of the massless Dirac-like Hamiltonian, one applicablenear K, and the other around K′ [34]. In terms of first quantization, we have two 2D Dirac equations formassless fermions valid close to the Dirac points

− i~vF σ∇ψ1(r) = εψ1(r) (near K),

−i~vF σ∗∇ψ2(r) = εψ2(r) (near K′), (13)

where σ = (σx, σy, σz) are the Pauli matrices and ψi are the two-component electron wave functions. Inmomentum space we have

ψ±1 (q)=eiqr(e−iθq/2

±eiθq/2), ψ±2 (q)=eiqr

(eiθq/2

±e−iθq/2), (14)

where the ± signs correspond to two bands ε(1)q and ε

(2)q [see Eq. (10)]. The phase is defined according to

θq = arctan(qy/qx), and the normalization factor is omitted.

3.1.3. Density of states

The density of states (DOS) per unit cell ρ(ε), derived for the Hamiltonian Eq. (2), is plotted in Fig. 3. Itshows semimetallic behavior [4]. For the case considered, when we take into account only nearest-neighborshopping, it is possible to derive the analytical expression for the DOS per unit cell, which has the form [35]

ρ(ε) =4|ε|

π2t2√Z0(ε)

F

(π

2,

√Z1(ε)

Z0(ε)

), (15)

11

Figure 3: Density of states for single-layer graphene. Left panel: the density of states per unit cell as a function ofenergy in units of t. To calculate this density, the single-electron dispersion, Eq. (8), was used. For one electron per carbonatom (undoped graphene) the Fermi level corresponds to ε = 0. The right panel shows a zoom-in of the density of states closeto the Dirac point. Reprinted figure with permission from A.H. Castro Neto et al., Rev. Mod. Phys. 81 109 (2009). Copyright2009 by the American Physical Society. http://dx.doi.org/10.1103/RevModPhys.81.109

where F(π/2, x) is the complete elliptic integral of the first kind and

Z0 =

(

1 + |ε|t

)2

− [(ε/t)2−1]2

4 , |ε| ≤ t,4|ε|t , t ≤ |ε| ≤ 3t,

(16)

Z1 =

4|ε|t , |ε| ≤ t,(1 + |ε|

t

)2

− [(ε/t)2−1]2

4 , t ≤ |ε| ≤ 3t,

Close to the Dirac point

ρ(ε) ≈ 3√

3a20

πv2F

|ε|, (17)

that is, the DOS vanishes linearly when the energy approaches the Fermi level.

3.2. AA bilayer graphene

3.2.1. Single-electron tight-binding description

First, we derive the electronic spectrum of the AA bilayer graphene. The crystal structure of the AAbilayer graphene is shown in Fig. 4. The AA-stacked bilayer consists of two graphene layers, 1 and 2. Eachcarbon atom of the upper layer is located above the corresponding atom of the lower layer. Since layerconsists of two triangular sublattices, A and B, the elementary unit cell of the AA-stacked bilayer graphenecontains four carbon atoms, A1, A2, B1, and B2. The system is modeled by the tight-binding Hamiltonianfor pz electrons of carbon atoms, which includes in-plane and interplane tunneling [36]

H = −t∑〈ij〉ασ

a†iασbjασ + t0∑iσ

(a†i1σai2σ +b†i1σbi2σ

)− t′

∑〈〈ij〉〉ασ

(a†iασajασ + b†iασbjασ

)+tg

∑〈ij〉σ

(a†i1σbj2σ + a†i2σbj1σ

)+ h.c. (18)

The first sum in this expression is the in-plane nearest-neighbor hopping, as in a graphene sheet [see Eq. (2)],the second sum describes the nearest-neighbor inter-plane hopping with amplitude t0, the third and the

12

A1

A2

B1

B2

Figure 4: (Color online) Crystal structure of the AA-stacked bilayer graphene. The circles denote carbon atoms in the A (red)and B (blue) sublattices in the bottom (1) and top (2) layers. The unit cell of the AA-stacked bilayer graphene consists of fouratoms A1, A2, B1, and B2. Hopping integrals t and t0 correspond to the in-plane and interplane nearest-neighbor hopping, t′

and tg correspond to the in-plane and interplane next-nearest-neighbor hopping.

fourth sums correspond to the in-plane and interplane next-nearest-neighbor hopping with amplitudes t′

and tg, respectively. The symbol 〈〈. . .〉〉 denotes summation over the next-nearest-neighbor sites.The values of the hopping integrals can be obtained from the ab initio calculations and tight-binding fit

to experiments. The value of t is well-established and lies within t = 2.5–3 eV [4, 37, 38, 39]. The interplanenearest-neighbor hopping integral is much weaker, t0 = 0.3–0.4 eV [4, 37, 38, 39]. The integral t′ is notwell known. The ab initio calculations performed by S. Reich et al. [40] indicate that 0.02t < t′ < 0.2tdepending on the tight-binding parametrization. A fit to cyclotron resonance experiments in the single-layergraphene done by R. S. Deacon et al. [41] finds t′ ≈ 0.1 eV. The interplane next-nearest-neighbor integraltg is significantly smaller than the others. Ab initio calculations performed in Ref. [38] estimated thattg ≈ −0.03 eV.

At first, we disregard next-nearest-neighbor hoppings (which will be considered at the end of this Section)keeping only the first two terms in the Hamiltonian Eq. (18). The unit cell of the AA bilayer contains fouratoms, and electronic spectrum consists of four bands εs0k, where s = 1, 2, 3, 4. The eigenenergies εs0k can beobtained by the same method we used for the single-layer graphene. We transform the Hamiltonian Eq. (18)into the k-space representation, and introduce the four-component spinor

Ψkσ = (ak1σ, ak2σ, bk1σ, bk2σ)T . (19)

Without the next-nearest-neighbor hopping, the Hamiltonian Eq. (18) can be written asH =∑

kσ Ψ†kσHkΨkσ,

where the 4×4 matrix Hk has the form

Hk =

0 t0 −tf(k) 0t0 0 0 −tf(k)

−tf∗(k) 0 0 t00 −tf∗(k) t0 0

. (20)

The spectrum of this Hamiltonian is comprised of four energy bands

ε(1)0k = −t0 − t|f(k)|, ε

(2)0k = +t0 − t|f(k)|, ε

(3)0k = −t0 + t|f(k)|, ε

(4)0k = +t0 + t|f(k)|, (21)

which are plotted in Fig. 5. The spectrum consists of two copies of the single-layer spectrum. One copy(bands 2 and 4) is shifted to higher energies by the amount t0. The other copy (bands 1 and 3) is shifted

13

Figure 5: (Color online) (a) Single-particle band structure of the AA-stacked bilayer graphene.It consists of two single-layered

graphene spectra shifted relative to each other by the energy 2t0. (b) The k dependence of the spectra ε(s)0k near the Dirac point

K. Here, k = K + qey . The bands s = 2 and 3 cross each other exactly at zero energy, which corresponds to the Fermi levelof the undoped system. (c) The first Brillouin zone (hexagon) and the reciprocal-lattice unit cell (rhombus) of the AA-stackedgraphene bilayer. The (green) circles around K and K′ points represent (degenerate) Fermi surfaces (Fermi arcs).

down by the amount −t0. In this approximation the spectrum possesses electron-hole symmetry. Near theDirac points, the bands 1 and 2 are hole-like, whiel the bands 3 and 4 are electron-like. Under the action ofthe electron-hole transformation, bands 1 and 4 are transformed into each other. The same is true for bands2 and 3. The first Brillouin zone, shown in panel (c) of Fig. 5, is the same as that for single-layer graphene(see Fig. 1). If the bilayer is undoped, bands s = 2 and 3 cross the Fermi level near the Dirac points K andK′. In such a situation, the Fermi surfaces are given by the equation |f(k)| = t0/t. Since t0/t 1, we canexpand the function |f(k)| near the Dirac points and find that the Fermi surface consists of two circles withradius kr = 2t0/(3ta0). Thus, the AA-stacked graphene bilayer is a metal even in the case of zero doping.

A striking feature of this tight-binding band structure is that for zero doping the Fermi surfaces of bothbands coincide. That is, the electron and hole components of the Fermi surface are perfectly nested. Thissingle-electron property is quite stable against changes in the tight-binding Hamiltonian. It survives evenif longer-range hoppings are taken into account, or a system with two nonequivalent layers is considered(e.g., similar to the single-side hydrogenated graphene [42, 43, 44]). However, an arbitrarily small electroninteraction can destabilize such a degenerate spectrum, generating a gap (see subsection 10.1). On the otherhand, upon doping the nesting is violated, and the Fermi surfaces transform into four circles.

As in the case of the single-layer graphene, the spectrum of the AA-stacked graphene bilayer is linearnear the Dirac points. Expanding Eq. (21) near the Dirac points in powers of |q| = |K−k|, |K′−k| |K|,we derive in the lowest-order approximation

ε(1,2,3,4)0K+q = ∓t0 ∓ ~vF |q|. (22)

The Fermi velocity for the AA-stacked graphene bilayer is the same as for the single-layer graphene.The electron-hole symmetry breaks, if we take into account the next-nearest-neighbors hopping. In this

case, the Hamiltonian in k-representation becomes

Hk =

−t′F (k) t0 −tf(k) tgf(k)

t0 −t′F (k) tgf(k) −tf(k)−tf∗(k) tgf

∗(k) −t′F (k) t0tgf∗(k) −tf∗(k) t0 −t′F (k)

, (23)

where

F (k) = |f(k)|2 − 3 = 2 cos(√

3kya0)+4cos

(√3kya0

2

)cos

(3kxa0

2

). (24)

14

The electron bands satisfy the equations

ε(1)k = −t′F (k)− t0 − (t+ tg)|f(k)|, ε

(2)k = −t′F (k) + t0 − (t− tg)|f(k)|,

ε(3)k = −t′F (k)− t0 + (t+ tg)|f(k)|, ε

(4)k = −t′F (k) + t0 + (t− tg)|f(k)|. (25)

The expansion of the spectrum around the Dirac point, up to second order in |q|/|K|, is given by

ε(1,2)q = 3t′∓t0−~vF

(1± tg

t

)|q|− 3

4

(3t′− t±tg

2sin(3θq)

)a2

0|q|2, (26)

ε(3,4)q = 3t′∓t0+~vF

(1± tg

t

)|q|− 3

4

(3t′+

t±tg2

sin(3θq)

)a2

0|q|2.

These equations demonstrate that, to lowest order in |q|, the next-nearest-neighbor hopping t′ shifts theposition of the Fermi level: the first term 3t′ is the same for all four bands, and can be absorbed into thechemical potential µ. The interlayer next-nearest-neighbor hopping tg breaks the electron-hole symmetrymore dramatically: if tg 6= 0, the renormalized electron and hole Fermi velocities become unequal to eachother. Corrections to the linear dispersion are also electron-hole asymmetric. Note that up to order q2/K2

the dispersion depends on the direction in momentum space and has a threefold symmetry (so-called trigonalwarping of the electronic spectrum [4]).

Despite electron-hole asymmetry and the trigonal warping, the nesting of the Fermi surface persists. To

prove this claim one must solve the equations for the electron Fermi surface (ε(3)k = µ), and the hole Fermi

surface (ε(2)k = µ), and demonstrate that the resultant surfaces (lines) coincide. The required equations are:

[−t′F (k) + tg|f(k)|] + t0 − t|f(k)| = µ, (27)

[−t′F (k) + tg|f(k)|]− t0 + t|f(k)| = µ. (28)

We can demonstrate that the solution of these equations correspond to the perfect nesting: both Fermisurfaces are defined by the relation

|f(k)| = t0t,

with the chemical potential

µ = −t′(t20/t2 − 3) + (t0tg/t).

These statements are easy to check, if one remembers that the function F (k) can be expressed in terms ofthe function f(k) according to Eq. (24). The stable nesting has important implications for the robustnessof the broken symmetry phases, which will be discussed below.

3.2.2. Density of states

The density of states of the AA-stacked bilayer graphene can be calculated using the expression

ρ(ε) =∑s

ˆ

VBZ

d2k

VBZδ(ε− ε(s)

k

), (29)

where the integration is taken over the volume of the Brillouin zone VBZ = 8π2/3√

3a20, and δ(x) is the

Dirac delta-function. The results are shown in Fig. 6. As it is seen from this figure, the DOS is non-zeronear the Fermi-level even in the case of the undoped system. The function ρ(ε) is flat near ε = 0, whereenergy bands s = 2 and 3 intersect: the DOS is almost constant in the energy range |ε| < t0, and

ρ(0) =4πt0

~2v2FVBZ

=2t0

π√

3t2.

Each band of the bilayer has one van Hove peak, inherited from a single-layer graphene spectrum. As aresult, the bilayer DOS has four van Hove singularities, clearly seen in the graph. If we take into accountnext-nearest-neighbor hopping, the electron-hole symmetry of the DOS is violated. This effect, however, isnot strong, especially in the energy range smaller than van Hove singularities.

15

Figure 6: (Color online) Density of states of the AA-stacked bilayer graphene. Red solid curve is calculated for tg = 0 andt′ = 0, while blue dashed curve corresponds to tg = −0.03 eV and t′ = 0.1 eV. For both cases t = 2.57 eV, t0 = 0.36 eV.Density of states of the single-layer graphene (t′ = 0) is shown by black dotted curve for comparison.

3.2.3. Effect of the bias voltage

The electronic properties of graphene systems can be tuned by the application of electric field transverseto the layers [45]. For the bilayer systems, the corresponding term in the Hamiltonian reads

HV =eV

2

∑jσ

(nj1σ − nj2σ) , where njασ = a†jασajασ + b†jασbjασ, (30)

and V is the bias voltage produced by the applied electric field in the bilayer. Operator njασ is the electronoccupation number corresponding to spin σ and lattice site Rj in the layer α = 1, 2. In the bi-spinorrepresentation, the corresponding 4×4 matrix is

HV =e

2

V 0 0 00 −V 0 00 0 V 00 0 0 −V

. (31)

The quantity V is the effective, not “bare”, voltage. It differs from the bare voltage V0 due to the partialscreening of the external electric field by the redistribution of the charge between the layers. This screeningmay significantly modify the resultant spectrum, as seen experimentally in, e.g., Ref. [46]. Combining HV

with the tight-binding Hamiltonian (20), we derive the spectrum of biased graphene, which coincides withEq. (21), if we substitute the interlayer hopping integral t0 by a renormalized value

t0 →

√t20 +

(eV

2

)2

. (32)

Thus, as far as the band energies ε(s)k are concerned, the application of the bias voltage to the bilayer

effectively increases the interlayer hopping, but the qualitative structure of the electronic spectrum remainsthe same. However, the quantitative details of the band structure may be affected by the transverse electric

16

Figure 7: Bernal stacking. If we start from AA stacking (see Fig. 4) and then shift the top layer by the vector −δ3, wearrive at the AB, or Bernal, stacking of the bilayer. In this arrangement A2 sublattice lies opposite to B1 sublattice. “Thedimer sites” from these sublattices are connected by green lines. The “non-dimer” sites lie against the centers of the hexagonsin the opposite layer. Besides the hopping between the dimer sites t0, one can introduce the hopping t3 from a non-dimer siteto nearest non-dimer sites in the opposite layer (shown by black dashed lines), and hopping t4 from a dimer site to nearestnon-dimer sites of the opposite layer (shown by dashed red lines). The amplitude t3 introduces so-called “trigonal warping” tothe single-electron dispersion, while t4 breaks the electron-hole symmetry of the single-electron states.

field of realistic strength: if the applied electric field E0 is 107 V/cm, then, the value eV0 = eE0c0 ≈ 0.33 eV iscomparable to t0. Nonetheless, one has to remember that the substitution rule Eq. (32) may be inapplicablefor evaluation of other physical properties of the biased AA bilayer graphene. For example, the wavefunctions should not be calculated with the help of Eq. (32).

3.3. AB bilayer graphene

3.3.1. Single-electron tight-binding description

Starting from the AA-stacked bilayer it is possible to construct a bilayer with AB, or Bernal, stacking.To obtain the AB stacking (see Fig. 7) we must shift one of two layers by the vector −δ3, shown in Fig. 1.Under such a displacement sublattice A of the shifted layer ends up over the sublattice B of the immobilelayer. A pair of opposite sites from these sublattices is called “dimer sites”. Two other sublattices (B ofthe shifted layer and A of the immobile layer) will be over the centers of the hexagons of the opposite layer.The sites from these sublattices are “non-dimer”.

From the general geometry of carbon p-orbitals one expects that the overlap between the orbitals of thedimer sites is the largest. Consequently, the hopping t0 between the dimer sites is the strongest of all possibleinterlayer tunneling processes. Thus, the simplest possible description of the AB bilayer is to include onlythese tunneling amplitudes. In such an approximation, using the notation of Eq. (20), one can write for theHamiltonian in k-space

HABk =

0 0 −tf(k) 00 0 t0 −tf(k)

−tf∗(k) t0 0 00 −tf∗(k) 0 0

. (33)

For the AB bilayer, the Hamiltonian parameters are estimated as follows [47, 48, 49]

2.9 eV ≤ t ≤ 3.16 eV, 0.3 eV ≤ t0 ≤ 0.4 eV. (34)

The matrix from Eq. (33) is easy to diagonalize. The corresponding eigenenergies satisfy the equation

ε4 − 2ε2

(t2|f(k)|2 +

1

2t20

)+ t4|f(k)|4 = 0 , (35)

17

Figure 8: (Color online) Single-particle band structure of AB-stacked bilayer graphene. At large energy the spectra of AB andAA bilayers resemble each other. However, near the Dirac points thier structures are quite dissimilar. Instead of degenerateFermi surface of AA-stacked graphene (see Fig. 5), the AB bilayer has two Fermi points at which two parabolic bands toucheach other (see inset, which zooms on the area bounded by the dashed line).

which can be solved to find the following four bands(ε

(1,4)k

)2

= t2|f(k)|2 +1

2t20 +

√t20t

2|f(k)|2 +1

4t40 , (36)(

ε(2,3)k

)2

= t2|f(k)|2 +1

2t20 −

√t20t

2|f(k)|2 +1

4t40 . (37)

These bands are plotted in Fig. 8.In the vicinity of the Dirac points K (or K′), where

|f(k)| t02t, (38)

equation (36) can be expanded, and the approximate formulas for the energy bands are derived

ε(1,4)K+q ≈ ±

(t0 +

t2

t0|f(k)|2

)≈ ±

(t0 +

~2v2F

t0|q|2

), (39)

ε(2,3)K+q ≈ ±

t2

t0|f(k)|2 ≈ ±~2v2

F

t0|q|2, (40)

where we used Eq. (10) for vF, valid near the corners of the Brillouin zone. Unlike both the monolayer andAA bilayer graphene, AB bilayer bands have parabolic dispersion near K and K′ points. The bands s = 2, 3touch each other at the Dirac points. If the AB bilayer is not doped, the bands touch exactly at the Fermienergy. Two other bands (s = 1, 4) do not reach the Fermi energy.

If one is interested in the effective description of the bilayer at |ε| t0, the bands s = 1, 4 may be

neglected, since |ε(1,4)k | ≥ t0. Further, one can easily check that, if k ≈ K (k ≈ K′), the wave functions for

s = 1, 4 bands are non-zero only at the dimer sites. Conversely, the low-energy states of s = 2, 3 bands arelocalized at the non-dimer sites. Therefore, only the electrons at the non-dimer atoms participate in thelow-energy processes. The two-band (thus, superscript ‘2b’) effective Hamiltonian is equal to [5, 50]

H2bξq ≈ −

~2

2m

(0 (iqx + ξqy)2

(iqx − ξqy)2 0

), m =

t02v2

F

, (41)

18

Figure 9: Trigonal warping. When the interlayer tunneling between non-dimer sites is taken into account, the parabolicdispersion at the Dirac point is split into four Dirac cones with linear dispersion. This distorted dispersion surface is shown onthe left panel, while the right panel shows top view of the same surface, with equal-energy contours visible. The point (0,0)corresponds to a corner of the Brillouin zone, and qx,y are momenta measured from this corner. Of the four emerged Diraccones, the central is located at the corner of the Brillouin zone, while three others are shifted from the corner by the amountpL. The resultant structure complies with the underlying geometrical symmetry of the bilayer. This distortion of the originalparabolic dispersion is called “trigonal warping”. Note, however, that for t3 = 0.3 eV (the value of t3 has been estimated inRefs. [51, 52]) the warping effect is very weak. The energy εL, at which the saddle points are located, is estimated [5] to be ofthe order of 1 meV. The quantity pL is ∼ 0.007a−1

0 .

where the integer-valued index ξ is equal to +1 (-1) at the K (K′) Dirac point. The effective mass m canbe expressed in terms of the free-electron mass m0 as m = 0.033m0.

The described band structure, however, is easy to spoil. For example, the gap opens in the spectrum ifwe apply an electric field perpendicular to the bilayer plane. We will discuss this type of perturbation below,in subsection 3.3.2. In addition to the transverse field, the dispersion given by Eq. (39) may be destroyedby hopping from non-dimer sites in one layer to non-dimer sites in another layer. In Fig. 7 the tunnelingprocesses of this type are shown by dashed lines labeled by t3. The corresponding Hamiltonian matrix reads

HABk = −

0 0 −tf(k) t3f

∗(k)0 0 t0 −tf(k)

−tf∗(k) t0 0 0t3f(k) −tf∗(k) 0 0

. (42)

The spectrum of this matrix can be found exactly [50]. However, since the analytical formulas are quitecomplicated, we will not discuss them. Instead, let us direct our attention to Fig. 9. In this figure thetwo bands reaching the Fermi level are plotted in the vicinity of a Brillouin zone corner. The bands arecalculated for non-zero t3, whose value was extracted from experiment [51] and DFT calculations [52]:

t3 = 0.3 eV. (43)

As we can see, the interlayer hopping between the non-dimer sites introduces a qualitative distortion of thesingle-electron bands: the parabolic dispersion near the K and K′ points is replaced at low energy by astructure consisting of four Dirac cones. The apexes of these cones lie at the Fermi energy. The apex ofthe central cone coincides with a corner of the Brillouin zone (K, or K′). Three others are shifted from the

19

corner by a small quantity pL. This low-energy fine structure is called “trigonal warping” [50]. To accountthe warping within the two-band approximation one may work with the following effective Hamiltonian [5]:

H2bξq = H2b

ξq +H2bξqw, where H2b

ξqw = ~v3

(0 ξqy − iqx

ξqy + iqx 0

), v3 =

3a0t32~

. (44)

It is necessary to remember, however, that this warping is a very weak effect, which become noticeable onlyvery close to the K,K′ points at small energies. Specifically, the six saddle points (three for ε > 0 andanother three for ε < 0), clearly visible in Fig. 9, are at the energies ε = ±εL, where [5, 50]

εL =t04

(v3

vF

)2

≈ 1 meV, and pL =t0v3

~v2F

∼ 0.007a−10 (45)

Both εL and pL are quite small. As a result, in experiment, disorder may easily mask the warping.Finally, let us mention that to fit experimental data to the theoretically-calculated dispersion additional

tunneling amplitudes and on-site energies are often included [47, 48, 49, 51, 53, 54, 55]. As an example,in Fig. 7 the tunneling t4 between dimer and non-dimer sites is shown. This tunneling process introducessmall, however, experimentally measurable asymmetry between hole and electron states of the AB bilayer.

3.3.2. Effect of the bias voltage

The asymmetry between the layers due to, for example, the application of the transverse voltage, opensa gap in the single-electron spectrum [50, 56]. To account for the applied voltage we can generalize Eq. (33)

HABk (V ) =

eV/2 0 −tf(k) 0

0 −eV/2 t0 −tf(k)−tf∗(k) t0 eV/2 0

0 −tf∗(k) 0 −eV/2

. (46)

The eigenenergies of HABk (V ) satisfy the equation:(

ε2 − e2V 2

4

)2

−(

2ε2 − e2V 2

2

)(t2|f(k)|2 +

1

2t20

)+ t4|f(k)|4 − e2V 2t2|f(k)|2 = 0, (47)

which has four solutions:

ε(1,2,3,4)k = ±

√e2V 2

4+

1

2t20 + t2|f(k)|2 ±

√t2|f(k)|2(e2V 2 + t20) +

1

4t40. (48)

The bands s = 2, 3, which touch at the Fermi level when V = 0, do not reach the Fermi energy for V > 0.To prove this, it is convenient to expand the expression Eq. (48), assuming that the condition Eq. (38) isvalid. Thus, near the Dirac point we derive

ε(2,3)q ≈ ±

√e2V 2

4−e2~2v2

FV2

4t20|q|2 +

~4v4F

t20

(1 +

e2V 2

4t20

)|q|4. (49)

It is easy to check that the expression under the root sign is always positive when V 6= 0. If we put V = 0in this formula, Eq. (40) is recovered.

For the low-energy description, we can use the generalized Eq. (41)

H2bξk(V ) ≈

(eV/2 −~2v2F

t0(ξqy + iqx)2

−~2v2Ft0

(ξqy − iqx)2 −eV/2

). (50)

20

The dispersion relation for this Hamiltonian is as follows

ε2b±ξk = ±

√e2V 2

4+

~4v4F

t20|q|4. (51)

Apparently, this expression does not coincide with Eq. (49). The effective Hamiltonian given by Eq. (50)is a fairly coarse approximation to Eq. (46). Despite that it is being used in the theoretical literature: theHamiltonian H2b

ξk(V ), Eq. (50), is able to reproduce the gapped dispersion and significantly simplify theformalism.

As we have commented earlier, Eqs. (49) and (51) show that, for finite transverse electric field, thebilayer becomes an insulator with gap ∆ of the order of |eV |. Experiments confirmed the existence of thisgap [46, 51, 54, 57, 58, 59, 60]. For example, A. B. Kuzmenko et al. [51, 54] observed the band gap aslarge as 0.1 eV. As an additional support, the emergence of the gap was also reported by workers employingdensity functional methods (e.g., Ref. [61] discussed free-standing samples, Refs. [62, 63] investigated thesamples on a substrate). The ability to engineer the gap attracted a lot of attention, both from theoristsand experimentalists. The possibility of turning a graphene sample into a semiconductor with controlledgap appears to be a promising notion with a variety of applications, some of which will be discussed below.

3.3.3. Density of states

The density of states for AB graphene calculated by E. V. Castro et al. in Ref. [64] is shown in Fig. 10.In panel (a) the general shape of the density of states is demonstrated. Unlike the single-layer graphene, theAB bilayer has finite density of states at the Fermi energy. This is a consequence of the parabolic dispersionin two-dimensional systems:

ˆ. . .

dqxdqy(2π)2

=

ˆ. . .

d(q2)

4π=

ˆ. . . ρ(0) dε. (52)

This point is illustrated more explicitly in Fig. 10(b), where the density of states for t3 = 0 (no trigonalwarping) is presented (in the notation of E. V. Castro et al. [64] the quantity γ3 is the same as our amplitudet3).

In Fig. 10(c), the trigonal warping is accounted for. In the presence of the warping, the density ofstates vanishes linearly near the zero energy. However, this effect becomes significant only at very smallenergy/temperature.

In panel (d), the spectrum with a gap due to the transverse voltage is plotted. When the field is appliedthe gap opens, see Eq. (49). The electron states pushed from the sub-gap region pile up into two peaks atthe edges of the gap.

3.3.4. Immediate consequences of the single-electron band theory

As we have mentioned above, significant amount of experimental data concerning the electronic propertiesof the AB bilayer may be explained with the help of single-electron concepts. Thus, it is often assumed that,at not too low temperatures, single-particle models are sufficient to describe how the external perturbations(strain, disorder, radiation, electric or magnetic field, etc.) affect the electronic properties of a graphenebilayer.

For example, the AB bilayer in a magnetic field was discussed in Refs. [58, 65, 66, 67]. For low magneticfield, the semi-classical cyclotron mass for a biased AB bilayer was calculated by E. V. Castro et al. inRef. [65] for different carrier densities and bias electric fields. The effects of disorder on the bias-inducedgap were investigated. The authors [65] concluded that the gap induced by the transverse electric field isquite insensitive to the diagonal disorder. The paper also discusses the formation of Landau levels in bilayernanoribbons, using the tight-binding approximation.

Reference [58] compared the theoretical results for the cyclotron mass with experiments. The theorywas consistent with the data for samples with electron doping. Tangible disagreement between the theoryand the experiment for the hole doping was attributed to poor performance of the Hartree approximation

21

Figure 10: Density of states for graphene bilayer with AB stacking. In panel (a) the general shape of the DOSis demonstrated. Unlike single-layer graphene, the AB bilayer has a finite density of states at the Fermi energy. This is aconsequence of the parabolic dispersion, which in two-dimensional systems leads to finite density of states. In panel (b) theDOS for t3 = 0 (no trigonal warping) is presented (γ3 in the Figure is the same as our amplitude t3). In panel (c) the trigonalwarping is accounted for. In the presence of the warping, the density of states vanishes linearly near the zero energy. However,this effect becomes significant only at very small temperatures. In panel (d) the spectrum with a gap due to a transversevoltage is plotted. Reprinted from E.V. Castro et al., New J. Phys. 11, 095017 (2009).

used for calculating the electrostatic screening of the bias field. In addition, Ref. [58] consider quantumHall conductivity of a bilayer sample (see also Section 5). The gap was estimated from the data. It wasconcluded [58] that the gap could be as large as ∼ 0.1 eV. The results of Refs. [58, 65] were summarized andgeneralized in Ref. [66].

In Ref. [67], N. Nemec and G. Cuniberti calculated the magnetic-field-induced Hofstadter butterflypatterns for samples of different stackings (AA, AB, and intermediate) at zero bias.

The effects of strain on the single-electron dispersion were discussed in Refs. [61, 68, 69]. In particular,the uniaxial strain perpendicular to the layers was studied by B. R. K. Nanda and S. Satpathy [61] usingDFT. Such a perturbation changes the interlayer distance. The authors [61] concluded that the strain cannotopen the gap for AB and for AA bilayers.

The situation in which the strain of the top layer is unequal to the strain of the bottom layer was investi-gated by S.-M. Choi et al. in Ref. [68] with the help of DFT. The authors noticed that the asymmetric straininduces and electric field perpendicular to the layers. The electric field appears because the deformationssignificantly alter the layers work function. According to [68], this field generates gap in the single-electronspectrum. The authors proposed that the studied system may be used as an electromechanical switch.

The modifications to the single-electron dispersion and the Landau levels in a strained AB bilayer were

discussed by M. Mucha-Kruczynski et al. in Ref. [69]. The strain splits the parabolic bands ε(2,3)k , Eq. (39),

into several Dirac cones (this splitting resembles the trigonal warping phenomena). The number of thesecones, as well as other details of the dispersion surface, depends on the strain. The energy scale for theseeffects was estimated to be of order of a few meV. The changes in the dispersion affect the behavior of theLandau levels energies.

22

4. Dirac electrons: chirality and Klein paradox

4.1. Chiral electrons

As we have already seen, the wave functions of single-layer and bilayer graphene are spinors. Thesespinors are solutions of the Dirac equation for massless fermions, which implies specific symmetries andrelated topological properties of the charge carriers in these systems. These effects have been intensivelystudied in single-layer graphene. Let us briefly review them following Ref. [4].

Consider once more the wave functions ψ±1,2(q) of single-layer graphene near two Dirac points K and K′,Eqs. (14). According to these equations, if the phase of θq is rotated by 2π, the wave function changes sign,since it acquires a phase of π (this is commonly called Berry’s phase). This change of phase under rotationis characteristic of spinors of the particle with spin 1/2. However, this property is unrelated to a real spinof the electron, which enters the problem in a trivial manner. It is associated with a pseudospin variable,related to the two components of the wave function, and usually referred to as helicity, or chirality, whichis defined as the projection of the momentum on the pseudospin direction. To work with the chirality it isnecessary to introduce the corresponding operator. The states near K, and the states near K′ have differentchirality operators:

near K : χ1 =σq

2|q|; near K′ : χ2 =

σ∗q2|q|

. (53)

These operators commute with the respective Dirac Hamiltonians Eqs. (13). It follows from the abovedefinition that the states ψ±1,2 are also eigenstates of χ1,2,

χ1ψ±1 = ±1

2ψ±1 , χ2ψ

±2 = ±1

2ψ±2 . (54)

Therefore, electrons (holes) have a positive (negative) chirality, or helicity. Thus, the pseudospin can beeither parallel, or antiparallel to the momentum q. The chirality values are good quantum numbers only nearthe Dirac points, as long as Eqs. (13) are valid, and the spectrum is linear. Thus, it is only an asymptoticproperty, and at larger energies the chirality stops being a good quantum number.

The states near a particular Dirac point, either K or K′, are commonly referred to as valleys [4]. Eachvalley can be characterized by a valley index ξ = ±1, where ξ = +1 corresponds to K, and ξ = −1 toK′, respectively. Using this index, we can rewrite the Dirac equations Eq. (13) for electrons in single-layergraphene in the form

Hψξ(r) = εψξ(r), H = −i~vF

(0 ∂

∂x − iξ∂∂y

∂∂x + iξ ∂∂y 0

)(55)

Thus, if we consider only low-energy processes and disregard hopping, which can break electron-holesymmetry, then, the intervalley scattering is absent, and the valley index is conserved. However, the inter-actions, which break both the inversion symmetry of the lattice and time-reversal, also break the symmetrybetween the two valleys [4]. Therefore, the electron scattering becomes valley dependent, and, in general,electrons from different valleys propagate along different paths. The chiral Dirac nature of fermions ingraphene might be of use for applications where one can control the valley flavor of the electrons besides itscharge, the so-called valleytronics [4, 70, 71].

4.1.1. AA bilayer graphene

Here we consider the chiral properties of AA bilayer graphene. Note, however, that up to now only afew works treated this subject.

As it is readily seen from the previous consideration, the low-lying energy spectrum (ε t0) of theAA graphene is made up of two Dirac cones, one shifted to higher energy, and other one shifted to lowerenergy, see panel (b) of Fig. 5. These cones intersect each other at ε = 0, forming a circular Fermisurface, instead of the Fermi point for single-layer graphene. Similar to single-layer graphene, the low-lying electronic excitations in AA-stacked bilayer graphene can be treated asymptotically as massless Dirac

23

fermions. Expanding the function f(k) [see Hamiltonian of Eq. (20)] to lowest order in either q = K − k,or q = K′ − k, one obtains f(k) ≈ ~vF|q|e∓iθq , where the ‘minus’ (‘plus’) sign corresponds to the K(K′) valley. It is convenient to express the four-component spinor Ψq = (aq1, bq1, aq2, bq2)T in the formΨq = (ψ1q, ψ2q)T , where ψiq = (aqi, bqi)

T are the two-component spinors constructed from the electronoperators in layer i = 1, 2. We also introduce two sets of Pauli matrices σ and τ , where the σ matrices acton the sublattice index, while the τ matrices act on the layer index. Then, in the real-space representation,the corresponding Dirac equation can be written as

HΨq(r) = εΨq(r) , (56)

withH = τx ⊗

(t0I − i~vFσ∇

)(near K), H = τx ⊗

(t0I − i~vFσ

∗∇)

(near K′), (57)

where the symbol A⊗B denotes the direct product of the matrices A and B, and symbol I is the 2× 2 unitmatrix.

Following notations by M. Sanderson et al. in Ref. [72], we introduce the band indexes η1 = ±1 andη2 = ±1. In this notation the spectrum Eq. (22) can be rewritten as

εqη1η2 = η1 (η2t0 + ~vF|q|) , (58)

with eigenvectors

ψqη1η2 =eiqr

2

η1e−iθq

η1η2

η2e−iθq

1

. (59)

For the Hamiltonians of Eq. (57) we can define two operators for two conserved quantities

C = γ5 = τx ⊗ I , χ1 = τx ⊗σq

q(near K), or χ2 = τx ⊗

σ∗qq

(near K′). (60)

where γ5 is the fifth Dirac gamma matrix. The operators χ1,2 can be considered as chirality operators

(the analog of the chirality operators for single-layer graphene). Regarding C, it can be referred to as thecone operator [72]. Both C, and χ1,2 are the direct products of τx, with either I or chirality operators forsingle-layer graphene, Eq. (54). The authors of Ref. [72] introduced the cone c ≡ η1η2, and chirality χ ≡ η1

indexes. The energy bands can now be labeled by these indexes as

εqcχ = ct0 + χ~vF|q|, (61)

with the eigenvectors

ψqcχ = eiqr

χe−iθq

ccχe−iθq

1

. (62)

Thus, each band is characterized by two numbers (c, χ): the first band has (c = χ = −1), the second(c = +1, χ = −1), the third (c = −1, χ = +1), and the fourth (c = χ = +1).

It can be readily shown that Cψqcχ = cψqcχ, and χ1,2ψqcχ = χψqcχ. A quasiparticle state belongs to theupper (lower) cone, if c = +1 (c = −1). The physical significance of the χ eigenvalue becomes immediatelyobvious if we consider the group velocity vqcχ ≡ ∂εqcχ/∂q = χvFq/|q|. A quasiparticle state is electron-like(i.e., vqcχ is parallel to q) if χ = +1, and hole-like (i.e., vqcχ is anti-parallel to q) if χ = −1. Finally, let usnote that these discrete quantum numbers can also be defined for the lattice model [36, 73].

In addition, as in the case of single-layer graphene, we could introduce also the valley index ξ, and rewritethe Hamiltonian Eq. (57) as

H = τx ⊗

[t0I − i~vF

(0 ∂

∂x − iξ∂∂y

∂∂x + iξ ∂∂y 0

)]. (63)

Here ξ = +1 corresponds to the point K and ξ = −1 corresponds to the K′ point.

24

Figure 11: (Color online) Klein tunneling in single-layer graphene. Left panel: schematic of the scattering of Diracelectrons by a rectangular potential. Right panel shows the definition of the angles θ and φ used in the scattering formalism inregions I, II, and III.

4.1.2. AB bilayer graphene

If we are interested only in electrons whose energy is low (ε t0), but not too low [ε εL, see Eq. (45)],we can neglect the trigonal warping and use the effective Hamiltonian of the AB-stacked graphene bilayer inthe form of Eq. (41). In this effective Hamiltonian, the valley index ξ is already included. Hamiltonian (41),together with the Hamiltonian of single-layer graphene, may be viewed as the first two members of theinfinite sequence of chiral Hamiltonians HJ (J = 1, 2, . . . ), corresponding to Berry’s phase Jπ [5]

HJ ∝(

0 (π†)J

(π)J 0

), (64)

whereπ = ξ∂/∂x+ i∂/∂y and π† = ξ∂/∂x− i∂/∂y. (65)

It is convenient to generalize this series for negative J as well

HJ ∝(

0 (π)|J|

(π†)|J| 0

), for J < 0. (66)

The chiral Hamiltonian (41) has a single Dirac point at q = 0, the spectrum is rotationally invariant, and thephase difference between sublattices changes by 2× 2π when the quasiparticle-momentum circles the Diracpoint. This property is referred to as J = 2 chirality, or winding number +2. When trigonal warping isincluded, the conduction and valence bands touch each other not only at q = 0, but also at three additionalq 6= 0 points (see Fig. 9). The central Dirac point at q = 0 has winding number J = −1, whereas the threesurrounding points have J = 1.

4.2. Klein tunneling and chiral scattering

A striking peculiarity of electron scattering in graphene systems is the so-called Klein tunneling, whichis a characteristic of electrons with linear dispersion. We start by calculating the transparency of therectangular barrier in single-layer graphene for electrons near the Dirac point [4]. In Fig. 11 we depict thescattering process due to the square barrier of width D and height V0. We further assume that the scatteringdoes not mix the momenta around the K and K′ points.

Using the spinor representation Eq. (14), we can rewrite the wave function of the electron with momentumk (near the K point) and energy E in the different regions ψI,II,III in terms of incident and reflected waves

ψI = ψ(χ, φ)eikxx + rψ(χ, π − φ)e−ikxx,

ψII = aψ(χ′, θ)eiqxx + bψ(χ′, π − θ)e−iqxx,ψIII = τψ(χ, φ)eikxx, (67)

25

Figure 12: (Color online) Angular behavior of the transmission coefficient T (φ) for single-layer graphene calculated for twodifferent values of the barrier height V0: V0 = 200 meV, dashed (blue) curve; V0 = 285 meV, solid (red) curve. The barrierwidth is D = 110 nm for the top panel and D = 50 nm for the bottom panel. For all curves the energy of the transmittedelectrons is E = 80 meV, and the Fermi momentum is kF = 2π/50 nm−1 Reprinted figure with permission from A.H. CastroNeto et al., Rev. Mod. Phys. 81 109 (2009). Copyright 2009 by the American Physical Society. http://dx.doi.org/10.1103/

RevModPhys.81.109

where

ψ(χ, φ) =

(1

χeiφ

)eikyy, (68)

and φ = arctan(ky/kx), kx = kF cosφ, ky = kF sinφ, kF is the Fermi momentum, θ = arctan(ky/qx),

qx =√

(V0 − E)2/v2F − k2

y, with chiralities χ = sign(E) and χ′ = sign(E − V0). Unlike the non-relativistic

Schrodinger equation, we only need to match the wave function, but not its derivative. As a result, we findthe transmission coefficient of the barrier T (φ) = |τ |2 in the form [4]:

T (φ) =cos2 φ cos2 θ

[cos(Dqx) cosφ cos θ]2 + sin2(Dqx)(1−χχ′ sinφ sin θ)2. (69)

The transmission is ideal [T (φ) = 1] for normal incident electrons (φ = 0, and θ = 0) even for very high(V0 E) and long (Dqx 1) barriers. This property is referred to as the Klein paradox, and it does notoccur for non-relativistic electrons. Note, that chirality is not conserved in the process of scattering. Thedependence of the transmission coefficient T on the incident angle φ is shown in Fig. 12.

As it follows from Eq. (67), the electrons moving through a barrier separating the regions of n- andp-doped graphene (regions I and II in Fig. 11) are transmitted as holes. For a hole, the momentum andvelocity are opposite vectors. This behavior is the same as that of photons moving in a medium with negativerefraction index [4].

Klein tunneling and related phenomena in graphene were discussed in numerous papers [74, 75, 76, 77, 78]and reviews [4, 79, 18] Note, however, that typically the authors assume a ballistic regime; that is, they

26

suppose that the mean free path of the charge carriers exceeds D. Otherwise, some delicate effects mightdisappear [80].

4.2.1. Klein scattering in AA-stacked bilayer graphene

The scattering of the charge carriers by barriers in AA bilayer graphene was studied theoretically byseveral authors. The scattering of electrons by a rectangular potential barrier in AA-stacked bilayer graphenewas analyzed in detail by M. Sanderson et al. in Ref. [72]. A standard barrier geometry shown in Fig. 11 wasconsidered. The wave function of the electron with momentum k near the K point has the same structureas the wave function in Eq. (67). This time, however, instead of the two-component spinor ψ(χ, φ), Eq. (68),we have the four-component spinor Eq. (62), which is convenient to write in the form

ψ(c, χ, φ) =

χeiφ

ccχeiφ

1

eikyy. (70)

As compared with the single-layer graphene, the electron in AA bilayer graphene is characterized by thesecond topological number c (cone index).

The calculation described in the previous subsection can be adopted for the derivation of the transmissioncoefficient for AA bilayer graphene. As a result, we obtain that Eq. (69) is valid for the AA-stacked bilayergraphene, if we consider electrons with the same cone index [72]. While the electron can change its chiralityin the scattering process, the cone index is conserved. This can be understood by considering the steppotential as a sudden perturbation [72]. The probability for an initial wave function ψ(c, χ, φ) to undergo asudden transition into a new state of ψ(c′, χ′, φ′) is given by

P = 〈ψ†(c′, χ′, φ′)ψ(c, χ, φ)〉 ≡ (1+cc′)(1+χχ′ei(φ′−φ)). (71)

This means that the transition probability c→ −c is strictly zero.Due to the orthogonality of states with different cone indexes, electron transport across a potential

barrier must conserve the cone index, and this leads to protected cone transport, which is unique in AAbilayer graphene. Together with the negative refraction of electrons, electrons residing in different cones canbe spatially separated according to their cone index when transmitted across an n-p junction. This suggeststhe possibility of ‘cone-tronic’ devices based on AA-stacked bilayer [72]. A detailed study of conductance ofthe junctions is also performed in Ref. [72]

The Klein tunneling in AA bilayer graphene in the presence of a magnetic field and a bias voltage wasstudied by D. Wang and G. Jin in Ref. [81].

4.2.2. Klein scattering in AB-stacked bilayer graphene

A comprehensive study of chiral Klein tunneling in AB-stacked bilayer graphene is presented in the reviewpaper by T. Tudorovskiy et al., Ref. [79], where different barrier configurations were analyzed. Here we onlypresent some general ideas and apply these to calculate the transmission coefficient for the rectangularbarrier in Fig. 11.

As usual for the problem of Klein tunneling of chiral electrons in graphene, we consider low-energyexcitations, |E|, |E − V0| t0. In this case, the effective Hamiltonian is given by Eq. (41). Further, fordefiniteness, we consider the valley with ξ = 1. For not-too-small wave vectors k, the effects of trigonalwarping may be neglected [79]. Indeed, if k pL, the warping is not important (see subsection 3.3).

Let us now consider an electron incident on the potential step barrier u(x) shown in Fig. 11 at an angleφ. Since the potential is constant in the y-direction, we can write the solution as ψ(x, y) = ψ(x) exp (ikyy).Inserting this into the Schrodinger equation with the Hamiltonian Eq. (41), we obtain(

d2

dx2− k2

y

)2

ψ =

[m (E − u(x))

~2

]2

ψ, (72)

27

where m is the effective mass of the quasiparticle in the AB bilayer [see Eq. (41)]. Equation (72) has foursolutions: two propagating waves exp(±ikxx), one exponentially growing, and one exponentially decayingmodes exp(±κxx). The presence of evanescent modes is markedly different from both the Schrodinger case,and the Dirac case [79]. The parameters kx,y and κx satisfy the relations

k2x + k2

y =m |E − u(x)|

~2, κ2

x − k2y =

m |E − u(x)|~2

. (73)

In what follows, we assume that the barrier is high, V0 > E + ~2k2y/2m.

Now let k =√

2mE/~ be the wave vector for the propagating modes in the region I and III (see Fig. 11),while q =

√2m(E − V0)/~ is the wave vector in the region II. Then, the solution in regions I, II, and III is

given by

ψI =

(1

χe2iφ

)eikxx + r

(1

χe−2iφ

)e−ikxx + c1

(1

−χh1(φ)

)eκxx,

ψII = a2

(1

χ′e2iθ

)eiqxx + b2

(1

χ′e−2iθ

)e−iqxx (74)

+c2

(1

−χ′h1(θ)

)eiλxx + d2

(1

−χ′/h1(θ)

)e−iλxx,

ψIII = τ

(1

χe2iφ

)eikxx + c3

(1

−χ/h1(φ)

)e−κxx,

where ky = k sinφ, kx = k cosφ, κx = k√

1 + sin2 φ, h1(φ) =(√

1 + sin2 φ− sinφ)2

, qx = q sin θ, and

λx = q√

1 + sin2 θ. To obtain constants in Eqs. (74), we have to match the spinor ψ and its derivativedψ/dx, as in the case of the usual Schrodinger equation.

For the case of normal incidence φ = θ = 0, we can solve the problem analytically. The transmissioncoefficient is given by [79]

T (0) =8k2q2

(k2 + q2)2 cosh (2qD) + 6k2q2 − k4 − q4. (75)

When 2qD 1, the transmission probability becomes exponentially small, even at normal incidence.In the general case, the transmission T (φ) = |τ |2, or reflection R(φ) = |r|2 coefficients can be found only

numerically [79]. Similar to the case of single-layer and AA bilayer graphene, there are angles, at whichthe transmission is perfect. The existence of such angles in bilayer graphene means that we cannot lock aconventional transistor made of AB-stacked bilayer graphene.

The results obtained in considering the Klein tunneling can be applied for analyzing pn-junctions [79](see also Section 7.4).

5. Bilayer graphene in a magnetic field: Landau levels and quantum Hall effect

One of the most common approaches for investigating the band structure of metals and semiconductorsis to study Landau levels using magneto-optics or magneto-transport measurements. In this section weconsider the properties of bilayer graphene in a magnetic field. In the tight-binding approximation, thehopping integrals are replaced by a Peierls substitution

tRR′ ⇒ tRR′ exp

(ie

~c

ˆ R′

R

A · dr

)= tRR′ exp

(2πi

Φ0

ˆ R′

R

A · dr

), (76)

where tRR′ is the hopping integral between the sites located at R and R′ (calculated at zero magneticfield), the quantity A is the vector potential of the magnetic field, and 2π~c/e = Φ0 is the flux quantum.Correspondingly, for the effective Hamiltonian, near the Dirac points, we should replace

− i~∇ ⇒ −i~∇ + eA/c . (77)

28

When a uniform magnetic field B is applied perpendicular to the graphene plane, we can use the Landaugauge: A = B(−y, 0). For the case of single-layer graphene, such a problem was analyzed in details in manypapers (see the review Ref. [4]). Here we are interested in the low-energy electron states with momenta nearthe Dirac points. For massless charge carriers with linear dispersion, the cyclotron frequency is [4]

ωc =√

2vFlB, (78)

where

lB =

√c~eB

(79)

is the magnetic length. The energies of the Landau levels are given by

E±LL(n) = ±~ωc√n, (80)

where n = 0, 1, 2, .... The Landau levels for both Dirac points, K and K′, have exactly the same spectrum.Hence each Landau level is doubly-degenerate due to the valley factor, and also doubly degenerate due tothe spin factor. Thus, the total degeneracy of each level in single-layered graphene is four. The Landau levelenergies for graphene scale as

√Bn (while for the electrons with quadratic dispersion: ELL ∝ Bn). Such a

behavior for single-layer graphene was confirmed in a number of experiments. The energy scale associatedwith the magnetic field for Dirac fermions is rather different from that found in the ordinary 2D gas ofmassive non-relativistic electrons. For instance, for fields of the order of B = 10 T, the cyclotron energy ~ωcin the 2D electron gas is of the order of 10 K, while in graphene it is about 400 K. This implies that thequantum Hall effect can be observed at room temperature [82].

The Landau level spectrum of a conventional two dimensional semiconductor is

ELL = ~eB

mc

(n+

1

2

), n ≥ 0, (81)

where eB/mc is the cyclotron frequency for massive charge carriers with quadratic dispersion [83]. As theelectron density is changed, there is a step in the Hall conductivity whenever a Landau level crosses theFermi level, and the separation of steps on the density axis is equal to the maximum carrier density perLandau level, NfB/Φ0, where Nf is a degeneracy factor. Each plateau of the Hall conductivity occursat a quantized value of nNfe

2/2π~, where n is an integer labeling the plateau. Steps between adjacentplateaus have height Nfe

2/2π~. In single-layer graphene there exist a zero-level state and all of the levelsare fourfold degenerate. The corresponding steps of the Hall conductivity have the height 2e2/π~ betweeneach plateau, but the plateaus occur at half-integer values of 2e2/π~ instead of integer ones, which wasobserved experimentally [24, 84]. This is due to the existence of the level at zero energy, which contributesto a step of height 2e2/π~ at zero density.

5.1. Landau levels and integer quantum Hall effect in AA-stacked bilayer graphene

5.1.1. Landau levels

The effects on the AA-stacked bilayer graphene due to a constant uniform magnetic field were discussedby several authors (see, e.g., Refs. [85, 86, 87, 88, 89]). In all of these studies the electron-electron interactionwas neglected and the electronic spectrum considered was gapless (see Fig. 5). One must remember, however,that the interaction could open a gap in the bilayer single-electron spectrum (Section 10). The presence ofsuch a gap may significantly affect the system behavior in a magnetic field.

Following Refs. [85, 87] we consider electrons near the Dirac cone in AA-stacked bilayer graphene placedin a constant uniform transverse magnetic field B with a bias voltage V across the layers. Then, in theLandau gauge we have to replace in the Hamiltonian Eq. (57) the term

− i~ ∂/∂x ⇒ −[i~ ∂/∂x+ (e/c)yB] (82)

29

and renormalize the interlayer hopping integral t0 according to Eq. (32). The solution Ψ(x, y) of the Diracequation HΨ = EΨ with renormalized Hamiltonian Eq. (57) is sought in the form eikxΨ(y). Solving theeigenvalue problem, we obtain the Landau levels for AA bilayer graphene [85, 87]

EηλLL(n) = −η~ωc√n− λ

√t20 +

(eV

2

)2

. (83)

The corresponding eigenfunctions are

Ψ1λk0(y) =

1√2

[0, Q0(ζ), 0, λQ0(ζ)]T, if n = 0 ,

Ψηλkn(x) =

1

2[Qn−1(ζ), ηQn(ζ), λQn−1(ζ), ηλQn(ζ)]

Tif n ≥ 0 . (84)

In these equations, η = ±1, λ = ±1, and

Qn(ζ) = 2−n/2(n!)−1/2 exp(−ζ2/2

)Hn(ζ), (85)

where Hn(ζ) are the Hermite polynomials and dimensionless variable ζ = y/lB + klB . Clearly, the Landaulevels of the AA bilayer graphene are nothing but two copies of the Landau levels of single-layer grapheneshifted up and down by

√t20 + e2V 2

0 /4. The Landau levels in the AA bilayer are four-fold degenerate, as inthe case of the single-layer graphene.

Five Landau energy levels (n = 1, ...5) with ηλ = −1 are shown in Fig. 13 (a) and (b) as functions of themagnetic field (figures are taken from the D. Wang, Ref. [87]).The levels with ηλ = −1 cross each other. TheLandau levels of the AA-stacked bilayer graphene can be effectively modified by the bias potential betweenthe layers [see Fig. 13 (c)]. In general, one could adjust B and V , and fine tune the energy of a particularLandau level to Fermi energy. For this to happen, V and B must satisfy the equation [87]

B =c

2n~v2F e

√t20 +

e2V 2

4. (86)

The obtained dependence B(eV = U) is shown in Fig. 13 (d).The effect of the strong spatial inhomogeneity of the magnetic field on the Landau levels in the AA-

stacked bilayer graphene was studied by D. Wang and G. Jin in Ref. [89].The magneto-optical absorption spectra of AA-stacked bilayer graphene was analyzed theoretically by

Y.-H. Ho et al. in Ref. [86]. They showed that these spectra exhibit two kinds of absorption peaks resultingfrom two groups of Landau levels classified from the selection rule based on electronic band symmetry. Onlyintragroup excitations that satisfy the selection rule take place. The magneto-optical absorption spectraof AA-stacked bilayer graphene are different from the spectra of AB-stacked bilayer graphene. This resultcould offer a way to distinguish AA-stacked bilayer graphene from AB stacking and monolayer graphene.However, it should be taken into account that the results for the absorption spectra of AA-stacked bilayergraphene were obtained in Ref. [86] disregarding the possible existence of the gap in the electronic spectrum.

5.1.2. Conductivity in the magnetic field and integer quantum Hall effect

The conductivity of AA-stacked bilayer graphene in a magnetic field can be easily derived in the cleanlimit using the Kubo formalism described in Section 9. The corresponding calculations were done in Refs. [85,87] in the case of zero temperature (that is, T ~ωc/kB). The resultant expression for the Hall conductivityis

σxy = − e2

π~sgn(eB)sgn(µ)

θ(g+)θ(g−) +

[g2

+

2

]+[θ(g+ +

√2) + θ(g− −

√2)− 1

] [g2−2

], (87)

30

Figure 13: (Color online) Five (n = 1, ...5) Landau levels in the AA-stacked bilayer graphene (from Ref. [87]) with ηλ = −1 asfunctions of the magnetic field B for two interlayer potential differences U = eV : (a) U = 0 and (b) U = 200 meV. (c) Landaulevels in AA-stacked bilayer graphene as a function of U for B = 16 T. (d) It is possible to adjust the bias voltage and thetransverse magnetic field in such a manner that the energy of a particular Landau level becomes equal to the Fermi energy. Forthis to happen V and B must satisfy Eq. (86). The latter condition defines a function B(n, V ), which is plotted in this panelfor several values of the index n. All curves in this figure are calculated for vF = 106 m/s. Reprinted from Physics LettersA, 375, D. Wang, “Electric- and magnetic-field-tuned Landau levels and Hall conductivity in AA-stacked bilayer graphene”,page 4070, Copyright 2011, with permission from Elsevier. http://dx.doi.org/10.1016/j.physleta.2011.09.025

where e2/π~ is the conductance quantum, [x] denotes the integer part of x, θ(x) is the Heaviside step-function, and the functions g± are defined as

g± =lB~vF

[µ±

√t20 +

e2V 20

4

]. (88)

Thus, the Hall conductance in AA-stacked bilayer graphene is quantized according to ±(e2/π~)n (n =0, 1, 2, ...), and the positions of the steps in the Hall conductivity depend on both the chemical potentialµ and the magnetic field B. A step occurs when a certain Landau level crosses the chemical potential.The dependence of the quantized Hall conductivity versus magnetic field and chemical potential (that is,doping) is presented in Fig. 14. Naturally, the height of the steps in the Hall conductivity corresponds tothe four-fold degeneracy of the Landau levels in AA-bilayer graphene.

The magnetic field also affects the longitudinal conductivity σxx of AA-stacked bilayer graphene. Thecalculation of σxx was performed by Y.-F. Hsu and G.-Y. Guo in Ref. [85] using the same Kubo approach. At

31

Figure 14: (Color online) Quantized transverse conductivity σxy for the AA-stacked bilayer graphene (from Ref. [85]): (a) asa function of 1/B for µ < t0, (b) as a function of 1/B for µ > t0, and (c) as a function of µ for different B. The longitudinalconductivity σxx as a function of 1/B is shown by the dashed (red) curve in figures (a) and (b) when taking into accountthe Landau level broadening Γ. The data were calculated for T = 0, t0 = 0.2 eV, and vF = 106 m/s. Reprinted figure withpermission from Ya-Fen Hsu and Guang-Yu Guo, Phys. Rev. B 82, 165404 (2010). Copyright 2010 by the American PhysicalSociety.

zero temperature, this conductivity is non-zero only if one of the Landau levels coincides with the chemicalpotential µ. In particular, this means that the application of an infinitesimally small magnetic field can giverise to a metal-insulator transition in the system. To overcome this unphysical result, one should take intoaccount the Landau level broadening due to the presence of disorder [85]. This disorder can be characterizedby a parameter Γ, which is defined [90] as a correction to the Matsubara frequency

iωn = iωn + µ/~ + i sgn(ωn)Γ/~. (89)

The dependence of σxx on 1/B, calculated in Ref. [85], is shown in Fig. 14 (a) and (b) by the dashed (red)curves.

5.2. Landau levels and integer quantum Hall effect in AB-stacked bilayer graphene

5.2.1. Landau levels

The study of Landau quantization in AB-stacked bilayer graphene began soon after the fabrication ofgraphene samples (see, e.g., Refs. [50, 56, 91, 92]), since it was then recognized that the bilayer systemcould display even more intriguing properties than the single-layer one. As we already saw in the previoussection, the bias voltage affects significantly the electronic properties of the AA bilayer graphene placed ina magnetic field. In the case of the AB bilayer, this effect is even more pronounced because the small bias

32

voltage opens a gap in the electronic spectrum of this system. Below we consider an AB-stacked bilayergraphene in a transverse dc magnetic field B with bias voltage V . As in the case of the AA bilayer, weconsider only low-energy states. This is a common approximation used in the original papers cited in thissubsection.

The exact solution for the band structure problem in magnetic fields for AB-bilayer graphene cannothas not been found in the general case, even in the tight-binding approach. The problem can be solvednumerically [93, 94], by semiclassical methods [95, 96], or by using simplified Hamiltonians [50, 56, 91, 97,98, 99, 48, 100].

Here, following Refs. [91, 97], we will use a simplified analysis disregarding trigonal warping (that is,neglecting the t3 hopping amplitude) and electron-hole asymmetry (that is, neglecting t4). In this approach,we rewrite the Hamiltonian of the AB bilayer Eq. (46) in the form [91, 97]

HAB = −

eV/2 0 Π 0

0 −eV/2 t0 Π

Π∗ t0 eV/2 0

0 Π∗ 0 −eV/2

, (90)

where in the gauge chosen above the operator Π is defined as

Π = −vF i~ (∂/∂x+ ∂/∂y) + eBy/c . (91)

As in the case of the AA bilayer, we seek a solution of the Schrodinger equation corresponding to thisHamiltonian in the form Ψ(x, y) = eikxΨ(y). The appropriate eigenvalue problem can be solved explicitly [91,97]. In the notations of the present review, the energies EnLL of the Landau levels are determined by theequation [

(εn + u0)2 − n)

] [(εn − u0)

2 − (n− 1)]

=

(ε2n − u2

0

)t20

~2ω2c

, (92)

whereεn = ELL(n)/~ωc and u0 = eV/2~ωc. (93)

The eigenfunctions for n ≥ 2 can be expressed as [91]

Ψkn(y) = dn

[Qn−1(ζ),

√n− 1

εn − u0Qn−2(ζ), fnQn−1(ζ),−fn

√n

εn + u0Qn(ζ)

]T, (94)

where the functions Qn and variable ζ are defined in the text after Eq. (84),

fn =~ωct0

(εn − u0)2 − (n− 1)

εn − u0, dn =

f2n

[1 +

n

(εn + u0)2

]+ 1 +

n− 1

(εn − u0)2

−1/2

. (95)

These results for the Landau levels become invalid for large n, when ELL(n) & t0, and the Hamiltonian inEq. (90) is not applicable. As it follows from Eqs. (92) and (94), for each integer n there exist four stateswith unequal energies. Within such an approach, the trigonal warping can be taken into account usingperturbation theory with respect to the small parameter (t3/t)

2 [97, 101].In the case of an unbiased bilayer, u0 = 0, Eq. (92) simplifies considerably, and the eigenenergies can be

expressed as

ε(1,2,3,4)n = ±

(2n− 1) + (t0/~ωc)2

2±

√[(2n− 1) + (t0/~ωc)2]

2

4− n(n− 1)

1/2

. (96)

If n = 0 or n = 1, we have

ε(1,2)0,1 = 0, ε

(3,4)0,1 = ±

√t20

(~ωc)2+ 1 . (97)

33

Figure 15: (Color online) First five electron-like Landau levels (n = 1, 2, 3, 4, 5) in biased (U = eV ) AB graphene bilayersfrom Ref. [103]. Panels (a, b): Landau levels as function of magnetic field. The level corresponding to n = 1 is shown by thesolid black curve, n = 2 – (red) dashed curve, n = 3 – (blue) dotted curve, n = 4 – (green) dot-dashed curve, and n = 5 –(purple) double-dot-dashed curve. Two different bias potentials are used: (a) U = 50 meV, and (b) U = 200 meV. (c) First fiveelectron-like Landau levels in the graphene bilayer as a function of the interlayer potential difference U = eV at B = 2 T. (d)Dependence of the crossings of the adjacent Landau levels on the combination of applied magnetic field and interlayer potentialdifference. The symbol Ln1n2 denotes the crossing of the Landau levels with indices n1 and n2. Figure from EPL 92, 57008(2010), by Dali Wang and Guojun Jin. Reprinted with permission from IOP.

The Landau levels have four-fold degeneracy due to spin and valley degrees of freedom. In the unbiasedcase (V = 0), zero level is eight-fold degenerate, which corresponds to experimental observations (see below).However, if we take into account the trigonal warping, the total degeneracy of the zero-energy Landau levelis 16, due to four Dirac minicones near the zero energy level [50]. As argued by S. Berciaud et al. inRef. [102], the electron-electron coupling destroys the ideal picture of the trigonal warping, e.g., reducingthe number of minicones near each K point from four to two, restoring eight-fold degeneracy.

In the biased AB bilayer, the valley degeneracy is lifted [50]. In particular, the zero-energy level splits

in two levels independent on the magnetic field ε(1)0,1 = −ξu0, where ξ = ±1 is the valley index.

The dependence of the Landau levels eigenenergies on the combination of the magnetic field and theinterlayer voltage bias is illustrated in Fig. 15. This dependence is different from that of the AA bilayer,Fig. 13. This discrepancy is due to the different electron energy spectra of these two systems. In particular,the applied interlayer voltage opens a gap in the spectrum of the AB graphene bilayer, in contrast to theAA system.

The Landau quantization in AB bilayer graphene was observed and experimentally studied in many

34

Figure 16: (Color online) (a) Position of the Landau levels in an AB bilayer as a function of the magnetic field extractedfrom the transport measurements [26]. Symbols represent experimental data points, and curves correspond to theoreticalcalculations. From A.S. Mayorov et al., Science, 333, 860 (2011). Reprinted with permission from AAAS. Panels (b) and(c): The Landau levels in a single layer (b) and AB bilayer (c) graphene from Ref. [102]. Left panels show false-color maps ofthe micro magneto-Raman scattering spectra as a function of the magnetic field. The corresponding peak frequencies of theelectronic Raman features extracted from Lorentzian fits are shown in the right panels. The theoretical results are shown bysolid lines. The interlayer hopping was t0 = 0.4 eV, while the Fermi velocity vF that best fits the results is indicated in eachpanel. Reprinted with permission from S. Berciaud et al., Nano Letters, 14, 4548 (2014). Copyright 2014 American ChemicalSociety.

experiments, not only devoted to the analysis of the Landau levels themselves [26, 102, 104, 46, 105, 106],but also in numerous papers studying the quantum Hall effect, which will be discussed in the next subsection.The experimental results are in a satisfactory agreement with the theoretical analysis presented above. Thediscrepancies between the theory and experiment can be attributed to experimental errors, sample qualityand, which is more important, to the approximations made when deriving Eq. (92), especially, neglectingthe t3 and t4 hopping amplitudes responsible for the trigonal warping and electron-hole symmetry breaking,disregarding electron-electron interaction, and continuous medium approach. For example, E. A. Henriksenand J. P. Eisenstein in Ref. [104] measured the Landau levels in AB bilayer using infrared spectroscopy inmagnetic fields up to 18 T. They observed four distinct intraband transitions in both the conduction andvalence bands. The transition energies are roughly linear in B between the lowest Landau levels, whereasthey follow

√B for the higher transitions. This behavior represents a change from a parabolic to a linear

energy dispersion. These observations, as well as the density of states derived from the data, generally agreeswith the existing lowest order tight-binding calculation for AB bilayer graphene discussed above. However,in comparing data to theory, a single set of fitting parameters fails to describe the experimental resultsquantitatively.

In Ref. [26], A. S. Mayorov et al. extracted the position of the Landau levels from experiments on elec-tronic transport in free-standing AB bilayer graphene in magnetic fields, see Fig. 16(a). The calculated valuesare shown in this figure by dashed lines. In contrast to results by E. A. Henriksen and J. P. Eisenstein [104],the range of parameters that fit the theoretical and experimental results was very narrow, which indicatesthat the proposed tight-binding Hamiltonian is appropriate for the analysis of the electronic properties ofthe AB bilayer. From Fig. 16 (a) it is seen that at energies below 5 meV, the almost parabolic electronicdispersion at higher energies is replaced with a linear spectrum at lower energies. Such a behavior couldbe attributed to the effect of the trigonal warping, which becomes significant at low energies. However, theauthors of Ref. [26] show that a more detailed analysis of the data reveals a significant deviation from theideal picture of trigonal warping, which could be attributed, e.g., to the effects of electron-electron coupling.In Ref. [102] by S. Berciaud et al., the electronic excitations between Landau levels in free-standing N-layergraphene were measured using micro magneto-Raman scattering spectroscopy. A characteristic evolutionof electronic bands in up to five Bernal-stacked graphene layers was observed. Their behavior is describedremarkably well by the simple tight-binding theoretical approach. The results for single-layer and AB bilayer

35

samples are shown in Figs. 16 (b) and (c). The calculations done with the help of Eq. (92) are shown bysolid curves. As it is seen, the theoretical and experimental results are in a good agreement. Note alsothat the measurements of the quantum Hall conductivity confirmed that the zero Landau level is eight-folddegenerate, while other levels are four-fold degenerate (see subsection 5.2.3).

Thus, we can conclude, the commonly-used simple tight-biding approach presented above is valid for thedescription of the main electronic properties of the AB bilayer graphene.

Several theoretical papers generalized the models discussed above. The Landau level spectrum for ABbilayer graphene in a tilted magnetic field was studied by Y.-H. Hyun et al. in Ref. [107]. In the low-energyapproximation of the tight-binding model, the authors found analytically the Landau level spectrum in termsof spheroidal functions and their respective eigenvalues. In the limit of large in-plane field, this spectrumbecomes two-fold degenerate, which is a consequence of the Dirac point splitting, induced by the in-planefield. The effect of disorder was analyzed in Refs. [65, 108]. It was shown that the Landau spectrum,especially the zero-energy level, is rather stable against disorder.

5.2.2. Conductivity in a magnetic field and magneto-optic phenomena

The electronic structure can be probed by spectroscopic measurements in magnetic field. Naturally, thistechnique was applied to study AB graphene bilayer. In particular, in Refs. [26, 104, 106], the Landau levelsenergies were extracted from the magneto-optic transport measurements. On the theory side, the magneto-optical spectrum of the biased and unbiased AB graphene was calculated in the tight-binding approximationin several papers [91, 97, 103, 109, 110]. Generalizing the approach used in Section 9 [see Eq. (122)] to thecase of finite dc magnetic field, it is possible to compute the dynamical conductivity and absorption. Theeffect of disorder is included with the phenomenological constant Γ as it was done in Section 9. In a magneticfield, an optical excitation by normally-incident light is only allowed between the Landau levels with indexvalues n and n±1, since the matrix element of the velocity operator vx in Eq. (122) vanishes otherwise [109].Figure 17 shows an example of such calculations of the magneto-optical absorption spectrum performed byD. Wang and G. Jin in Ref. [103].

The Hall conductivity σxy can be calculated the same way as σxx, Eq. (122) with (α, β) = (x, y).The optical Hall conductivity is directly related to the Faraday rotation angle ΘF of the incident light,ΘF = 2πRe(σxy)/c. The Faraday rotation in AB bilayer graphene was computed in Refs. [97, 100].

5.2.3. Integer quantum Hall effect

The integer quantum Hall effect in the AB bilayer has some specific peculiarities at low carrier density Ndue to the eight-fold degeneracy of the zero-energy Landau level at V = 0. It has been studied theoretically inseveral papers [50, 56, 97, 101, 111, 112]. As it was mentioned above, the calculation of the Hall conductivityis a straightforward procedure based on the Kubo approach, Eq. (122). However, even in the tight-bindingapproximation and neglecting the trigonal warping the result can be obtained only numerically.

Theoretical predictions regarding the integer quantum Hall effect in the AB bilayer graphene (E. McCannand V. I. Fal’ko [50], E. McCann [56], M. Nakamura et al. [112]) are illustrated in Fig. 18. Experimentalresults (E. V. Castro et al. [58], K. S. Novoselov et al. [111]) are shown in Fig. 19. In Figs. 18 (a), (b), andFig. 19 (a) the Hall conductivity is shown as function of the carrier density N , while in Fig. 18 (c) it isshown as function of 1/B. The measured dependencies of σxy on the applied voltage V0 are shown in Fig. 19(c) for undoped and chemically doped AB bilayer samples. Note that physically the applied voltage changesthe carrier density, and the dependencies of σxy on both N and V0 are in some sense similar. The measureddependence of the longitudinal resistivity ρxx on N is shown in Fig. 19 (b). As it follows from the theory,Eq. (122), the steps in the quantum Hall conductivity corresponds to peaks in the longitudinal resistance(see also Fig. 14). For comparison, the dependencies σxy on N and 1/B for single-layer graphene are shownschematically in Figs. 18 (a) and (c).

The data shown in Figs. 18 and 19 demonstrate that, on both theoretical and experimental pictures, theplateaus in the Hall conductivity σxy occur at integer multiples of 4e2/h, and each plateau corresponds tothe quantized change in the charge density value of 4B/Φ0. This behavior is due to the four-fold degeneracyof the AB bilayer arising from the spin and valley degrees of freedom. Deviation from the conventionalinteger quantum Hall effect occurs near σxy = 0. In the unbiased AB bilayer, there is a step in σxy of height

36

Figure 17: (Color online) Calculated intraband magneto-optical absorption for AB bilayer graphene as a function of photonenergy at a fixed bias potential (from Ref. [103] by D. Wang and G. Jin). The absorption peaks correspond to transitionsbetween adjacent Landau levels. The curves are plotted for transverse bias voltage eV = 200 meV, and the several differentvalues of the magnetic field B; the notation Li → Lj denotes transitions between levels i and j. Figure from EPL 92, 57008(2010), by Dali Wang and Guojun Jin. Reprinted with permission from IOP.

8e2/h due to additional degeneracy of the zero-energy Landau level. This big step is accompanied by aplateau separation of 4B/Φ0 in density, arising from the eight-fold degeneracy of the zero-energy Landaulevels. These features are clearly seen on the experimental curves, see Fig. 19 (a) and blue curve (undopedsample) in Fig. 19 (c). In many papers studying Landau levels and quantum Hall effect, the value of thecharge density N is expressed as a dimensionless filling factor ν = NΦ0/B. In terms of ν, the steps in theHall conductivity in the AB bilayer are observed when ν changes by the value ±4, except ν = 0, when thestep is 8.

Thus, the manifestation of the integer quantum Hall effect in AB bilayers differs significantly from thatin AA bilayers and single layer graphene. First, there is no zero-energy Landau level in AA bilayer andsingle layer graphene, therefore, there is no step across zero density [the dashed line in Fig. 18 (a)]. AllLandau levels in AA bilayer and single-layer graphene have four-folded degeneracy, therefore, there is no“double” step in the Hall conductivity σxy.

The application of the transverse voltage splits the valley degeneracy as shown theoretically by E. Mc-Cann and V. I. Fal’ko in Ref. [50]. In particular, as it was mentioned in Section 5.2.1, zero-energy levelsplits as E0,1 = ±eV/2. The splittings of the non-zero levels are weaker. When the energy scale eV is largeenough, then the splitting eV of the zero energy levels from each valley results in a sequence of quantumHall plateaus at all integer values of 4e2/h, including a plateau at zero density, Fig. 18 (a) (dotted line), as

37

Figure 18: (Color online) Integer quantum Hall effect in AB bilayer graphene. (a) The calculated Hall conductivity σxy asa function of carrier density N for unbiased AB bilayer (solid line) is compared to that of a monolayer (dashed line), fromRef. [50]. (b) The calculated Hall conductivity as a function of carrier density for unbiased (dashed curve) is compared tothat for large V (solid curve), from Ref. [56]. (c) Dependence of σxy on 1/B for monolayer (left picture) and unbiasedAB bilayer (right picture) graphene, from Ref. [112]. The insets show the dispersion relations of both systems. The twicelarger step at N = 0 and 1/B = 0 in the unbiased AB bilayer is due to the additional two-fold degeneracy of the Landaulevel at zero energy. Disorder is phenomenologically taken into account in (a) and (b), and disregarded in (c). Credits.Panel (a): Reprinted figure with permission from E. McCann, V.I. Fal’ko, Phys. Rev. Lett., 96, 086805 (2006). Copyright2006 by the American Physical Society. http://dx.doi.org/10.1103/PhysRevLett.96.086805 Panel (b): Reprinted figure withpermission from E. McCann, Phys. Rev. B, 74, 161403 (2006). Copyright 2006 by the American Physical Society. http:

//dx.doi.org/10.1103/PhysRevB.74.161403 Panel (c): Reprinted figure with permission from M. Nakamura et al., Phys. Rev.B, 78, 033403 (2008). Copyright 2008 by the American Physical Society. http://dx.doi.org/10.1103/PhysRevB.78.033403

observed experimentally, Fig. 19 (c), (red curve, for a doped sample).Recall that in this section we have assumed that the degeneracy of the Landau levels is preserved, i.e.,

any splitting of the levels is negligible as compared to the temperature and level broadening in experiments.

5.2.4. Fractional quantum Hall effect

Fractional quantum Hall effect is observed in two-dimensional systems with electron correlations [83]. Insuch systems the quasiparticles can have fractional charge. As a result, the steps in the Hall conductivitycould arise at fractional filling factors. Usually such steps can be distinctly extracted from measurements onlyat very low temperatures. The fractional quantum Hall effect has been observed in monolayer graphene [113,114, 115]. The observation of this effect in a high-quality AB bilayer graphene samples was reported inRefs. [59, 116]. More detailed experimental studies of the factional quantum Hall effect in the AB bilayerwere performed [117, 118].

In Ref. [116], W. Bao et al. performed magneto-transport measurements of a suspended bilayer graphenedevice with charge carrier mobilities up to 2.7×105 cm2/Vs in magnetic field up to 31 T. A small conduc-tance plateau was observed at ν = 1/3. This plateau scales appropriately with N and B and disappearsat temperature above T ≈ 2 – 2.5 K. In Ref. [117], A. Kou et al. presented local electronic compressibilitymeasurements of the fractional quantum Hall effect in the lowest Landau level of a bilayer graphene device

38

Figure 19: (Color online) Experimental observation of the integer quantum Hall effect in AB bilayer graphene. The Hallconductivity σxy (a) and ρxx (b) are plotted as functions of the electron density N at a fixed B and temperature T = 4 K.Positive and negative N correspond to field-induced electrons and holes, respectively. The Hall conductivity crosses zerowithout any sign of the zero-level plateau that would be expected for a conventional 2D system. The inset shows the energyspectrum for AB bilayer graphene. Reprinted by permission from Macmillan Publishers Ltd: Nature Physics, 2, 177 (2006),copyright 2006. http://www.nature.com/nphys/index.html Panel (c): measured Hall conductivity as function of the appliedvoltage V0 of pristine (undoped) and chemically doped AB bilayer graphene (N0 ≈ 5.4 × 1012 cm2). Reprinted figure withpermission from E.V. Castro et al., Phys. Rev. Lett., 99, 216802 (2007). Copyright 2007 by the American Physical Society.http://dx.doi.org/10.1103/PhysRevB.78.033403

fabricated on hexagonal boron nitride (h-BN). Peaks were observed in the compressibility, correspondingto the fractional quantum Hall effect states at filling factors ν = 2p + 2/3, with hints of additional statesappearing at ν = 2p + 3/5, where p = −2 ,−1, 0,, and 1. According to Ref. [117], this sequence breaksparticle-hole symmetry and obeys a ν → ν+ 2 symmetry, which highlights the importance of the orbital de-generacy for many-body states in bilayer graphene. Robust fractional quantum Hall states at ν = −1/2 and−4/3 in suspended AB samples were revealed in low-temperature magneto-transport measurements [118].The experimental dependence of the longitudinal, Rxx, and Hall, Rxy, resistances on the magnetic field fromRef. [118] are shown in Fig. 20; panels (a) and (b) illustrate the fractional quantum Hall effect with ν = −1/2and ν = −4/3, respectively. Note that the observation of the quantum Hall effect requires high-quality ABbilayer graphene samples, low temperatures (below 2 – 2.5 K), and strong magnetic fields (about 5 – 10 Tand higher).

The nature of fractional quantum Hall states is determined by the interplay between the Coulomb inter-action and the symmetries of the system. The distinct combination of spin, valley, and orbital degeneraciesin AB bilayer graphene is predicted theoretically to produce an unusual and tunable sequence of fractionalquantum Hall states in the lowest Landau level [119, 120, 121, 122, 123, 124, 125].

Strongly correlated states at fractional filling factors and the prospect of tuning their properties havebeen the focus of recent theoretical attention [119, 121, 124, 123, 125, 126, 127]. Z. Papic et al. [122] proposeda method to continuously tune the effective electron interactions in graphene and its bilayer by the dielectricenvironment of the sample. Using this method, the charge gaps of prominent fractional quantum Hall states,including ν = 1/3 or ν = 5/2 states, can be increased several times, or reduced to zero. The tunability

39

Figure 20: (Color online) Observation of fractional quantum Hall effect at T = 0.25 K. Magneto-resistance Rxx (blue curve)and Rxy (black curve) at V0 = −27 V. Panels (a) and (b) illustrate the features associated with the ν = −1/2 and ν = −4/3fractional quantum Hall states, respectively. Reprinted with permission from D.-K. Ki et al., Nano Letters, 14, 2135 (2014).Copyright 2014 American Chemical Society.

of the interactions can be used to realize and stabilize various strongly-correlated phases and explore thetransitions between them. The fact that different sample preparations result in different fractional quantumHall states could be a sign of the theoretically predicted tunability of the fractional quantum Hall effectin bilayer graphene [121, 123, 125]. Applying a perpendicular electric and/or a parallel magnetic field tothe sample may provide insight into the conditions under which different fractional quantum Hall states arefavored.

The effects of the electron-electron interaction on the properties of AB bilayer graphene in a strong mag-netic field were the focus of a many theoretical studies. In particular, D. S. L. Abergel and T. Chakrabortypredicted that the interactions can cause the mixing of Landau levels in moderate magnetic fields [128].Broken-symmetry states induced by electron-electron coupling and phase diagram of the lowest Landaulevel in the Bernal or AB bilayer graphene in a magnetic field were investigated in Refs. [129, 130, 131, 132,133, 123].

6. Spin-orbit coupling

Spin-orbit coupling is a relativistic effect, which can be derived from Dirac’s model of the electron.Spin-orbit coupling describes a process in which an electron changes simultaneously its spin and angularmomentum or, in general, moves from one orbital wave function to another. The spin-orbital mixing is largein heavy ions, where the average velocity of the electrons is higher.

Single-layer graphene has been proposed to be a two-dimensional quantum spin Hall system when theintrinsic spin-orbit interaction is taken into account [134, 135, 136]. Spin-orbit coupling (SOC) in grapheneopens a gap at the Dirac points and the system becomes a topological insulator. However, carbon isa light atom, and the spin-orbit interaction is expected to be weak. Tight-binding and band-structurecalculations provide estimates for the intrinsic and extrinsic spin-orbit interactions in the range 0.01 –0.2 K, and hence much smaller than the other energy scales in the problem [4]. The artificial enhancementof the spin-orbit coupling strength in graphene can open up new possibilities in graphene-based spintronics.Several theoretical and experimental works have addressed the effects of enhanced spin-orbit coupling ingraphene by doping with heavy adatoms such as indium or thallium [137], doping with 3d/5d transitionmetal atoms [138, 139, 140], and interfacing with metal substrates, e.g., Ni(111). [141, 142, 143, 144]

In bilayer graphene the effect of spin-orbit coupling was investigated in several theoretical works [145,146, 147, 148, 149, 150, 151, 152, 153]. The Hamiltonian of the problem is usually written in the form

H = H0 + HR + HM . (98)

40

Here H0 is the Hamiltonian of bilayer graphene, either AB of AA, which includes the terms describingboth in-plane and inter-plane hopping, the gate voltage contribution, and disregards all interactions (seeSection 3). The term HR describes Rashba spin-orbit interaction. If one takes into account only nearestneighbor interaction this term can be expressed as [148, 151]

HR = itR∑〈ij〉aαβ

z · (σαβ × dij)a†iaαbjaβ + h.c. , (99)

where tR is the Rashba spin-orbit coupling strength, z is the unit vector perpendicular to the layers, dij isa vector pointing from sites j to i, a = 1, 2 is the layer index, and σαβ are spin Pauli matrices with α and β

denoting up spin or down spin. The term HM is the exchange field contribution with magnetization M

HM = M∑iaαβ

(a†iaασ

zαβaiaβ + b†iaασ

zαβbiaβ

). (100)

Such an exchange field effect can arise due to the proximity coupling between graphene and magnetic adatomsor ferromagnetic substrate materials (see Ref. [151]). This term is of importance for several reasons, whichwill be discussed below.

According to Refs. [147, 151], the effect of spin-orbit coupling in AA-stacked bilayer graphene is insignifi-cant, unless tR becomes of the order or larger than interlayer hopping amplitude t0, which seems unrealistic.Thus, the main research efforts for this problem were devoted to the AB bilayer graphene.

The electronic band structure of the AB bilayer in the presence of spin-orbit coupling and a transverseelectric field was calculated from “first principles” using the linearized augmented plane-wave method byS. Konschuh et al. in Ref. [150]. The main conclusion of the latter paper is that the spin-orbit effects inAB-stacked bilayer graphene differ essentially from the single-layer spin-orbit coupling. The intrinsic spin-orbit splitting (anticrossing) around the K points is about 24µeV for the low-energy valence and conductionbands, which are closest to the Fermi level, similarly as in single-layer graphene. An applied transverseelectric field breaks space-inversion symmetry, and leads to a Rashba spin-orbit splitting. This splitting isusually linearly proportional to the electric field. The peculiarity of AB-stacked bilayer graphene is thatthe low-energy bands remain split by 24µeV, independently of the applied external field. The electric field,instead, opens a semiconducting band gap separating these low-energy bands. In the remaining two high-energy bands the spin degeneracy is lifted. The strength of this splitting is proportional to the electricfield; the proportionality coefficient is given by the second intrinsic spin-orbit coupling, whose value is20 µeV. All the band-structure effects and their spin splittings can be explained by a tight-binding model,in which the spin-orbit Hamiltonian is derived from symmetry considerations. The magnitudes of intra- andinterlayer couplings (their values are similar to the single-layer graphene ones) are determined by fitting tofirst-principles results.

A systematic study on the influence of Rashba spin-orbit coupling, interlayer potential difference, andexchange field on the topological properties of bilayer graphene was performed by Z. Qiao et al. in Refs. [148,151]. Due to the band gap opening from broken out-of-plane inversion symmetry, gated AB bilayer grapheneis a quantum valley Hall insulator characterized by a quantized-valley Chern number. The presence of Rashbaspin-orbit coupling turns the gated bilayer graphene system from a quantum valley Hall insulator into atopological insulator. The phase boundary is given by [148]

9t2R = t20 + (eV/2)2. (101)

In the presence of different Rashba spin-orbit coupling strengths on the top and bottom layers, t(1)R 6= t

(2)R ,

the topological insulator phase remains robust as long as [151]

9t(1)R t

(2)R > t0. (102)

When the time-reversal symmetry is broken by an exchange field M , Eq. (100), the AB-stacked bilayergraphene hosts different topological phases characterized by different Chern numbers. The phase boundaries

41

associated with the topological phase transitions are given by eV = ±M and

9t2R = t20 + (eV/2)2 −M2. (103)

The effects of next-nearest-neighbors spin-orbit coupling interaction and stability limits of the topologicalphases against trigonal warping and staggered sublattice potential were investigated by E. Prada et al. inRef. [147].

A theoretical study of the band structure and Landau levels in AB bilayer graphene at low energiesin the presence of a transverse magnetic field and Rashba spin-orbit interaction was done by F. Mirelesand G. Schliemann in Ref. [149]. These authors predicted an unexpected asymmetric spin splitting andcrossings of the Landau levels due to the interplay between the Rashba interaction and the external biasvoltage. The edge modes in AB-stacked bilayer graphene arising due to spin-orbit interactions were analyzedin Refs. [145, 147].

Let us conclude this section with a reminder that all spin-orbit effects discussed above have not beenobserved experimentally. Thus, realistic values of the gaps, associated with the spin-orbit interaction, arenot known.

7. Bilayer-based mesoscopic systems

The list of bilayer-based mesoscopic objects studied by theorists is quite similar to the list of single-layer graphene mesoscopic systems (for a summary of single-layer mesoscopic research, see, e.g., the reviewby A. Rozhkov et al. [18]). The items on such a list are: quantum dots, nanoribbons (narrow stripes ofgraphene), pn-junctions, edge states, and conducting channels. However, since the electronic spectra of thebilayers are different from the single layer, the electronic properties of the bilayer mesoscopic objects maybe quite dissimilar from their single-layer counterparts.

Most of this section is dedicated to mesoscopic structures made of AB bilayer graphene. The number ofstudies of AA-based system is fairly small and it is reviewed in subsection 7.2.1 below. In addition, Kleintunneling for AA bilayer graphene was discussed in subsection 4.1.1. Klein tunneling in twisted bilayergraphene is discussed in subsection 13.5.4. Finally, there is a small number of theoretical [154, 155] andexperimental [156] studies where mesoscopic systems based on twisted bilayer graphene have been studied.

7.1. AB bilayer graphene quantum dots

Quantum dots are simplest mesoscopic objects. In the theoretical literature, both single-layer and ABbilayer graphene quantum dots are discussed. Studies of quantum dots made of AA bilayer are virtuallyabsent.

A simple quantum dot can be a small piece of material. As a first example of a quantum dot let, usconsider a nanoribbon of finite length. Sahu et al. [157] investigated a finite-length AB bilayer nanoribbonusing DFT. According to this paper, the system ground state is magnetic: it demonstrates interlayer anti-ferromagnetic arrangement of magnetic moments. The confinement-induced gap is enhanced by the internalmagnetism. The application of an external electric field weakens this gap. A related study of an infinitelength nanoribbon, Ref. [158], will be reviewed below.

For single-layer and AB bilayer graphene, tearing a macroscopic sample into small pieces is not the onlymethod to define a quantum dot. Alternatively, a dot may be created within a larger sample with the helpof a position-dependent external potential, either chemical or electric. For AB bilayer samples, appropriateideas were explored theoretically in Refs. [159, 160]. If the symmetry between the layers is broken (e.g., by atransverse electric field, see subsection 3.3.2), a gap opens up in the bulk of the bilayer. In such an insulatingenvironment, one can induce a well-defined quantum dot. This can be done by introducing dopants to asmall area of the sample, as discussed theoretically by J. Pereira et al. in Ref. [160]. If the donor or acceptorlevels lie inside the gap, the wave functions associated with these states are localized near the region wherethe dopants are placed. As a result, several discrete subgap states emerge (in connection with single-layergraphene similar proposals were considered by G. Giavaras and F. Nori in Ref. [161]).

42

Experimentally, this type of dot was realized by M. T. Allen et al. [162] with the help of a complicatedgating system in suspended AB bilayer graphene samples. The tunable bulk gap in this experiment wasup to 250 meV. Inside this insulating bulk an electric-field-defined quantum dot was created. Dots withdiameters ranging from 150 to 450 nm were reported. Measurements performed on a particular dot at 0.1 Kdemonstrated well-defined Coulomb blockade with charging energy EC ≈ 0.4 meV. The same principle wasused by A.M. Goossens et al. [163], to define a quantum dot within a bilayer sample on a hexagonal boronnitride substrate. A related experiment was described in Ref. [164].

If the electric potential varies in space, but it is identical for both layers, the gap does not emerge.In such a situation it is impossible to create true bound states: the electron wave function would “leak”away from the dot into a gapless environment. In this situation, a set of quasi-bound states (resonances)can be induced. This can occur both in single-layer graphene [159, 165, 166, 167], and in gapless bilayergraphene [159]. However, the application of the external magnetic field may confine these states.

This method of creating quantum dots is very appealing, since it allows one, at least in principle, tocontrol the properties of the dots by varying external fields. Using an appropriately-designed gating systemit is possible to engineer, for example, quantum dots of non-trivial shapes. Specifically, a ring-shapedquantum dot was studied theoretically by M. Zarenia et al. in Ref. [168]. To generate such a dot we need agating system creating a bias potential, which vanishes within a finite-width ring: U(r) = eV (r) = 0 whenRmin < r < Rmax, where r is a polar radius, Rmin and Rmax are the internal and external radii of the ring.The required potential is non-zero and has the same polarity for both r < Rmin, and r > Rmax. As a result,several discrete subgap states may localize at the ring. The behavior of these states in an external magneticfield and other properties are discussed in [168].

A ring with a different confining mechanism was proposed by L. J. P. Xavier et al. in Ref. [169]. This“topological” confinement is based on the idea of I. Martin et al. [170] (it will be discussed in more detailin subsection 7.3). According to Ref [170], when the transverse electric potential applied to an AB bilayersample changes sign as a function of coordinate [for example, U(x > 0) > 0, but U(x < 0) < 0], the electricpotential kink at x = 0 becomes the source of topological states. The wave functions of such subgap statesare extended along the y-axis and localized in the x-direction. If the gate system creates the transversepotential U(r), which changes sign at some finite r = R > 0, then the topological states are localized at thering of radius R. Due to the finite circumference of this ring, instead of a one-dimensional band, a set ofquantized levels appears.

7.2. Bilayer graphene nanoribbons

7.2.1. AA bilayer nanoribbons

Nanoribbons (narrow stripes of the material) prepared from bilayer graphene are another popular ob-ject of research. Similar to single-layer graphene nanoribbons, AA bilayer nanoribbons are also classifiedaccording to their edge type: there are zigzag and armchair nanoribbons.

The Landauer-Buttiker transport through AA bilayer nanoribbon was studied in Refs. [171, 172]. InRef. [172], N. Xu et al. studied a transport through the AA nanoribbons with both zigzag and armchairedges. The effects of interlayer electron hopping and ripples were discussed. For the armchair nanoribbonthe current decreases at fixed voltage when the interlayer hopping grows. This effect is virtually absent forthe zigzag nanoribbons. Ripples act to suppress the current, especially for zigzag systems. S.-J. Sun andC. Chang [171] compared AA-stacked and AB-stacked nanoribbons. The influence of both bias voltage andperpendicular magnetic field were studied. The bias voltage affects the AA and AB nanoribbons differently:the bias electric field in the interval E < 4 V/nm suppress the current through the AB nanoribbon, but doesnot significantly change the current through the AA nanoribbon. Current oscillations, which are predictedto occur at higher E, are likely to be difficult to observe due to electrical breakdown. As for the magneticfield, it appears that the magnetoresistance is extremely weak (< 10−5 at 10 T) in both cases.

Transport between two overlapping single-layer nanoribbons was studied by J. W. Gonzalez et al. inRef. [173] within the framework of the Landauer-Buttiker formalism. Both AA and AB types of stacking inthe overlap region were discussed. Reference [173] found that for both stackings the Landauer conductanceoscillates as a function of the overlap region width. The period of oscillations is about 20 unit cells. Since the

43

Figure 21: AB bilayer edges. Edge classification developed for single-layer graphene is incomplete for AB-stacked bilayer.Both armchair edge (horizontal edges in both panels) and zigzag edge (vertical edges) can appear in any of the two varieties,α-alignment [panel (a)] and β-alignment [panel (b)]. In both panels one layer is shown by (red) solid hexagons, another isrepresented by (black) dashed hexagons.

conductance is very sensitive to the geometry of the system, the authors proposed to use such a setup as anelectromechanical switch. Experimentally, electromechanical properties of both AB bilayer and monolayergraphene were studied in Ref. [174].

In Ref. [175], K. M. M. Habib et al. investigated the same system of two overlapping single-layer nanorib-bons in a non-equilibrium regime. Similar to [173], Ref. [175] assumed that the overlap area is either ofAA, or AB type. Using DFT and non-equilibrium Green’s function approach Ref. [175] proved that sucha system would demonstrate a region of negative differential resistance at sufficiently large applied voltage.Details of the IV curve, however, depend on the type of stacking.

7.2.2. AB bilayer nanoribbons

For AB bilayer nanoribbons, the usual classification of the edge types (armchair versus zigzag edges) isnot entirely complete: both types must be further split into α-alignment and β-alignment (see Fig. 21).

It is known that single-layer graphene allows for a flat band of edge states near the zigzag termination(localized states near the armchair termination are also possible under suitable circumstances [176]). Similarlocalized states were described theoretically by E. V. Castro et al. [177] for β-aligned AB bilayer zigzagsemiplane and AB bilayer zigzag nanoribbons. There are two edge bands per edge; thus, a nanoribbon hasfour such bands. The wave functions corresponding to different edge bands are quite dissimilar. Namely,in the nearest-neighbor-hopping model of Ref. [177] there are two bands whose wave functions are localizedexclusively on a single layer of the bilayer. The wave functions for the two other bands arespread over bothlayers. This disparity explains the different behavior of the edge states under the action of the transversebias voltage V . When V = 0, all four bands are dispersionless, with zero eigenenergy εk = 0. For V 6= 0,the single-layer localized bands shift rigidly from εk = 0 to εk = ±eV/2. The localized states whose wavefunctions are spread over both layers remain in the bulk gap, and acquire a pronounced dispersion.

This model was generalized by A. Cortijo et al. in Ref. [178]. They included longer-range hopping andinteraction into their Hamiltonian. The longer-range hopping lifted the degeneracy of the perfectly flatedge bands, introducing the dependence of the eigenenergies on momentum k along the nanoribbon. Thecombined effect of the longer-range hopping and non-zero transverse bias V creates a disparity between thenanoribbon edges. The authors identify “fast” and “slow” edge: the velocity of the band localized at the “fastedge” of the nanoribbon is higher than that at the “slow edges”. The electron-electron interaction inducessingle-electron gaps at both edges. According [178], “the slow edge” must have a higher gap value. Measuringthe conductance of an individual edge, an experimentalist could extract each gap value independently.

44

It is theoretically predicted for single-layer graphene that the edge-state band is unstable with respectto ferromagnetic order when considering the repulsive interaction between electrons (see, e.g., the reviewRef. [18]). Likewise, AB bilayer zigzag nanoribbons were actively researched in connection with their mag-netic properties [157, 158, 179, 180]. At the bilayer edge one might expect that both layers would bemagnetized. Indeed, this type of magnetic structure has been reported in several theoretical papers wheredifferent versions of density functional theory (DFT) calculations were employed. However, one must re-member that the relative stability of the magnetic and non-magnetic states turns out to be very sensitiveto numerous details: the type of density-functional approximation, edge structure (α-alignment versus β-alignment), relaxation of the atom positions at the edge. For example, Sahu et al. [158] concluded that forα-aligned zigzag graphene nanoribbons, the DFT calculations cannot reliably determine if the stable stateis magnetic or not. Also, [158] claimed that β-aligned zigzag nanoribbons are magnetic: every edge of everylayer carries finite magnetization. However, the method was unable to assess if the magnetization vectors atthe same edge of the nanoribbon have the same (ferromagnetic) or opposite (antiferromagnetic) orientations.

The results of a similar DFT study were described by M. P. Lima et al. in Ref. [180]. Unlike Ref. [158],where the graphene strips comprising the nanoribbon were assumed to be perfectly flat, Ref. [180] allowedfor bending of the nanoribbon layers. Therefore, they found that in the stable configuration the “thickness”of the nanoribbon is not constant, but rather changes from point to point as one moves from one edge toanother. This thickness variation is the result of the interlayer interaction variation: a local value of theinterlayer interaction in the proximity of an edge becomes sensitive to the distance from the edge. Foran α-aligned nanoribbon, this additional interaction can be thought of as an extra attraction between thelayers, while for a β-aligned nanoribbon acts as repulsion. Thus, the α-aligned nanoribbon was determinedto be more stable than its β-aligned counterpart. Regarding magnetism, α-aligned nanoribbons were foundto be non-magnetic. For β-aligned nanoribbon [180] confirmed the conclusion of [158] about the stability ofa magnetic configuration. However, the energy differences between competing states, possessing dissimilarmagnetic structures, were smaller than the temperature. As a result, which of theses states was the “true”ground state, remained unknown.

The papers [158, 180] discussed the situation of a nanoribbon with no contact with the substrate. Thus,they are most relevant for suspended ribbons. The effect of silicone substrate on nanoribbon electronproperties was investigated by Z. Zhang et al. in Ref. [179]. According to this DFT study, the carbonatoms at the edges of the nanoribbon bottom layer form covalent Si-C bonds to the silicone atoms of thesubstrate. Thus, the top layer, which interacts with the bottom layer only through weak van der Waalsforces, behaves as an almost isolated single-layer zigzag nanoribbon. The latter object is known to havea magnetic ground state. Consequently, a bilayer nanoribbon on a silicone substrate is magnetic: eachedge carries a finite ferromagnetic magnetization, while the coupling between the edges is antiferromagnetic.Further, the authors proposed to control the magnetization of the nanoribbon by an external electric field.

Thus, it appears that the zigzag bilayer nanoribbons have several competing low-energy states, some ofwhich are magnetic, some of which are not. Which state wins in a laboratory experiment may depend ona variety of conditions: type of nanoribbon edge, substrate, sample history, etc. Unfortunately, relevantexperimental data are not available at the time of writing.

Optical properties of the zigzag and armchair nanoribbons were studied by A. R. Wright et al. inRef. [181] using the tight-binding approximation. According to those calculations, AB bilayer armchairnanoribbons should demonstrate strong optical response in the far infrared and terahertz regimes. Thefrequency-dependent dimensionless optical conductivity σ was predicted to be as large as 150(e2/4~). Sucha response strength greatly exceeds the values typical for graphene. The authors claimed that the requirednanoribbons were already created in laboratory experiment, Ref. [182].

Numerical calculations of the Landauer conductance of AB bilayer nanoribbons were performed by H. Xuet al. in Ref. [183]. This paper discusses both zigzag and armchair nanoribbons with ideal and disorderededges, with and without a magnetic field. The electron-electron and electron-phonon interactions weredisregarded. The authors reported that the dimensionless conductance π~σ/e2 for the bilayer nanoribbonquantizes as n for the armchair edge and (2n + 1) for the zigzag edge. The edge disorder quickly destroysthis quantization, and opens a so-called transport gap. This phenomenon is particularly strong for armchairnanoribbons. The transport through the zigzag nanoribbons is more robust, possibly due to edge states.

45

However, that paper investigated a very idealized object. Since the model disregarded the effects of electron-electron and electron-phonon interaction, several mechanisms, which may affect the transport of single-layerribbon (see, e.g., Refs. [184, 185, 186]), were neglected. The authors themselves assessed their results as“a necessary first step” toward developing a reliable theoretical description of nanoribbon transport. Arelated theoretical study of a bilayer nanoribbon in a spatially inhomogeneous magnetic field was reportedin Ref. [187].

As mentioned in the previous paragraph, Ref. [183] reaffirmed the expected conclusion that edge disorderis very harmful for the ballistic propagation of the carriers. However, the fabrication of nanoribbons withsmooth edges is a very difficult task, and experimental attempts in this direction are ongoing (see, forexample, Ref. [156]).

7.3. Topologically-protected conducting channels in AB bilayer samples

As we already mentioned, the bias voltage applied to the AB bilayer opens a gap in the electron spectrum,turning the sample into a semiconductor. I. Martin et al. [170] noticed that, if the bias potential U(r) = eV (r)passes through zero and changes its sign upon crossing some line r = r`, then a set of conducting single-electron subgap states binds to this line.

To demonstrate the existence of these modes, the authors of Ref. [170] modified the effective two-bandHamiltonian, Eq. (50). They assumed that the transverse bias potential is position-dependent V = V (r),and satisfies the following relations

V (r) = V (x), V (x) = −V (−x). (104)

That is, the bias voltage changes sign on the straight line x = 0. The corresponding Schrodinger equationmay be solved [170] rather straightforwardly, if we choose

U(x) = U0 sgn (x), where U(x) = eV (x). (105)

Since the system remains invariant under translations along the y-axis, one can replace −i∂/∂y → qy. Thus,for positive x the following system of ordinary differential equations needs to be investigated:

~2v2Ft0

(ξqy + ∂x)2ϕb(x, qy) = (U0

2 − ε)ϕa(x, qy),~2v2Ft0

(ξqy − ∂x)2ϕa(x, qy) = −(U0

2 + ε)ϕb(x, qy),(106)

where ξ = ±1 is the valley index, defined in subsection 4.1. The system has four solutions. However, ofthese four only two are normalizable at x→ +∞. The divergent solutions must be discarded. Likewise, forx < 0 the following system of equations must be solved:

~2v2Ft0

(ξqy + ∂x)2ϕb(x, qy) = −(U0

2 + ε)ϕa(x, qy),~2v2Ft0

(ξqy − ∂x)2ϕa(x, qy) = (U0

2 − ε)ϕb(x, qy).(107)

Only two solutions are normalizable, and can be kept.Once the solutions in each half-plane are found, they must be matched, together with their derivative,

at x = 0. The matching condition cans be cast in the form of a homogeneous system of four linear equationsfor four unknown coefficients. To have a non-zero solution the system’s determinant has to vanish. Thisimplicitly defines two dispersion relations εξ1,2 = εξ1,2(qy) for two bands localized at the line x = 0. In k-space these bands are located near the Dirac point specified by the value of ξ. Reference [170] explained thatthe presence of exactly two bands per Dirac point is related to the topological properties of the insulatingbilayer state. This set of four bands may be visualized as a one-dimensional conducting channel inside atwo-dimensional insulating host system.

While the approximation Eq. (105) accounts for many qualitative features of the topological bands,it is still quite crude. Unfortunately, this is the only known limit which admits an analytic solution.For more realistic choices one has to resort to numerical calculations. Let us examine Fig. 22, where the

46

Figure 22: Dispersion relation for localized bands near a particular Dirac point. The two solid curves crossing the ε = 0level represent the dependence of the energy [measured in units of (~vF)2/(3a20t0)] versus dimensionless momentum py =√

3a0qy (note that√

3a0 is the graphene lattice constant). These curves were estimated numerically for the dimensionless

bias potential (3a20t0U(x))/(~2v2F) equal to 2 tanh(x/w), where the length scale w was chosen to be w =√

3a0/2. Bothbands demonstrate negative group velocity. Their time-reversal partners are located at the other Dirac point, both havingpositive group velocities. If tanh(x/w) is approximated by sgn (x), the dispersion curves for this case are shown by dashedcurves. One can see that for such choices of parameters the latter approximation works extremely well. Reprinted figure withpermission from I. Martin et al., Phys. Rev. Lett., 100, 036804 (2008). Copyright 2008 by the American Physical Society.http://dx.doi.org/10.1103/PhysRevLett.100.036804

dispersion of the localized bands are shown. These dispersion relations were obtained numerically in [170] forU(x) ∝ tanh(x/w), where w has the dimension of length. The figure shows two subgap modes (solid curvescrossing the ε = 0 level) near a particular Dirac point. Both curves have negative group velocity. Theirtime-reversal partners are located at the other Dirac point, and they both have positive group velocities.The dashed curves represent the dispersions corresponding to the approximation Eq. (105). One can seethat for such a value of w and U , the approximate dispersion gives a very accurate estimate for the numericalresult. Similar results were obtained by M. Zarenia et al. in Ref. [188].

As can be seen, the localized modes have non-trivial valley structure: the direction of propagation fora particular band depends entirely on its valley index ξ. Reference [170] proposed to use this property tocreate “valley filters” and “valley valves”. Reference [189] discussed the use of the topological bands to splitCooper pairs.

Electronic states localized near the bias voltage kinks were studied in some detail in Ref. [188]. Theauthors showed that, in addition to the topological bands crossing the zero energy, for a sufficiently smoothfunction U(x), non-topological subgap bands also appear. For zero doping, the non-topological bands donot reach the Fermi energy, and remain separated from the Fermi level by a gap ∼ U0. They also consideredthe more general case when U(x) changes sign at some finite x = d > 0, and then again changes sign atx = −d < 0. If d is not too large, the topological bands at x = d hybridize with the bands at x = −d.Therefore, the bands acquire small, but finite, gaps, which may be useful for the control of transportproperties. The presence of the magnetic field does not influence strongly the topological bands.

The transport properties of these bands were studied by Z. Qiao et al. in Ref. [190]. Unlike the papersmentioned above, they used a tight-binding Hamiltonian, thus, avoiding the perils of the low-energy effectivemodels, such as the non-physical absence of intervalley scattering. Of course, the study relies exclusivelyon numerical calculations. Using the Landauer-Buttiker approach and non-equilibrium Green’s function

47

technique, it was shown [190] that the topological bands have excellent transport properties. They propagatewell even when the channel bends: the authors report “zero bend resistance” even for sharp turns of thepropagation paths. Disorder-induced backscattering is also predicted to be very weak both for long-rangeand short-range disorder. These properties may be useful for applications.

Topological bands could be used as a Tomonaga-Luttinger-like liquid with tunable parameters. Thisproposal was formulated by M. Killi et al. in Ref. [191]. Since these systems have two bands propagatingalong the y-axis and two bands propagating in the opposite direction, the resultant one-dimensional liquiddoes not coincide with the standard Tomonaga-Luttinger concept, which has only one propagating modeper direction of propagation (so-called “left-moving” and “right-moving electrons”). Nonetheless, this one-dimensional liquid is an interesting object in its own right. Its effective low-energy description was outlinedin Ref. [191]. In particular, the authors noted that the effective parameters of such a generalized Tomonaga-Luttinger liquid may be varied by the bias voltage.

Finally, we would like to mention two variations of the ideas reviewed in this subsection. (I) It waspredicted [192, 193] that certain stacking-fault domain walls may host similar modes in the presence ofcoordinate-independent bias U(r) = U0 6= 0. Experimentally, such domain walls were studied in Refs. [194,195]. (II) In the context of edge states, related concepts were discussed in Ref. [196].

7.4. pn-junctions and similar structures

A junction of pn type is both a cornerstone of modern electronics and an interesting object for funda-mental research. This type of mesoscopic structure has been studied for single-layer graphene (see Ref. [18]for a review). It is no wonder that bilayer-based junctions are also discussed in the literature.

Similar to single-layer graphene, the physics of Klein tunneling, reviewed in subsection 4.2, also affectsthe properties of bilayer junctions as well. However, the setups discussed in subsection 4.2 are too idealizedto be directly relevant for experiments. To develop a realistic description of the transport through thejunctions other important factors, such as disorder and interaction, must be accounted for.

The AB bilayer graphene has two obvious differences when compared to a single-layer graphene: itsdispersion is quadratic, and it can become a gapped insulator (semiconductor) when the transverse bias ispresent. Thus, the properties of a bilayer pn-junction differ from the properties of a single-layer junction. Asemiclassical theoretical investigation of transport through a ballistic junction was presented by R. Nand-kishore and L. Levitov in Ref. [197]. The geometry of the system under study is shown in the inset forFig. 23.

As one can expect, the junction’s IV curve demonstrates asymmetry with respect to the source-drainvoltage polarity change (see Fig. 23). In addition, for a certain range of source-drain voltages the differ-ential conductivity of the junction is negative. In Ref. [197] it was explained that the negative differentialconductivity is a consequence of quantum-mechanical interference between two semiclassical trajectoriesin a classically-forbidden region, separating p and n electrodes of the junction. Such under-the-barrierinterference is uncommon for usual semiconducting junctions.

The interference is very sensitive to the disorder inside the sample. However, estimates suggest thatthe currently available experimental purity is sufficient to guarantee the observation of the theoretically-predicted behavior.

A model of a pn-junction with a step-like barrier was discussed in Refs. [198, 199]. In particular, theauthors of Ref. [199] studied a pn-junction and the tunneling across a potential barrier (the latter systemmay be viewed as a pnp-junction). A disorder-free configuration was assumed. The paper investigatedthe accuracy of different effective models of the bilayer graphene. Predictions of the four-band and two-band models were compared, and the importance of the longer-range single-electron hopping processes wasassessed. It was found that the longer-range hopping amplitudes are unimportant for energies in excessof 4 meV. On the other hand, the two-band effective theory prediction may deviate significantly from thefour-band theory at higher energies.

The effects of strain on the properties of ballistic pn-, pnp-, and other types of junctions were discussedin Ref. [198]. Uniaxial strain, when applied to an AB bilayer sample, qualitatively modifies the low-energydispersion of electrons: the parabolic dispersion surface is replaced by two Dirac cones separated by a

48

Figure 23: Calculated IV characteristics for a pn-junction made from an AB graphene bilayer, Ref. [197]. Three curvesrepresent three values of the gate-induced potential difference across the junction U (curve 1 corresponds to the smallest U ,curve 3 corresponds to the largest U). The curves are asymmetric with respect to polarity change of the source-drain voltageVsd. Negative differential conductivity regions are clearly visible. Inset: Structure of the junction under finite Vsd. Reprintedfrom: R. Nandkishore and L. Levitov, PNAS 108, 14021 (2011).

saddle point. The resultant dispersion surface is somewhat similar to the trigonal warping, Fig. 9, butwith two emergent cones instead of four. The saddle point at ±5 meV may be induced by strain of about1%. Reference [198] concluded that in the presence of strain the ballistic conductance of both pn- andpnp-junctions may demonstrate non-monotonous dependence on doping and temperature.

Above we have already mentioned Refs. [198, 199] investigating pnp-junctions. Another paper dedicatedto this topic is Ref. [79]. It developed a semiclassical formalism for the theoretical study of a ballistic ABbilayer pnp-junction. The bilayer was assumed to be in the gapless regime (no transverse bias voltage).They showed that there is a set of “magic” incident angles for which an electron passes the junction withoutreflection (for the single-layer graphene and rectangular barrier these angles can be seen on the transmissionplot of Fig. 12, for more general case see, e.g., Ref. [76]). This reflectionless transmission is a manifestationof the Klein tunneling. The authors concluded that it would be difficult to lock a transistor based on agapless AB bilayer because of the perfect transmission at the “magic angles”. Of course, one might tryusing a gapped biased bilayer to circumvent this difficulty, but this route is not without a flaw either (seesubsection 8.3, where the experiment on biased AB bilayer graphene is discussed). Yet another opportunity isa relatively new theoretical proposal, Ref. [200]. The latter paper demonstrated that the tunneling accrossthe barrier for any angle can be small provided that the barrier shape is suitably chosen. Recently, thetunneling through a smooth barrier was examined in Ref. [201]. The latter paper also discussed the effectsof the trigonal warping on the tunneling.

A theoretical proposal to use an AB bilayer heterojunction as a detector of radiation in terahertz andinfrared range was presented by V. Ryzhii and M. Ryzhii in Ref. [202]. The setup is depicted in Fig. 24and that heterojunction resembles a npn-junction. However, unlike the latter, the electrochemical potentialin the central area lies inside the gap. Therefore, it is not a p-type doped semiconductor, but rather aninsulator with a small gap. The “dark current” (the source-drain current in the absence of any radiation)of the detector is small, since the charge carriers from the source must overcome the gap in this insulatingarea to reach the drain. The radiation excites electron-hole pairs across the gap, and these pairs contributeto the source-drain current. Observation of the photocurrent in excess of a dark current signifies thefinite radiation flux. The authors calculated different characteristics (spectral characteristics, dark current,responsivity, dark current limited detectivity) of their detector. They concluded that at optimal parametersit can demonstrate better performance than the detectors of other types. The experimental realization of aphotodetector working in the terahertz range was reported by D. Spirito et al. [203].

Experimental realizations of pn-junctions and related heterostructures have been described in many

49

( a )

D r a i n

tL

S o u r c etW

bW

B a c k g a t e

T o p g a t e

V b > 0

( b )

b i l a y e r

V t < 0

V d > 0

G r a p h e n e

de V

Eg

sL

dL

wh

sgE d

gE

e F

de F

s

Figure 24: Photodetector based on gapped AB bilayer graphene. In panel (a) Vd is the source-drain voltage, Vt (Vb) isthe top-gate (back-gate) voltage. The huge red arrow denotes the incoming radiation. Panel (b) describes the operationof the detector. The incoming radiation (red arrows) excites electron-hole pairs. Under the action of the source-drain fieldthe photoholes move mostly to the source, and the photoelectrons move mostly to the drain. The motion in the oppositedirection is also possible due to thermal fluctuations. The latter are responsible for “the dark current”. Reprinted figure withpermission from V. Ryzhii, M. Ryzhii, Phys. Rev. B, 79, 245311 (2009). Copyright 2009 by the American Physical Society.http://dx.doi.org/10.1103/PhysRevB.79.245311

papers. For example, the properties of pn-junction were studied experimentally by B. Chakraborty et al.in Ref. [204]. The authors also offered a simple theory explaining the observed IV curve. The formulatedtheory fits well the data. However, according to the paper, the described device becomes pn-junction onlyunder substantial source-drain voltage: it was assumed that the areal charge density near the drain electrodechanges its polarity due to spillage of the charge from the electrode itself. Clearly, such a situation does notcorrespond to any of the discussed theoretical models.

Many workers are attempting to create a field-effect transistor, which may serve as a cornerstone offuture potential graphene-based electronics (for a general discussion on this issue one may consult Ref. [19]).For example, a series of papers [205, 206, 207] studied this type of devices. A theoretical proposal for atunnel field-effect transistor was put forward in Ref. [208].

In Ref. [209] H. Miyazaki et al. investigated a setup consisting of several junctions connected in series.The purpose of that study was to check if multiple junctions can suppress leakage current in the “off” stateof the transistor. The junctions were created by a comb-like top gate. Depending on the voltage on the topand back gates, the system may be in one of four regimes: pn-, np-, nn’-, and pp’-junction. The ambipolarregimes (pn and np) are indeed characterized by a lower source-drain current.

50

Unfortunately, these setups do not yet demonstrate the characteristics required for successful commercialexploitation. For example, the on/off ratio (the ratio of currents in “on” and “off” states) for the transistorsdevised in Ref. [206] is less than 50, while for logic applications [19] this ratio must be higher than 104. Ofcourse, at lower temperature this ratio grows: Ref. [210] described a device with the on/off ratio of severalthousands at 20 K. However, such a restriction on the operation temperature makes the device useless formass market applications.

8. Electronic transport through an AB bilayer sample

Both theoretical and experimental research of the electric transport through AA bilayer graphene isnon-existent. Current experimental and theoretical efforts are focused on the electrical conductivity of ABbilayers. Consequently, in this section we will only review the transport through AB bilayer samples.

The relevant papers may be roughly divided into three groups. The papers in the first group study theconductivity of doped AB bilayer graphene. A doped sample has a well-defined Fermi surface. Despitesome peculiarities, such a system may be viewed as a metal, and its transport properties can be investigatedaccordingly. We review this topic in subsection 8.1.

The second group involves work with the so-called minimum conductivity, that is, the conductivity of anundoped sample. While the undoped bilayer with no disorder has no charge carriers, they can be induced(by random variations of an external potential, or by impurities) and contribute to the transport. This andother mechanisms for the minimum conductivity are discussed in subsection 8.2.

The third group of papers is dedicated to transport in samples to where the transverse bias is applied.While the reasoning outlined in subsection 3.3.2 implies that a system of this kind should demonstrate insu-lating behavior, transport measurements paint a more complicated picture. Theoretical proposals explainingthis discrepancy are reviewed below, in subsection 8.3.

8.1. Transport through doped bilayer

One of the earliest theoretical papers studying the conductivity through AB-stacked bilayer graphenewas Ref. [211] by M. Koshino and T. Ando. There it was assumed that the band structure of the bilayeris described by only two bands closest to the Dirac point energy. In addition to the parabolic dispersionterms, the trigonal warping was also included into the model. Speaking technically, we can say that such amodel corresponds to the low-energy sector of the Hamiltonian, Eq. (42).

Within formalism, the doping level x was controlled by a finite Fermi energy εF, measured from theDirac point energy. The authors estimated that for a typical experimentally-available sample, the dopingis ∼ 1012 cm−2, or higher. Such electron concentration corresponds to the Fermi energy εF ∼ 10ε0, wherethe energy scale ε0 ≈ 3.9 meV used in Ref. [211] characterizes the trigonal warping. It can be related tothe quantity εL, defined by Eq. (45), as the energy of the saddle points of the dispersion surface: ε0 = 4εL.According to the estimates presented in the paper, when the Fermi energy εF ∼ 10ε0 the trigonal warpingexerts significant modifications to the single-electron dispersion.

The only mechanism of current relaxation discussed in Ref. [211] is disorder scattering. Two types ofdisorder were studied separately: long-range and short-range potential disorder. The difference betweenthe two is the presence (absence) of intervalley scattering for the short-range (long-range) scatterers. Thedisorder potential was assumed to be weaker than the amplitude t0. The violation of this condition impliesthe necessity to use the full four-band model, instead of the two-band description employed in the paper. Tocalculate the electric conductivity the authors resorted to the self-consistent Born approximation. Withinthis framework the single-electron self-energy Σ(εF) can be found as a solution of the non-linear integralequation.

If we want to evaluate a transport coefficient, in a typical situation the single-electron self-energy is notsufficient: one needs to know vertex corrections as well. However, for the case of short-range scatterers, thevertex corrections vanish, and the knowledge of Σ(εF) is sufficient to derive σ. The conductivity calculatedin such a manner depends on the Fermi energy εF, which, in turn, is a function of doping x.

51

For general value of disorder, the self-energy may be found only numerically. Yet, for the case of weakshort-range disorder an analytic solution is available. Specifically, in the Σ(εF) → 0 limit, the followingexpression for the self-energy was established in Ref. [211]:

Σ(εF + i0) = − iπ2Wε0

ρ0(εF)

ρ∞, where W =

niu2

2

ρ∞ε0. (108)

Here ρ0(εF) is the density of states at the Fermi energy εF for a pristine bilayer, the quantity ρ∞ is the“high-energy” asymptotic value of the density of states: ρ0(εF) ≈ ρ∞, if t0 εF ε0. The disorder ischaracterized by the product niu

2, where ni gives the concentration of scatterers, while u stands for typicalstrength of an individual scatterer. The parameter W quantifies the strength of the disorder relative tothe strength of the trigonal warping: for W > 1 the disorder scattering smears the fine effects due to thewarping.

Using the above expression for the self-energy, Ref. [211] derived for the conductivity:

σ =e2

π2~×

1W

(|εF|ε0

+ 1), if |εF| > ε0,

34W , if |εF| ε0.

(109)

These results demonstrate that for weak short-range disorder the conductivity is non-universal, and dependson the disorder strength W .

The dependence on W disappears for strong disorder: in the regime W > 1 we have

Σ(εF + i0) ≈ −iΓ, where Γ =π

2Wε0. (110)

The conductivity is equal to

σ =e2

π2~

[(εF

Γ+

Γ

εF

)arctan

(εF

Γ

)+

1

W+ 1

]. (111)

If εF < Γ the conductivity becomes

σ =e2

π2~

(2 +

1

W

). (112)

As disorder grows, this expression approaches the finite universal value: σ ≈ 2e2/(π2~) per spin projection.In addition to these analytic estimates, the results for σ(εF) with numerically-calculated self-energy were

also presented. For weak disorder, the numerical data revealed that at very small εF the conductivity dropsfrom large non-universal value to the universal value of 6e2/(π2~) per spin projection.

For long-range disorder the vertex corrections are finite, and must be taken into account. However, thedependence of the conductivity on the disorder strength and the Fermi energy are similar to the case of short-range disorder. It was demonstrated [211] that at weak disorder the conductivity is inversely proportionalto W . When the disorder is strong (W > 1), the conductivity approaches the universal value 2e2/(π2~).

The theory predictions [211] were compared against transport data in Ref. [111]. The authors of Ref. [211]concluded that in the doping range < 2 × 1012 cm−2, their theory was consistent with the experiment,provided that 1 . W . 2. For larger doping, the experimental resistivity decreased faster than anticipatedby the theory. The authors of Ref. [211] discussed briefly possible reasons of such deviations.

The study of Ref. [211] was later generalized in Refs. [212, 213]. The formalism of the latter papersincluded all four bands of the bilayer. Reference [212] concluded that the two higher-energy bands contributeto the conductivity at large Fermi energy. At the same time, these bands do not significantly affect transportat the charge-neutrality point, even if the disorder is large. In Ref. [213] the effects of the trigonal warpingwere neglected. However, Ref. [213] discussed more general disorder models (impurities with Gaussianpotential and impurities with screened Coulomb potential). For the Gaussian-shape impurity potential

v(r) =v0

πd2exp(−r2/d2) ,

52

Figure 25: Measured AB bilayer graphene conductivity as a function of gate voltage vg for different temperatures [29]. Theconductivity passes through a minimum at non-zero value of the gate voltage. This minimum is believed to occur when theaverage doping level is zero. Away from the minimum, the conductivity demonstrates almost ideal linear behavior as a functionof the gate voltage. The temperature dependence of the conductivity is particularly pronounced at the minimum, see Fig. 26.Reprinted figure with permission from S.V. Morozov et al., “Giant intrinsic carrier mobilities in graphene and its bilayer”, Phys.Rev. Lett., 100, 016602 (2008). Copyright 2008 by the American Physica Society. http://dx.doi.org/10.1103/PhysRevLett.

100.016602

it was found that σ is sensitive both to the strength v0 of the potential, and to its range d. At zero Fermienergy, the conductivity becomes non-universal at larger d. The screened charged impurities also destroythe universality of the conductivity.

The conductivity of a sample with short-range scatterers was numerically studied by M. Trushin et al. [214]using the Kubo formula and kinetic equation formalism. This paper [214] generalized ideas, previously for-mulated for transport in single-layer graphene [215, 216].

J. Nilsson et al. [217] used the Kubo formula and the coherent-potential approximation to discuss theeffects of short-range impurity disorder on the single-electron and transport properties of the AB bilayer andmultilayers. The coherent-potential approximation is considered to be superior to the self-consistent Bornapproximation of Ref. [211]. The paper [217] presented the dependence of the dc conductivity on doping fordifferent impurity concentrations. The zero-doping value of the conductivity was found to be universal.

The electric transport through a bilayer in the presence of screened charged impurities was studiedtheoretically by S. Adam and S. Das Sarma in Ref. [218]. In the limit of higher carrier density the authorsargued that the impurity potential is strongly screened. Such an impurity can be treated as a short-range scatterer with a doping-independent effective potential. The influence of these impurities on thecharge transport was accounted with the help of the Boltzmann equation. For not-too-small doping x, thecalculated conductivity demonstrates a linear dependence on x. As the doping x grows, weak deviation fromthis linear behavior becomes observable.

If the doping x drops below a certain disorder-dependent value, a crossover to a different regime occurs: atlow x disorder-induced electron and hole puddles appear. Such ‘charge puddles’ are thought to be unipolarlycharged areas, which may appear within a sample, whose average doping x is small or zero. In this limit theconductivity saturates near a finite non-universal value and shows only very weak dependence on x. The

53

transport in the presence of puddles will be discussed in more detail in subsection 8.2.It was concluded in Ref. [218] that the developed formalism is consistent with the experimental data (see

Fig. 25). Namely, the authors stressed that they explained both the saturation of the conductivity at lowcarrier density, and obtained a σ(x) ∝ x behavior at higher doping levels.

The analysis of Ref. [218] was re-examined in Ref. [219]. It was claimed that Ref. [218], “consideringonly screened Coulomb disorder, included drastic approximations (e.g. complete screening) which are bothunreliable and uncontrolled”. The authors of Ref. [219] argued that not only the screened Coulomb disorder,but also short-range disorder must be accounted to describe experiments [29, 220]. It was determined thatin a wide range of dopings the conductivity dependence on x is approximately linear, and the temperaturedependence of σ is very weak for higher x. Both features are consistent with the experimental data. Theconductivity at x = 0 was also analyzed.

Another theoretical study of the Coulomb disorder was presented by M. Lv and S. Wan in Ref. [221].This paper investigated the screening of a charged impurity in a doped bilayer sample. The obtained resultswere used to calculate the conductivity as a function of temperature.

Consequences of a different type of disorder were explored in Ref. [222]. The authors noted that, forsingle-layer graphene, experimental studies [223, 224, 225] suggested that radicals adsorbed on a samplebecome an important source of scattering. According to Ref. [222], the same scattering mechanism isrelevant in bilayer samples at large doping levels. The paper developed a theoretical framework to describesuch a disorder, and discussed in detail several subtleties of the formalism. The authors concluded that theproposed mechanism alone is sufficient to explain the linear relation between the conductivity of a bilayerand the sample’s doping level observed in experiments [29] for large doping.

The scattering by the adsorbed atoms, together with other types of disorder (short-range and long-range impurities, vacancies, and others), were considered in Ref. [226]. The authors employed a numericaltechnique called time-evolution method [227]. They claimed that the latter method allows “to carry outcalculations for very large systems, up to hundreds of millions of sites, with a computational effort thatincreases only linearly with the system size”. The paper numerically calculated the conductivity σ as afunction of the doping level x. Depending on the type and strength of the disorder, the function σ(x)demonstrated linear or sublinear behavior.

In Ref. [228] the carrier mobility was measured as a function of both temperature and carrier con-centration. The experimental data for the mobility was analyzed with the help of the scattering timeapproximation. The authors concluded that for a bilayer on a substrate “the mobility is dominated byCoulomb scattering”.

F. Kisslinger et al. [229] observed a linear behavior in the magnetoresistance of epitaxial AB bilayergraphene in a magnetic field up to 62 T at and above room temperature. The authors argued that such abehavior can be attributed to dislocations in epitaxial AB bilayer, “a system that is frequently assumed tobe dislocation-free”.

8.2. Minimum conductivity of a bilayer

As can be seen from Fig. 25 and Fig. 26, even at zero doping, the experimentally-measured conductivityof an AB bilayer sample is small, but finite even at very low temperatures. Apparently, in such a regime,the sample is able to conduct current, although, formally speaking, at zero doping and temperature thesystem has no charge carriers (single-layer graphene also demonstrates a finite minimum conductivity [24]).This property was investigated theoretically using several approaches, defined by nonequivalent sets ofassumptions and technical tools. Some of these methods have already been mentioned in Section 8.1. Otherswill be reviewed below. However, choosing a most suitable technique for a particular experimental situation,one has to be aware of certain theoretical subtleties, important for both monolayer, and AB bilayer grapheneat low doping. Specifically, Refs. [215, 216] developed a kinetic-equation approach to disordered single-layergraphene. It was demonstrated that the use of a simple Boltzmann equation might be unjustified. Instead, amore general kinetic equation accounting for the “chiral” nature of the single-electron states near the Diracpoints must be employed. The ideas put forward in these papers were extended for a bilayer by M. Trushinet al. in Ref. [214]. The function σ(x) approaches finite minimum of the order of e2/(π~), when x→ 0. [214]

54

Figure 26: Experimental data for the minimum conductivity: The blue and red curves demonstrate the measured minimumconductivity of two suspended AB bilayer samples as a function of temperature. The inset shows fine details of the low-temperature data. The conductivity of the bilayer remains finite even for very low temperature. Reprinted by permission fromMacmillan Publishers Ltd: Nature Physics, 5, 889 (2009), copyright 2009. http://www.nature.com/nphys/index.html

Further, if a sample with low or zero average doping is placed on a substrate, charged impurities inthe substrate affect the system in a highly non-perturbative manner. The smooth random variation of theelectrostatic potential due to these impurities could induce so-called “charge puddles” in the sample. Thepuddles are defined in subsection 8.1 as areas with finite unipolar charge density, generated by Coulombdisorder in the substrate. Puddles of both polarities coexist within a single sample. For monolayer graphene,the puddles were discussed theoretically [230] and observed experimentally [231]. It is only natural to alsoapply this concept to the bilayer. For example, above we already discussed Ref. [218] by S. Adam andS. Das Sarma, which invoked this notion in connection with the transport through the bilayer. Using theseideas, W. Zhu et al. [228] offered a semi-phenomenological fitting expression to describe the behavior of theminimum conductivity. A more rigorous approach was adopted in Ref. [232] by S. Adam and M. D. Stiles,where an effective medium theory was used to investigate the conductivity of a sample with a disorderedensemble of puddles (this approximation was also employed in Refs. [219, 233]).

The effective medium theory is a fairly old method designed to study macroscopic properties of a com-posite material. According to a version of the effective medium theory used in Ref. [232], the effectiveconductivity of a macroscopic sample σEMT must satisfy the following equation⟨σ(x)− σEMT

σ(x) + σEMT

⟩= 0. (113)

Here σ(x) is the local conductivity of a small patch of the sample with local doping x. Patches with differentx are randomly distributed over the sample. To account for such a disorder we should view the local dopingas a random variable characterized by some distribution function P [x]. The triangular brackets in Eq. (113)denote averaging over P [x]. Overall, Eq. (113) defines σEMT as an implicit functional of P and the bilayergraphene dispersion. Extracting σEMT from Eq. (113), S. Adam and M. D. Stiles [232] found that theconductivity σEMT possesses interesting universal properties, which we now briefly review.

To discuss universality we need to introduce some notation. Obviously, 〈x〉 = x, which may be treatedas a mathematical definition of the averaged doping level x. In addition, it is convenient to define theroot-mean-square deviation xrms

x2rms = 〈x2〉 − x2. (114)

In the ensemble of puddles, the quantity xrms characterizes fluctuations of the local doping x around itsaverage value x. Disorder introduces additional characteristic scales into our system. We can define the

55

0 0.5 1

0.5

1

1.5

2

σmin

nrmseµc

T

T ∗

Linear Dispersion

Parabolic

Dispersion

Hyperbolic

0 150 3000

1

2

3

σ(10−

4S)

T (K)

Figure 27: Scaling property of the minimum conductivity of the AB bilayer graphene, as described by the effective mediumtheory by S. Adam and M. D. Stiles [232]. Points are experimental data, lines are calculations for different band dispersionsspecified in the picture [linear dispersion ε(k) ∝ k, parabolic ε(k) ∝ k2, and hyperbolic ε(k) ∝ 1/(k + k0)]. The raw minimumconductivity data from different papers [27, 29, 228] are shown in the inset. After the scaling procedure developed in Ref. [232]the experimental points collapse on a single theoretical (red solid) curve. Reprinted figure with permission from S. Adam,M.D. Stiles, “Temperature dependence of the diffusive conductivity of bilayer graphene”, Phys. Rev. B, 82, 075423 (2010).Copyright 2010 by the American Physical Society. http://dx.doi.org/10.1103/PhysRevB.82.075423

dimensionless doping x, temperature T , and conductivity σEMT according to the equations

x =x

xrms, (115)

T =T

εF(x = xrms), (116)

σEMT =σEMT

exrmsµc. (117)

In these formulas εF(x = xrms) is the doping-dependent Fermi energy of a clean sample with x = xrms, andthe charge mobility is µc. If xrms is sufficiently large, we need an additional dimensionless parameter tocharacterize the deviation of the single-electron dispersion from a simple parabola. Assuming that the dis-tribution function P [x] is completely characterized by x and xrms (for example, in Ref. [232] the distributionP was taken to be a Gaussian), the authors demonstrated that σEMT is a universal function of x and T .

Once this universal function is determined, numerically or analytically, the theoretical predictions canbe compared against experimental data. As a crude approximation, one can ignore the dependence of themobility on temperature. Under such a premise one can use experimental low-temperature values for µc.In principle, the quantity xrms could be measured experimentally. However, due to lack of the requireddata, xrms was treated in Ref. [232] as a fitting parameter. With these approximations, the experimentalconductivity reported in Refs. [27, 29, 228], when plotted on a (T , σEMT) plane, collapsed on a singleuniversal curve, see Fig. 27. The authors of Ref. [232] commented that “in the appropriate limits” theirresults agree with the findings of Refs. [217, 228].

A different mechanism for the minimum conductivity was discussed in Refs. [234, 235, 236, 237]. Thesepapers evaluated the conductivity of bilayer samples in the ballistic regime. Assuming that the sample’slength is smaller than its width, the conductivity of e2/(4π~) per valley per spin projection was derivedby M. I. Katsnelson [234]. In such a regime, the charge is transported by evanescent modes to which theLandauer-Buttiker formalism was applied.

Similar Landauer-Buttiker study was reported by I. Snyman and C. W. J. Beenakker in Ref. [236], wherethe conductivity of a disorder-free bilayer sample was evaluated as a function of the Fermi energy εF. The

56

conductivity demonstrated a non-monotonous dependence on the Fermi energy. At the charge neutralitypoint, εF = 0, the conductivity value σ = 4e2/(π2~) of Ref. [236] deviated from the minimum conductivitye2/(π~) of Ref. [234]. The analysis of Ref. [236] suggested that the discrepancy was due to nonidenticalassumptions about the metallic electrodes, which supply current to the sample. The authors of Ref. [236]commented that their value for the εF = 0 conductivity agreed with the result of Ref. [235], where the Kuboformula was used.

Unlike Refs. [234, 235, 236], which all neglected the trigonal warping, J. Cserti et al. [237] accounted forsuch a complication. The trigonal warping drastically changes the minimum conductivity: σ = 12e2/(π2~).

Recently, P. San-Jose et al. [238] presented a comprehensive experimental study of the minimal con-ductivity in AB bilayers. Authors argued that the non-zero minimal conductivity in AB bilayers can beexplained by scattering on boundaries between domains with different stacking order (AB and BA). Theyalso presented experimental evidence, reinforcing their interpretation, of reversible switching between ametallic and an insulating regime in suspended bilayers when subjected to thermal cycling or high currentannealing.

8.3. Transport through an AB bilayer in a transverse electric field

As we explained in subsection 3.3.1, in a transverse electric field, the bilayer becomes an insulator with afield-dependent gap in the single-electron spectrum. Clearly, if the temperature is small, the presence of thisgap suppresses charge transport. In an ideal undoped sample with gap ∆, one expects that when T < ∆the conductivity would demonstrate the activation behavior

− lnσ(T ) ∝ ∆/T . (118)

However, experimental data does not support such a simple picture. For example, Ref. [30] reported thatat zero doping the measured resistivity R(T ) as a function of temperature is best fitted by the law

lnR(T ) ∼ (T0/T )1/3, (119)

where the characteristic temperature scale T0 ∼ 0.5–0.8 K. This behavior is observed for T < 5 K and strongtransverse fields. The exponent of 1/3 in Eq. (119) is consistent with variable-range hopping transport viain-gap impurity states in two dimensions. The emergence of such states in a bilayer sample with the gapwas discussed theoretically in Ref. [239].

The authors of Ref. [240] used a more complicated fitting expression

1

R(T )=

1

R1 exp(E1/T )+

1

R2 exp(E2/T )+

1

R3 exp[(T3/T )1/3](120)

to describe their experimental data. Here R1,2,3 are the fitting parameters with dimension of resistivity, whileE1,2 and T3 have the dimension of energy. This formula aims to describe three transport channels: variable-range hopping and two activation channels. One of the activation channels corresponds to the transportvia the carriers excited thermally above the transport gap E1. Reference [240] reported that E1 > ∆/2 forsmall ∆. When the gap ∆ grows, however, E1 ∼ ∆/2. The second activation channel is “associated withthe hopping conduction between nearest neighboring impurity states”. It is characterized by E2 and R2,and dominates the transport in the interval between 50 K and 5 K. Below 5 K, the variable-range hopping(characterized by T3 and R3) is the strongest contribution to the conductivity.

Another experimental study, Ref. [241], investigated transport in the regime of large electric fields.The strong electric field induces a large single-electron gap; thus, the activation behavior becomes morepronounced. The authors estimated that the field in their setup was three times stronger than the fieldreported in Ref. [30]. The resistivity data obtained in Ref. [241] was fitted by a formula similar to Eq. (120).However, the activation energy extracted from the transport data was two orders of magnitude smaller thanthe single-electron gap, whose value was obtained by infrared spectroscopy. The authors used an impurityband model to qualitatively explain the data.

To address these obvious deviations from the simple Eq. (118), various theorists discussed several mecha-nisms. In Ref. [242] the interplay between the smoothly-varying disorder potential and the gap was studied.

57

If the disorder is strong then charge puddles may appear. The authors [242] identified several transportregimes for the proposed model. Among them, they particularly focused on a case of strong disorder in whichthe variation of the disorder potential is larger than the local value of the gap. In such a situation, mostof the sample surface is covered by puddles, with narrow charge-free insulating strips separating puddles ofopposite polarities. Neither electron nor hole puddles form percolating clusters. Thus, the gapped bilayer“is expected to behave like a bad metal in which transport is dominated by hopping processes betweenelectron and hole puddles that cover most of the sample”. It was hypothesized that this theoretical pictureis relevant for the experimental situation of Refs. [30, 240, 241].

Reference [243] investigated theoretically the conductivity of the gapped bilayer in the presence of short-range disorder. The paper concluded that, due to a certain interband coherence effect, specific to the ABbilayer, the short-range disorder generates a finite conductivity even at T = 0. As a function of temperature,the conductivity may demonstrate a non-monotonous behavior. Related ideas were reviewed in Section 8.2,in our discussion of Ref. [214].

It was demonstrated experimentally [194] that the AB bilayer sample may possesses certain topologicalstacking defects. These defects were already mentioned in Section 7.3: they may host subgap topologicalmodes [193]. These modes give additional contributions to the conductivity at low temperatures. Similarmodes bound to the sample edges [196] also affect the low-T conductivity.

The phase diagram summarizing the stacking-dependent gap openings of biased bilayer graphene wasobtained by C. Park et al. [244] using density functional theory and perturbation analysis. The authors alsoidentified high-density midgap states, localized on grain boundaries, even under a strong field, which canconsiderably reduce the overall transport gap.

Thus, it appears that both theory and experiment agree that for a non-ideal bilayer sample there areseveral mechanisms contributing to the low-temperature transport violating Eq. (118). This indicates thatcreating field-effect transistors based on AB bilayers may be a challenging task: in a gaped “off” state ofthe transistor, unless we have a very clean sample, there are various transport pathways, which allow theflow of the unwanted leak currents.

In recent paper [245], transport measurements were reported in low-doped biased AB bilayer graphenein a perpendicular magnetic field and at low temperatures. Near charge neutrality point the resistivity wasfound to increase exponentially with decreasing temperature from 10 K to 1.4 K at B = 14 T, “indicating anemergence of transport energy gap induced by magnetic field”.

9. Dynamic conductivity and optical spectra

The dynamic (or optical) conductivity of single-layer graphene has been extensively studied theoreti-cally [246, 247, 248, 249, 250], and experiments have largely verified the expected behavior [251, 252, 253,254]. The dynamic conductivity of graphene could elucidate features that would demonstrate unique prop-erties of this system and allow for the identification of characteristic energy scales associated with the bandstructure. Moreover, as the optical properties of graphene are of considerable importance for technologicalapplications, all variants of graphene are also of potential interest and should be examined.

9.1. Dynamic conductivity in AA-stacked bilayer graphene

Let us analyze theoretically the dynamic conductivity of the AA and AB bilayers within the frameworkof the Kubo formalism for the current-current response function and the Green’s function approach [90].To derive an expression for the dynamic conductivity it is useful to determine the Green’s function G(z)from G−1(z) = zI − H, where I is the unit matrix and H is the system’s Hamiltonian. Following Ref. [255]by C. J. Tabert and E. J. Nicol, we choose our Hamiltonian in its simplest form, given by Eq. (20). ThisHamiltonian accounts for nearest-neighbor hopping only, and neglects the possibility of symmetry-breakingand energy gap generation (symmetry breaking and related issues in AA-stacked system are discussed below,

58

in subsection 10.1). Keeping these assumptions in mind, one can write [255]

G−1(z,k) =

z −t0 tf(k) 0−t0 z 0 tf(k)tf∗(k) 0 z −t0

0 tf∗(k) −t0 z

, (121)

where z = iωn, with ωn = πT (2n+1) being the nth (n = 0,±1,±2, ...) fermionic Matsubara frequency. Thefinite frequency conductivity is calculated through the standard procedure based on the Kubo formula [90].Within this formalism, the conductivity is expressed in terms of the retarded current-current correlationfunction. The real part of the conductivity can be written as [255, 256]

σαβ(ω) =Nfe

2

2ω

+∞ˆ

−∞

dε

2π[f(ε− µ)− f(ε+ ~ω − µ)]

ˆ

VBZ

d2k

(2π)2Tr[vαA(ε+ ω,k)vβA(ε,k)

], (122)

where, Nf = 4 is a degeneracy factor, α and β represent the spatial coordinates x, y, z (the axis Oz isperpendicular to the graphene plane), f(ε) = 1/[exp (ε/T ) + 1] is the Fermi function, µ is the chemicalpotential, and the velocity operator is defined as ~vα = ∂Hk/∂kα. The spectral function A(ε,k) is relatedto the Green’s function according to the usual spectral representation

G(z,k) =

+∞ˆ

−∞

dε

2π

A(ε,k)

z − ε. (123)

If T = 0, straightforward calculations in the continuum approximation around the K point of thegraphene Brillouin zone (|v(k)|2 = v2

F ) give the longitudinal σxx and transverse σzz conductivities [256]

σxx(ω) =8e2v2

F

ω

µ

µ−~ω

dε

2π

ˆ

VBZ

d2k

(2π)2

[A11(ε+ ~ω)A11(ε) +A12(ε+ ~ω)A12(ε)

], (124)

σzz(ω) =8e2v2

F

ω

µ

µ−~ω

dε

2π

ˆ

VBZ

d2k

(2π)2

[A11(ε+ ~ω)A11(ε) +A∗13(ε+ ~ω)A13(ε)

−A12(ε+ ~ω)A12(ε)−A∗14(ε+ ~ω)A14(ε)]. (125)

The components of the spectral function are equal to

A11 =π

2

[δ(ε+ε

(3)0k )+δ(ε−ε(3)

0k )+δ(ε+ε(4)0k )+δ(ε−ε(4)

0k )],

A12 =π

2

[δ(ε+ε

(3)0k )−δ(ε−ε(3)

0k )−δ(ε+ε(4)0k )+δ(ε−ε(4)

0k )],

A13 =πf(k)

2|f(k)|

[δ(ε−ε(3)

0k )−δ(ε+ε(3)0k )−δ(ε+ε

(4)0k )+δ(ε−ε(4)

0k )],

A14 =πf(k)

2|f(k)|

[δ(ε+ε

(4)0k )+δ(ε−ε(4)

0k )−δ(ε+ε(3)0k )−δ(ε−ε(3)

0k )], (126)

where the energy bands ε(3,4)0k are defined by Eqs. (21).

Following Ref. [256] we can perform integration in Eqs. (124) and obtain analytical formulas for the realparts of the dynamic conductivities

σxx =e2

4~[8δ(~ω)max(µ, t0) + θ(~ω − 2|µ− t0|) + θ(~ω − 2|µ+ t0|)

],

σzz =e2t0c

20

~3v2F

δ(~ω − 2t0)[(t0 − µ)2θ(t0 − µ) + 2t0µ

], (127)

59

where θ(x) is the Heaviside step-function. To obtain the conductivity of single layer graphene we shall putt0 = 0 and take a half of the obtained value of σxx. The curve σxx(ω) for the AA-stacked bilayer graphenehas a zero frequency Drude peak for any doping and two steps at ω = |µ± t0|/~, due to the existence of twoconductivity bands. In contrast, the conductivity σxx(ω) for the single-layer graphene is a smooth functionof ω in the case of zero doping, µ = 0. The Drude peak and a step at ω = |µ|/~ in single-layer graphenearise only if µ 6= 0 and the DOS at the Fermi level becomes non-zero. The Kramers-Kronig relations allowsone to calculate the imaginary parts of the conductivities [256]. The bias voltage V acts to renormalize theinterlayer hopping parameter t0: for finite voltage it becomes

t′0 =√t20 + (eV )2/4 .

Thus, the bias voltage does not introduce new features into the conductivity [256]. Note that the resultsreviewed here need further generalization, because they are valid only if T = 0, and the possible existence of agap in a single-particle spectrum due to spontaneous symmetry breaking (see subsection 10.1) is disregarded.

9.2. Dynamic conductivity in AB-stacked bilayer graphene

We start our discussion of the dynamic (or optical) conductivity of AB bilayer graphene using a the-oretical approach similar to the one employed in the previous subsection for AA system. As the simplestapproximation, we neglect trigonal warping (hopping amplitude t3) and electron-hole asymmetry (hoppingamplitude t4) as it was done in Refs. [255, 257, 258, 259, 260]. This model successfully explains the majorfeatures of frequency-dependence of the conductivity as well as its dependence on the gate voltage V . Inthis approximation, the conduction and valence bands are symmetric. In the absence of an electrostaticpotential difference between the layers, the two conduction (valence) bands have the same shape and areshifted by t0. Except for the range of very small momenta k, where the trigonal warping is of importance,their shape remains nearly identical even in the presence of a finite V . As a result, there is a high opticaldensity of states for transitions between the two pairs of bands at frequency ωm = t0/~, which gives rise to asharp peak in the real part of the conductivity at ω = ωm. Taking for estimate t0 = 0.40 eV, we obtain thatωm = 3200 cm−1 or 96 THz. Other transitions give more gradually-varying contributions to Reσ, eventuallyleading to asymptotic “universal” value at high frequency equal to e2/(2~), which is twice the value for themonolayer graphene. Finally, in real graphene systems the conductivity features are never sharp because offinite lifetime due to, e.g., disorder scattering. This broadens the peaks and can also merge together severalfeatures that are close in energy.

We use the tight-binding Hamiltonian given by the sum of Hamiltonians in Eqs. (30) and (33) to accountfor the effect of the gate voltage, which opens the gap in the spectrum of the AB bilayer. The equation forthe corresponding Green’s function can be expressed in the following form [255]

G−1(z) =

z + eV/2 0 tf(k) 0

0 z − eV/2 −t0 tf(k)tf∗(k) −t0 z + eV/2 0

0 tf∗(k) 0 z − eV/2

. (128)

Applying Eqs. (122) and (123) in the continuum approximation around the Dirac K point, we derive theformula for the longitudinal conductivity [255]

σxx =2e2v2

F

ω

∞

−∞

dε

2π

ˆ

VBZ

d2k

(2π)2

A11(ε, V )A33(ε+ ~ω, V ) +A33(ε, V )A11(ε+ ~ω, V )

+A11(ε,−V )A33(ε+ ~ω,−V ) +A33(ε,−V )A11(ε+ ~ω,−V )

+2 [A12(ε, V )A∗12(ε+ ~ω,−V ) +A∗12(ε,−V )A12(ε+ ~ω, V )]. (129)

If we take the limit of this expression for t0 = V = µ = 0, we find a constant equal to 2e2/(4~), whichis twice the value of the single-layer graphene conductivity. The spectral functions Aij can be writtenexplicitly [255]. However, these formulas are too cumbersome, and we do not present them here.

60

Figure 28: (Color online) The calculated dynamic conductivity of AB bilayer graphene as a function of the frequency [48].(a) Examples of the allowed optical transitions for the chemical potential indicated by the dashed line. Occupied states areshown by the thicker lines. The dots and the arrows mark the initial and the final states, respectively, of the transitions thatproduce features at frequencies Ej , j = 1, 2, ..., 6 in panel (b). (b) Real and (c) imaginary parts of the conductivity in unitsof σ0 = e2/~ for the gate voltage V = −100 V. The solid curves are for broadening Γ = 0.02t0. The dashed curve is forΓ = 0.002t0. Reprinted figure with permission from L.M. Zhang et al., Phys. Rev. B, 78, 235408 (2008). Copyright 2008 bythe American Physical Society. http://dx.doi.org/10.1103/PhysRevB.78.235408

The analytical expression for σ(ω) can be derived if the temperature is zero and the sample is unbiased(T = 0, V = 0) [17, 255]

σxx =e2

8~

[~ω + 2t0~ω + t0

+~ω − 2t0~ω − t0

θ(~ω − 2t0)

]θ(~ω − 2µ) (130)

+t20

~2ω2

[θ(~ω − 2µ− t0) + θ(~ω − 2µ+ t0)

]θ(~ω − t0) + a(µ)δ(~ω) + b(µ)δ(~ω − t0)

,

where the functions a(µ) and b(µ) are defined according to the equations

a(µ) =4µ(µ+ t0)

2µ+ t0+

4µ(µ− t0)

2µ− t0θ(µ− t0) , b(µ) =

t02

[ln

2µ+ t0t0

− ln2µ− t0t0

]θ(µ− t0) .

In the general case, the function σ(ω) can be calculated numerically. Note also that we derive here only thereal part of the conductivity; the imaginary part can be calculated using a similar approach [48, 101].

A calculated dependence of the real and imaginary parts of the conductivity of AB bilayer graphene [48]is shown in Fig. 28. The calculations were performed with a phenomenological broadening constant Γ (i.e., tomimic the effects of the impurity scattering, the delta-function δ(x) is replaced by (Γ/π)/(x2 +Γ2) [48, 255]).The real part of the conductivity Reσ(ω) has a Drude peak at ω = 0, a characteristic high peak at ω = ωm,and several steps and peaks correspond to the interband optical transitions shown in Fig. 28(a).

Recently, a theoretical study of infrared absorption of graphene samples, both single-layer and bilayer,on hexagonal boron nitride substrate was published by D.S.L. Abergel and M. Mucha-Kruczynski [261].

An experimental study of the infrared conductivity, transmission, and reflection of AB gated bilayergraphene has been performed by L. M. Zhang et al. in Ref. [48]. In addition, this paper presented theoreticalcalculations of the real and imaginary parts of the dynamic conductivity. The authors took into accountboth t3, and t4 hopping amplitudes. Such an approach allowed not only a more complete interpretation ofthe experimental observations, but also to derive from the experimental data the values of t0 = 0.4 eV andt4 = 0.15 eV, and obtain the estimates t ∼ 3 eV and t3 ∼ 0.3 eV. For illustration, the results of calculations

61

Figure 29: (Color online) The dynamic conductivity of AB bilayer graphene as a function of the frequency [48]. Panels (a)and (b) present theoretical, and (c) experimental results for the conductivity Reσ(ω). The deviation V of the gate voltagefrom the charge-neutrality point is indicated next to each curve. For clarity, the curves are offset vertically by 0.5σ0 from oneanother, where σ0 = e2/~. For the plots in panel (b) the parameters are chosen as follows t = 3 eV, t0 = 0.4 eV, t3 = 0.3 eV,and t4 = 0.15 eV. In panel (a) the parameters are the same, except that t3 = 0. The dashed curves superimposed on theV = +50 Volts (−50 Volts) traces in (a) and (b) are the arithmetic means of all the positive (negative) V curves. Reprintedfigure with permission from L.M. Zhang et al., Phys. Rev. B, 78, 235408 (2008). Copyright 2008 by the American PhysicalSociety. http://dx.doi.org/10.1103/PhysRevB.78.235408

and measurements of the real part of the dynamic conductivity taken from Ref. [48] are shown in Fig. 29.The correspondence of the measurements and calculations is satisfactory. As it is seen from the comparisonof the data in Figs. 29 (a) and (b), the effect of the trigonal warping (that is, t3) on the conductivity ispractically negligible.

10. Broken symmetry phases

The electron-electron coupling in carbon systems can be rather large. However, the single-electronapproximation is a good theoretical approach for solving many problems in the case of single-layer graphene.Indeed, the most striking effect of the strong Coulomb repulsion between charge carriers is the opening ofthe insulating gap in the electronic spectrum. The DOS at the Fermi level in undoped single-layer grapheneis zero (see Fig. 3). Thus, the insulating gap should arise in such a system only if the electron-electroncoupling is larger than some threshold value [262, 263]. It is commonly accepted that for single-layergraphene this coupling is close to, but lower than the critical value. In undoped bilayer graphene, the DOSis non-zero at the Fermi level. Thus, the correlation effects are much more pronounced. Moreover, the holeand electron Fermi surfaces (Fermi arcs) of undoped AA bilayer graphene are perfectly nested (see Fig. 6).The latter feature means that at zero temperature a symmetry breaks and the gap opens at an arbitraryweak electron-electron repulsion.

For graphene systems, a specific difficulty arises when we wish to take into account the electron-electroncoupling. These materials are two-dimensional and the electrons interact through three-dimensional electricfields. As a result, the long range part of the Coulomb potential is not strongly screened in graphene, as

62

Reference U0 [eV] U01 [eV] U02 [eV] Method

[264] 9.3 5.5 4.1 cRPA

Table 2: Coulomb potentials in graphene. Parameters U0, U01, and U02 are the on-site, nearest-neighbor, and next-nearest-neighbor in-plane Coulomb repulsions, respectively. Here cRPA stands for the constrained random phase approximation.

it usually occurs in 3D materials. The second problem is the strong effect of the substrate on the electroncoupling, especially on the long-range part of this coupling.

To avoid serious mathematical difficulties associated with the description of the long-range Coulombinteraction, the majority of researchers consider either only on-site Coulomb repulsion U0, or work in thecontinuum-media (or long-wave) limit. The latter approach is the most convenient when the effect of thesubstrate is of importance. However, the nearest-neighbor in-plane repulsion U01, or inter-plane U11 terms aresmaller, but comparable to U0. Thus, to obtain realistic results one has to take these terms in considerationeither directly, or by an appropriate renormalization of U0. Note also that the continuum-media approachis valid only to study the low-lying electronic states, and could be inappropriate in the case of high dopingor for the calculation of thermodynamic properties.

The values of the Coulomb potentials are usually calculated [264] using some ab initio methods orestimated from the comparison of the theoretical results with the experimental findings. In table 2 wepresent data on the Coulomb potentials in graphene taken from Ref. [264]. In this table U02 is the in-planenext-nearest-neighbors repulsion potential, other U ’s are defined in the text above.

10.1. Low-temperature broken symmetry phases of AA bilayer graphene

In the AA-stacked bilayer graphene the effect of the electron-electron correlations is the most pronounced.The presence of two bands with identical Fermi surfaces makes the AA-stacked bilayer graphene unstablewith respect to spontaneous symmetry breaking. This instability can open a gap in the electronic spectrumto decrease the free energy of the system for arbitrary small interaction. Since there is no experimental dataon the electronic properties of the AA graphene bilayer, we below review only theoretical results.

10.1.1. Electron correlations: symmetry analysis

The specific symmetries of the Hamiltonian can be used to narrow the choices of the possible sym-metry breakings and order parameters. Such an analysis has been performed at the mean-field level byA. L. Rakhmanov et al. in Ref. [36]. In the mean-field approximation, the interaction operator

Hint ∝∑

ψ†αψβψ†γψδ

is replaced by a single-particle operator

HMFint ∝

∑〈ψ†αψβ〉ψ

†γψδ ,

where the average 〈ψ†αψβ〉 represents different types of possible order parameters. To be at least metastable,the order parameter must open a gap at the Fermi level. The authors of Ref. [36] started from a tight-bindingHamiltonian similar to Eq. (23) (with t′ = 0), but written in the basis

Ψkσ = (ak1σ, ak2σ, e−iϕkbk1σ, e

−iϕkbk2σ)T ,

where ϕk = arg f(k). In this basis, the matrix Hamiltonian (23) becomes real and equals

Hk =

0 t0 −tζk tgζkt0 0 tgζk −tζk−tζk tgζk 0 t0tgζk −tζk t0 t0

, (131)

63

where ζk = |f(k)|. The Hamiltonian is invariant under the transpositions of both the layers and thesublattices. The authors showed that, to open a gap at the Fermi level for arbitrary small interaction,it is necessary to break both of these symmetries. The general expression for the mean-field interactionHamiltonian HMF

int , which breakes both symmetries and induces a gap at the Fermi level, is

HMFint =

∑kσ

ψ†kσδHkσψkσ, δHkσ =

∆zz

kσ −i∆yzkσ −i∆zy

kσ −∆yykσ

i∆yzkσ −∆zz

kσ ∆yykσ i∆zy

kσ

i∆zykσ ∆yy

kσ −∆zzkσ i∆yz

kσ

−∆yykσ −i∆zy

kσ −i∆yzkσ ∆zz

kσ

, (132)

where the real-valued functions ∆yykσ, ∆zz

kσ, ∆yzkσ, and ∆zy

kσ, are different components of the multi-componentorder parameter.

To calculate the renormalized spectra near the Fermi level, one should diagonalize the matrix Hkσ =Hk + δHkσ. This gives

E(2,3)kσ =

ε(2)k + ε

(3)k

2∓

√√√√(ε(2)k − ε

(3)k

2

)2

+ |∆kσ|2, (133)

where ε(2,3)k are given by Eq. (25) (these two bands cross the Fermi level when interactions are neglected),

and∆kσ = ∆zz

kσ + ∆yykσ + i (∆zy

kσ + ∆yzkσ) . (134)

The gap between renormalized bands is equal to

∆0 = 2mink |∆kσ| .

The order parameters in Eq. (134) are found by minimization of the grand potential. Which type of ordercorresponds to the ground state depends on the features of the interaction Hamiltonian. The parameter∆zz

kσ can be related to the so called G-type antiferromagnetic (AFM) order (all nearest neighboring spinsin the lattice are antiparallel to each other). It is controlled by the on-site Coulomb repulsion energy. Theorder parameter ∆yy

kσ can be attributed to the instability toward the homogeneous shift of one graphenelayer with respect to another one. To consider this type of order one has to take into account the electron-phonon interaction. The order parameters ∆zy

kσ and ∆yzkσ can be viewed as excitons, which produce circular

currents flowing inside and between the layers, respectively. These parameters are controlled by the in-planeand out-of-plane nearest neighbor Coulomb repulsion energies. All these types of order compete againsteach other. The ground state of the system corresponds to antiferromagnetism, when the on-site Coulombrepulsion energy U0 is the strongest interaction constant.

10.1.2. Electron correlations and antiferromagnetic order

The AFM order in AA-stacked bilayer graphene was considered first in Ref. [36], and then studied indetail in Refs. [73, 265]. The authors used a Hubbard-like model, where the single-particle part of theHamiltonian is given by Eq. (20), while the Hubbard interaction term has a form

Hint =U0

2

∑iαaσ

(niαaσ −

1

2

)(niαaσ −

1

2

). (135)

Longer range Coulomb interactions were neglected. It is commonly accepted that in this limit one shoulduse the estimate for U0 smaller than that predicted by the ab initio (see Table 2) calculations [266]. Theauthors used the characteristic values U0 = 5–7 eV.

In Refs. [36, 73, 265] it was shown that the on-site Coulomb repulsion stabilizes so-called G-type AFMorder. In such a state the localized spin at any given site is antiparallel to spins at nearest-neighbor sites.Other types of AFM order are either unstable or metastable. Thus, the order parameter can be written as

∆αA ≡ U0

⟨a†nα↑anα↓

⟩, ∆αB ≡ U0

⟨b†nα↑bnα↓

⟩, ∆1A = ∆2B = −∆2A = −∆1B ≡ ∆ , (136)

64

Figure 30: (Color online) Dependence of the AFM gap ∆(x, T ) on doping x, calculated for U0 = 5.5 eV and different valuesof the normalized temperature T/∆0, from Ref. [73]: (1) T/∆0 = 0.06, (2) T/∆0 = 0.17, (3) T/∆0 = 0.33, (4) T/∆0 = 0.41,(5) T/∆0 = 0.47, (6) T/∆0 = 0.52, (7) T/∆0 = 0.55, and (8) T/∆0 = 0.58; note that ∆0 = ∆(0, 0) is the value of the AFMgap at zero temperature and doping. Inset: The dependence of the mean-field transition temperature TMF on doping x. Thereentrance from the PM to AFM state exists in the doping range xc < x < 1.231xc; xc = 0.128 and ∆0 = 0.124 eV. PM meansparamagnetic phase, and AFM means antiferromagnetic phase.

and ∆ is real. In the mean-field approximation, the interaction Hamiltonian has the form [73]

Hint = N[

4∆2

U0− U0(n2 − 1)

]+U0x

2

∑nαaσ

nnαaσ −∑nα

(∆αAa

†nα↑anα↓ + ∆αBb

†nα↑bnα↓ + h.c.

), (137)

where x = n − 1 is the doping, n is the number of electrons per site, and N is the number of unit cells.Mean-field spectra are obtained by diagonalizing of H0 + Hint. The spectra are

ε(1,4)k = ∓

√∆2 + (t|f(k)|+ t0)

2, ε

(2,3)k = ∓

√∆2 + (t|f(k)| − t0)

2. (138)

To determine the AFM gap ∆ one has to minimize the grand potential per unit cell

Ω =4∆2

U0− U0(n2 − 1)− 2T

4∑s=1

ˆdk

VBZln

[1 + e

(µ′−ε(s)k

)/T], (139)

where µ′ is the renormalized chemical potential, µ′ = µ− U0x/2. The equation

∂Ω

∂∆= 0 (140)

specifies the gap as a function of the chemical potential and temperature. To find ∆ as a function of dopingx, one needs to relate the doping and the chemical potential [73]

n = 1 + x = −1

4

∂ (Ω− E0)

∂µ′. (141)

Equations (140) and (141) implicitly define the AFM gap ∆(x, T ) and the chemical potential µ(x, T ). Ifonly the nearest-neighbor hopping is taken into account, the gap obeys the particle-hole symmetry relation,

∆(−x, T ) = ∆(x, T ) .

65

Figure 31: (Color online) The dependence of the AFM gap ∆ (red solid curve) and |q| (blue dashed curve) on the doping x,calculated for T/∆0 = 0.06 and U0 = 8 eV, from Ref. [73]. The dot-dashed curve is the gap calculated for q = 0. The dopingx is normalized by the critical doping xc, calculated for the commensurate AFM state. The incommensurate AFM exists in aslightly larger doping range than the commensurate AFM.

The next-nearest-neighbor hopping breaks this symmetry; however, this effect is small. The gap as a functionof doping x(> 0) is shown in Fig. 30. The gap decreases monotonously when the doping level x grows. Thegap becomes zero at some x = xc(T ).

In two-dimensional systems no long-range order is possible if T > 0. In such a situation, the mean-fieldsolutions characterize the short-range order, which survives for sufficiently low T . The effects beyond themean-field approximation are discussed in Ref. [73]. The gap ∆(T ) decreases when temperature increases,and the crossover from (short-range) AFM insulating state to the paramagnetic (PM) metallic state (seeinset of Fig. 30) occurs at temperatures about mean-field transition temperature TMF(x). It is interestingto observe that the transition temperature is not a single-valued function of doping. Instead, it exhibits apronounced reentrant behavior. This feature will be discussed below.

The maximum value of the crossover temperature depends on the on-site Coulomb repulsion U0. Forexample, AFM ordering can exist up to temperatures of about 50 K for U0 = 5.5 eV and to temperaturesmuch higher than room temperature for U0 & 6.5 eV. The critical doping value xc, at which the AFM stateis replaced by the PM one, also strongly depends on U0, changing from about 0.1% for U0 = 5.5 eV to about10% for U0 ' 8 eV. [73]

10.1.3. Incommensurate antiferromagnetic order

The G-type AFM state has the smallest value of the thermodynamic potential Ω among states withcommensurate magnetic order. Further optimization of Ω can be achieved if the local direction of theantiferromagnetic vector is allowed to rotate slightly from site to site [267]. Such a state is referred to asincommensurate (or helical) AFM. The complex order parameter for this state has the form

∆nαA = U0〈a†nα↑anα↓〉 = eiqn∆αA, ∆nαB = U0〈b†nα↑bnα↓〉 = eiqn∆αB , (142)

where q describes the spatial variation of the direction of the AFM vector. The averaged electron spin Snαa

in the unit cell n, layer α, sublattice a lies in the x–y plane and is related to the order parameter by

Snαa =∆αa

U0[cos (qn), sin (qn)] . (143)

Therefore, the grand potential becomes a function of q. Thus, one should add the minimization condition∂Ω/∂q = 0 to derive equilibrium value of q. The corresponding calculations were done in Ref. [73]. The

66

Figure 32: (Color online) The phase diagram of the AA-stacked bilayer graphene [73], calculated for U0 = 5.5 eV (a) andU0 = 6.5 eV (b). Solid (red) curves are mean-field AFM to PM transition temperature TMF(x); (blue) dashed curves areT q(x), at which the commensurate-incommensurate transition occurs. The dotted (red) curves are TMF(x), calculated withouttaking into account the incommensurate AFM state. The dot-dashed (green) curves show the region of phase separation (seesubsection 10.1.4).

plots of the AFM gap ∆(x) and |q(x)| are shown in Fig. 31. For comparison, the curve ∆(x) calculated forthe commensurate AFM (q = 0) is also presented. We see that the incommensurate AFM state exists in aslightly wider doping range than the commensurate one. The phase diagram of the model in the x–T planeis shown in Fig. 32 for two different values of U0. The diagrams for U0 . 6 eV and U0 & 6 eV demonstratea qualitative difference. Namely, for smaller U0 the reentrance, seen in the inset of Fig. 30, disappears.For larger U0 it survives. On the other hand, for large U0 the mean-field approximation is not an accuratemethod. Thus, it is not clear, whether the reentrance is a genuine feature of the system, or it is an artifactof the mean-field approximation.

Note, the incommensurate AFM phase is mathematically equivalent to the Fulde-Ferrel-Larkin-Ovchinni-kov state in superconductors [268, 269, 270, 271, 272]. Such incommensurate order is known to be sensitiveto disorder. However, the effect of disorder on the incommensurate AFM state was not analyzed in Ref. [73].

10.1.4. Phase separation

The formation of the inhomogeneous or phase separated states is an inherent property of multibandsystems with significant electron-electron coupling. In Refs. [73] and [265] it was predicted that at non-zerodoping, the AA bilayer graphene can separate in two phases with unequal electron densities n1,2 = 1 + x1,2.A typical dependence of the chemical potential on doping, µ(x), for nonzero temperature is shown in Fig. 33.The derivative ∂µ(x)/∂x is negative in some range of doping. This indicates that the system is unstable, andcan experience phase separation into commensurate (q = 0, x1 < x) and incommensurate (q 6= 0, x2 > x)AFM phases. The doping levels x1,2 are found using the Maxwell construction [273]: the (black) horizontalline is drawn in such a manner that the areas of the shaded regions in Fig. 33 are equal to each other. Theregion of phase separation in the (x–T )-phase diagram is bounded, in Fig. 32, by (green) dot-dashed curves.If the possibility of an incommensurate AFM is ignored, then phase separation occurs between the AFMinsulator (x1 = 0) and the PM (U0 & 6 eV), or the AFM (U0 . 6 eV) metal (x2 > 0).

The separated phases have different electron concentrations, and the phase separation will be frustratedby long-range Coulomb repulsion [274, 275, 276, 277]. Unless the Coulomb interaction completely arrests theseparation, the formation of nanoscale inhomogeneities is likely. If the electron-rich phase (incommensurateAFM) is a metal, and the electron-poor phase is an insulator or “bad” metal, then, the percolative insulator-metal transition could occur when the doping x exceeds some threshold value, which is about 0.5(x1 + x2)in 2D systems. Phase separation can exist in the doping range x1 < x < x2. Depending on U0, phaseseparation could be observed in a temperature range from 30–40 K to room or even higher temperatures(see Fig. 32).

67

Figure 33: (Color online) Chemical potential µ versus doping x from Ref. [73]; U0 = 5.5 eV and T = 0.014 eV. The verticaldot-dashed line separates the AFM states with q = 0 and q 6= 0. In the doping range x1 < x < x2, phase separation occurs.The values x1,2 are determined by the Maxwell construction: the horizontal (black) line is drawn in such a manner that theareas of the shaded regions are equal to each other.

10.1.5. Nearest-neighbor Coulomb repulsion, bias voltage, and exciton order parameter

The nearest neighbor terms in the interaction part of the Hamiltonian can lead to the appearanceof different ordered states. However, according to Ref. [36] all these order parameters compete againstantiferromagnetism, and only the AFM order parameter survives [36, 73, 265], because U0 is the strongestinteraction constant (see Table 2). A nonzero bias voltage V breaks the symmetry between two graphenelayers. It was shown by R. S. Akzyanov et al. [45], that in this case, there exists an order parameterdriven by the inter-layer interaction coexisting with antiferromagnetism. The analysis based on symmetryconsiderations (see subsection 10.1.1) shows that this order parameter should have the form [45]

∆Aexc = U11

⟨a†n1↑an2↓

⟩, ∆B

exc = U11

⟨b†n1↑bn2↓

⟩, ∆A

exc = −∆Bexc ≡ ∆exc, (144)

and the ∆exc is real. This order parameter corresponds to a bound state of an electron and a hole in differentlayers, and can be referred to as the exciton order parameter.

The calculation of ∆exc was performed in Ref. [45] for an undoped sample at T = 0 using the mean-fieldapproach similar to that described in Section 10.1.2. The exciton order parameter was found to increasewhen the bias voltage V grows. However, the full gap in the spectrum decreases when V increases, since theAFM gap is much larger than the exciton one, |∆| |∆exc|. At non-zero temperature, the applied voltagecan fully suppress the gap giving rise to a voltage-driven metal-insulator transition. For the typical valuesof parameters U0 = 2.2t, U11/U0 = 1/4, and eV/t0 = 0.1, the values of the order parameters are estimatedas ∆ ≈ 0.17 eV and ∆exc ≈ 8 meV. [45]

The expressions for the order parameters can be rewritten in terms of magnetization: S = ∆/U0 is theaveraged spin on the site A1, and φ = ∆exc/U11 can be viewed as the spin located on the link connectingthe nearest sites A1 and A2 in different layers. The spin on the link connecting carbon atoms B1 andB2 has opposite sign. The dimensionless exciton magnetization φ(V ) (and the order parameter as well)increases almost linearly with V , while S decreases with increasing bias voltage. Nevertheless, φ S(and, consequently, ∆exc ∆), even for relatively large V . The exciton condensation could be observedby measuring the Coulomb drag [278, 279, 280]. The experimental observation of the Coulomb drag inan artificial structure of two graphene sheets with a dielectric barrier between them has been reported byR. Gorbachev et al. in Ref. [281].

68

The crossover temperature T ∗, at which the transition from ordered phase to PM state occurs, is of theorder of ∆. Consequently, ∆exc T ∗. However, the exciton order parameter is correlated with the AFMone, and it could be expected that they both have the same crossover temperature. According to resultspresented in the previous sections, doping suppresses the AFM ordering. It is natural to expect that it willalso suppress the exciton gap [45].

10.1.6. Long-range Coulomb interaction

Since in 2D systems the screening of the long-range Coulomb repulsion is not so effective as in 3Dsystems, taking it into account is of special interest. Proper treatment of the long-range effects improves theaccuracy of the calculations. Further, this long-range interaction also stabilizes additional order parameters,which can be important for the analysis of the phase separated state. However, for AA bilayer graphenethis problem was considered only in a few theoretical papers.

In Ref. [282] D. S. de la Pena et al. analyzed ordering in undoped AA-stacked bilayer graphene takinginto consideration the on-site Coulomb repulsion, both in-plane and out-of-plane nearest-neighbor Coulombrepulsion terms, and in-plane next-nearest-neighbor Coulomb repulsion. They studied the possible groundstates of AA-stacked bilayer graphene using a functional renormalization group approach. The authorsanalyzed a set of possible electronic instabilities: AFM ordering of the type considered above, charge densitywave (CDW), quantum spin Hall instability (QSH), etc. They concluded that, in the range of parameterscharacteristic of AA-stacked bilayer graphene, the only stable phase is the AFM order, while additionalorders could exist in the AA honeycomb bilayer at a smaller value of the on-site interaction. However, apossible existence of significant QSH fluctuations in the AA-stacked bilayer graphene was predicted.

The long-range Coulomb repulsion was taken into account by L. Brey and H. A. Fertig in Ref. [283]. Theauthors consider a single-valley model Hamiltonian for electrons in undoped AA bilayer near the Dirac pointusing the Hartree-Fock approximation. They observe the instability of a single-electron spectrum with theformation of the energy gap and analyzed several possible order parameters arising due to the long-rangeCoulomb repulsion. However, they neglect the spin of the electrons, which automatically excludes the AFMordering from their consideration. As it was stated above, the AFM instability competes with other possibleinstabilities and could suppress them. Thus, the question about possible additional order parameters in theAA-stacked bilayer graphene and their coexistence with the AFM ordering is still open.

A Monte Carlo study of the AFM ordering of AA bilayer graphene was reported by A. Nikolaev andN. Ulybyshev in Ref. [284, 285]. The authors used long-range interaction Hamiltonian. They concludedthat long-range terms act to destroy the AFM order on finite clusters. It is not clear at the moment how toapply this result to an infinite sample. However, it seems to imply that a longer-range interaction weakensthe AFM order.

10.2. Low-temperature broken symmetry phases of AB bilayer graphene

Since the AB bilayer has a finite density of states at the Fermi energy, it is natural to inquire aboutthe stabilization of a broken symmetry phase in such a system at sufficiently low temperature. Indeed,there are several experimental observations [23, 26, 27, 28, 32, 286, 287, 288, 289, 290], which support thisnotion. However, the exact nature of the ordering transition is not known. For example, some experimentsfound that the low-temperature state has a single-electron gap, while others reported gapless behavior.This may indicate an experimental artifact, or could be a manifestation of a competition between severalnon-equivalent ordered states. Below we will discuss some candidate broken-symmetry states, which areconsidered by theorists.

10.2.1. Ferromagnetic and antiferromagnetic states

One of the earliest papers on the subject is Ref. [291] by J. Nilsson et al. The authors investigatedthe effects of the long-range and short-range repulsion on the low-temperature symmetry breaking for theunbiased AB bilayer. To study the long-range Coulomb interaction the authors used the two-band Hamilto-nian (at both Dirac points only two bands touching the Fermi energy are kept) augmented by the following

69

interaction term

H longint =

1

2S

∑α=±,q

Vα(q)ραqρα−q , (145)

where

V±(q) =1± e−qc0

2V (q) =

πe2

q(1± e−qc0), and ρ± = ρ1 ± ρ2 . (146)

In these equations, the symbol S denotes the sample area, and c0 is the distance between the layers, thebare Coulomb potential in the momentum space is

V (q) =2πe2

|q|. (147)

The layer density operators ρ1,2 correspond to smooth components of the total electron density: ρ1,2 are

sums of the terms ψ†KψK and ψ†K′ψK′ , which conserves the valley index. The oscillating components of the

density, ψ†KψK′e−i(K−K′)r and ψ†K′ψKe

i(K−K′)r, were initially omitted.To investigate the stability of a ferromagnetic state the authors [292] applied the variational approach

due to Bloch, adopting it to the AB bilayer. The corresponding wave function was constructed in such away that at each Dirac point the density of spin-up electrons was unequal to the spin-down density, whilethe total density was kept constant. The authors shown that the state with finite magnetization in eachvalley is more stable than the paramagnetic state. The phase diagram at finite doping was also discussed.

Unlike the case of a single Fermi surface, for the bilayer one has to worry about two K-points. Thus,finite magnetizations at individual valleys do not immediately imply that the sample has finite magneticmoment, since the magnetizations of two valleys may be either add up, or cancel each other out, resultingin either a finite, or zero total magnetic moment of the whole system. Within the variational calculationsoutlined above, these states are degenerate. To lift this degeneracy, the authors [292] added the exchangeterm describing the interaction between the oscillating components of the electron density. For such amodel, the most stable state is the one with a finite ferromagnetic moment (related theoretical studies offerromagnetism in biased AB bilayers were reported in Refs. [293, 294]).

Thus, the results of J. Nilsson et al. [291] suggest that the long-range interaction favors a ferromagneticground state. To study the effects of the short-range interaction, the authors of Ref. [291] used the Hubbardmodel on the lattice of the AB bilayer. Applying the mean-field approximation to such a Hamiltonian itwas shown that, at one electron per carbon atom, the mean-field ground state is antiferromagnet. Since thegraphene bilayer lattice with nearest-neighbor hopping is bipartite, this result is not that surprising.

The described investigation demonstrated that the competing long-range and short-range interactionsmay act to stabilize different types of ordered states. This means that the phase diagram of a particularsample could depend on delicate details of the system, which shift the balance between the competing states.

However, one must not take the results of Ref. [291] too literally. It is necessary to remember that thejustification of the two-band model may be problematic when the effects of the interaction are studied.Indeed, the single-site interaction constant for graphene is estimated to be of the order of several eV, whilethe discarded “high-energy” bands are separated from the Fermi level by a fraction of eV. Further, thediscussed variational ferromagnetic wave function is only one possible type (among many) of ordered statepromoted by the long-range interaction. Consequently, other options must also be explored.

10.2.2. “Pseudospin magnetic” states

Several ordered states are considered theoretically as alternative to ferromagnetic and AFM ones. Forexample, H. Min et al. argued in Ref. [295] that the long-range Coulomb interaction establishes a gappedbroken symmetry state, which they called a “pseudospin magnet”. The paper suggested that, by neglectingthe chiral structure of the single-electron states, the authors of Ref. [291] ignored a very effective routeto minimize the electron interaction energy. The Hartree-Fock calculations of Ref. [295] demonstrated

70

that, at each valley and for each spin projection, the bilayer may experience the spontaneous generation of“pseudospin polarization”, which may be viewed as a finite expectation value of some “pseudospin” operator.In the context of the latter study, the pseudospin is the layer index, or, equivalently, the sublattice index.Therefore, the finite pseudospin polarization (for a given spin projection σ and a given valley ξ) implies thatthe electron density

ρσξ = ψ†σξψσξ

associated with σ and ξ is spontaneously shifted toward a particular layer. Summing the pseudospin polar-izations over all values of σ and ξ, the total polarization for a given many-electron trial state is determined.It could be either zero (“pseudospin antiferromagnet”), or finite (“pseudospin ferromagnet/ferrimagnet”).These order parameters are of excitonic origin in the sense that they describe condensation of electron-holepairs. A particular ordered phase corresponds to electron-hole pairs with specific spin and orbital quan-tum numbers. At the charge neutrality point the most stable state is “pseudospin antiferromagnet”. InRef. [296] these conclusions were checked with the help of renormalization group calculations. It was judgedthat the results of this renormalization group study were consistent with the Hartree-Fock findings of H. Minet al. [295]. A related renormalization group investigation was reported in Ref. [297].

R. Nandkishore and L. Levitov [298] also studied long-range interactions, but used a different technique.They argued in favor of the stability of “the ferroelectric” state. The ferroelectric state is characterizedby a finite value of the electric charge polarization vector, directed normally to the bilayer plane. In otherwords, some electrons from one layer are spontaneously shifted to the other layer, creating a local violationof charge neutrality. The energy associated with the ordering was estimated to be ∼ 4 meV, that is, withinthe experimentally accessible range. In the language of Ref. [295], this ferroelectric state is a “pseudospinferromagnet”. The results of both papers are consistent with each other.

It is worth noting that an earlier paper by E. McCann et al. [257] reasoned against stability of such aferroelectric state, pointing out that the electric polarization increases the Hartree energy. In Ref. [298] thisargument was criticized: the exchange interaction, neglected in Ref. [257], overcomes the Hartree term. Thismakes the transition into the ferroelectric state possible. Such a conclusion agrees with the calculations ofH. Min et al. [295], which also identified the exchange contribution as the driving force behind the symmetrybreaking.

In Ref. [299] R. Nandkishore and L. Levitov pointed out that if V− = 0 in Eq. (145), then the Hamil-tonian symmetry is significantly enhanced. For a generic value of V−, the Hamiltonian symmetry groupis SU(2)×SU(2), where one instance of SU(2) corresponds to the rotation of electron spin, while the otherdescribes the rotation in the valley space. When V− vanishes, the symmetry group is augmented to SU(4).

Working with such a highly symmetric Hamiltonian, Ref. [299] developed a classification of the brokensymmetry states. It covers the states discussed in Refs. [295, 298], as well as some others. The classificationformalized and extended the ideas in Ref. [295] about “pseudospin (anti)ferromagnet”. To explain the originof this classification more rigorously, let us examine the following mean-field Hamiltonian [299]:

H = −v2F

t0

(0 (qy + iqx)2 ⊗ 1⊗ 1

(qy − iqx)2 ⊗ 1⊗ 1 0

)+ ∆

(Q 0

0 −Q

). (148)

In this expression, the first term corresponds to the kinetic energy of the bilayer. The product 1 ⊗ 1is an identity matrix in the spin-valley space. While the kinetic energy differs from Eq. (41), the tworepresentations are unitary equivalent [299]. The second term shows the mean-field contribution due tobroken symmetry caused by the Coulomb interaction. Specifically, the parameter |∆| represents the absolutevalue of the order parameter. It is proportional to the single-electron gap. The hermitian 4 × 4 matrix Q,acting in the spin-valley space, and satisfying the condition Q2 = 1, sets a “direction” of the multicomponentorder parameter. This quantity is analogous to the vector n, with n2 = 1, which describes, for example,the direction of the magnetization for a ferromagnet. Unlike the magnetization, however, the number ofindependent components of Q is much higher.

The value of |∆| is found by solving the mean-field equation [298]. However, the sign of ∆ and the matrixelements of Q, beyond the constraint Q2 = 1, are completely arbitrary within the framework of the mean-

71

field theory. We can say that all mean-field states form a degenerate manifold parametrized by matrices Q,such that Q2 = 1, and a specific matrix Q encodes a particular mean-field state from this manifold.

It was noticed in Ref. [299] that the latter manifold has some internal structure: it can be split into threeequivalence classes. To explain the division into the classes, let us note that, because of the constraint, alleigenvalues of Q are equal to ±1. Thus, one can define three equivalence classes, which will be denotedbelow as (4, 0), (3, 1), and (2, 2). The first class corresponds to matrices with four positive eigenvalues. Thesecond class, to matrices with three positive eigenvalues and one negative. Finally, the matrices with twopositive and two negative eigenvalues constitute the third class. Within a particular class, any two matricesare unitary equivalent, but a pair of matrices from different classes cannot be connected by an SU(4)transformation. For example, if the eigenvalues of some Q1 are all positive, while the eigenvalues of someother Q2 are both positive and negative, it is impossible to find a unitary matrix such that Q2 = UQ1U

†.Therefore, the SU(4)-symmetric Hamiltonian has only three types of non-equivalent mean-field ground

states, corresponding to the three equivalence classes. Specifically, the first and the second classes contain theso-called quantum anomalous Hall (QAH) states. These states have finite non-diagonal (Hall) conductivityσxy (at zero doping). Depending of the type of QAH state, it equals to either 4e2/h, or to 2e2/h. The finitevalue of the Hall conductivity is a manifestation of the time-reversal symmetry breaking.

As for the third class, it is called the quantum flavor Hall state. For this class σxy = 0, thus, time-reversal symmetry is preserved. Instead, these states are characterized by either finite non-diagonal spinconductivity, non-diagonal valley conductivity, or non-diagonal spin-valley conductivity. All quantum flavorHall states are equivalent in the sense that they can be connected by a transformation from the HamiltonianSU(4) symmetry group. This equivalence is an artifact of the initial approximation, which mixes spin andvalley spaces, making them indistinguishable from each other. A more detailed analysis reveals that differentflavor Hall states are quite dissimilar, and have non-identical physical properties: the valley Hall state hasfinite interlayer electric polarization (it is the ferroelectric state of Ref. [298]), the spin-valley Hall state islayer antiferromagnet [300] (total magnetization of the layer antiferromagnet is zero, but the magnetizationsof each layer is finite). Therefore, the less symmetric Hamiltonian lifts the degeneracy between these states.The degeneracy between the SU(4) multiplets may be lifted by fluctuations and a weak external magneticfield [299].

To overcome the shortcomings of the continuous effective models, the same set of pseudospin-orderedphases was studied with the help of a lattice model by J. Jung et al. in Ref. [300]. It was found that theordered states are stable even in the lattice model. The quantum anomalous Hall states and flavor Hallstates have different energies; however, this difference is very small, of the order of 10−9 eV per carbonatom. The paper [300] evaluated the energy gap as ∼ 10 meV. The latter value is roughly consistent withthe estimate of ∼ 4 meV reported in Ref. [298]. It was also claimed that the developed theoretical picture isin agreement with experimental results [23, 286].

Experimental signatures of these broken symmetries were discussed by theorists in Refs. [301, 302].

10.2.3. Antiferromagnetic state

As one can see from the previous discussion, the antiferromagnetic phase is considered by many theoriststo be a viable candidate for the low-temperature broken-symmetry state of the bilayer. Thus, its proper-ties have been investigated in several publications. For example, a first-principle calculations reported inRef. [303] confirmed the stability of the antiferromagnetic ordering. The gap was found to be ∼ 1.8 meV,and the surface magnetization was ∼ 10−2µB nm−2.

A very popular tool to study antiferromagnetism is the Hubbard model. It was used, for example, inRefs. [291, 304, 305, 306, 307, 308]. The latter references employed Monte Carlo simulations [305, 307], differ-ent versions of the renormalization group approach [304, 305, 308], and mean-field theories [291, 305, 306]. Inparticular, the perturbative renormalization group study of Ref. [304] concluded that the antiferromagneticinstability is the strongest instability of the Hubbard model.

A continuous model was used in Ref. [130], which offered a mean-field treatment of the antiferromagneticstate in a magnetic field. It was found that the insulating gap grows as a function of the magnetic field. Theauthor [130] reported that, after adjusting two parameters of the proposed theory, the experimental datawas described quantitatively by the theory.

72

Experimentally, the low-temperature layer-antiferromagnetic order was mentioned as a possibility inRefs. [289, 290].

10.2.4. Nematic phase

A completely different way to eliminate the finite density of states at the Fermi energy was proposed byO. Vafek and K. Yang in Ref. [309]. This paper used a perturbative renormalization group approach, whichwas applied to a two-band effective Hamiltonian with interactions. The authors assumed that the electroninteraction potential V (r) vanishes, if |r| > r0, where r0 a is some finite length scale. According to thisstudy, the strongest instability corresponds to the order parameter, which breaks rotation symmetry of theHamiltonian. The mean-field Hamiltonian in the broken-symmetry phase can be written as follows:

Hnem = −v2F

t0

(0 (ξqy + iqx)2

(ξqy − iqx)2 0

)+

(0 ∆′ − iξ∆′′

∆′ + iξ∆′′ 0

), (149)

where different values of ξ = ±1 correspond to different valleys, K or K′. The complex number

∆ = ∆′ + i∆′′ ,

with

∆′ = 〈Ψ†KσxΨK + Ψ†K′σxΨK′〉 , ∆′′ = 〈Ψ†KσyΨK −Ψ†K′σyΨK′〉 , (150)

is the order parameter. This order parameter changes its sign, when the real space is rotated by π/2. Inanalogy with the nematic state of liquid crystals, which has the same symmetry, this order parameter iscalled nematic. Note that this ordered state is insensitive to the electron spin: the rotation of spins doesnot change ∆.

The eigenenergies of the Hamiltonian (149) are given by the relation:

ε = ±|(ξqy − iqx)2 + ∆| . (151)

Upon the transition into the nematic phase, the Fermi point at q = 0 with parabolic dispersion splits intotwo Fermi points at

q∗x + iξq∗y = ±√

∆ , (152)

both with linear dispersion. Unlike the states discussed in subsections 10.2.2, 10.2.3, the nematic state isgapless. However, below the energy scale set by |∆|, the electron density of states vanishes linearly near theFermi energy.

Within the framework of the two-band model, the absolute value of the order parameter |∆| is fixed, butits complex phase is completely undetermined. Unlike the superconducting order parameter phase, whosevalue is of no significance, the phase of the nematic order parameter has a physical consequence: as one cansee from Eq. (152), the locations of the emergent Dirac points in k-space depends on arg ∆. The presence ofthe lattice, however, reduces the degeneracy relative to arg ∆ down to a set of three discrete angles, definedwith respect to the crystallographic axis. Once the direction of the vector (q∗x, q

∗y) is chosen (randomly) from

this discrete set, in the resultant nematic state the effective hopping along the bonds parallel to a particularδi, (for definition of δi see Fig 1) is enhanced. In this regard Y. Lemonik et al. in Ref. [310] pointed outthat the nematic order parameter is “mimicking the effect of anisotropic hopping along bonds with differentdirections on the honeycomb lattice”.

The nematic order, its stability, and competition against other ordered states is a subject of several the-oretical publications. In a comprehensive renormalization group study of O. Vafek, Ref. [304], the nematic,antiferromagnetic, and quantum anomalous Hall states were listed as possible broken-symmetry states for amodel with short-range interaction. According to the latter paper, which state wins depends on values of the“microscopic” Hamiltonian coupling constants. For example, the very short-range interaction of the Hub-bard model leads to antiferromagnetic order. These conclusions are consistent with the results of Ref. [311],

73

which argued that short-range interactions favor antiferromagnetic order, while longer-range interactionsstabilize the nematic state. The antiferromagnetic phase is associated with short-range scattering, sincesuch a phase requires inter-valley scattering, which decreases as the interaction range grows. A related per-turbative renormalization group study was reported by V. Cvetkovic et al. in Ref. [312]. It was shown thatthe two-band model with generic choice of interaction constants has a very diverse phase diagram. However,“nematic appears to be the unique dominant instability when forward scattering dominates. Similarly, thelayer antiferromagnet appears upon inclusion of sufficiently strong back and layer imbalance scattering”.

Analogous conclusions were reached in Refs. [310, 313], where a different version of the perturbativerenormalization group was used (among these two papers Ref. [310] presented the latest and most extensiveaccount of the calculations, it also corrected some misprints of an earlier publication, Ref. [313]). Thesepapers derived the renormalization group flow in the presence of screened Coulomb interaction. Accordingto Ref. [310], the nematic, antiferromagnetic, and quantum spin Hall phases are the most probable groundstates of the bilayer.

A different approach to the question of the relative stability of the nematic order and other ordered phaseswas adopted by E.V. Gorbar et al. in Ref. [314]. That paper, using a two-band model with Coulomb long-range interaction, obtained, in the random-phase approximation, the energies of different ordered phases inthe presence of a transverse bias voltage and external strain. The authors showed that at zero strain theground state is gapped: one of the “pseudospin magnetic” phases discussed in subsection 10.2.2 wins overthe nematic state. The transverse bias voltage can be used to stabilize the otherwise unstable/metastableferroelectric state (also referred to as “pseudospin ferromagnet”, or quantum valley Hall state). Since thepolarization vector couples to the electric field, the energy of the ferroelectric state decreases when the biasgrows, and at sufficiently strong bias the ferroelectric state becomes the ground state. The strain, on theother hand, couples to the nematic order parameter. Thus, if the bias is zero, a sufficiently strong externalstrain destroys the pseudospin order, which is replaced by a gapless phase with a finite expectation valuecorresponding to the nematic order parameter. This, of course, is not spontaneous nematic order, since therelated symmetry is already broken in the Hamiltonian by the outside condition (strain). At arbitrary strainand bias, the ground state is one of the “pseudospin magnetic” states with an admixture of the nematicorder parameter. This phase diagram in the plane strain versus bias-voltage contains two phases “separatedby a critical line of first- and second-order phase transitions” [314].

There are several experimental papers [23, 26, 286], whose findings were interpreted as consistent withthe nematic low-temperature state. However, there are other experiments (e.g., Refs. [32, 315]), which areinconsistent with this hypothesis. J. Zhang et al. [316] suggested that disorder might explain the discrepancybetween experiments. They demonstrated that, in mean-field approach, the ground state of AB bilayerundergoes a transition between different ordered states as a function of the disorder strength. In particular,they predicted that small amounts of disorder can drive the gapped ground state into a nematic state, andboth gapped and nematic orders vanish if the impurity density exceeds some critical value.

10.2.5. Other types of order

Other types of ordered states have been investigated in the theoretical literature [312, 317, 318, 319]. Forexample, Refs. [318] discussed the charge density wave. The phase diagram of Ref. [312] contains numerousordered states, some of which were mentioned above, some others, like superconducting phases, were not.

The authors of Ref. [319] argued that the bilayer lattice Hamiltonian may stabilize a particular “currentloop order”, provided that the only interaction term included into the Hamiltonian is the nearest-neighborrepulsion. While such a choice of the interaction seems highly peculiar, some reasoning behind this ap-proximation was offered. The proposed symmetry-breaking state was called “magnetoelectric”. It has somesimilarities with the quantum anomalous Hall state, but, unlike the latter, breaks layer-inversion symme-try. The authors stated that the phenomenology of the magnetoelectric symmetry violation offered a morecomprehensive explanation to the experimental data of Refs. [28, 32] than the explanation in terms of theantiferromagnetic order, or quantum anomalous Hall state.

Exciton order was investigated in Refs. [317], where the authors performed a mean-field analysis ofa lattice model with Hubbard-like interaction. To stabilize the exciton phase the repulsion between theelectrons located in different layers was taken into account. Conversely, the discussed excitons are formed

74

by electrons in one layer and holes in the other. The authors concluded that, to stabilize the exciton phase,the interaction constant must exceed a threshold value of the order of 10t ∼ 30 eV. Such high value of thecoupling constant is unrealistic. The paper noticed that this threshold may be reduced by a transverseelectric field. However, for realistic fields the effect is quite weak. Thus, it is likely that such an orderparameter cannot be stabilized in graphene bilayers.

As the above discussions demonstrate, the non-interacting ground state of AB bilayer graphene is unstablewith respect to a variety of symmetry breakings. In such a situation, a theorist’s ability to predict the“true” ground state is quite limited: the theory allows one to compile a list enumerating various possibleordered states, which could be stabilized under realistic conditions. Such a list may serve as a guide to anexperimentalist. However, which ordered state wins under a particular set of external conditions can bedetermined only experimentally.

11. Many-body and non-Fermi liquid effects in bilayer graphene

Highly doped AB bilayer behaves almost as an ordinary metal and is described by Fermi liquid theory.However, if one is interested in the many-body properties of the undoped AB bilayer graphene, it is necessaryto remember that, unlike a metal with its well-developed Fermi surface, it has no Fermi surface, only Fermipoints. This circumstance has dramatic consequences for the many-body physics of the electronic liquid ofthe bilayer. Even at weak doping, when the Fermi points are replaced by a Fermi surface, many electronicproperties are dominated by the proximity of the charge-neutrality regime.

Since the undoped AB bilayer does not have the Fermi surface, it lacks the quasiparticles as definedby the Landau theory of the Fermi liquid. This feature of the system was investigated in Refs. [320, 321].Assuming that the RPA adequately describes the effective interaction between charge carriers, Y. Barlasand K. Yang [320] calculated the self-energy to second-order in the screened interaction. It was found thatthe quasiparticle spectral weight Z vanishes as the energy approaches zero

Z ∝ 1

(ln ε)2→ 0 , when ε→ 0 . (153)

The disappearance of the quasiparticle residue is inconsistent with the quasiparticle notion of the Landautheory. This means that the undoped bilayer is not a Fermi liquid. At the same time, while the residue Zvanishes, the effective mass remains unchanged by the interaction.

This perturbation-theory treatment was improved by R. Nandkishore and L. Levitov in Ref. [321], wherethe renormalization group approach was used. Those renormalization group calculations confirmed thedestruction of the quasiparticles: as the energy approaches zero, the quasiparticle residue vanishes as theinverse of the square of ln ε, in agreement with Eq. (153). The disappearance of the quasiparticles impliesthe suppression of the tunneling density of states, which may be measured experimentally. A weaker (log-arithmic) renormalization of the mass was also discovered. Since the mass renormalization is a subleadingeffect, the perturbation theory of Ref. [320] was unable to capture it. Interactions also introduce logarithmiccorrections to the compressibility. However, the authors of Ref. [321] concluded that these corrections areweak, and difficult to detect in experiments.

For doped bilayer, the electronic liquid properties were discussed in Refs. [322, 323, 324]. Specifically,it was argued in Ref. [324] that, upon doping, the Fermi surface emerges, and the Fermi liquid behavioris restored. In Ref. [322] the compressibility of the bilayer electronic liquid was calculated within theframework of the Hartree-Fock approximation for different values of the Fermi momentum kF. In general,the compressibility was found to be a non-monotonous function of kF. At low density it was negative. Theseresults have to be contrasted with those of Ref. [321], where only weak corrections to the compressibility werefound. This discrepancy may be related to the fact that Ref. [322] disregarded the screening of the Coulombinteraction [321]. The renormalization of mass as a function of the doping density was discussed in Ref. [323].The ground state wave function was constructed with the help of the Hartree-Fock approximation. Toaccount for the screening, the Coulomb potential in the Hamiltonian was replaced by a static Thomas-Fermipotential. The authors concluded that the mass is strongly suppressed by the interaction but, nonetheless,it remains finite even at low doping levels.

75

Reference [325] investigated many-body corrections to the cyclotron resonance in the monolayer andAB bilayer graphene, and compared the theoretical conclusions with the experimental data [104]. As theauthor admitted, the data “defy good fit by theory but certainly suggest nontrivial features of many-bodycorrections”. The high resolution ARPES measurements of low doped AB bilayer samples done in Ref. [326]confirmed directly non-Fermi liquid quasiparticle behavior in AB bilayer.

The dielectric function ε(k, ω) is among the physical quantities affected by the peculiar band structureof AB bilayer graphene. Most generally, ε may be written as follows

ε(k, ω) = 1− V (k)Π(k, ω) . (154)

In this expression, Π is the irreducible polarization, and V (k) is the Fourier transform of the bare Coulombpotential, Eq. (147). The dielectric function, due to its importance for both fundamental and appliedresearch, was investigated very actively [219, 221, 327, 328, 329, 330, 331, 332]. For example, the staticCoulomb screening was discussed in Refs. [219, 221] in the context of electric transport, see subsection 8.1.

As another instance of this type of study, we would like to mention Ref. [331] by X.-F. Wang andT. Chakraborty, where ε(k, ω) was determined with the help of the extremely common random-phase ap-proximation (RPA). In the framework of RPA, the full polarization Π in Eq. (154) is replaced by the one-looppolarization Π0, which may be viewed as the polarization of the system with no electron-electron interaction.To find Π0, the authors of Ref. [331] used a two-band effective Hamiltonian with the trigonal warping term,see Eq. (44). Because of the warping, the RPA static dielectric function ε(k, 0) demonstrated noticeableanisotropy for k ∼ pL [the momentum pL characterizes the scale below which the trigonal warping is im-portant, see Eq. (45)]. At k = 0 the value of the static ε was as high as 102 at zero temperature, and evenbigger at finite temperature.

Studies of Coulomb screening were presented in Refs. [327, 328, 329, 330, 333]. In Ref. [327], besidesscreening, the Kohn anomaly, RKKY interaction, and Friedel oscillations were investigated for both dopedand undoped bilayer, modeled by the two-band Hamiltonian. Finite temperature RKKY interaction forboth bilayer and single-layer graphene was calculated in Ref. [334].

The many-body properties of AA bilayer were recently studied by Y. Mohammadi [335]. He derived ananalytical formula for the static polarization function for a biased AA bilayer using random phase approxi-mation and the simplest tight-binding Hamiltonian taking into account only nearest neighbors hopping andneglecting electron-electron interaction. The obtained results were applied to calculate Coulomb screeningand the electrical conductivity. It was argued that the short-range scattering is not affected by the perpen-dicular electric filed, while the conductivity limited by the (long-range) Coulomb scattering is enhanced bythe bias voltage.

12. Dielectric function and plasmonics in AB bilayer

Numerous investigations have covered photonics of graphene systems and AB bilayer in particular, in-cluding plasmonics, the nonlinear optical, and optoelectronic properties. Here we discuss these topics verybriefly. Interested reader may consult recent reviews [13, 14, 15]. We also restrict our focus to AB bi-layer as being experimentally relevant. Studies of plasmon physics in AA bilayer are limited to theoreticalpublications [336, 337, 338, 339].

The knowledge of the dynamic dielectric function ε(k, ω) was used by several authors to determine thedispersion of the plasmons. Briefly recall that plasmons are quanta of the longitudinal collective chargedensity oscillations. Their dispersion relation ω = ωk is a solution to the equation

ε(k, ωk) = 0 . (155)

Reference [331] reported that the undoped AB bilayer at T = 0 has a single plasmon mode. When thetemperature is finite, however, an additional weakly-damped lower-frequency mode emerges. The effectsof doping on the plasmons were briefly mentioned as well. Reference [332] of the same authors discussedplasmons in a situation when the bilayer is subjected to a transverse bias voltage, which generates a gap inthe single-particle spectrum.

76

To analyze screening and the plasmon mode, the author of Ref. [329] used a four-band model at finitechemical potential, but neglected the trigonal warping. This paper reported the technical details of the thepolarization operator calculations. References [328, 330] discussed different plasmon properties. Plasmonsin the presence of a magnetic field were considered in Ref. [340].

In Ref. [341] S.A. Mikhailov and K. Ziegler argued theoretically that, besides the longitudinal plasmons,a single-layer graphene sample can support an additional transverse electrodynamic mode. Their analysiswas based on previous theoretical study of electrodynamics of a thin metallic film [342]. In the context ofAB bilayer such ”transverse plasmons” were discussed in Ref. [343], for the twisted bilayer in Ref. [344].

Interesting results were obtained in recent studies of plasmons in the AB bilayer [345, 346, 347, 333, 339].T. Low et al. [345] theoretically studied plasmonic response in biased Bernal-stacked bilayer graphene. Theauthors found that the AB bilayer “accommodates optically active phonon modes and a resonant interbandtransition at infrared frequencies”. As a result, the plasmonic properties of bilayer graphene are stronglymodified “leading to Fano-type resonances, giant plasmonic enhancement of infrared phonon absorption,a narrow window of optical transparency, and a new plasmonic mode at higher energy than that of theclassical plasmon.” This suggests that bilayer graphene may be considered as an interesting and importantplasmonic material. These conclusions were supported in the experiments by Z. Fei et al. [346]. Usinginfrared nanoimaging, the authors determined that “bilayer graphene supports plasmons with a higherdegree of confinement” when compared to single-layer graphene or an artificial double-layer (subnanometerseparated) graphene characterized by a random stacking order. The plasmons mode were attributed to aninterlayer tunneling process. The authors were able to tune the plasmonic mode by a gate voltage andconclude that their observation “uncovers essential plasmonic properties in bilayer graphene and suggests apossibility to achieve novel plasmonic functionalities in graphene few-layers”. It should be also mentionedhere that an analog of the effect of plasmon-induced transparency was observed by H. Yan et al. [347] inAB nanoribbons.

13. Twisted bilayer graphene

In addition to bilayer graphene with AB and AA stacking, there is a class of bilayers characterizedby a non-zero (twist) angle θ between two graphene layers. Such twisted bilayers can be synthesized usingdifferent preparation techniques. For example, bilayer samples with rotation misorientation can be producedin the process of growth on the SiC substrate (see, e.g., Refs. [6, 348, 349, 350]). They can be synthesizedalso by chemical vapor deposition (CVD) [351, 352, 353, 354, 355, 356, 357, 358]. Another approach is thefolding of single graphene sheet [359, 360, 361]. Reference [362] reported the preparation of twisted bilayergraphene (tBLG) by transferring the graphene monolayer synthesized by CVD onto another monolayerepitaxially grown on SiC. Similar techniques were used also in Ref. [363]. Note also that in graphite crystalsthe top layer is often rotated with respect to the deeper layers [364].

Twisted bilayer graphene has a more complex crystal structure than the AA and AB bilayers. Thereview of the geometrical properties of the tBLG requires a separate subsection. The crystal structure ofthe twisted bilayer affects significantly its electronic properties. Due to its complex geometry, even thesingle-particle models for the tBLG are quite involved. Because of this complexity, the majority of thepublished papers on the subject are devoted to study electron spectra (both at zero or non-zero magneticfield) in the single-electron approximation. The papers recently studying the effects of electron-electroninteractions in twisted bilayer graphene are virtually absent. We hope this gap will be addressed in futurestudies. The peculiarities of the system and theoretical methods used for its study require to review thetwisted bilayer graphene in a separate Section.

13.1. Geometrical properties: Moire pattern and superstructure.

The twist of one graphene layer with respect to another one manifests itself in the appearance of aMoire pattern, which can be visualized using STM techniques. Such structures have been observed in manyexperiments using scanning microscopy [6, 348, 349, 351, 352, 365, 366] and dark-field transmission electronmicroscopy [353, 354] (DF-TEM). For different values of the twist angle θ, the STM images of the Moire

77

Figure 34: (Color online) Scanning tunneling microscope images of bilayer graphene samples with different twist angles θrevealing a Moire pattern. The twist angle is estimated by measuring the Moire period. Reprinted figure with permissionfrom I. Brihuega et al., Phys. Rev. Lett., 109, 196802 (2012). Copyright 2012 by the American Physical Society. http:

//dx.doi.org/10.1103/PhysRevLett.109.196802.

patterns are shown in Fig. 34. The value of the twist angle is determined from the measured Moire periodL. The latter length is defined as the distance between light (or dark) regions in the STM images. Theangle θ and L are related according to the following formula [364]:

L =a0

√3

2 sin(θ/2), θ < 30. (156)

where a0 = 1.42 A is the in-plane C-C distance. The Moire pattern is a peculiar feature of twisted bilayergraphene, which has no analog for the AA or AB bilayers. In general, for non-zero θ, the lattice propertiesof the twisted bilayer are quite singular. This subsection is dedicated to their description.

The details of the crystal structure of tBLG have been considered in many papers (see, e.g., Refs. [3, 16,367, 368, 369]). Here, we will follow, mainly, Ref. [367] by J. M. B. Lopes dos Santos et al. Each graphenelayer in tBLG consists of two sublattices (A1, B1 in the layer 1, and A2, B2 in the layer 2). The positionsof the carbon atoms in each sublattice in the bottom layer 1 are

r1An ≡ rn = na1 +ma2 , r1B

n = rn + δ , (157)

where δ = a0(1, 0). The quantity n = (n,m) is an integer-valued vector, and a1,2 are the basis vectors ofthe graphene elementary unit cell, Eq. (1). The distance between graphene layers is c0 = 3.35 A. When thelayers are not rotated (θ = 0), we assume that the system is a perfect AB bilayer.

Let us, for definiteness, assume that layer 2 is rotated around the axis connecting the atoms A1 and B2with n = 0, while layer 1 remains fixed. In this case, the atoms of the top layer (layer 2) have the positionsezc0 + r2α

n , where ez is the unit vector in the z direction, and

r2Bn ≡ r′n = na′1 +ma′2 , r2A

n = r′n − δ′ . (158)

In these equations,

a′1,2 = a1,2

(cos θ ∓ sin θ√

3

)± a2,1

2 sin θ√3

, (159)

78

and δ′ = a0(cos θ, sin θ).While the Moire exists for any θ, the superstructure, that is, strictly periodic repetition of some large

multiatomic supercell, occurs for the so-called “commensurate” θ only. The supercell may coincide with theMoire cell, but, generically, contains many Moire cells. For the superstructure to emerge, after the rotation,a certain atom of the sublattice B2 from layer 2 must end up exactly over an atom of the sublattice A1 fromlayer 1. This happens when the twist angle satisfies the following relation [3, 16, 367, 368]

cos θ =3m2

0 + 3m0r + r2/2

3m20 + 3m0r + r2

, (160)

where m0 and r are mutually-prime positive integers. The number of sites in the elementary unit cell of thesuperlattice N is

N(m0, r) =4

g

(3m2

0 + 3m0r + r2), (161)

where g = 1 if r 6= 3n, and g = 3 if r = 3n (n is integer). In the notation used by E. J. Mele [16, 370, 371],the structures with r 6= 3n (r = 3n) are called ‘odd’ (‘even’). The superlattice vectors can be expressed interms of the single-layer graphene lattice vectors as:

R1 = m0a1 + (m0 + r)a2 ,

R2 = −(m0 + r)a1 + (2m0 + r)a2 , (162)

if r 6= 3n, and

R1 =(m0 +

r

3

)a1 +

r

3a2 ,

R2 = −r3a1 +

(m0 +

2r

3

)a2 , (163)

if r = 3n. In both cases, the size of the superlattice cell LSC ≡ |R1,2| = a0

√3N/2

Due to the symmetry of the single-layer graphene lattice, the rotation on the angle θ = 2π/3 transformsthe AB bilayer to itself. In addition to that, rotations on angles θ and −θ are equivalent to each other. Asa result, one can consider only twist angles in the range 0 < θ < 60. A rotation on the angle θ = π/3transforms the bilayer from AB to AA stacking. Moreover, if the angle θ corresponds to some commensuratestructure (m0, r), the angle θ′ = π/3− θ is also commensurate with m′0 = r/g and r′ = 3m0/g, where g = 1if r 6= 3n, and g = 3 otherwise. Thus, rotations for angles θ > 30 can be considered as rotations for theangle θ′ = π/3− θ < 30, but starting from the AA-stacked bilayer graphene as a reference structure. Notethat Eq. (156) for the Moire period is valid only for θ < 30: for larger θ we have to replace θ → θ′.

In addition to the twist angle, the bilayer graphene can also be characterized by a non-zero shift of onelayer with respect to another one. In the majority of the papers, however, this shift is not considered.

The authors of Ref. [372] constructed an effective Hamiltonian in the continuum (low-energy) approx-imation for tBLG with a non-zero shift % between the layers. They found, however, that this effectiveHamiltonian coincides with that for % = 0 upon a unitary transformation, so the electronic spectrum isindependent on %. This is because, in the continuum approximation, the detailed information about thesuperlattice is averaged out, and the effect of non-zero % is reduced only to shifting the Moire pattern inspace [372], which does not affect the electronic spectrum.

Among the superstructures (m0, r) with θ < 30, there is a special subset corresponding to r = 1. Itcan be shown from Eq. (160) that in the vicinity of the angle θ, corresponding to some m0 and r = 1, thereis an infinite set of commensurate angles with different m′0 and r′ > 1. These structures have larger sizesupercells. However, as it was shown in Ref. [367], such structures are almost periodic repetitions of thestructure with m0 and r = 1. Figure 35 illustrates this fact. The structure (7, 3) shown there is quite similarto the structure (2, 1) with the smaller size of supercell.

For structures with r = 1, the size of the superlattice LSC coincides with the Moire period L, whilefor all other structures LSC > L. This can be easily checked using Eq. (160) for the twist angle and the

79

Figure 35: (Color online) Structure of the twisted bilayer graphene with (m0, r) = (7, 3) (θ ∼= 12.95). The large blackhexagon is the Wigner-Seitz cell of the superlattice, while R1,2 are the superlattice vectors. This structure is an almostperiodic repetition of the structure with (m0, r) = (2, 1) (θ ∼= 13.17) having a smaller size of the superlattice (gray hexagons).Reprinted figure with permission from J. M. B. Lopes dos Santos et al., Phys. Rev. B, 86, 155449 (2012). Copyright 2012 bythe American Physical Society. http://dx.doi.org/10.1103/PhysRevB.86.155449.

relation (156) for the Moire period [367]. The supercell of the structure (m0, r) with r > 1 contains a r2/gnumber of Moire cells, where g = 1, if r 6= 3n, or g = 3 otherwise. The arrangements of carbon atomsinside these cells are slightly different from each other and approximately correspond to the superstructure([m0/r], 1), where [a] means the integer part of a. For angles θ > 30, the corresponding subset is (1, 3m0),and

θ(m0, 1) = π/3− θ(1, 3m0) . (164)

The basis vectors of the reciprocal superlattice can be written as

G1 =4

N[(2m0 + r)b1 + (m0 + r)b2] ,

G2 =4

N[−(m0 + r)b1 +m0b2] , (165)

if r 6= 3n, and

G1 =4

N

[(m0 +

2r

3

)b1 +

r

3b2

],

G2 =4

N

[−r

3b1 +

(m0 +

r

3

)b2

], (166)

if r = 3n. In these equations, b1,2 are the reciprocal lattice vectors of the bottom layer, Eq. (4).The Brillouin zone of the superlattice has the shape of a hexagon with sides QBZ = |G2 − G1|/3.

In the particular case r = 1, this side is equal to ∆K = |Kθ − K|, where K = 4π(0, 1)/(3√

3a0) andKθ = 4π(− sin θ, cos θ)/(3

√3a0) are the Dirac points of the bottom and top layers, respectively. For r > 1,

QBZ is smaller than ∆K and is equal to QBZ =√g∆K/r, where g = 1 if r 6= 3n, and g = 3 otherwise.

Figure 36 shows the Brillouin zones of the superstructures (1, 1) and (2, 3) having twist angles θ ∼= 21.798

and θ ∼= 27.796, respectively. For comparison, the Brillouin zones of the rotated and static layers are also

80

K2

K1

G2

K'K'

kyK

kx

(a) K

G1

K

K

K2

K1

G2

K'K'

ky

K

kx

(b)K

G1

K

K

Figure 36: (Color online) Geometry of the reciprocal lattice for the twisted bilayer graphene. The green thick solid hexagonnew the center shows the Brillouin zone of the tBLG with the superstructures (1, 1) [panel (a), θ ∼= 21.798] and (2, 3) [panel(b), θ ∼= 27.796]. The large hexagons show the Brillouin zones of individual layers: the red dashed hexagon corresponds tothe bottom layer, the blue dot-dashed hexagon corresponds to the top layer. The next several Brillouin zones of the tBLG aredepicted by (black) thin solid hexagons. For the twisted bilayer, the Dirac point K′ (K′θ) is equivalent to the point Kθ (K)if r 6= 3n. When r = 3n, Kθ ∼ K and K′θ ∼ K′ (see the text), where the symbol ‘∼’ means equivalent. The twisted bilayergraphene Dirac points K1,2 are doubly degenerate: each of them is equivalent to one of two Dirac points of each graphenelayer. For the particular case of the (1, 1) superstructure [panel (a)], K1 ∼ K ∼ K′θ and K2 ∼ K′ ∼ Kθ, while for the (2, 3)superstructure [panel (b)], we have K1 ∼ K ∼ Kθ and K2 ∼ K′ ∼ K′θ. The vector ∆K = Kθ−K is shown for both structures.For the structure in panel (b) it coincides with the reciprocal vector of the superlattice, in panel (a) vector ∆K does not equalto the reciprocal vector of the superlattice.

shown in this figure. Recall that each graphene layer has two non-equivalent Dirac points, K and K′(= −K)for the bottom layer, and Kθ and K′θ(= −Kθ) for the top (rotated) layer. To find out where these Diracpoints are located in the Brillouin zone of the superstructure one can express their co-ordinates in terms ofreciprocal superlattice vectors. For r 6= 3n we have

K = −K′ = m0G2 +r

3(G1 + 2G2) ,

Kθ = −K′θ = m0G2 +r

3(G2 −G1) , (167)

while for r = 3n

K = −K′ =r

3G2 +

m0

3(G2 −G1) ,

Kθ = −K′θ = −r3G1 +

m0

3(G2 −G1) . (168)

It follows from these formulas, that the points K′ and Kθ (as well as K and K′θ) are equivalent to each otherif r 6= 3n [see Fig. 36(a)], that is, the difference K′ −Kθ is the reciprocal vector of the superlattice. Whenr = 3n, other pairs of Dirac points are equivalent: K ∼ Kθ and K′ ∼ K′θ [see Fig. 36(b)]. Thus, for anycommensurate angle, there are two doubly-degenerate non-equivalent Dirac points of the twisted bilayer.Inside the reciprocal cell of the superlattice, these two non-equivalent tBLG Dirac points are located at:

K1 =G1 + 2G2

3, K2 =

2G1 + G2

3, (169)

81

for any superstructure (see Fig. 36). This double degeneracy affects the electronic structure of the tBLG,leading to band splitting and band-gap formation (see subsection 13.2.4).

13.2. Effective low-energy theories of twisted bilayer graphene electronic spectrum

13.2.1. Low-energy Hamiltonians

The specific electronic properties of tBLG are mostly determined by the interlayer single-electron hoppingand the twist angle. For commensurate structures, numerical studies based on density functional theoryand tight-binding calculations were performed in numerous papers [154, 348, 368, 369, 373, 374, 375, 376,377, 378, 379, 380, 381, 382, 383]. Since the elementary unit cell of the tBLG superlattice contains a largenumber of sites, especially at small twist angles, the ab initio calculations incur a significant computationalcost.

To avoid this difficulty, several semi-analytical theories have been developed for describing the low-energyelectronic properties of tBLG [3, 367, 370, 371, 372, 384, 385, 386, 387, 388, 389, 390]. These theories operatemainly on the electronic states near the Dirac cones, which the tBLG inherits from its two constituent layers.In tBLG, the Dirac cones having their origins at K and Kθ (as well as K′ and K′θ) are located close to eachother in momentum space (for θ < 30). This allows constructing an effective low-energy Hamiltonian forthe Dirac electrons moving in each graphene layer and hybridized by inter-layer hopping.

The first such low-energy theory was proposed by J. M. B. Lopes dos Santos et al. [3] and further developedin Ref. [367]. The authors consider the following effective Hamiltonian of tBLG:

H = ~vF∑kαβ

d†1kασαβ

(k +

∆K

2

)d1kβ + ~vF

∑kαβ

d†2kασθαβ

(k− ∆K

2

)d2kβ +

∑kαβ

∑G

(tβα⊥ (G)d†1k+Gαd2kβ + h.c.

). (170)

The first two terms here describe the Dirac quasiparticles moving in layers 1 and 2 respectively, where d†ikαand dikα (i = 1, 2) are the creation and annihilation operators of the electron with the momentum k, inlayer i, in the sublattice α. The momentum k is measured from the point K0 = (Kθ + K)/2, and additionalterms ±∆K/2 in brackets (where ∆K = Kθ −K), appear due to the position of the Dirac points of thebottom and top layers with respect to K0. The labels α, β are the sublattice indices, σ are Pauli matricesacting in the sublattice space, while σθ is defined as σθ = eiθσz/2σe−iθσz/2. The use of σθ instead of σ isassociated with the rotation of the second layer. Spin and valley degeneracy are assumed in this model, andthe corresponding indices in the electronic operators are omitted.

The last term in Eq. (170) describes inter-layer hopping. The second summation is performed over the

vectors G = nG1+mG2 (n,m are integers) lying inside the single-layer graphene Brillouin zone, and tβα⊥ (G)are the Fourier transform of the interlayer hopping amplitudes, which can be written in the following form

tβα⊥ (G) =4

N

∑n∈SC

t⊥[δβα(r1αn )]e−iG

′r1αn , (171)

where G′ = ∆K+G and the summation is performed over the sites inside the superlattice cell. The functiont⊥[δβα(r1α

n )] is the amplitude of the electron hopping from the site in the layer 1 located at r1αn to the nearest-

neighbor site in the layer 2 located at c0ez + r1αn + δβα. Only nearest-neighbor hopping is considered, even

though the authors mention that results are not changed qualitatively if the more distant hopping will betaken into account. These hopping amplitudes are calculated numerically using the procedure proposed inRef. [391] (see also Section 13.3 for more details).

The authors showed that the amplitudes tβα⊥ (G) decay rapidly with increasing |G|. As a result, inthe first approximation, one can keep only three terms in the sum over G in Eq. (170) with G = 0,G = G1, and G = G1 + G2. The corresponding values of G′ = ∆K + G have the same magnitude,

82

(c)

Figure 37: (Color online) (a) Spectra of the low-energy tBLG bands calculated for θ = 3.9 (m0 = 8, r = 1) in Ref. [3]; themomentum k changes from k = K0 −∆K to k = K0 + ∆K passing the Dirac points, K and Kθ (points k/∆K = ∓1/2 in theplot). (b) The same as for (a), but for the momentum k varying in the perpendicular direction and passing the Dirac point K(k = 0 in the plot). Reprinted figures with permission from J. M. B. Lopes dos Santos, et al., Phys. Rev. B, 99, 256802 (2007).Copyright 2007 by the American Physical Society. http://dx.doi.org/10.1103/PhysRevLett.99.256802. (c) Schematic of thelow-energy spectrum according to Eq. (186). Reprinted figure with permission from M.-Y. Choi et al., Phys. Rev. B, 84,195437 (2011). Copyright 2011 by the American Physical Society. http://dx.doi.org/10.1103/PhysRevB.84.195437.

|G| = |G′| = ∆K = 2K sin(θ/2), where K = |K| = 4π/(3√

3a0). The tunneling amplitudes for these valuesof G are not independent, and satisfy the following symmetry relations:

tαβ⊥ (0) = t⊥

(1 11 1

), tαβ⊥ (G1) = t⊥

(z 1z z

), tαβ⊥ (G1 + G2) = t⊥

(z 1z z

), (172)

where z = e2πi/3 and the bar over z means complex conjugation. Thus, all interlayer hopping amplitudesdepend on the single parameter t⊥, which the authors calculated numerically. Their result, t⊥ ∼= 0.4t0, wheret0 is the inter-plane nearest neighbor hopping amplitude for the AB bilayer, shows very weak dependenceon θ.

Due to the hybridization between electrons with momenta k and k + G with different G, the Hamilto-nian (170) cannot be diagonalized analytically. The authors diagonalize it numerically by truncating thematrix Hamiltonian (the minimum rank of truncated matrix used is 12), but some results can be obtainedby perturbation theory on parameter t⊥. An analysis of the spectrum for the commensurate structureswith r = 1 shows that, as we explained above, all different structures are almost periodic repetitions ofthe structures with r = 1 [367]. As a result, the low-energy Hamiltonian for structures with m′0 andr′ 6= 1 can be effectively reduced to the Hamiltonian (170) for the structure with m0 and r = 1 such thatθ(m′0, r

′) ≈ θ(m0, 1).Similar approach based on continuum approximation was proposed by R. Bistritzer and A.H. MacDon-

ald [372]. In the latter reference the interlayer hopping Hamiltonian in real space was expressed as

Tαβ(r) =

3∑j=1

e−iqjrTαβj , (173)

where q1 = ∆K, vectors q2,3 are obtained by the rotation of the vector q1 by angles ±2π/3, respectively,

and matrices Tαβj are given by Eq. (172). In the limit of θ = 0, corresponding to the AB bilayer, the matrix

Tαβ is reduced to

3t⊥

(0 10 0

).

This gives the value t⊥ = t0/3, which deviates somewhat from the result t⊥ ∼= 0.4t0, obtained by J. M. B. Lopesdos Santos et al. The total Hamiltonian can be written as

H =

(−i~vFσ

−θ2 ∇ T (r)

T †(r) −i~vFσθ2∇

). (174)

83

Hamiltonian (174) is periodic with a Moire period L. The authors [372] calculated the tBLG spectrumemploying a technique similar to that used in Ref. [367]. This approach [372] is valid for arbitrary twistangles, not necessarily commensurate ones. If the twist angle corresponds to the commensurate structurewith r = 1, the Hamiltonian (174) becomes equivalent to the Hamiltonian (170) (when only three termsshown by Eq. (172) in the summation over G are taken into account).

The Hamiltonian (174) can be generalized [372] to include not only the relative rotation of the layers,

but also the relative shift between the layers %. For non-zero shift, the matrices Tαβj acquire addition phasefactors

e−iBj% , where B1 = 0 , B2 = b1 , and B3 = −b2 .

These factors, however, can be eliminated by a unitary transformation. Therefore, the effective Hamilto-nian H for non-zero % is equivalent to that for % = 0, Eq. (174). Thus, in the continuum (low-energy)approximation, the tBLG spectrum is independent of the shift %.

Typical curves of the low-energy spectrum of tBLG for r = 1, calculated by diagonalizing the Hamilto-nian (170), are presented in Fig. 37. The dispersion surface ε = ε(k) forms two Dirac cones near the Diracpoints of two graphene layers, K and Kθ. The cones merge at higher energies. For tBLG, the Fermi velocityv∗F near the Dirac points turns out to be smaller than the Fermi velocity vF for the single-layer graphene.The authors of Ref. [367] calculated the dependence v∗F = v∗F (θ), both numerically and analytically, usingperturbation theory on the parameter t⊥. In the latter approach, they obtained

v∗F = vF

[1−

(3t⊥

~vF∆K

)2]. (175)

This formula shows that the accuracy of the perturbation theory is controlled by the dimensionless parametert⊥/~vF∆K. For t⊥ = 0.11 eV, the deviation of the numerical result from Eq. (175) is significant if θ . 5,and higher-order contributions should be taken into account. The renormalized Fermi velocity goes tozero at some critical angle θc. The value of θc cannot be found by perturbation theory, and numericalcalculations are needed. R. Bistritzer and A.H. MacDonald [372] obtained the relation for the renormalizedFermi velocity

v∗F = vF

[1− 1− 3α2

1 + 6α2

], α =

t⊥~vF∆K

, (176)

which coincides with Eq. (175) in the limit of small α. It is interesting to note that such a spectrum of thetBLG is equivalent to the spectrum of the AB bilayer subject to the large in-plane magnetic field [392].

Using further simplifications of the low-energy Hamiltonian, R. de Gail with coauthors [385] constructeda simple effective 2 × 2 Hamiltonian of tBLG allowing to obtain analytical expressions for the low-energyspectrum. They started from a 4× 4 Hamiltonian in the form

H =

(H0(k + ∆K/2) H⊥

H†⊥ H0(k−∆K/2)

), (177)

where H0(k) = ~vFσk, and H⊥ is the operator describing interlayer hopping. In the real-space representa-tion, H⊥ has a form of Eq. (173). The authors consider the limit of small angles, when t⊥ ~vF∆K. Asa first simplification, the operator H⊥ is replaced to that corresponding to the AB bilayer (θ = 0),

H⊥ → t0

(0 10 0

). (178)

The system of Schrodinger equations for the bi-spinor wave function ψ = (ψA1, ψB1, ψA2, ψB2)T thenbecomes

~vF k+ψB1 + t⊥ψB2 = EψA1 , (179)

~vF k+ψA1 = EψB1 , (180)

~vF k−ψB2 = EψA2 , (181)

~vF k−ψA2 + t⊥ψA1 = EψB2 , (182)

84

wherek± = (kx ±∆Kx/2) + i(ky ±∆Ky/2). (183)

For t⊥ ~vF∆K and small |E|, we determine from the above equations that ψA1 ∼ ψB2 ψA2 ∼ ψB1.Thus, the right-hand sides of equations (179) and (182) can be set to zero. As a result, one obtains from theseequations ψA1 = −~vF k−ψA2/t⊥ and ψB2 = −~vF k+ψA2/t⊥. Substituting these relations to Eqs. (181)and (180), the following expression is derived

Heff(k)

(ψA2

ψB1

)= E

(ψA2

ψB1

). (184)

Here, the effective 2× 2 Hamiltonian is

Heff(k) = −~v∗F∆K

(0 k+k−

k+k− 0

), v∗F =

~v2F∆K

t0. (185)

The eigenvalues of this Hamiltonian are

ε(k) = ±~v∗F∆K

∣∣∣∣k +∆K

2

∣∣∣∣ ∣∣∣∣k− ∆K

2

∣∣∣∣ . (186)

The spectrum is schematically shown in Fig. 37(c). It qualitatively captures the main features of the low-energy bands calculated by the numerical diagonalization of the Hamiltonians (170) or (174): there are twoDirac cones located at±∆K/2 merging at higher energies, which are characterized by the renormalized Fermivelocity. However, the dependence of v∗F on θ differs from the result of the numerical calculations [3, 372].The estimates given by Eq. (175) or Eq. (176) are consistent with Eq. (186) only in the range θc < θ . 5.Moreover, numerical calculations [367, 372] show that the picture with Dirac cones becomes completelyirrelevant for angles below the critical θc ≈ 1, while Eq. (186) predicts the existence of Dirac cones forarbitrary-small twist angles.

In Ref. [371], E. J. Mele considered the effects of the lattice symmetry on the electronic properties ofthe tBLG in the framework of the continuum approximation. He derived a more general expression for thematrices describing the interlayer hopping [cf. with Eq. (172)]

tαβ⊥ (0) =

(caa cabcba cbb

), tαβ⊥ (G1) =

(zcaa cabzcba zcbb

), tαβ⊥ (G1 + G2) =

(zcaa cabzcba zcbb

), (187)

where the parameters caa, cab, cba, and cbb are expressed via the interlayer hopping amplitudes for the ABbilayer graphene, t0, t3, and t4 (for definition, see Fig. 7), as

caa = cbb =t0 − t3

3+ t4 , cab = cba =

t0 + 2t33

. (188)

The form of the matrices in Eq. (187) coincides with the previously discussed result (172) only for the‘isotropic’ case t3 = t4. For t3 = t4 = 0, the matrices in Eq. (187) exactly coincide with that foundby R. Bistritzer and A.H. MacDonald [372]. It is known, however, that the parameters t3 and t4 cansubstantially deviate from each other, despite the fact that the distances separating the corresponding pairs ofcarbon atoms are the same [39, 393, 394]. For example, the estimate of these parameters for graphite [39, 393]produces a t3 which is only slightly smaller than t0 (the largest interlayer hopping amplitude), while t4is about 10 times smaller. E. J. Mele [371] calculated the electron spectrum for different values of twoindependent parameters caa(= cbb) and cab(= cba). He reproduced the results of Refs. [3, 367, 372] for the‘isotropic’ case. However, when caa cab, or caa cab, the spectrum structure differs from the picture withDirac cones described above, especially when caa or cab is comparable to ~vF∆K. For caa > cab, that is,when t4 > t3, the reduction of the Fermi velocity of the Dirac cones is strongly suppressed. E. J. Mele [371]suggested that this can be a possible explanation of the lack of Fermi velocity reduction experimentallyobserved for some tBLG samples [350, 352, 395, 396, 397].

85

vF*/vF

(b)(a)

Figure 38: (Color online) (a) Energies of the Landau levels En measured at different values of the magnetic field B in Ref. [351].The twist angle is θ = 21.8± 1.7. The solid line is a linear fit following Eq. (189). (b) Dependence of the renormalized Fermivelocity v∗F on the twist angle θ. Triangles are the experimental data in Ref. [351]. The solid (red) curve is the theoreticalprediction, Eq. (175). Reprinted figures with permission from A. Luican et al., Phys. Rev. Lett., 106, 126802 (2011). Copyright2011 by the American Physical Society. http://dx.doi.org/10.1103/PhysRevLett.106.126802.

13.2.2. Fermi velocity reduction and low-energy van Hove singularities

Many experimental studies, using STM [6, 348, 349, 351, 352, 365, 366, 395, 398, 399, 400, 401, 402](both at zero and non-zero magnetic field), ARPES [350, 396, 403], and Raman [354, 355, 356, 357, 359, 360,361, 404, 405, 406, 407, 408] spectroscopies revealed the persistence of the Dirac cones in tBLG. The effect ofthe Fermi velocity reduction was also confirmed using a variety experimental techniques, e.g., ARPES [403],Raman [360], and Landau level (LL) spectroscopies [351, 398, 399, 402]. For example, the STM topographymade by A. Luican et al. in Ref. [351] for bilayer graphene samples prepared by chemical vapor depositionshows large regions characterized by different twist angles, which are estimated by measuring the Moireperiod. In each such region, the LL spectroscopy reveals the sequence of the Landau levels En characteristicfor the massless Dirac fermions:

En = sgn(n)v∗F√

2e~|n|B . (189)

The dependence of the En on the level’s number n for the region characterized by θ ∼= 21.8 is shown inFig. 38(a). From these data, one can extract the Fermi velocity v∗F using Eq. (189). It turns out that v∗Fis different for the regions characterized by different θ, and correlates well with the theoretical predictionEq. (175) [see Fig. 38(b)].

Another important feature of the tBLG spectrum is the existence of van Hove singularities (VHS) atenergies much lower than that for the single-layer graphene. The VHS of the twisted bilayer appear due tothe merging of two Dirac cones leading to saddle points in the low-energy bands, both below and above theFermi level [see Fig. 37(a)]. Van Hove singularities manifest themselves as peaks in the density of states inSTM measurements [6, 352, 365, 400]. The energy difference between two VHS peaks, ∆EvHs, is smaller forsmaller twist angles. In the framework of the continuum approximation [3, 367, 372], this energy differencecan be estimated as

∆EvHs = 2~v∗FK sin(θ/2)− 2t⊥ . (190)

For a rough estimate of the ∆EvHs at angles not close to the critical value θc, one can neglect the dependenceof v∗F on θ. The decrease of the ∆EvHs with a twist angle was observed in different experiments [6, 352, 365,400]. For example, Fig. 39(a) shows the DOS spectra for different tBLG, obtained by STM measurementsin Ref. [6]. The two peaks are closer to each other for samples with smaller twist angle. The VHS splitting,∆EvHs, as a function of θ is shown in Fig. 39(b). The fitting of the experimental data with formula (190)with a constant v∗F is also shown in this figure.

86

TB vF=1.09 106 m/s

Experimental data

(a) (b)

Figure 39: (Color online) (a) Local DOS spectra for samples with different twist angles measured by STM in Ref. [6]. (b) Thedependence of the van Hove singularities splitting ∆EvHs on 2 sin θ/2. Orange circles are the experimental data. The dashed(blue) line is the best fit of the experimental data by Eq. (190) with v∗F = 1.12×106 m/s and t⊥ = 0.108 eV. The (black) trianglesand solid (green) line are described in Ref. [6]. Reprinted figures with permission from I. Brihuega et al., Phys. Rev. Lett., 109,196802 (2012). Copyright 2012 by the American Physical Society. http://dx.doi.org/10.1103/PhysRevLett.109.196802.

Similar results were obtained in Ref. [365]. In the range of the twist angles 2 < θ < 5, the VHS splittingmeasured in the latter reference is approximately described by Eq. (190) with constant v∗F . At the same time,the best fitting of the experimental data reported in Ref. [352] corresponds to ∆EvHs = 2~vFK sin(θ/2),with vF equal to the Fermi velocity of single-layer graphene. The authors concluded that the Fermi velocityremained non-renormalized for their tBLG samples. From the viewpoint of low-energy theories [3, 367, 372],this corresponds to the limit of uncoupled graphene layers, t⊥ → 0. No Fermi velocity reduction was observedalso in ARPES measurements of Refs. [350, 396], and by the Landau level spectroscopy in Ref. [395]. Theseresults are in contradiction with those obtained by Landau level [351] and Raman [360] spectroscopies (seethe previous paragraph). It is likely that these discrepancies can be explained by different sample preparationtechniques, influence of the substrate, disorder, etc.

Related results were obtained in Ref. [400] by W. Yan et al. Scanning tunneling microscopy datagathered in this paper demonstrated the existence of low-energy VHS for bilayer samples with twist anglesθ . 3.5. For these samples, the energy difference between VHS peaks, ∆EvHs, with a good accuracy followsEq. (190). At the same time, no traces of the low-energy VHS were found for samples with θ & 5.5: themeasured dI/dV spectra are “almost identical to those of the graphene monolayer”. In the intermediaterange, 3.5 . θ . 5.5, some samples show VHS peaks, but some others do not.

Measurements of both the Fermi velocity and the VHS splitting were performed in Ref. [402] for sampleswith different twist angles prepared on two different substrates. The Fermi velocity was determined withthe help of LL spectroscopy and Eq. (189). Using Eq. (190) and measured ∆EvHs, the authors extractedthe inter-layer hopping parameter t⊥ for each sample. They found that the tBLG properties demonstratedsignificant sample-to-sample variation, which cannot be explained by the sample-to-sample variation of thetwist angle. For example, in several systems t⊥ ≈ 0. The authors speculated that this variation maybe caused by the influence of “the stacking fault, tilt grain boundary, atomic defects, and roughness ofsubstrate” on the inter-layer distance. However, in agreement with the theory, strong correlation betweenFermi velocity reduction and the inter-layer coupling was found: the authors [402] showed that the v∗F iswell described by Eq. (175) with experimentally obtained t⊥ and θ.

The effect of doping on the VHS has been studied using STM in Ref. [401]. For these bilayers a doping

87

of the order of 1012 cm−2 arose by charge transfer from the substrate. The doping leads to asymmetricpositions of the VHS peaks with respect to the Fermi level, while the energy difference, ∆EvHs, is almostdoping independent, as it is expected from theory. For the doping ∼ 5× 1012 cm−2, the Fermi level exceedsthe energy of the upper VHS for the tBLG with θ . 3. They [401] also mentioned that doping leads tosmall (< 100 mV) potential difference between layers.

In Ref. [409] both VHS as well as higher-energy spectroscopic features were detected using STM tech-nique. Consistency between experimental data and theoretical predictions was found.

13.2.3. Low-energy spectrum at very small angles

The band structure with Dirac cones described above is valid only for angles larger than the criticalangle θc, below which the renormalized Fermi velocity v∗F vanishes. For angles close to θc the low-energybands become almost flat, and for θ < θc the cone-like band structure becomes completely irrelevant. Thevalue of θc, which actually depends on the interlayer hopping, was estimated by different groups, using bothlow-energy theories [367, 372] and tight-binding calculations [374, 410]. For t⊥ ≈ 0.1 eV, J. M. B. Lopes dosSantos et al. [367] concluded that θc ≈ 1. This value correlates well with that found by R. Bistritzer andA.H. MacDonald [372]. Tight-binding studies reported similar value (e.g., calculations done in Ref. [410]give θc ∼= 1.89).

The physical properties of tBLG differ qualitatively for θ above and below θc. Specifically, Ref. [367]calculated the density of states for different twist angles. When θ > θc, the DOS is zero at the Fermi leveland increases linearly at small energies, consistent with the existence of Dirac cones. For θ < θc, the densityof states has a very pronounced double-peak structure at small energies (see Fig. 40). Moreover, the DOS ρ0

at the Fermi level is non-zero. The width of this double-peak, as well as the value of ρ0, oscillate as a functionof θ. For small twist angles, the tBLG can be considered as composed of large regions with almost AB andAA stacking. They [367] explain the peak in the density of states by the localization of the electrons at theregions with AA stacking (for details, see Section V in Ref. [367]). This interpretation was confirmed bythe calculation of the local density of states (LDOS) at the Fermi level, which demonstrated that almost allelectrons are located inside regions with AA stacking. The oscillations of ρ0 with the twist angle are relatedto the quantization conditions for the confined electrons: kFL(θ) ∼ 2πn, where n is integer, kF = t⊥/(~vF )is the Fermi momentum of electrons at zero energy localized inside the AA regions, and L(θ) ≈ a0

√3/θ is

the Moire period. As a result, the maxima of ρ0 (and the minima of the peak’s width) occur at angles

θn ∼t⊥a0

√3

2π~vFn. (191)

Similar conclusions were reached in Ref. [375], which relied on tight-binding calculations. They alsoshowed the electron localization inside the regions with almost AA stacking (for details of the tight-bindingcalculations, see the next Section). Further, the band flatness and the localization of the single-electronstates inside the AA regions was also confirmed by P. San-Jose et al. [387] in the framework of the continuumapproximation. The authors proposed an approach treating the inter-layer hopping as a spatially-modulatednon-Abelian gauge potential. The calculations [387] showed the appearance of flat bands for certain valuesof the twist angles. For these angles, the local density of states has pronounced peaks in the regions withAA stacking [see Fig. 40(d)]. The sequence of these ‘magic’ angles satisfies approximately the law θn ∝ 1/n,in agreement with Eq. (191).

The oscillation of the DOS at the Fermi level is also consistent with the results of R. Bistritzer andA.H. MacDonald [372] showing oscillations of the Fermi velocity v∗F calculated at one of the Dirac pointwith the twist angle. The Fermi velocity vanishes at discrete angles θn, whose values are approximatelydescribed by Eq. (191), indicating the electron localization. The value θ1 corresponds to θc.

Such a behavior of the density of states at small twist angles has been confirmed in STS and STMmeasurements in Ref. [411] by L.-J. Yin et al. The authors observed a pronounced peak in the dI/dVspectra at the charge-neutrality point for bilayer with θ = 1.11. The authors associated this angle with thecritical angle θc described above. For bilayers with θ 6 θc (data for θ = 0.88 and θ = 1.11 are presented),the peak is observed only in the region with AA stacking, in agreement with theoretical predictions. For

88

(a) (b)

(c) (d) m

0=31 m

0=68

Figure 40: (Color online) (a) – (c) The low-energy DOS, calculated for three twist angles, is shown by gray rectangles. Thesolid (red) line is the DOS of the single-layer graphene. (a): θ > θc. The DOS has an almost linear dependence on E atsmall energies, consistent with the existence of Dirac cones. It is zero at zero energy (Fermi level). (b) and (c): θ < θc.The DOS has a double-peak structure at small energies, and it is non-zero at zero energy. Reprinted figures with permissionfrom J. M. B. Lopes dos Santos, et al., Phys. Rev. B, 86, 155449 (2012). Copyright 2012 by the American Physical Society.http://dx.doi.org/10.1103/PhysRevB.86.155449. (d) Patterns of the local density of states at the Fermi level calculated fortwo different structures (m0, 1) corresponding to the ‘magic’ angles, Eq. (191). The twist angles are θ ∼= 1.05 (m0 = 31)and θ ∼= 0.48 (m0 = 68). A logarithmic scale is used, the white color corresponds to the maxima of the local DOS.These patterns show single-electron localization inside the regions with approximately AA stacking. Reprinted figure withpermission from P. San-Jose et al., Phys. Rev. Lett, 108, 216802 (2012). Copyright 2012 by the American Physical Society.http://dx.doi.org/10.1103/PhysRevLett.108.216802.

the sample with θ = 0.88 the peak is broader than the peak for the critical angle, which is also consistentwith theoretical calculations. For angles θ > θc no peak at the charge neutrality point is observed, and thedI/dV spectra are almost position independent. For these angles, the dI/dV spectra have a minimum atthe charge-neutrality point, and two peaks below and above it, which is consistent with the Dirac conespicture.

13.2.4. Fine structure of the low-energy bands: band splitting and band gap

In the low-energy theories described above, the valley degeneracy is assumed. For any tBLG super-structure, however, the two Dirac points of one layer coincide with the Dirac points of another layer upontranslations of the reciprocal superlattice vectors. Which pairs of Dirac points are equivalent depends onthe type of superstructure. It was shown in Section 13.1 that when r 6= 3n, K′ ∼ Kθ and K ∼ K′θ. Whenr = 3n, other pairs of Dirac points are equivalent: K ∼ Kθ and K′ ∼ K′θ. In a generic situation, the single-electron states near equivalent cones are hybridized by some finite matrix element. E. J. Mele in Ref. [370]took this into account by adding a mass term into the effective low-energy Hamiltonian. He considered theHamiltonian at the momenta close to one of two tBLG Dirac points. The Hamiltonian has the form of a4×4matrix. It is different for ‘odd’ (r 6= 3n) and ‘even’ (r = 3n) superstructures. For r 6= 3n, the effective

89

Figure 41: (Color online) Low-energy spectra of tBLG for ‘odd’ (left panel) and ‘even’ (right panel) superstructures. Reprintedfigures with permission from E. J. Mele, Phys. Rev. B, 81, 161405 (2010). Copyright 2010 by the American Physical Society.http://dx.doi.org/10.1103/PhysRevB.81.161405.

Hamiltonian is

Hodd =

(−i~v∗Fσ∇ H−int

(H−int)† i~v∗F σ∇

), (192)

where σ are the complex conjugate Pauli matrices σ. The mass term H−int is a 2×2 matrix which couples theelectron states near the Dirac points K and K′θ (∼ K). Since these Dirac points belong to different valleys,

the diagonal blocks in Hodd have a different structure. The velocity v∗F is the renormalized Fermi velocity,not the bare vF . By retaining v∗F , as opposed to the bare vF, the proposed technique attempts to account“phenomenologically” for more robust effects discussed in the previous subsection. For ‘even’ structures, themass term, H+

int, couples the electrons near the Dirac points in the same valley, K and Kθ (∼ K). Therefore,the effective Hamiltonian has identical diagonal blocks:

Heven =

(−i~v∗Fσ∇ H+

int

(H+int)† −i~v∗Fσ∇

). (193)

Furthermore, the structure of the matrices H+int and H−int is different. Using symmetry considerations,

E. J. Mele [370] proposed the following general form of these matrices:

H+int = Veiϑ

(eiϕ/2 0

0 e−iϕ/2

), H−int = Veiϑ

(1 00 0

). (194)

The parameter V describes the strength of the cone hybridization, while ϑ and ϕ are phase factors allowedby symmetry. E. J. Mele estimated the parameter V as V ∼ 10 meV for superstructures (m0, r) = (1, 1),θ ∼= 21.787 and (m0, r) = (1, 3), θ ∼= 38.213.

The low-energy spectrum consists of four bands. It is different for ‘odd’ and ‘even’ structures. Typicalcurves are shown in Fig. 41. For r = 3n, the spectrum is gapped with a gap proportional to V. For r 6= 3n,all four bands have parabolic dispersion near the Dirac point, and the spectrum is gapless: two middlebands touch each other at the Dirac point. The band splitting was experimentally found by ARPES [403]and Raman spectroscopy [404]. The band gap in the tBLG was also observed in transport measurements inRef. [412] (for more details about the latter reference, see next subsection).

90

13.3. Tight-binding calculations of the twisted bilayer graphene spectrum

The applicability of the approximations described above is restricted to low energies and relatively smalltwist angles. To lift up these restrictions, different approaches are required. One possibility is ab initiocalculations. Unfortunately, the ab initio band structure calculations of the tBLG require huge computationefforts because of the large number of atoms inside the supercell N . Numerical calculations based ontight-binding approximations are also quite time-consuming for the same reason, especially for small twistangles. Indeed, to find the tBLG spectrum, one needs to diagonalize the N ×N matrix of the tight-bindingHamiltonian on a 2D momentum grid, covering the tBLG Brillouin zone. For example, for the structure(16, 1) with the twist angle θ ∼= 2, the rank of this matrix is N = 3286. For these reasons, in manypapers the authors combine DFT and tight-binding calculations [154, 374, 375, 376, 378]. They performDFT calculations only for a few structures with moderate N , and then use these results to extract thehopping amplitudes in the tight-binding Hamiltonian. In the general case, the second-quantized tight-binding Hamiltonian of the tBLG can be written as

H =∑nmiαβσ

[t(i)‖ (riαn ; riβm)d†inασdimβσ + h.c.

]+∑nmαβσ

[t⊥(r1α

n ; r2βm )d†1nασd2mβσ + h.c.

], (195)

where d†inασ and dinασ are the creation and annihilation operators of an electron with spin projection σ inthe site n in the layer i (= 1, 2) on the sublattice α (= A,B). The first term describes the in-plane hopping,

with t(i)‖ (r; r′) being the in-plane hopping amplitude. The second term describes the interlayer hopping, with

t⊥(r; r′) being the hoping amplitude between sites in layers 1 and 2, located in positions r and ezd + r′,respectively.

Different groups use different parametrizations for the hopping amplitudes in Eq. (195). In the simplest

case of two-center approximation, the functions t(i)‖ (r; r′) and t⊥(r; r′) depend entirely on the relative posi-

tions of the orbitals participating in the hopping event. The amplitudes can be expressed via Slater-Kosterparameters [413], Vppσ and Vppπ, as follows:

t(i)‖ (r; r′) = Vppπ(|r− r′|) ,

t⊥(r; r′) = cos2γ Vppσ(√

c20 + (r− r′)2)

+ sin2γ Vppπ(√

c20 + (r− r′)2), (196)

where the functions Vppσ(r) and Vppπ(r) depend only on the distance between two sites, and γ is the anglebetween the z axis and the line connecting the sites in the positions r and c0ez + r′:

cos2γ =c20

c20 + (r− r′)2. (197)

In Refs. [374, 375], Trambly de Laissardiere et al. exploited the exponentially-decreasing function Vppπand Vppσ

Vppπ(r) = −t exp [qπ (1− r/a0)]Fc(r) , (198)

Vppσ(r) = t0 exp [qσ (1− r/c0)]Fc(r) , (199)

with equal spatial exponential-decreasing coefficients

qπa0

=qσc0. (200)

In these equations, Fc(r) is the cutoff function, reducing the long-range hopping amplitudes. In Ref. [375]it is taken to be

Fc(r) =1

1 + exp[(r − rc)/lc], (201)

91

Figure 42: (Color online) Fermi velocity versus twist angle θ, calculated for several superstructures in Ref. [374]. The pairs ofintegers denote superstructures, but the superstructure indices (n,m) in the figure correspond to (n,m − n) in our notation.Crosses are the tight-binding calculations, (red) circles correspond to ab initio calculations. The solid (blue) curve correspondsto the approximate formula (175) by J. M. B. Lopes dos Santos et al. [3]. The inset shows the data for small angles. Reprintedwith permission from G. Trambly de Laissardiere et al., Nano Letters, 10, 804 (2010). Copyright 2010 American ChemicalSociety. http://dx.doi.org/10.1021/nl902948m.

where the authors used rc = 2.5√

3a0 = 6.14 A, and lc = 0.265 A. In an earlier paper, Ref. [374], the cutofffunction is not introduced, that is, Fc(r) = 1. To fix the parameters t and qπ in Eq. (198), the authorstake the in-plane nearest-neighbor and the next nearest-neighbor hopping amplitudes to be equal to theircharacteristic values in the single-layer graphene [4]: t = 2.7 eV, t′ = 0.1t. This yields for the ratio

qπ/a0 = qσ/c0 = ln(t/t′)/[a0(√

3− 1)] = 2.22 A−1.

The largest inter-plane hopping amplitude is chosen to be t0 = 0.48 eV. Thus, three hopping amplitudes, t,

t′, and t0, together with Eq. (200), allows to fix all the fitting parameters in functions t(i)‖ (r; r′) and t⊥(r; r′)

describing all the hoppings in the twisted bilayer for any rotation angle. Density functional calculations werealso performed for several tBLG superstructures, and a good agreement was found between tight-bindingand DFT results.

The findings of Refs. [374, 375], in general, confirm the conclusions of the low-energy theories [3, 367,372, 387], such as the Fermi velocity reduction at larger twist angles, the band flattening, and wave functionlocalization at smaller angles (the band splitting and the deviation from the linear dispersion near the Diracpoints were not discussed in these papers). The calculated Fermi velocity at the Dirac cones is found to bea smooth function of the twist angle. The dependence of the Fermi velocity versus θ is symmetric aroundthe angle θ = 30, see Fig. 42. For not too small angles θ & 3 the Fermi velocity is very well describedby the approximate formula (175). In further work, Ref. [375], the authors focused on the small angles.They demonstrated the appearance of flat bands, and the non-zero density of states at the Fermi level forθ < θc ∼ 2. The authors calculated the local density of states of the tBLG in regions with almost AB andAA stacking [see Fig. 43(a,b)]. The local DOS at the AA region shows a pronounced peak at the Fermi

92

E-m [eV]

r(E)

[eV-1]

(a)

E-m [eV]

r(E)

[eV-1]

(b)

Figure 43: (Color online) Local densities of states (LDOS) for two different superstructures calculated for atoms located in thecenter of the nearly AB (a) and nearly AA (b) regions. For the left panel: the curve “at. A” (“at. B”) corresponds to the A1 orB2 (B1 or A2) atoms. Dotted curves are the LDOS for pure AB (a) and AA (b) bilayers. Note that G. Trambly de Laissardiereet al., Ref. [375], used different parametrization for the superstructures: (n,m) in the figures corresponds to (n,m− n) in ournotation. The superstructures (100, 101) and (200, 201) have twist angles θ ∼= 0.33 and θ ∼= 0.16, respectively. Reprintedfigures with permission from G. Trambly de Laissardiere, et al., Phys. Rev. B, 86, 125413 (2012). Copyright 2012 by theAmerican Physical Society. http://dx.doi.org/10.1103/PhysRevB.86.125413.

level, while this peak is absent for sites in the AB region. The oscillations of the DOS at the Fermi level, aswell as ‘magic’ angles, were also found.

The existence of flat bands at small angles is also shown by E. Suarez Morell et al. [376]. They used asimpler dependence for the interlayer hopping:

t⊥(r; r′) = t0 exp

1

β

[c0 −

√c20 + (r− r′)2

]. (202)

To check the accuracy of the tight-binding calculations, they also compared the tight-binding spectra withab initio data for several twist angles and found no difference at low energies. Typical spectra for smallangles are shown in Fig. 44. Two low-energy flat bands exist for θ . 1.5. No Dirac spectrum near K pointis observed for these θ. The bandwidth ∆E of the low-energy flat bands is determined as the differencein energies of the lower and the upper bands at the Γ point (see Fig. 44). The bandwidth ∆E is a non-monotonous function of the twist angle, which is consistent with the oscillations of the width of the DOSpeak predicted in Refs. [367, 372, 375].

The same parametrization of the inter-layer hopping is used in Ref. [377]. The authors were interested inthe effect of the bias voltage applied to the twisted bilayer. The application of the gate voltage leads to theredistribution of the charge carriers in the bilayer: one layer acquires additional electrons with a density n,while another layer loses the same amount of electrons (no doping is assumed). They [377] did not analyzethe modification of the electronic spectrum by the bias voltage V , but instead discussed the dependenceof the excess electron density n on the twist angle (the effect of the bias voltage on the tBLG spectrumwas studied in Refs. [3, 380, 414, 415]). Figure 45(a) shows the dependence of n on V for bilayers withdifferent θ. At a fixed bias voltage, the smaller θ, the larger the charge redistribution becomes. The authorsinterpreted this result as a demonstration of the reduction of the effective interlayer coupling for larger θ.

The next interesting effect is the inhomogeneous spatial distribution of the excess electron density.Ref. [377] found that the spatial local distribution of electrons is substantially different for the A and Bsublattices in the layer. They plotted the patterns of the electron density inside the supercell of the bilayer,separately for A and B sites of the layer [see Fig. 45(b)]. The authors distinguished three different regionsinside the supercell. In the regions with nearly AA stacking, the electron densities at A and B atoms areapproximately equal to each other and correspond to the averaged value n. In the regions with nearly ABstacking, the areas where the local density near the A sites is larger than the local density at the B sitesis changed by areas where the local electron density at the B sites exceeds the local density at the A sites(authors of Ref. [377] referred the latter areas as BA stacking regions). This observation correlates very well

93

Figure 44: (Color online) Twisted bilayer graphene spectra for three twist angles of about 1.5 calculated in Ref. [376] (blue solidcurves). For comparison, the spectra of the AB bilayer (green dashed curves) and single-layer graphene (red dotted curves) areadded. In panels (a) and (b), there are two nearly-flat bands closest to zero energy. For θ ∼= 1 [panel(c)] the bandwidth of theselow-energy bands is relatively large. This is consistent with the oscillatory behavior of the peak’s width of the DOS at smallangles (see Fig. 40). Insets in panels (a) and (b) show the spectra close to the Dirac point. The numbers (n,m) in the figurescorrespond to the structures (n,m−n) in our notation. Reprinted figures with permission from S. Morell et al., Phys. Rev. B,82, 121407 (2010). Copyright 2010 by the American Physical Society. http://dx.doi.org/10.1103/PhysRevB.82.121407.

with the calculations of the local density of states of the twisted bilayer done in Ref. [375]. Indeed, insidethe nearly AB region, the LDOS at the B atoms is larger than that for the A atoms [see Fig. 43(a)].

In Ref. [415], P. Moon et al. studied the effects of the bias voltage V on the tBLG spectrum and thedynamical conductivity using a tight-binding model with hopping amplitudes described by Eqs. (196) – (199)[with Fc(r) = 1]. For the range of twist angles studied (1 . θ . 15), the spectrum is doubly degeneratenear the tBLG Dirac points when V = 0. The bias voltage lifts this degeneracy. For θ > θc, where Diraccones exist, the resulting band structure is similar to that for the AA-stacked bilayer graphene; near eachDirac point there are two cones shifted upwards and downwards from the Fermi level (at zero doping) by theenergy value proportional to V . The coefficient of proportionality depends on the twist angle. It decreaseswhen θ decreases going to zero when θ → θc. Experimental investigation of the tBLG under the transversebias was reported in Ref. [358].

In all theoretical studies mentioned in this subsection, the authors relied on the two-center approximationto describe the interlayer hopping, see Eq. (196). In addition, the Hamiltonians themselves were typicallyformulated with the help of the second-quantization formalism. The approach developed by O. Pankratov etal. in Refs. [154, 368, 369, 378] differs in several respects. First, the authors started from the first-quantizedsingle-electron Hamiltonian:

H =p2

2m+ V (1)(r) + V (2)(r) , (203)

94

(a) (b)

AB

AA

BA

n

Figure 45: (Color online) (a) The average density n of extra electrons in the top (negatively charged) tBLG layer as a functionof the applied gate voltage for different twist angles. The electron density for the AB bilayer is also shown (orange triangles).(b) Spatial distribution of the electron density in the A (upper panel) and B (lower panel) sublattices of the top layer insidethe tBLG supercell. The superstructure is (15, 1), θ ∼= 2.13. The gate voltage applied is V = 0.08 V. The electron density isin units 1012 cm−2, and the averaged value is n = 0.7× 1012 cm−2. The x and y axes are in A. Arrows show the regions withnearly AB, BA, and AA stacking. Reprinted figures with permission from S. Morell et al., Phys. Rev. B, 84, 195421 (2011).Copyright 2011 by the American Physical Society. http://dx.doi.org/10.1103/PhysRevB.84.195421.

where m is the electron mass and V (i) is the potential of the i-th(=1, 2) graphene layer. The potential V (1)

(V (2)) is invariant with respect to translations by the single-layer graphene lattice vectors a1,2 (a′1,2), whilethe total Hamiltonian (203) is invariant with respect to translations by the superlattice vectors R1,2. The

authors used the basis constructed of the single-layer graphene eigenstates of each layer, |φ(i)siki〉 satisfying

the equation

H(i)|φ(i)siki〉 ≡

(p2

2m+ V (i)

)|φ(i)siki〉 = ε

(i)siki|φ(i)siki〉 , (204)

where ε(i)siki

is the eigenenergy, with si being the band index and ki is the momentum. For every momentumk belonging to the Brillouin zone of the twisted bilayer graphene, we can define a complete basis |Ψk〉 =

|φ(1)s1k1〉, |φ(2)

s2k2〉, where the momenta k1 belong to the Brillouin zone of the first layer, momenta k2 belong

to the Brillouin zone of the second layer, and the admissible k1,2 satisfy the following relation

k1,2 = k + n1,2G1 +m1,2G2 , (205)

where n1,2 and m1,2 are some properly chosen integers. It is easy to show that the number of eigenfunctions

in the set |Ψk〉 = |φ(1)s1k1〉, |φ(2)

s2k2〉 is equal to the number of atoms in the supercell N . Thus, |Ψk〉 is the

N -component spinor (only pz electrons are considered, the number of single-layer graphene bands is equalto 2; that is, si = 1, 2).

In the basis |φ(1)s1k1〉, |φ(2)

s2k2〉, the Hamiltonian (203) is a 2× 2 block matrix

H =

(H11 H12

(H12)† H22

), (206)

where the matrices Hii are diagonal, (Hii)siki,s′ik′i = δsis′iδkik′iε(i)siki

, and the matrix H12 describing theinter-layer hopping has the form:

(H12)s1k1,s2k2 =1

2

⟨φ

(1)s1k1

∣∣∣(V (1) + V (2))∣∣∣φ(2)

s2k2

⟩. (207)

95

According to Eq. (205), the difference k2−k1 is the reciprocal vector of the superlattice. Using geometricalconsiderations, the authors showed that the matrix elements in Eq. (207) are negligible if

k2 − k1 6= n1G(c)1 + n2G

(c)2 , (208)

where n1,2 are integers and

G(c)1 = rG1 , G

(c)2 = rG2 , (209)

if r 6= 3k, and

G(c)1 =

r

3(G1 + 2G2) , G

(c)2 =

r

3(2G1 + G2) , (210)

otherwise1. The authors of Ref. [378] emphasized the appearance of a new momentum scale in the tight-

binding model, which is described by the G(c)1,2 vectors. Their magnitude |G(c)

1,2| = 8π sin(θ/2)/(a√

3) depends

only on the twist angle, and the reciprocal vectors G(c)1,2 correspond to the real-space hexagonal superlattice

with the size L equal to the Moire period, Eq. (156).

For k2 − k1 = n1G(c)1 + n2G

(c)2 , the matrix elements (H12)s1k1,s2k2

decrease exponentially when |n1,2|grows, and in numerical calculations one can keep only matrix elements with the first several |n1,2|. Since thematrix (206) is sparse, it is possible to apply the efficient Lanczos algorithm to find the tBLG spectrum at lowenergies. The efficiency of the numerical scheme can be increased substantially by using the truncated basis

|φ(1)s1k1〉, |φ(2)

s2k2〉, which includes only states with energies within certain window |ε(n)

snkn| . W [368, 378].

The authors claim, that at small twist angles, their algorithm works about 103 times faster than standardtight-binding methods [378].

In general, the numerical calculations of the spectrum in Refs. [368, 369, 378] are in agreement withthe results of both tight-binding calculations and the low-energy theories described above. The calculationsshow the existence of the Dirac cones and the Fermi velocity reduction at sufficiently large angles, as wellas the band flatness and the charge localization at small angles. The authors [378] obtained also severalanalytical results. Specifically, using perturbation theory and their tight-binding model, they re-derived theformula for v∗F = v∗F (θ), Eq. (175), and demonstrated that it works well for θ & 5.

The important analytical result confirmed by numerical calculations is the twofold degeneracy of theDirac cones when the number of atoms in the supercell N is large [369]. The analysis is based on thecalculation of the inter-layer matrix elements (H12)s1k1,s2k2

, for k1 = K′, k2 = Kθ, if r 6= 3n, or for k1 = K,k2 = Kθ otherwise. According to Eqs. (167) and (168), the difference k2−k1 is the reciprocal vector of thesuperlattice for both cases, and, strictly speaking, the corresponding matrix elements, describing the bandsplitting, are non-zero. However, the value (H12)s1k1,s2k2

decays fast when N grows, and the splitting ofDirac cones becomes negligible for N larger than some critical value. For smaller N , where the band splittingis relevant, the low-energy spectrum deviates from the linear dispersion near the Dirac cones, in agreementwith the low-energy theory by E. J. Mele [370]. Figure 46 presents the dependence of the band splitting ∆s

on the number of atoms in the supercell N (for a definition of ∆s, see the inset in Fig. 46). The value of∆s depends on N non-monotonously, and it becomes negligible when N & 102. The maximum splitting,∆s ≈ 7 meV, corresponds to the superstructures (1, 1) with θ = 21.79, and (1, 3) with θ = 38.21, bothhaving N = 28 atoms per unit supercell. A similar estimate ∆s ∼ 10 meV was obtained by E.J. Mele [370].The character of the spectrum near the Dirac point, as it was reported in Ref. [369], is qualitatively differentfor the r 6= 3n (‘odd’) and r = 3n (‘even’) superstructures. In the former case, the spectrum is gapped,while for r = 3n it is gapless, with two parabolic bands touching each other at the Dirac point (see the insetin Fig. 46). Such a situation is opposite to that was found by E. J. Mele [370] (cf. inset in Fig. 46 withFig. 41).

A different analysis of the band splitting has been done by A. O. Sboychakov et al., Ref. [410]. The

authors studied the tight-binding Hamiltonian (195), where the in-plane hopping amplitudes t(i)‖ (riαn ; riβm)

1The authors of Refs. [154, 368, 369, 378] characterized a superstructure by two co-prime integers p and q, which can beconnected to our notation (m0, r) as follows: p = r/2, q = m0 + r/2 for even r and p = r, q = 2m0 + r for odd r.

96

N/4

odd even

Figure 46: (Color online) Dependence of the band splitting (∆s in the text) on the number of atoms N in the supercellcalculated in Ref. [369]. Inset shows the low-energy spectrum near the Dirac point for the (1, 1) (‘odd’) and (1, 3) (‘even’)superstructure. Reprinted figure with permission from S. Shallcross et al., Phys. Rev. Lett., 101, 056803 (2008). Copyright2008 by the American Physical Society. http://dx.doi.org/10.1103/PhysRevLett.101.056803.

are non-zero only for a nearest-neighbor hopping equal to t = 2.57 eV. To calculate the interlayer hoppingamplitudes t⊥(r1α

n ; r2βm ), the authors use the approach proposed by M. S. Tang et al. [391], which takes

into account the environment dependence of the hopping. The inter-layer hopping amplitude, t⊥(r; r′), isexpressed via Slater-Koster parameters according to Eq. (196). However, in contrast to the widely-usedtwo-center approximation, the functions Vppσ(r; r′) and Vppπ(r; r′) depend also on the positions of othersites in the lattice via the factor [1− S(r; r′)], where the screening function is

S(ri; rj) = tanh

(β1

∑l

exp

[−β2

(Ril +RljRij

)β3])

. (211)

In this equation, Rij is the distance between sites i and j, the summation is performed over all sites in thelattice, and β1, β2, and β3 are fitting parameters. It follows from this equation, that the closer some of theneighboring atoms are to the line connecting the sites ri and rj , the larger is the screening. The inclusionof the screening helps to describe more correctly the longer-range inter-layer hopping amplitudes in bilayergraphene systems. Indeed, it is known from experiment and ab initio calculations [39, 393, 394], that thenext-nearest-neighbor interlayer hopping amplitudes for the AB graphene bilayer and graphite, t3 and t4(for definitions, see Fig. 7), are different by about an order of magnitude, even though the distance betweenthe corresponding pairs of sites are equal to each other. Taking the first three largest inter-layer hoppingamplitudes of the AB bilayer, t0 = 0.4 eV, t3 = 0.254 eV, and t4 = 0.051 eV, the authors of Ref. [410],found the fitting parameters β1, β2, and β3 of the screening function. The interlayer hopping amplitudesfor the tBLG are calculated then by using these βs. The same approach was used also by O.A. Pankratovet al. in Refs. [154, 368, 378]; the fitting parameters are found in these papers by comparison of the tight-binding spectra with the DFT results. The parametrization of M.S. Tang et al. [391] for inter-layer hoppingamplitudes was used also by J. M. B. Lopes dos Santos et al. in Refs. [3, 367].

The authors of Ref. [410] showed that near the Dirac point K the low-energy tight-binding spectrum canbe approximated as

E(ν)K+k = µ±

√∆2 + v2

F (|k| ± k0)2, ν = 1, . . . , 4 , (212)

97

Figure 47: (Color online) Dependence of the band splitting ∆s on the twist angle θ, calculated for all superstructures withN < 2000 (gray solid line). Different dashed curves connect the points corresponding to superstructures with a fixed r. Figureis from Ref. [410].

if r 6= 3n, or

E(1,4)K+k = µ∓

√∆2s + v2

Fk2 , E(2,3)K+k = µ∓

(√∆2s + v2

Fk2 −∆s

). (213)

otherwise. Qualitatively, these dependencies are similar to those found by O. A. Pankratov et al. [368, 369,

378] (see the inset in Fig. 46). The band splitting is defined as ∆s = E(4)K −E

(1)K , and for r 6= 3n structures,

it is related to the band gap according to ∆s =√

∆2 + v2F k

20. The dependence of ∆s on the twist angle is

shown in Fig. 47. It is not a continuous function of θ: any small deviation of the twist angle from a givenvalue changes drastically the band splitting. However, the band splitting for superstructures with a given rmonotonously decreases with θ. Among all superstructures in some range of the twist angle, the maximumband splitting corresponds to r = 1 superstructures. The maximum value ∆s

∼= 80 meV corresponds to the(1, 1) superstructure, and it is one order of magnitude larger than estimate of O. A. Pankratov et al. [368, 369].For m0 < 7 (and r = 1) the band splitting exceeds 1 Kelvin, which is an experimentally observable quantity.However, the discontinuous behavior of ∆s on θ can make the band splitting (and a band gap) non-observable,because any infinitesimal deviation δθ of the twist angle from its value θ0 ≡ θ(m0, 1) totally suppresses theband splitting. In real situation, however, the twist angle is known with a finite error. Rotational disorderof the twisted bilayer graphene was studied experimentally in Ref. [407]. They observed local variations ofthe twist angle ∆θ ∼ 2 in samples with θ & 15.

The authors of Ref. [410] pointed out that taking into account the finite mean-free-path of electrons orthe sample’s size will make the band splitting a continuous function of the twist angle. Indeed, calculationsof the band gap performed for a finite sample with θ ∼= 21.79 showed [410], that the band gap changescontinuously with θ. The value of ∆ has a peak at θ corresponding to the (1, 1) superstructure, the widthof this peak is ∆θ ∼ a0/L, where L is the sample’s size.

Reference [410] also mentioned the presence of low-energy edge states with a characteristic localizationlength much smaller than the sample’s size. In the band gap calculations these states were ignored. Theexistence of edge states was reported also by O. A. Pankratov et al. in Ref. [154], where they studied the

98

Figure 48: (Color online) (a) and (b) Fermi surfaces of the superstructures (17, 1) [θ ∼= 1.89, panel (a)] and (18, 1) [θ ∼= 1.79,panel (b)] calculated at half-filling in Ref. [410]. Different colors correspond to different bands intersecting the Fermi level.Brillouin zone (hexagon), the reciprocal supercell (rhombus) and the Dirac points K1,2 are also shown. (c) Low-energy densityof states calculated for three superstructures with close twist angles θ < θc. The density of states is calculated at finitetemperature T/t = 10−5 by numerical integration over the momentum. Figures are from Ref. [410].

electronic properties of the tBLG flakes. Edge states in the twisted bilayer graphene nanoribbons werestudied theoretically in more detail in Ref. [155]. The authors found, in particular, that the edge states withenergies close to the Fermi level (for undoped bilayer) are localized at the AB-type regions of the edge, whilestates localized at the AA-type regions of the edge become split; they have energies either above or belowthe Fermi level by a value of about 0.2 eV.

The band gap in twisted bilayer graphene has been observed experimentally in transport measurementsby J. Park et al. in Ref. [412]. They estimated the twist angle of their sample as θ ∼ 30. The band gapwas extracted both from the IV characteristics and from the temperature dependence of the conductivityand the carriers concentration obtained by Hall measurements. Thus, the authors [412] showed that bothconductivity and the concentration of the charge carriers follow the thermal activation law, lnσ, lnn ∝ ∆/T ,with gap ∆ ∼ 80 meV (the estimate of the gap from the width of the flat region in the IV curve gives amuch larger value of the gap). The authors explain such a big value of the band gap by the local formationof the sp3 interlayer C-C bonding arising due to the peculiarities of the sample’s preparation techniquesthey used. The theoretical background for such a possibility can be found in Refs. [416, 417]. Note, however,that the estimate ∆ ∼ 80 meV coincides with the gap found in Ref. [410] using the tight-binding calculationsdescribed above.

Band gap engineering by the intercalation of twisted bilayer graphene by alkali metal ions has beenproposed in Ref. [418]. Using DFT calculations, the authors found the equilibrium positions for the inter-calated ions inside the supercell of the bilayer. Intercalation modifies the electronic spectrum leading tothe gap opening at the Dirac points. They mentioned that the gap can be “several times larger than roomtemperature”. The modification of the tBLG electron spectrum by point defects has been studied, alsousing DFT, in Ref. [419].

The authors of Ref. [410] also found the estimate for the critical value of the twist angle θc ∼= 1.89.If θ 6 θc, no Dirac spectrum exists, and the tBLG has a Fermi surface and a finite density of states atthe Fermi level. Figure 48 shows the Fermi surfaces calculated at half-filling for the superstructures (17, 1)(θ = θc ∼= 1.89) and (18, 1) (θ ∼= 1.79). The peak in the density of states existing near the Fermi level forθ 6 θc has a complex structure [see Fig. 48(c)]. Calculating the density of states allows a direct comparisonof the electronic properties of superstructures with different r. 2 The authors found that, neglecting somefine structures, the electronic properties of the tBLG change continuously with the twist angle when θ < θc.Another theoretical study of the Fermi surface structure and properties in the regime of small θ was reportedin Ref. [390].

2Structures with different r but similar θ have Brillouin zones of greatly dissimilar sizes. Thus, to compare the spectraand/or Fermi surfaces of these structures one has to work with folded Brillouin zones.

99

In all theoretical investigations described above it is assumed that the graphene layers are flat, andthe distance between layers is a constant. Experiments shows, however, that the interlayer distance c0 isspatially modulated [6]. Using STM, Ref. [6] showed that c0 is larger at regions with almost AA stackingand smaller in regions with almost AB stacking. The corrugation of graphene layers in tBLG was foundtheoretically using DFT in Refs. [382, 383]. The authors used their own efficient computation code allowingto perform DFT calculations for systems consisting of 104-105 atoms. In particular, they showed that fortwist angles [383] θ . 20 (or θ & 40) the layers are corrugated; the intralayer distance c0 is a Moireperiodic function of the real-space coordinate r, having a maximum (minimum) for r in the region withalmost AA (AB) stacking, which correlates with the experiment [6].

13.4. Twisted bilayer graphene in a magnetic field

13.4.1. Landau levels and quantum Hall effect

Landau quantization and quantum Hall effect are two issues which are the main focus for both theoreticaland experimental studies of the tBLG in an applied perpendicular magnetic field. As in the previoussubsection, the theoretical papers on this topic can be classified according to the level of approximationof the tBLG Hamiltonian. Here we follow the order of the previous section and consider first the worksusing effective low-energy Hamiltonians. The analysis based on tight-binding Hamiltonians will be consideredafterwards. We compare theoretical predictions with experimental results, both for the Landau quantizationand the quantum Hall effect.

In Refs. [385, 386], the structure of Landau levels is studied in the framework of a simplified 2×2 effectiveHamiltonian (185). In the presence of a magnetic field perpendicular to the bilayer, the Hamiltonian (185)can be rewritten as

H = ~ω∗c(

0 a2 − β2

a†2 − β2 0

), (214)

where

ω∗c =2eBv∗F~∆K

(215)

is the cyclotron frequency, the complex number β is defined as

β =

√~

8eB(∆Kx + i∆Ky) , (216)

and the operators a and a†, such that [a, a†] = 1, are the usual lowering and raising operators of the harmonicoscillator [420]. Note that the cyclotron frequency ω∗c , given by Eq. (215), is different from ωc introducedin Section 5, Eq. (78). The authors of Ref. [385] solve the eigenvalue problem Hψ = Eψ by numericallyexpanding the spinor wave function ψ = (ψ1, ψ2)T in the harmonic-oscillator basis |m〉:

ψ(n) =

∞∑m=−[n/2]

(φ1

2m+n

φ22m+n

)|2m+ n〉 , (217)

where the index n = 0, 1, 2, . . . enumerates the eigenvalues and eigenfunctions, and the ket-vectors |m〉satisfy the equations

a |m〉 =√m|m− 1〉 , a†|m〉 =

√m+ 1|m+ 1〉 , m = 0, 1, 2, . . . . (218)

For an odd (even) value of the index n, the expansion (217) contains only odd (even) basic states |m〉.The authors of Ref. [385] found that for any value of the magnetic field, the tBLG Hamiltonian has twozero-energy eigenstates with n = 0 and n = 1. The corresponding eigenfunctions can be found analytically.They are [385]

ψ(0) = N0 cosh(βa†)

(0|0〉

), ψ(1) = N1

sinh(βa†)

β

(0|0〉

). (219)

Thus, together with the spin and valley degeneracy, the zero-energy eigenstate is eight-fold degenerate.

100

The eigenvalue problem for the spinor wave function ψ = (ψ1, ψ2)T can be reduced to a single equationof the form

(a†2 − β2)(a2 − β2)ψ1 = λψ1 , λ =

(E

~ω∗c

)2

. (220)

The authors of Ref. [386] consider this equation in its holomorphic representation

a† 7→ ξ , a 7→ d

dξ. (221)

As a result, they derived a second-order differential equation, and solved it numerically. In the general case,there is no analytical expressions for the eigenenergies En. However, the authors of Ref. [386] were able tofind asymptotic expansions for the Landau levels in two limiting cases of small and large |β|. In the formercase they obtained(

En~ω∗c

)2

∼= n(n− 1)

[1− 2|β|4

(2n+ 1)(2n− 3)+

4n(n− 1)(4n(n− 1)− 39) + 63

(2n+ 3)(2n+ 1)3(2n− 3)3(2n− 5)|β|8 + . . .

]. (222)

When |β| 1, the result is(En~ω∗c

)2

∼= 4[n

2

]|β|2

(1−

[n2

] 1

2|β|2−[n

2

]2 1

4|β|4+ . . .

). (223)

For small |β|, the non-zero Landau levels are four-fold degenerate due to the spin and valley degeneracy.The case |β| 1 can be only realized either for very small twist angles or very high magnetic fields. Indeed,since |∆K| = 8π sin(θ/2)/(3

√3a0) ∼= 4πθ/(3

√3a0) and a0 = 1.42 A, one obtains from Eq. (216):

|β| ∼= 2.7θ[deg]√B[T]

. (224)

For the characteristic twist angle θ = 3 for which the effective 2 × 2 Hamiltonian (185) is best applicableand the magnetic field B = 10 T, one obtains |β| ≈ 2.57, which is closer to the limit of |β| 1. It followsfrom Eq. (223), that a level with n = 2` and another level with n = 2`+ 1, where ` is an integer, have thesame energy. Keeping only the leading term in Eq. (223), one obtains

E2`∼= E2`+1

∼= εLL(`) ≡ ±v∗F√

2e~|`|B , (225)

which coincides with Eq. (189). Thus, in the limit |β| 1, all Landau levels are eight-fold degenerate.Under more scrutiny, however, one discovers that for large |β|, the difference between E2` and E2`+1 isfinite, but exponentially small. The authors of Ref. [386] obtained an estimate

E22`+1 − E2

2`

~2ω∗2c≈ 2(2|β|)4`+2

(`− 1)!`!e−2|β|2 . (226)

The parameter |β| is smaller for smaller twist angles or for higher magnetic fields. Thus, the degeneracybetween the levels with n = 2` and n = 2` + 1 is lifted by stronger magnetic field. Due to the factor(2|β|)4`+2 in Eq. (226), the larger ` is, the smaller the magnetic field is required to lift the degeneracy. Thedegeneracy of the levels n = 2` and n = 2` + 1 is lifted when the right-hand-side of Eq. (226) becomes ofthe order of unity. For ` = 1 this happens when |β| ∼= 2.18, while for ` = 2 one obtains |β| ∼= 2.99.

Figure 49 shows the dependencies of the Landau levels energies on the magnetic field [panel (a)] and onthe twist angle at fixed magnetic field [panel (b)] calculated in Ref. [386]. The same results are obtainedalso in Ref. [385]. In these figures we see a crossover from the massless behavior at small fields (or relativelylarge twist angles) to the equidistant massive behavior at larger fields.

Measurements of the Landau levels in twisted graphene samples fabricated by chemical vapor depositionhave been performed in Ref. [351]. The magnetic field was varied in the range 2 T < B < 10 T. The bilayer

101

B[T]

E [eV] (a)

q[deg]

E/ħwC (b)

Figure 49: (Color online) Energies of the first several Landau levels in tBLG versus applied perpendicular magnetic field (leftpanel, twist angle θ = 3.17) and on the twist angle at fixed magnetic field (right panel, B = 10 T). At small fields or largetwist angles, the non-zero Landau levels are eight-fold degenerate and form a sequence corresponding to massless particles, asin Eq. (225). In the opposite limit, Landau levels are approximately equidistant, corresponding to massive particles. In thislimit, the non-zero LLs are four-fold degenerate. For any values of B and θ there is one eight-fold degenerate Landau levelhaving zero energy. Reprinted figures with permission from M.-Y. Choi et al., Phys. Rev. B, 84, 195437 (2011). Copyright2011 by the American Physical Society. http://dx.doi.org/10.1103/PhysRevB.84.195437.

graphene sample studied had large regions within which the Moire pattern preserved its periodicity. Thatallowed the authors [351] to extract the local values of twist angles. For twist angles larger than about2, the data are presented in Fig. 38(a). The sequence of Landau levels is well described by a square-rootdependence, given by Eq. (225). This work [351] reported Fermi velocity renormalization for the samples[see Fig. 38(b)], with the dependence of v∗F on θ correlating well with the theoretical prediction Eq. (175).A deviation from Eq. (225) was observed when θ . 1.17. For these angles, the form of the tunnelingspectra depends substantially on the position of the STM tip inside the Moire cell, which is consistent withthe theoretical calculations of the local density of states for small angles. A square root dependence of theLandau levels is reported also in Ref. [395] for multilayer samples grown on SiC. No Fermi velocity reductionis found in these samples (for a discussion on this issue, see page 3 of Ref. [351]).

Landau quantization can also be observed in measurements of both the longitudinal, σxx, and Hall, σxy,conductivities. At zero temperature, the Hall conductivity is a step function of the chemical potential (orthe induced charge carrier density), σxy = (e2/2π~)ν, where the filling factor ν takes integer values whichdepend on the degeneracy of the Landau levels. When |β| 1, the zero-energy Landau level is eight-folddegenerate, while all other levels are four-fold degenerate, and the filling factor is

ν = ±4, ±8, ±12, . . . . (227)

In the opposite case of |β| 1, when Eq. (225) is valid, all Landau levels are eight-fold degenerate, and

ν = ±4, ±12, ±20, . . . . (228)

The Hall conductivity of the tBLG samples was measured in several works [399, 421, 422]. Figure 50shows the dependence of the σxy on the electron density n at different values of the magnetic field (fromD. S. Lee et al. [421]). The electron density is induced by the applying a gate voltage. From Fig. 50 wesee that the Hall conductivity is quantized according to Eq. (227), corresponding to the limit of |β| 1.For example, the step at filling factor ν = ±8, (which is absent in the opposite limit |β| 1), is clearlyseen in this figure for B = 5 T and larger. The twist angle for samples studied in Ref. [421] is estimated asθ ∼= 2.2, and for B = 5 T one obtains from Eq. (224) that |β| ∼= 2.66. This estimate is slightly below thevalue |β| ∼= 2.99 Where the eight-fold degeneracy of the second Landau level is lifted. The authors concludedthat the regime of small |β| was realized in their experiments.

102

n

Figure 50: (Color online) Hall conductivity of the tBLG sample versus the electron density, measured for different values ofthe magnetic field. Reprinted figure with permission from D. S. Lee et al., Phys. Rev. Lett., 107, 216602 (2011). Copyright2011 by the American Physical Society. http://dx.doi.org/10.1103/PhysRevLett.107.216602.

J. D. Sanchez-Yamagishi et al. [399] reported results on transport measurements for tBLG, obtained usingthe dual-gate device schematically shown in Fig. 51(a). The existence of the top and bottom gates allowsone to control both the total electron density n in the bilayer and the potential difference ∆V between twolayers or the difference in the electron density, ∆n, between two layers. The induced total electron densityis related to the top VTG and bottom VBG gate voltages as

n = (CTVTG + CBVBG)/e ,

where CT , CB are the capacitances per unit area of the top and bottom gates, respectively. The appliedelectric field

E = (CTVTG − CBVBG)/2

leads to the redistribution of the charge carriers between two graphene layers, which partially screens theelectric field. As a result, the potential difference between two layers ∆V can be written as [399]

−∆V =

(E − e∆n

2

)1

C, (229)

where C = ε/c0 is the interlayer capacitance per unit area and ε is the interlayer dielectric constant.In the case of completely uncoupled graphene layers, the potential difference gives rise to the shift of the

Dirac cones of the top (bottom) layer by the value −e∆V/2 (+e∆V/2). The calculations done in Ref. [3] inthe framework of low-energy theory show that similar situation takes place in tBLG with finite interlayerhybridization. In magnetic field, the shift of the Dirac cones leads to the lifting of the eight-fold degeneracy ofthe tBLG Landau levels, existing in the regime |β| 1, and to the appearance of additional steps in the Hallconductivity. This was experimentally observed in Ref. [399]: Figure 51(b) demonstrates distinctive stepsof 2e2/π~ in the Hall conductivity at non-zero E, while for unbiased bilayer only the steps of 4e2/π~ exist.

103

(a)

n

E

E/e0=0

E/e0=145mV/nm

(c) (d)

n

E/e

0

Figure 51: (Color online) (a) Schematic of the dual-gated twisted bilayer graphene device. Two central (red and blue) layerscorrespond to the tBLG. BN – hexagonal boron nitride layer. (b) Hall conductivity in units of e2/2π~ measured at B = 9 T. ForE = 0 the steps follow Eq. (228). If E 6= 0 addition steps exist, indicating the lifting of the eight-fold Landau levels degeneracy.(c) The Landau level energy spectra as a function of the interlayer potential difference ∆V calculated in the uncoupled layerapproximation; NU , NL are integers corresponding to the upper and lower layers, respectively. The Landau levels crossingsare indicated by black dots. (d) Longitudinal resistance with subtracted background value as a function of E and ν = nh/eBmeasured at B = 4 T. Peaks indicate the LL crossing. Black dots correspond to the theoretical prediction. Reprinted figureswith permission from J. D. Sanchez-Yamagishi et al., Phys. Rev. Lett., 108, 076601 (2012). Copyright 2012 by the AmericanPhysical Society. http://dx.doi.org/10.1103/PhysRevLett.108.076601.

Further increasing ∆V leads to Landau level crossing. The crossing occurs when the following condition issatisfied:

− e∆V = εLL(`1)− εLL(`2) , (230)

where `1,2 are integers. For uncoupled layers, `1 and `2 are the numbers of Landau levels of the top andbottom layer, respectively. In tBLG, the interlayer hybridization is non-zero, and this works only whenεLL(`1,2) is less than the energy of the van Hove singularity. Figure 51(c) presents the LL energy spectra asa function of the interlayer potential difference, as they were calculated in Ref. [399] in the approximation ofuncoupled layers. When LL crossing appears, the longitudinal conductivity has a peak, which was observedexperimentally in Ref. [399] [see Fig. 51(d)]. The positions of these peaks are in a good agreement withtheoretical predictions.

13.4.2. Fine structure of the Landau levels

According to the simple model, Eq. (214), the Landau levels in tBLG are eight-fold degenerate, when|β| ∝ θ/

√B 1. This picture is confirmed experimentally by both Landau-level spectroscopy [351, 395] and

transport measurements [422, 399]. However, a high-resolution LL spectroscopy measurements performedat low temperatures (T ∼ 10 mK) in Ref. [398] by Y. J. Song et al. revealed the fine structure of thetBLG Landau levels. The authors studied multilayer graphene samples grown on the carbon face of SiC.The estimated total number of layers in the sample was six. The STM images show the Moire patternwith period 5.7 nm [see the Fig. 52(a)], which corresponds to twist angle between the two top layers beingθ ∼= 2.3. Peaks in the tunneling spectra measured at low magnetic fields are well described by the squareroot dependence of B and of the level’s number, according to Eq. (225) [see Fig. 52(b)]. However, alreadyat B & 2 T, the fine structure of the Landau levels is clearly seen [see the Fig. 52(c)]. Each Landau levelwith ` 6= 0 splits into two pairs of levels. Thus, there are four sub-levels with energies E`L ±∆E`L/2 andE`R±∆E`R/2. The energy splitting ∆E` = E`L−E`R between two pairs of sub-levels is much higher thanthe splitting within each pair, ∆E`L and ∆E`R. The splitting demonstrates an almost-linear dependenceon the magnetic field,

∆E` ≈ g`µBB , ∆E`L,R ≈ g`L,RµBB ,

where the g-factors are estimated as g` ∼ 20 and g`L,R ∼ 2. The zeroth Landau level splits at higher magneticfields, B ∼ 12 T. The authors attributed the splitting ∆E` to the lifting of the valley degeneracy, while the

104

(a)

(b)

5.7

nm

( ) 2/1

Bl

Figure 52: (Color online) (a) STM image of epitaxial graphene grown on C-face of SiC showing a Moire pattern with the periodL = 5.7 nm, corresponding to the twist angle between two top layers θ = 2.3. Total number of graphene layers is six. (b)Energies of Landau levels ` versus the square root of `B. Solid (blue) line is the linear fit according to Eq. (225) with the Fermivelocity v∗F = (1.08 ± 0.03) × 106 m s−1. (c) A series of tunneling spectra as a function of the magnetic field taken along thesample. Each panel shows the dI/dV intensity in a color scale. The vertical axis within each panel is distance from 0 to 40 nm.A splitting of the Landau levels in different field ranges is clearly seen. Reprinted by permission from Macmillan PublishersLtd: Y. J. Song et al., Nature, 467, 185 (2010), copyright (2010). http://dx.doi.org/10.1038/nature09330.

splitting within sub-levels can be explained by Zeeman coupling to electron spin. The spatially-modulatedsplitting of the zeroth Landau level was also observed in Ref. [423].

The theoretical analysis of the fine structure of the Landau levels in tBLG has been done in Refs. [424,425, 426, 427]. In Ref. [424] M. Kindermann and E. J. Mele calculated the tBLG Landau levels in frameworkof the low-energy theory. They took into account the hybridization of electron states in different layers ifthese states are equivalent in the Brillouin zone of the superlattice. The result depends on the type ofsuperstructure. The effective Hamiltonian used is a 4 × 4 block matrix having a form similar to that ofEq. (192) for ‘odd’ structures (Hodd) or Eq. (193) for ‘even’ structures (Heven)

Hodd =

(HK(− θ2 ) H−int

(H−int)† HK′(

θ2 )

), Heven =

(HK(− θ2 ) H+

int

(H+int)† HK( θ2 )

), (231)

where the non-diagonal 2× 2 ‘mass’ matrices H∓int are given by Eq. (194), while

HK(θ) = −i~ωc(

0 ae−iθ

−a†eiθ 0

), HK′(θ) = σyHK(θ)σy = −i~ωc

(0 a†eiθ

−ae−iθ 0

), (232)

where a and a† are the Landau level lowering and raising operators, and cyclotron frequency ωc is givenby Eq. (78) with the renormalized Fermi velocity. The Hamiltonian (231) can be diagonalized analyticallyboth for ‘odd’ and ‘even’ structures. The mass terms in Eqs. (231) lead to the splitting of the eight-folddegenerate Landau levels ` (with the single exception of ` = 0 for the ‘odd’ structures) into two four-folddegenerate levels, which now can be described by the integers ` and κ = ±1. The energies of these levels

105

are [424]:

Eodd`κ = ±

[(`− κ

2

)~2ω2

c + V2 +κ

2

√~4ω4

c + 4(`− κ

2

)~2ω2

cV2 + V4

]1/2

, (233)

Eeven`κ = ±

[`~2ω2

c + V2 + 2κ~ωcV cosϕ

2

√`]1/2

, (234)

where V describes the strength of the LL splitting, and ϕ is the additional parameter entering throughH−int. If the structure is ‘odd’, the level with ` = 0 remains degenerate: Eodd

0κ = 0 both for κ = +1 andκ = −1. When ~ωc V, which corresponds to the experimental conditions [see Fig. 52(b)], the splittingof the `-th LL level is ∆Eeven

`∼= 2V cos(ϕ/2), while ∆Eodd

`∼= V2

√`/ωc if ` ωc/V or ∆Eodd

`∼= V/2 if

` ωc/V. Thus, this theory predicts the LL splitting, but it can not describe the linear dependence of ∆E`on magnetic field observed experimentally.

Similar ideas have been discussed in Ref. [425] in a more realistic model. The authors considered boththe bilayer and trilayer graphene samples. In addition, they took into account the non-zero potential energydifference Vij between graphene layers (i, j = 1, 2 or i, j = 1, 2, 3). In the limit V12 ωc V, the resultfor the ‘odd’ structures is

∆E0∼=V2

V12, ∆E` ∼=

2V2v∗2FV 3

12

eB , ` 6= 0 . (235)

Thus, indeed, the splitting of Landau levels linearly increases with the magnetic field. However, the effectiveg-factor estimated from Eq. (235) turns out to be much smaller than the experimental value. This is becauseof the smallness of V, which was estimated by the authors for the twisted bilayer as V ∼ t⊥θ2. For graphenetrilayer, however, the splitting is given by similar relations, in which one has to replace V → t0. Then, thediscrepancy between theory and experiment can be attributed to the effect of lower carbon layers in thesamples used in Ref. [398].

The authors of Ref. [426] calculated the optical absorption spectra in the presence of the magnetic field,using an approach related to that of Refs. [424, 425]. The LL splitting described above gives rise to themultipeak structure of the absorption spectra, which could be observed experimentally.

13.4.3. The Hofstadter butterfly spectrum

The analysis of the Landau levels described above does not take into account the superlattice periodicityof the tBLG. It is well known, however, that a periodic potential changes the Landau level spectrum ofthe electrons in a magnetic field, leading to a spectrum with a fractal structure. This phenomenon, theso-called Hofstadter’s butterfly [428], becomes experimentally observable when the magnetic flux throughthe elementary unit cell Φ becomes comparable to the magnetic flux quantum Φ0, or, alternatively, whenthe magnetic length satisfies

lB =√~c/eB . L ,

where L is the lattice period. For common materials, with L about several angstroms, this happens whenB ∼ 104–105 T, which significantly exceeds normally achievable magnetic fields. However, for superlatticeswith large supercells, the Hofstadter butterfly can be observed experimentally. Using Eq. (156) for the Moireperiod L, one can calculate the magnetic flux through the Moire cell and obtain the estimate for the fieldrequired for the observation of the fractal spectrum in the tBLG [429]

B &~θ2

3ea20

≈ 3.3(θ)2 [T] . (236)

Fractal spectra have been observed experimentally in single-layer graphene [430, 431] and also in Bernal-stacked bilayer graphene [432] placed on an hexagonal boron nitride (hBN) substrate. The mismatch betweenthe graphene and the hBN lattice constants (along with a small rotational misorientation between thegraphene layers and the substrate) creates a Moire pattern, which modifies the single layer or AB-stackedbilayer graphene’s electron spectrum. As a result, a Hofstadter’s butterfly spectrum was observed in a

106

magnetic field of the order of several Tesla. Unfortunately, similar observations for twisted bilayer grapheneare still absent. Note, however, that in Ref. [433], the magnetotransport measurements were reported fordifferent samples of the tBLG in a magnetic field up to B = 13 T. The authors observed a complex behaviorof the resistivity as a function of the magnetic field and the gate voltage if θ < 3, but the interpretation ofthe obtained data is not yet clear.

Theoretical studies of the fractal spectrum of tBLG were performed both in the framework of the con-tinuum approximation [434] and tight-binding models [429, 435, 436]. In Ref. [434], R. Bistritzer and A.H.MacDonald used the effective low-energy Hamiltonian having a block matrix of the form of Eq. (174), inwhich one should replace −i~∇→ −i~∇ + eA/c, that is,

H =

(H0(−θ/2) T (r)

T †(r) H0(θ/2)

), H0(θ) = vFσ

θ [−i~∇ + eA/c] , T (r) =

3∑s=1

e−iqsr Ts , (237)

whereq1 = ∆K(0,−1) , q2 = ∆K(

√3, 1)/2 , q3 = ∆K(−

√3, 1)/2 ,

and 2× 2 matrices Ts are given by Eq. (172). The Hamiltonian (237) has a Moire periodicity. The authorsof Ref. [434] used the Landau gauge A = B(−y, 0, 0). They expressed the Hamiltonian (237) in terms ofthe basis states |iαny〉 ≡ |iα〉 ⊗ |ny〉, where i = 1, 2 and α = A,B are the layer and sublattice indices,respectively. The ket-vector |iα〉 can be considered as a 4-component spinor [|1A〉 = (1, 0, 0, 0)T, etc]. Thesecond ket |ny〉 represents the nth Landau level wave function. The variable y being the y-coordinate of thecenter of the electron’s orbit [420] is related to the conserved momentum in the x-direction as y = kxl

2B . In

the real-space representation, the |ny〉 can be written as [420]

|ny〉 =eiyx/l

2B exp

[− (y−y)2

4l2B

][2nn!

√πlBLx]1/2

Hn

(y − ylB

), (238)

where Hn(ξ) are the Hermite polynomials and Lx is the sample’s length in the x-direction. In terms of thesewave functions, the intralayer part of the Hamiltonian (237) H0(θ) has the form

H0(θ) = −ωc∑ny

√n

(0 e−iθ|n− 1y〉〈ny|

eiθ|ny〉〈n− 1y| 0

). (239)

The spectrum is degenerate with respect to y if we neglect the interlayer hopping. Diagonalizing H0(±θ/2)one obtains the spectrum of the Landau levels corresponding to the decoupled graphene layers En = ±ωc

√n.

The interlayer hopping, however, hybridizes the states with y and y ± δy, where

δy =

√3 ∆K l2B

2, (240)

due to the factors exp(−iqr) in T (r). The states with y = y0 + nδy, where n = 0, ±1, ±2, . . . , form a ‘one-dimensional’ chain of states. Such a structure allows a partial diagonalization of the Hamiltonian. Eachchain is characterized by the momentum k1 = y0/l

2B , where k1 belongs to the interval

0 < k1 < δy/l2B =√

3∆K/2 .

Each chain is coupled to other chains. For the commensurate flux

Φ0/Φ = ∆K2l2B√

3/(8π) = p/q ,

where p and q are co-prime integers, one can define a ‘supercell’, introduce the second momentum k2, anddefine new basis vectors, |iαnjk〉 ≡ |iα〉 ⊗ |njk〉, according to the relation

|njk〉 =

√qδy

Ly

∑m

exp[ik2δy(mq + j)]|nk1l2B + δy(mq + j)〉 , (241)

107

Figure 53: (Color online) The low-energy spectrum of tBLG in magnetic field as a function of (rational) Φ0/Φ calculated forθ = 2 and t⊥ = 110 meV. For any vertical cut of this image a tiny dot corresponds to a Landau level, white areas representspectral gaps with no levels. The periodic inter-layer hopping leads to the Hofstadter-like structure of the spectrum. Reprintedfigure with permission from R. Bistritzer and A. H. MacDonald, Phys. Rev. B, 84, 035440 (2011). Copyright 2011 by theAmerican Physical Society. http://dx.doi.org/10.1103/PhysRevB.84.035440.

where j = 0, 1, . . . , q − 1, Ly is the sample’s size in the y-direction, and the momentum k = (k1, k2) liesinside the “magnetic” Brillouin zone

0 < k1 <∆K√

3

2, 0 < k2 <

∆K

2p. (242)

In the latter basis, the intralayer term H0(θ) is diagonal in k and j. It is given by Eq. (239) in whichone substitute |ny〉 → |njk〉 and the summation over y is replaced by the summation over k and j. Theinterlayer term T is diagonal in this basis in the wave vector k. It can be written as

T =∑nmkj

∑αβ

[Tαβ1 Fnm

(q1lB√

2

)e−i∆Kk1l

2Be−4πi pq j |2αnjk〉〈1βmjk|

+ Tαβ2 Fnm

(q2lB√

2

)ei∆Kk1l

2B/2eik2δyeiπ

pq (2j−1)|2αnj + 1k〉〈1βmjk| (243)

+Tαβ3 Fnm

(q3lB√

2

)ei∆Kk1l

2B/2e−ik2δyeiπ

pq (2j+1)|2αnj − 1k〉〈1βmjk|

],

where j is defined modulo q, and

Fnm(z) =

√m!

n!(−zx + izy)

n−mexp

(−z2

2

)Ln−mm

(z2), n > m, (244)

with Lam being the associated Laguerre polynomials. For n < m, the function Fnm is defined by Fnm(z) =[Fmn(−z)]∗.

108

R. Bistritzer and A.H. MacDonald [434] calculated the spectrum numerically by only considering first

N0 ∼ 2[max(vF∆K, t⊥)/ωc]2 (245)

Landau levels. Thus, for any k, the rank of the matrix, which has to be diagonalized, is equal to 4qN0.As it follows from the structure of Eq. (243), the interlayer hopping splits each Landau level into q finite-width sub-bands, and couples them to each other. Both of these effects change the spectrum. However, thecoupling of Landau levels is more important for smaller magnetic fields. The smaller the twist angle is, thesmaller the magnetic field is required to disturb the Landau level spectrum, because

Φ0/Φ ∝ θ2/B .

If θ < θc, this line of reasoning becomes invalid because the Dirac cones in the spectrum disappear even atB = 0). Figure 53 shows the spectrum of tBLG for rational Φ0/Φ < 1, calculated at θ = 2. It is seen that,in general, the gaps between sub-bands increase when Φ0/Φ decreases.

C.-K. Lu and H. A. Fertig in Ref. [437] used a similar low-energy model, Eq. (237), to analyze the effect ofthe bias voltage on the LL in tBLG. Besides the electronic spectrum in a magnetic field, they calculated theoptical absorption spectra. They [437] claimed that the bias voltage can help to distinguish the transitionsinvolving the states localized in one particular layer from the transitions involving the layer-delocalizedstates.

Tight-binding calculations of the tBLG spectrum in a magnetic field were performed in Refs. [429, 435,436]. The authors of Refs. [435, 436] used the exponential dependence of the hopping amplitudes t(r; r′) onthe distance between sites, while P. Moon and M. Koshino [429] applied the somewhat more complicatedparametrization given by Eqs. (196)–(201). In magnetic field, the hopping amplitude t(r; r′) acquires anaddition phase factor and becomes

t(r; r′) exp

(ie

~c

ˆ r′

r

Adr

). (246)

The gauge in which the vector potential A is parallel to the superlattice vector R2 is used in Ref. [429].When Φ/Φ0 = p/q, where p and q are co-prime integers, the tight-binding tBLG Hamiltonian (195) has aperiodicity described by the supercell vectors qR1 and R2. Consequently, the area of the magnetic Brillouinzone is q times smaller than the Brillouin zone area for B = 0, and the number of bands for (m0, r)superstructure is qN(m0, r).

The authors of Ref. [429] considered a spectrum in the energy window −0.5 eV< E < 0.5 eV, for severalsuperstructures with r = 1 and twist angles in the range 1.5 . θ . 10, in magnetic fields up to 180 T.In addition to the spectrum, they calculated the Hall conductivity σxy. When the Fermi level µ lies in theband gap, the conductivity σxy can be found according to [438]

σxy = −e(∂n

∂B

)µ

, (247)

where n is the number of electrons per unit area for a given µ. Some results of this study are presentedin Fig 54. Panels (a,d) and (b,e) show the dependencies of the spectrum and the Hall conductivity onthe magnetic field. Right panels (c,f) present the band structure in the case B = 0. When Φ/Φ0 1, thespectrum consists of a sequence of nearly-degenerate Landau levels [described by the square-root dependenceEq. (225)], and the Hall conductivity in units of e2/2π~ follows the law Eq. (228), corresponding to uncoupledgraphene layers [see panels (a,b) in Fig. 54]. For large twist angles, the regime of small Φ/Φ0 is maintainedup to very high magnetic fields. The deviation from the square-root dependence of the sequence of Landaulevels occurs when the absolute value of the LL energy, En, exceeds the energy of the van Hove singularities(if θ ∼= 3.89 this happens when |En| & 0.2 eV). Simultaneously, the Hall conductivity drops down to negativevalues and then grows in discrete increments equal four conductivity quanta [see panel (e) in Fig. 54]. Thebehavior of the tBLG spectrum in magnetic fields near the van Hove singularities has been also studied [439]using a semiclassical approach.

109

Figure 54: (Color online) Numerically calculated energy spectrum (a,d) and Hall conductivity (b,e) versus magnetic fieldfor tBLG samples with θ ∼= 9.43 (upper panels) and θ ∼= 3.89 (lower panels). The right panels (c,f) show the bandstructure at B = 0. The dashed (red) lines show the dispersion of monolayer graphene near the Dirac point. In panels(b) and (e) the values of the Hall conductivity are indicated by numbers and colors. Reprinted figure with permission fromP. Moon and M. Koshino, Phys. Rev. B, 85, 195458 (2012). Copyright 2012 by the American Physical Society. http:

//dx.doi.org/10.1103/PhysRevB.85.195458.

Even for small Φ/Φ0, the superlattice periodicity breaks the degeneracy of each Landau level: thedensity of states spreads in the energy domain to form several sub-bands separated by small gaps. Thesegaps increase when the magnetic field grows. As a result, the spectrum acquires a complicated fractalstructure dissimilar to the original Landau level picture [Fig. 54(d)]. Simultaneously, the Hall conductivitybecomes a non-monotonic function of the Fermi level. Characteristic magnetic fields of the crossover fromthe Landau level to fractal descriptions can be estimated from Eq. (236). For example, B = 50, 23, and7.2, T for θ = 3.89, 2.65, and 1.47, respectively [429].

Similar results for the tBLG electronic spectrum where obtained by Y. Hasegawa and M. Kohmoto inRef. [436]. The authors used the so-called periodic Landau gauge for the vector potential A. The spectrumthey calculated consists of many bands separated by the gaps. Each gap can be characterized by twointegers (s, ν), where ν is related to the Hall conductivity as σxy = (e2/2π~)ν. The authors [436] analyzedthe evolution of the spectrum when changing of the magnetic field and the twist angle. For example, theyshowed that for considerably small twist angles, there are several narrow low-energy bands separated bygaps having the same value of ν; that is, the passing of the chemical potential trough these bands does not

110

change the Hall conductivity.Reference [435] by Z. F. Wang et al. presents tight-binding calculations of the spectrum in a magnetic field

for finite samples with sizes up to 140×140 nm2. The Lanczos algorithm was used for calculating eigenstatesin the energy window |E| < 0.2 eV. Because of the finite size of the samples, the authors were able to considerboth commensurate and incommensurate twist angles. The authors distinguished three regions of twistangles where the spectra are qualitatively different from each other. In the ‘quasi-Bernal’ regime, 0 6 θ .0.3, the spectrum consists of nearly-degenerate Landau levels with energies corresponding to the AB bilayer.In the intermediate regime, 0.3 . θ . 3, the spectrum has a complex fractal-like structure (for B ∼ 10 T).At larger angles, the spectrum consists of Landau levels corresponding to effectively uncoupled layers; theenergies of these levels are described by Eq. (225) with a renormalized Fermi velocity, which monotonouslydecreases with the twist angle both for commensurate and incommensurate structures. The Supportinginformation to Ref. [435] presents a movie showing the evolution of the spectrum when changing the twistangle. This video can be downloaded from http://pubs.acs.org/doi/suppl/10.1021/nl301794t.

13.5. Electronic transport in twisted bilayer graphene

13.5.1. Dynamical conductivity

The response of the tBLG on the ac electromagnetic field has been studied both experimentally [441,442, 443] and theoretically [440, 444, 445, 344]. In Ref. [440] C. J. Tabert and E. J. Nicol calculated theoptical conductivity in the framework of the simplified low-energy theory proposed by R. de Gail et al. [385].They used the 4 × 4 Hamiltonian H(k) given by Eq. (177) with the interlayer term H⊥ in the form ofEq. (178). The use of the simplified expression for the interlayer hopping allows them to calculate thespectrum analytically. The results are shown in Fig. 55(a)–(c). The real part of the dynamical conductivityat zero temperature is calculated numerically using Eq. (122), which for T = 0 has the form

σxx(ω) =2e2

ω

µ

µ−ω

dω′

2π

ˆd2k

(2π)2Tr[vxA(k, ω′ + ω)vxA(k, ω′)

], (248)

where vx = ∂H/∂kx, and A(k, ω) is the spectral function (both are 4 × 4 matrices). As in the case of theAA and AB bilayers considered in the previous sections, the authors [440] use the Lorentzian broadeningfor the δ-function in A(k, ω), πδ(x)→ Γ/(x2 + Γ2), where Γ is associated with the transport scattering rateon the impurities.

Figures 55(d)–(f) show the in-plane dynamical conductivity as a function of frequency calculated forthe tBLG with θ = 5 at different values of the chemical potential µ. At zero doping, the conductivity isapproximately constant at low frequencies and equal to twice the background conductivity of single-layergraphene e2/(4~). At higher frequencies, the conductivity has a dip-and-peak structure associated with thetransitions from/to electron states near the low-energy van Hove singularities [see the black, green, andorange arrows in Fig. 55(a)–(f)]. Such a peak in the conductivity is similar to that for the AB bilayer [256,259] (see Figs. 28 and 29) but is located at higher energies, near the energy of the VHS splitting, ∆EvHs

(for definition, see subsection 13.2.2). Its position is closer to zero energy for smaller twist angles. Atlarge twist angles, ∆EvHs ∼ 1 eV, and the corresponding frequencies lie in the visible range. For example,the contrast spectroscopy measurements done in Ref. [441] revealed the peak in conductivity located atwavelength λ ≈ 595 nm (~ω ∼= 2.08 eV) for tBLG sample with θ ∼= 13.7. At smaller twist angles, the peakcan lie in the infrared and even terahertz frequency range. Thus, the peak at ω ∼= 2.64 THz was observedexperimentally using terahertz time-domain spectroscopy in Ref. [442]. The twist angle of the sample studiedin the latter work was estimated as θ ∼= 1.16.

At finite doping, the conductivity is modified in two aspects. First, it acquires a Drude peak centeredat zero frequency. Second, at frequencies ω < 2µ the interband transitions are not allowed due to the Pauliexclusion principle, and this leads to the suppression of the dynamical conductivity in the range 0 . ω < 2µ[see Fig. 55(b,e)]. At larger frequencies, the conductivity is the same as for µ = 0. For larger doping, whenµ lies between the van Hove singularity and the bottom of the upper band, the conductivity acquires an

111

(meV) wh

(meV) wh

(meV) wh

Figure 55: (Color online) Dynamical conductivity of twisted bilayer graphene. Panels (a)–(c): the low-energy single-electrontBLG spectrum along the line connecting the K and Kθ points calculated in Ref. [440] for θ = 5. Different significant opticaltransitions are indicated by arrows. Panels (d)–(f): the frequency dependence of the longitudinal conductivity calculated fordifferent values of the chemical potential µ. The arrows indicate the frequency of the transitions shown in panels (a)–(c).Reprinted figure with permission from C. J. Tabert and E. J. Nicol, Phys. Rev. B, 87, 121402 (2013). Copyright 2013 by theAmerican Physical Society. http://dx.doi.org/10.1103/PhysRevB.87.121402.

addition low-energy peak associated with the transitions between these two states [see Fig. 55(c,f), c.f. withFig. 28(b)].

Tight-binding calculations of the dynamical conductivity were performed by P. Moon and M. Koshino inRef. [445]. The hopping amplitudes are calculated according to the exponential parametrization Eqs. (196)–(201). The Lorentzian broadening of the spectral functions with Γ = 7 meV was used for calculating thedynamical conductivity. The authors considered undoped bilayers, and focused on the change of the dynam-ical conductivity with the twist angle. The dependencies of σ on ω calculated for several superstructures arepresented in Fig. 56. Since the tight-binding approach involves much more energy bands into consideration,in comparison to the low-energy theories, the obtained curves have a more complicated structure than thosepresented in Fig. 55. The curves σ(ω) have several peaks associated with the electron transitions betweendifferent VHS. Each singularity manifests itself as a peak in the density of states, shown in Fig. 56(a).Authors [445] distinguish three major types of VHS. Singularities of the types (i) and (ii) result from theintersection of the single-layer graphene bands caused by the interlayer coupling. Specifically, singularitiesof types (i) appear at momenta near the points K0 = (K + Kθ)/2 and K′0 = (K′ + K′θ)/2, while the

112

(a) (b)

Figure 56: (Color online) The density of states (a) and the dynamical conductivity (b) calculated in tight-binding approximationfor several undoped tBLG superstructures, as well for AB- and AA-stacked bilayers in Ref. [445]. Peaks marked by (•), (),and (O) symbols correspond to the three types of the VHS described in the text. The superstructures (n,m) in the figurecorrespond to structures (n,m−n) in our notation. Small peaks encircled by dashed blue lines in panel (b) exist only for r 6= 1(m 6= n + 1) superstructures. Reprinted figures with permission from P. Moon and M. Koshino, Phys. Rev. B, 87, 205404(2013). Copyright 2013 by the American Physical Society. http://dx.doi.org/10.1103/PhysRevB.87.205404.

type (ii) VHS exist near the middle point of the line connecting the points K0 and K′0. Finally, the type(iii) singularities originate from the VHS of single-layer graphene. Since VHS of different types appear atdifferent momenta, and the momentum of the absorbed photon is negligible, there can exist only transitionsbetween electron states near the VHS of the same type, and the peaks in the conductivity can be classifiedin the same manner. The peaks of type (i) in the conductivity curves in Fig. 56(b) approach zero energyfor structures with smaller twist angles. These peaks are similar to those given by the low-energy theories[see, Fig. 55(d)]. On the other hand, the peaks of type (ii) move to higher energies with decreasing twistangle. The position of the type (iii) peaks is almost independent of θ because these peaks are related tosingle-layer van Hove singularities. The peaks of types (ii) and (iii) are beyond the scope of the low-energytheories.

In addition, superstructures with r 6= 1 have extra small peaks in the conductivity. They are markedby the dashed blue circles in Fig. 56(b). The authors [445] associated these minor peaks with the electrontransitions at the corners of the Brillouin zone of the superlattice. Indeed, the Brillouin zone of the super-structure (m, r) with r 6= 1 is approximately r times smaller than that for the superstructure (m0, 1) havingsimilar θ, where m0 = [m/r]. According to calculations done in Ref. [410], the spectrum of the superstruc-ture (m, r) is similar to the spectrum of the (m0, 1) superstructure calculated in the r-times-folded Brillouinzone. The folding leads to an additional band crossings, which for the (m, r) superstructure can give riseto additional van Hove singularities resulting in these conductivity peaks. These peaks, when observed,would be a fingerprint of the r 6= 1 superstructures. Similar calculations, but for biased bilayers, have beenperformed in Ref. [415].

Detailed experimental studies of the optical conductivity of tBLG have been performed by R. W. Havener

113

Figure 57: (Color online) Optical conductivity spectra of the AB BLG (top) and for three tBLG samples with different twistangles θ from Ref. [446]. For clarity, neighboring curves are offset by the value 4(e2/4~). The dashed lines connect the peakswith energies EA, EB , and EM corresponding, respectively, to peaks of the types (i), (ii), and (iii) in the notation of P. Moonand M. Koshino [445] (see Fig. 56). Images on the right show the diffraction patterns of the bilayers and the correspondingvalues of the twist angle. Reprinted with permission from R. W. Havener et al., Nano Letters, 14, 3353 (2014). Copyright 2014American Chemical Society. http://dx.doi.org/10.1021/nl500823k.

et al. in Ref. [446]. The authors measured the optical conductivity in the energy range 1.2 < ~ω < 5.6 eV forbilayers with different twist angles and for AB samples as well. Some results are presented in Fig. 57. Theconductivity spectra of the twisted bilayers have three peaks which Ref. [446] associated with the peaks ofthe types (i), (ii), and (iii) mentioned above. The authors [446] compared their results with the tight-bindingcalculations by P. Moon and M. Koshino, Ref. [445], and found a qualitative agreement between theory andexperiment. However, according to the analysis done in Ref. [446], for better fitting of the obtained data onehas to take into account the effects of the electron-hole interactions and the existence of excitonic states.

The possibility of the formation of excitons in tBLG has been proposed theoretically in Ref. [447]. Theexciton is formed by the hole, located near the VHS above the Fermi level and the electron located closeto the bottom of the upper electron band. These quasiparticles can be excited by optical transitions shownby the two left (green) arrows in Fig. 55(a). According to calculations done in Ref. [447], the electron-holeinteraction leads to the formation of the bound exciton with binding energy Eb ∼ 0.5 eV. The existence ofthese excitonic states should result in increasing the lifetime of optical excitations. In particular, the decaytime of the photocurrent in the tBLG should be much larger than that for the AB bilayer. This effect hasbeen observed experimentally [448] using transient absorption microscopy.

The real and imaginary parts of the dynamical conductivity were calculated by T. Stauber et al. [344]in the framework of the continuum (low-energy) approximation developed in [3, 367, 372, 387]. The directcalculation of Im[σ(ω)] is impossible because it requires the integration over a wide energy range, includingenergies far beyond the low-energy approximation. The authors [344] obtained a regularized Kramers–Kronig relation allowing to calculate the imaginary part of the dynamical conductivity in this case. Theirapproach is based on the observation that at high frequencies, the real part of the conductivity is equal to2σ0, where σ0 = e2/4~ is the background conductivity of single-layer graphene. As a result, they obtained

114

the following equation

Imσ(ω) =2

πω

∞

0

dω′ω′2[Reσreg(ω′)− 2σ0]

ω2 − ω′2, (249)

where the bar in the integral represents the principal part. In this equation, σreg is the regular part ofthe total conductivity not including the δ-peak at zero frequency. The authors [344] calculated Re(σreg)numerically according to the relation

Re [σreg(ω)] =4πe2

~ω∑nm

ˆd2k

(2π)2[nF (εnk)− nF (εmk)]

∣∣∣〈mk|jx|nk〉∣∣∣2 δ[ω − (εmk − εnk)/~] , (250)

where εnk and |nk〉 are the eigenenergy and the eigenstate of the low-energy Hamiltonian, with n being theband index, and jx = −∂H/∂kx. The total conductivity, then becomes

σ(ω) = πDδ(ω) + σreg(ω) , (251)

where D is the the Drude weight, which is related to the imaginary part of σ as

D = limω→0

[ω Imσ(ω)] . (252)

Using Eqs. (249)–(252), the authors of Ref. [344] numerically calculated the Drude weight as a functionof the chemical potential µ. When the twist angle exceeds a critical value (which was estimated [344] asθc ∼= 1.05), for small µ, the Drude weight is approximately twice of its value for single-layer graphene,

D(µ) ≈ 2D0(µ) , D0(µ) =e2µ

π~2. (253)

If the chemical potential µ grows, the linear increase eventually changes to a sharp decrease. This happenswhen the chemical potential becomes larger than the low-energy VHS energy. After this, D starts increasingagain until µ reaches the next VHS, where D(µ) also has a dip, and so on. The function D(µ) never exceedstwice of its value for single-layer graphene for any µ.

The situation changes drastically for angles θ < θc. In this case, the Drude weight at low µ increasesinitially much faster than 2D0(µ), but then, at larger values of µ (about the width of the peak in the DOSexisting at θ < θc), it drops down to almost zero, indicating the existence of a flat band at low energies.At some twist angles, the Drude weight vanishes completely and the transport gap exists in the system atnon-zero µ.

Experimental data for interlayer conductivity as a function of θ for a tBLG sample was reported recentlyin Ref. [449]. The measured room-temperature conductivity demonstrated pronounced peaks at θ = 21.8

and θ = 38.2. It is easy to check that the former angle corresponds to the (1, 1) structure with the smallestpossible supercell size, the latter angle is for the (1, 3) structure, which is conjugate to (1, 1).

13.5.2. Plasmons

Knowledge of the imaginary part of the dynamical conductivity allows, in particular, to calculate theplasmon excitation spectrum in twisted bilayer. This was done in Ref. [344] in the random-phase approx-imation. The plasmon spectrum is derived from the solution of the equation ε(k, ω) = 0, where ε(k, ω) isthe dielectric function. The RPA result for the tBLG is [344]

ε(k, ω) = 1 +2πi

εs

|k|ωσ(ω) , (254)

where εs is the dielectric constant of the substrate. When the chemical potential lies below the low-energyVHS, the real part of the conductivity is strongly suppressed in the frequency range 0 < ω < 2µ [seeFig. 55(e)], Reσreg(ω) ≈ 0. Thus, well defined (low damped) plasmons can exist at these frequencies. At

115

Figure 58: (Color online) The interlayer RC-circuit equilibration rate, τRC , versus twist angle, calculated for slightly dopedtBLG samples with an excess electron density n = 5× 1012 cm−2 and εF /~τ = 3, where εF is the Fermi energy, and τ is theparticle’s lifetime due to scattering on impurities. Reprinted figure with permission from R. Bistritzer and A. H. MacDonald,Phys. Rev. B, 81, 245412 (2010). Copyright 2010 by the American Physical Society. http://dx.doi.org/10.1103/PhysRevB.

81.245412.

small frequencies, one can use the expansion Imσ(ω) ≈ D/ω, and obtain from Eq. (254) the followingdispersion relation for this type of plasmons

ωp(k) ∼=

√2πD|k|εs

, (255)

where D is given by Eq. (253). In general, the real part of the conductivity is non-zero, and the plasmonshave a non-zero damping. The dispersion relation in this case is determined from the peak in the lossfunction

S(k, ω) = − Im[1/ε(k, ω)] .

The authors [344] discussed different types of plasmonic excitations in twisted bilayers, in particular, “trans-verse plasmons” mentioned in Section 12.

13.5.3. Interlayer conductivity

Interlayer transport has been studied by R. Bistritzer and A. H. MacDonald [444] in the low-energyapproximation. The authors considered both linear and non-linear regimes. The current I, flowing betweentwo layers with a non-zero potential difference V , was found using second-order perturbation theory inpowers of the interlayer coupling. Both commensurate and incommensurate structures were discussed. Inthe linear regime, one can introduce the conductance G = [I(V )/V ]V→0, and the time constant τRC of theeffective resistor-capacitor circuit (RC-circuit) corresponding to the bilayer,

τRC = S/(4πGc0) ∼= 0.027S/G ,

where S is the sample’s area and c0 ∼= 3.3 A is the interlayer distance. The rate 1/τRC ∝ G as a function of thetwist angle is shown in Fig. 58. The conductance depends substantially on θ: it increases for commensurateangles. For example, the curve in Fig. 58 shows six maxima corresponding to the superstructures (2, 1)(θ ∼= 13.2), (1, 1) (θ ∼= 21.8), (2, 3) (θ ∼= 27.8), (1, 2) (θ ∼= 32.2), (1, 3) (θ ∼= 38.2), and (1, 6) (θ ∼= 46.8).

116

(a)

(c)

E/EvHs

(b)

Figure 59: (Color online) Klein tunneling in twisted bilayer graphene. (a) Schematic diagram of the system. The electron withenergy E tunnels through the potential barrier of height U0 = E + ∆U and width D in the x direction. The barrier is infinitealong the y direction. (b) Transmission probability of the normally-incident electrons versus incident energy E, calculatedfor different values of ∆U . (c) Transmission probability as a function of ∆U calculated for three values of the energy of theincident electrons. Reprinted figures with permission from W.-Y. He et al., Phys. Rev. Lett., 111, 066803 (2013). Copyright2013 by the American Physical Society. http://dx.doi.org/10.1103/PhysRevLett.111.066803.

Reference [444] also considered a non-linear regime, and calculated the IV characteristics for different twistangles. The IV curves are very sensitive to the commensuration of the underlying structure. In particular,at small bias voltage, the current for commensurate angles is several orders of magnitude larger than thatfor close incommensurate angles. For larger V , a region of negative differential conductance exists forcommensurate angles, whereas for incommensurate angles the value of dI/dV is always positive.

13.5.4. Klein tunneling

The transmission probability of the tunneling through the potential barrier in twisted bilayer graphenewas calculated by W.-Y. He et al. in Ref. [450]. The authors used a simple 2× 2 model Hamiltonian givenby Eq. (185). The potential barrier has a rectangular shape. It is infinite in the y direction and has awidth D in the x direction [see Fig. 59(a)]. Despite the simplicity of the model Hamiltonian, no analyticalexpression was derived for the transmission probability T . They [450] calculated T as a function of theincident angle ϕ, energy of incident electrons E, and the height of the barrier U0. Analyzing the dependenceT = T (ϕ), the authors revealed the existence of angles, at which T = 1. Such a behavior is similar to thatfor single-layer graphene, as well as for AA- and AB-stacked bilayers, as we discussed in subsection 4.2. Thetransmission probability of normally-incident electrons, ϕ = 0, as a function of the electron energy is shownin Fig. 59(b). At small energies, T is nearly 1 as in the case of single-layer graphene or AA-stacked bilayergraphene. When E increases, T (E) exhibits several oscillations and then vanishes at higher energies. It wasnoted [450] that the normal tunneling becomes zero for E > 2EvHs, where EvHs is the energy of the VHS.

117

Thus, at high energies the twisted bilayer behaves as a Bernal-stacked bilayer. They [450] also analyzed thebehavior of the transmission probability T as a function of barrier’s height. Figure 59(c) presents the resultsfor the normal transmission probability as a function of the parameter ∆U = U0 − E. The transmissionprobability oscillates with ∆U , which can be explained by a geometrical resonance. The period of suchoscillations scales as 1/D. It is interesting that at relatively high energies the tunneling is suppressed insome region of ∆U near ∆U = 0. The authors [450] attribute this fact to the absence of propagating wavesolutions to the Schrodinger equation inside the barrier when ∆U is close to zero.

14. Conclusions

Bilayers of graphene are interesting objects for further investigations. Their electronic properties arestacking-dependent, and, in many ways, differ from those of the single-layer graphene. The bilayers have anumber electronic and electrodynamic features, which may be of importance for fundamental research andpossible applications.

The bilayers are studied intensively in recent years. In 2014 and in the first half of 2015 only, more than1100 papers on this subject were published. However, despite significant efforts, several problems concerningthe electronic properties of the graphene bilayers are still unsolved. For example, we discussed the issuesrelated to identification of ordered states in AB bilayer graphene and a gap in its electronic spectrum.Different theoretical approaches predict different results. Moreover, experimental observations of the gapopening are also controversial in many cases. Whether these discrepancies are due to the sample quality orthe reasons lie in the intrinsic properties of the bilayer graphene is not clear.

Naturally, we are unable to overview here all questions concerning the properties of graphene bilayers.Analysis of effects of dopants, adsorbed atoms, special substrates and change in chemical composition ofthe layers is the next step in the study of bilayer graphene-based systems. In this review we have restrictedourselves to pure carbon bilayer graphene. We also presented here only a brief discussion of some specificfields (for example, photonics) referring the interested reader to recent reviews on these subjects.

Acknowledgements

We acknowledge partial support of the Russian Science Support Foundation, RFBR Grant No. 15-02-02128. FN is partially supported by the RIKEN iTHES Project, MURI Center for Dynamic Magneto-Opticsvia the AFOSR award number FA9550-14-1-0040, the Impact Program of JST, and a Grant-in-Aid forScientific Research (A), and a grant from the John Templeton Foundation. We are grateful to Ya. Rodionovfor his help with figures.

118

References

[1] K. Novoselov, A. Geim, S. Morozov, D. Jiang, Y. Zhang, S. Dubonos, I. Grigorieva, and A. Firsov, “Electric field effectin atomically thin carbon films,” Science 306, 666 (2004).

[2] Z. Liu, K. Suenaga, P. J. F. Harris, and S. Iijima, “Open and Closed Edges of Graphene Layers,” Phys. Rev. Lett. 102,015501 (2009).

[3] J. M. B. Lopes dos Santos, N. M. R. Peres, and A. H. Castro Neto, “Graphene Bilayer with a Twist: Electronic Structure,”Phys. Rev. Lett. 99, 256802 (2007).

[4] A. H. Castro Neto, F. Guinea, N. M. R. Peres, K. S. Novoselov, and A. K. Geim, “The electronic properties of graphene,”Rev. Mod. Phys. 81, 109 (2009).

[5] E. McCann and M. Koshino, “The electronic properties of bilayer graphene,” Rep. Prog. Phys. 76, 056503 (2013).[6] I. Brihuega, P. Mallet, H. Gonzalez-Herrero, G. Trambly de Laissardiere, M. M. Ugeda, L. Magaud, J. M. Gomez-

Rodrıguez, F. Yndurain, and J.-Y. Veuillen, “Unraveling the Intrinsic and Robust Nature of van Hove Singularities inTwisted Bilayer Graphene by Scanning Tunneling Microscopy and Theoretical Analysis,” Phys. Rev. Lett. 109, 196802(2012).

[7] P. L. de Andres, R. Ramırez, and J. A. Verges, “Strong covalent bonding between two graphene layers,” Phys. Rev. B77, 045403 (2008).

[8] Y. Shibuta and J. A. Elliott, “Interaction between two graphene sheets with a turbostratic orientational relationship,”Chem. Phys. Lett. 512, 146 (2011).

[9] M. S. Alam, J. Lin, and M. Saito, “First-Principles Calculation of the Interlayer Distance of the Two-Layer Graphene,”Jpn. J. Appl. Phys. 50, 080213 (2011).

[10] Z. Xu, X. Li, B. I. Yakobson, and F. Ding, “Interaction between graphene layers and the mechanisms of graphite’ssuperlubricity and self-retraction,” Nanoscale 5, 6736 (2013).

[11] J. Berashevich and T. Chakraborty, “On the Nature of Interlayer Interactions in a System of Two Graphene Fragments,”J. Phys. Chem. C 115, 24666 (2011).

[12] S. Das Sarma, S. Adam, E. H. Hwang, and E. Rossi, “Electronic transport in two-dimensional graphene,” Rev. Mod.Phys. 83, 407 (2011).

[13] H. Yan, “Bilayer graphene: physics and application outlook in photonics,” Nanophotonics 4 (2014).[14] T. Stauber, “Plasmonics in Dirac systems: from graphene to topological insulators,” J. Phys.: Condens. Matter 26,

123201 (2014).[15] M. Glazov and S. Ganichev, “High frequency electric field induced nonlinear effects in graphene,” Phys. Rep. 535, 101

(2014).[16] E. J. Mele, “Interlayer coupling in rotationally faulted multilayer graphenes,” J. Phys. D: Appl. Phys. 45, 154004 (2012).[17] D. Abergel, V. Apalkov, J. Berashevich, K. Ziegler, and T. Chakraborty, “Properties of graphene: a theoretical perspec-

tive,” Adv. Phys. 59, 261 (2010).[18] A. Rozhkov, G. Giavaras, Y. P. Bliokh, V. Freilikher, and F. Nori, “Electronic properties of mesoscopic graphene

structures: Charge confinement and control of spin and charge transport,” Phys. Rep. 503, 77 (2011).[19] P. Avouris, Z. Chen, and V. Perebeinos, “Carbon-based electronics,” Nat. Nanotechnol. 2, 605 (2007).[20] J.-K. Lee, S.-C. Lee, J.-P. Ahn, S.-C. Kim, J. I. B. Wilson, and P. John, “The growth of AA graphite on (111) diamond,”

J. Chem. Phys. 129, 234709 (2008).[21] P. Lauffer, K. V. Emtsev, R. Graupner, T. Seyller, L. Ley, S. A. Reshanov, and H. B. Weber, “Atomic and electronic

structure of few-layer graphene on SiC(0001) studied with scanning tunneling microscopy and spectroscopy,” Phys. Rev.B 77, 155426 (2008).

[22] J. Borysiuk, J. Soltys, and J. Piechota, “Stacking sequence dependence of graphene layers on SiC (0001) - Experimentaland theoretical investigation,” J. Appl. Phys. 109, 093523 (2011).

[23] J. Martin, B. E. Feldman, R. T. Weitz, M. T. Allen, and A. Yacoby, “Local Compressibility Measurements of CorrelatedStates in Suspended Bilayer Graphene,” Phys. Rev. Lett. 105, 256806 (2010).

[24] K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, M. I. Katsnelson, I. V. Grigorieva, S. V. Dubonos, and A. A.Firsov, “Two-dimensional gas of massless Dirac fermions in graphene,” Nature 438, 197 (2005).

[25] K. Bolotin, K. Sikes, Z. Jiang, M. Klima, G. Fudenberg, J. Hone, P. Kim, and H. Stormer, “Ultrahigh electron mobilityin suspended graphene,” Solid State Commun. 146, 351 (2008).

[26] A. S. Mayorov, D. C. Elias, M. Mucha-Kruczynski, R. V. Gorbachev, T. Tudorovskiy, A. Zhukov, S. V. Morozov, M. I.Katsnelson, V. I. Fal’ko, A. K. Geim, et al., “Interaction-Driven Spectrum Reconstruction in Bilayer Graphene,” Science333, 860 (2011).

[27] B. E. Feldman, J. Martin, and A. Yacoby, “Broken-symmetry states and divergent resistance in suspended bilayergraphene,” Nat. Phys. 5, 889 (2009).

[28] W. Bao, J. Velasco, F. Zhang, L. Jing, B. Standley, D. Smirnov, M. Bockrath, A. H. MacDonald, and C. N. Lau,“Evidence for a spontaneous gapped state in ultraclean bilayer graphene,” PNAS 109, 10802 (2012).

[29] S. V. Morozov, K. S. Novoselov, M. I. Katsnelson, F. Schedin, D. C. Elias, J. A. Jaszczak, and A. K. Geim, “Giantintrinsic carrier mobilities in graphene and its bilayer,” Phys. Rev. Lett. 100, 016602 (2008).

[30] J. B. Oostinga, H. B. Heersche, X. Liu, A. F. Morpurgo, and L. M. K. Vandersypen, “Gate-induced insulating state inbilayer graphene devices,” Nat. Mater. 7, 151 (2008).

[31] C. Dean, A. Young, I. Meric, C. Lee, L. Wang, S. Sorgenfrei, K. Watanabe, T. Taniguchi, P. Kim, K. Shepard, et al.,“Boron nitride substrates for high-quality graphene electronics,” Nat. Nanotechnol. 5, 722 (2010).

119

[32] J. Velasco Jr., L. Jing, W. Bao, Y. Lee, P. Kratz, V. Aji, M. Bockrath, C. Lau, C. Varma, R. Stillwell, et al., “Transportspectroscopy of symmetry-broken insulating states in bilayer graphene,” Nat. Nanotechnol. 7, 156 (2012).

[33] H. J. van Elferen, A. Veligura, E. V. Kurganova, U. Zeitler, J. C. Maan, N. Tombros, I. J. Vera-Marun, and B. J. vanWees, “Field-induced quantum Hall ferromagnetism in suspended bilayer graphene,” Phys. Rev. B 85, 115408 (2012).

[34] G. W. Semenoff, “Condensed-Matter Simulation of a Three-Dimensional Anomaly,” Phys. Rev. Lett. 53, 2449 (1984).[35] J. P. Hobson and W. A. Nierenberg, “The Statistics of a Two-Dimensional, Hexagonal Net,” Phys. Rev. 89, 662 (1953).[36] A. L. Rakhmanov, A. V. Rozhkov, A. O. Sboychakov, and F. Nori, “Instabilities of the AA-Stacked Graphene Bilayer,”

Phys. Rev. Lett. 109, 206801 (2012).[37] J.-C. Charlier, J.-P. Michenaud, and X. Gonze, “First-principles study of the electronic properties of simple hexagonal

graphite,” Phys. Rev. B 46, 4531 (1992).[38] N. B. Brandt, S. M. Chudinov, and Y. G. Ponomarev, Modern Problems in Condensed Matter Sciences, vol. 20.1

(North-Holland, Amsterdam, 1988).[39] M. S. Dresselhaus and G. Dresselhaus, “Intercalation compounds of graphite,” Adv. Phys. 51, 1 (2002).[40] S. Reich, J. Maultzsch, C. Thomsen, and P. Ordejon, “Tight-binding description of graphene,” Phys. Rev. B 66, 035412

(2002).[41] R. S. Deacon, K.-C. Chuang, R. J. Nicholas, K. S. Novoselov, and A. K. Geim, “Cyclotron resonance study of the electron

and hole velocity in graphene monolayers,” Phys. Rev. B 76, 081406(R) (2007).[42] H. J. Xiang, E. J. Kan, S.-H. Wei, X. G. Gong, and M.-H. Whangbo, “Thermodynamically stable single-side hydrogenated

graphene,” Phys. Rev. B 82, 165425 (2010).[43] B. S. Pujari, S. Gusarov, M. Brett, and A. Kovalenko, “Single-side-hydrogenated graphene: Density functional theory

predictions,” Phys. Rev. B 84, 041402 (2011).[44] L. Openov and A. Podlivaev, “Insulator band gap in single-side-hydrogenated graphene nanoribbons,” Semiconductors

46, 199 (2012).[45] R. S. Akzyanov, A. O. Sboychakov, A. V. Rozhkov, A. L. Rakhmanov, and F. Nori, “AA-stacked bilayer graphene in

an applied electric field: Tunable antiferromagnetism and coexisting exciton order parameter,” Phys. Rev. B 90, 155415(2014).

[46] E. A. Henriksen and J. P. Eisenstein, “Measurement of the electronic compressibility of bilayer graphene,” Phys. Rev. B82, 041412 (2010).

[47] L. M. Malard, J. Nilsson, D. C. Elias, J. C. Brant, F. Plentz, E. S. Alves, A. H. Castro Neto, and M. A. Pimenta,“Probing the electronic structure of bilayer graphene by Raman scattering,” Phys. Rev. B 76, 201401 (2007).

[48] L. M. Zhang, Z. Q. Li, D. N. Basov, M. M. Fogler, Z. Hao, and M. C. Martin, “Determination of the electronic structureof bilayer graphene from infrared spectroscopy,” Phys. Rev. B 78, 235408 (2008).

[49] Z. Q. Li, E. A. Henriksen, Z. Jiang, Z. Hao, M. C. Martin, P. Kim, H. L. Stormer, and D. N. Basov, “Band StructureAsymmetry of Bilayer Graphene Revealed by Infrared Spectroscopy,” Phys. Rev. Lett. 102, 037403 (2009).

[50] E. McCann and V. I. Fal’ko, “Landau-Level Degeneracy and Quantum Hall Effect in a Graphite Bilayer,” Phys. Rev.Lett. 96, 086805 (2006).

[51] A. B. Kuzmenko, I. Crassee, D. van der Marel, P. Blake, and K. S. Novoselov, “Determination of the gate-tunable bandgap and tight-binding parameters in bilayer graphene using infrared spectroscopy,” Phys. Rev. B 80, 165406 (2009).

[52] J.-C. Charlier, X. Gonze, and J.-P. Michenaud, “First-principles study of the electronic properties of graphite,” Phys.Rev. B 43, 4579 (1991).

[53] D. L. Mafra, L. M. Malard, S. K. Doorn, H. Htoon, J. Nilsson, A. H. Castro Neto, and M. A. Pimenta, “Observation ofthe Kohn anomaly near the K point of bilayer graphene,” Phys. Rev. B 80, 241414 (2009).

[54] A. B. Kuzmenko, E. van Heumen, D. van der Marel, P. Lerch, P. Blake, K. S. Novoselov, and A. K. Geim, “Infraredspectroscopy of electronic bands in bilayer graphene,” Phys. Rev. B 79, 115441 (2009).

[55] K. Zou, X. Hong, and J. Zhu, “Effective mass of electrons and holes in bilayer graphene: Electron-hole asymmetry andelectron-electron interaction,” Phys. Rev. B 84, 085408 (2011).

[56] E. McCann, “Asymmetry gap in the electronic band structure of bilayer graphene,” Phys. Rev. B 74, 161403 (2006).[57] T. Ohta, A. Bostwick, T. Seyller, K. Horn, and E. Rotenberg, “Controlling the electronic structure of bilayer graphene,”

Science 313, 951 (2006).[58] E. V. Castro, K. S. Novoselov, S. V. Morozov, N. M. R. Peres, J. M. B. Lopes dos Santos, J. Nilsson, F. Guinea, A. K.

Geim, and A. H. Castro Neto, “Biased bilayer graphene: Semiconductor with a gap tunable by the electric field effect,”Phys. Rev. Lett. 99, 216802 (2007).

[59] L. Jing, J. Velasco Jr., Ph. Kratz, G. Liu, W. Bao, M. Bockrath, and Ch. N. Lau, “Quantum Transport and Field-InducedInsulating States in Bilayer Graphene pnp Junctions,” Nano Lett. 10, 4000 (2010).

[60] Y. Hao, L. Wang, Y. Liu, H. Chen, X. Wang, C. Tan, S. Nie, J. W. Suk, T. Jiang, T. Liang, et al., “Oxygen-activatedgrowth and bandgap tunability of large single-crystal bilayer graphene,” Nat. Nano. 11, 426 (2016).

[61] B. R. K. Nanda and S. Satpathy, “Strain and electric field modulation of the electronic structure of bilayer graphene,”Phys. Rev. B 80, 165430 (2009).

[62] J. Slawinska, I. Zasada, and Z. Klusek, “Energy gap tuning in graphene on hexagonal boron nitride bilayer system,”Phys. Rev. B 81, 155433 (2010).

[63] A. Ramasubramaniam, D. Naveh, and E. Towe, “Tunable Band Gaps in Bilayer Graphene-BN Heterostructures,” NanoLett. 11, 1070 (2011).

[64] E. V. Castro, M. P. Lopez-Sancho, and M. A. H. Vozmediano, “Pinning and switching of magnetic moments in bilayergraphene,” New J. Phys. 11, 095017 (2009).

[65] E. V. Castro, N. M. R. Peres, and J. M. B. Lopes dos Santos, “Gaped graphene bilayer: disorder and magnetic field

120

effects,” Phys. Status Solidi (b) 244, 2311 (2007).[66] E. V. Castro, K. S. Novoselov, S. V. Morozov, N. M. R. Peres, J. M. B. Lopes dos Santos, J. Nilsson, F. Guinea, A. K.

Geim, and A. H. Castro Neto, “Electronic properties of a biased graphene bilayer,” J. Phys.: Condens. Matter 22, 175503(2010).

[67] N. Nemec and G. Cuniberti, “Hofstadter butterflies of bilayer graphene,” Phys. Rev. B 75, 201404 (2007).[68] S.-M. Choi, S.-H. Jhi, and Y.-W. Son, “Controlling Energy Gap of Bilayer Graphene by Strain,” Nano Lett. 10, 3486

(2010).[69] M. Mucha-Kruczynski, I. L. Aleiner, and V. I. Fal’ko, “Strained bilayer graphene: Band structure topology and Landau

level spectrum,” Phys. Rev. B 84, 041404 (2011).[70] A. Rycerz, J. Tworzyd lo, and C. Beenakker, “Valley filter and valley valve in graphene,” Nat. Phys. 3, 172 (2007).[71] Y. Shimazaki, M. Yamamoto, I. V. Borzenets, K. Watanabe, T. Taniguchi, and S. Tarucha, “Generation and detection

of pure valley current by electrically induced Berry curvature in bilayer graphene,” Nat. Phys. 11, 1032 (2015).[72] M. Sanderson, Y. S. Ang, and C. Zhang, “Klein tunneling and cone transport in AA-stacked bilayer graphene,” Phys.

Rev. B 88, 245404 (2013).[73] A. O. Sboychakov, A. V. Rozhkov, A. L. Rakhmanov, and F. Nori, “Antiferromagnetic states and phase separation in

doped AA-stacked graphene bilayers,” Phys. Rev. B 88, 045409 (2013).[74] M. I. Katsnelson, K. S. Novoselov, and A. K. Geim, “Chiral tunnelling and the Klein paradox in graphene,” Nat. Phys.

2, 620 (2006).[75] V. V. Cheianov, V. Fal’ko, and B. L. Altshuler, “The Focusing of Electron Flow and a Veselago Lens in Graphene p-n

Junctions,” Science 315, 1252 (2007).[76] Y. P. Bliokh, V. Freilikher, S. Savel’ev, and F. Nori, “Transport and localization in periodic and disordered graphene

superlattices,” Phys. Rev. B 79, 075123 (2009).[77] V. A. Yampol’skii, S. S. Apostolov, Z. A. Maizelis, A. Levchenko, and F. Nori, “Voltage-driven quantum oscillations of

conductance in graphene,” EPL 96, 67009 (2011).[78] V. A. Yampol’skii, S. Savel’ev, and F. Nori, “Voltage-driven quantum oscillations in graphene,” New J. Phys. 10, 053024

(2008).[79] T. Tudorovskiy, K. J. A. Reijnders, and M. I. Katsnelson, “Chiral tunneling in single-layer and bilayer graphene,” Phys.

Scripta 2012, 014010 (2012).[80] M. M. Fogler, D. S. Novikov, L. I. Glazman, and B. I. Shklovskii, “Effect of disorder on a graphene p-n junction,” Phys.

Rev. B 77, 075420 (2008).[81] D. Wang and G. Jin, “Tunneling magnetoresistance tuned by a vertical electric field in an AA-stacked graphene bilayer

with double magnetic barriers,” J. Appl. Phys. 114, 233701 (2013).[82] K. S. Novoselov, Z. Jiang, Y. Zhang, S. V. Morozov, H. L. Stormer, U. Zeitler, J. C. Maan, G. S. Boebinger, P. Kim,

and A. K. Geim, “Room-Temperature Quantum Hall Effect in Graphene,” Science 315, 1379 (2007).[83] A. H. MacDonald, ed., Quantum Hall Effect: A Perspective (Kluwer, Boston MA, 1989).[84] Y. Zhang, Y.-W. Tan, H. L. Stormer, and P. Kim, “Experimental observation of the quantum Hall effect and Berry’s

phase in graphene,” Nature 438, 201 (2005).[85] Y.-F. Hsu and G.-Y. Guo, “Anomalous integer quantum Hall effect in AA-stacked bilayer graphene,” Phys. Rev. B 82,

165404 (2010).[86] Y.-H. Ho, J.-Y. Wu, R.-B. Chen, Y.-H. Chiu, and M.-F. Lin, “Optical transitions between Landau levels: AA-stacked

bilayer graphene,” Appl. Phys. Lett. 97, 101905 (2010).[87] D. Wang, “Electric- and magnetic-field-tuned Landau levels and Hall conductivity in AA-stacked bilayer graphene,”

Phys. Lett. A 375, 4070 (2011).[88] S.-J. Tsai, Y.-H. Chiu, Y.-H. Ho, and M.-F. Lin, “Gate-voltage-dependent Landau levels in AA-stacked bilayer graphene,”

Chem. Phys. Lett. 550, 104 (2012).[89] D. Wang and G. Jin, “Effect of a nonuniform magnetic field on the Landau states in a biased AA-stacked graphene

bilayer,” Phys. Lett. A 377, 2901 (2013).[90] G. D. Mahan, Many Particle Physics (Plenum, New York, 1990).[91] J. Pereira, J. Milton, F. M. Peeters, and P. Vasilopoulos, “Landau levels and oscillator strength in a biased bilayer of

graphene,” Phys. Rev. B 76, 115419 (2007).[92] Y. H. Lai, J. H. Ho, C. P. Chang, and M. F. Lin, “Magnetoelectronic properties of bilayer Bernal graphene,” Phys. Rev.

B 77, 085426 (2008).[93] B. Partoens and F. M. Peeters, “From graphene to graphite: Electronic structure around the K point,” Phys. Rev. B

74, 075404 (2006).[94] A. Gruneis, C. Attaccalite, L. Wirtz, H. Shiozawa, R. Saito, T. Pichler, and A. Rubio, “Tight-binding description of the

quasiparticle dispersion of graphite and few-layer graphene,” Phys. Rev. B 78, 205425 (2008).[95] L. M. Zhang, M. M. Fogler, and D. P. Arovas, “Magnetoelectric coupling, Berry phase, and Landau level dispersion in a

biased bilayer graphene,” Phys. Rev. B 84, 075451 (2011).[96] A. Y. Ozerin and L. A. Falkovsky, “Berry phase, semiclassical quantization, and Landau levels,” Phys. Rev. B 85, 205143

(2012).[97] L. A. Falkovsky, “Magneto-optics of monolayer and bilayer graphene,” JETP Lett. 97, 429 (2013).[98] G. Li and E. Y. Andrei, “Observation of Landau levels of Dirac fermions in graphite,” Nat. Phys. 3, 623 (2007).[99] K.-C. Chuang, A. M. R. Baker, and R. J. Nicholas, “Magnetoabsorption study of Landau levels in graphite,” Phys. Rev.

B 80, 161410 (2009).[100] T. Morimoto, M. Koshino, and H. Aoki, “Faraday rotation in bilayer and trilayer graphene in the quantum Hall regime,”

121

Phys. Rev. B 86, 155426 (2012).[101] L. A. Falkovsky, “Quantum magneto-optics of graphite with trigonal warping,” Phys. Rev. B 84, 115414 (2011).[102] S. Berciaud, M. Potemski, and C. Faugeras, “Probing Electronic Excitations in Mono- to Pentalayer Graphene by Micro

Magneto-Raman Spectroscopy,” Nano Lett. 14, 4548 (2014).[103] D. Wang and G. Jin, “Combined effect of magnetic and electric fields on Landau level spectrum and magneto-optical

absorption in bilayer graphene,” Europhys. Lett. 92, 57008 (2010).[104] E. A. Henriksen, Z. Jiang, L.-C. Tung, M. E. Schwartz, M. Takita, Y.-J. Wang, P. Kim, and H. L. Stormer, “Cyclotron

resonance in bilayer graphene,” Phys. Rev. Lett. 100, 087403 (2008).[105] K. Lee, B. Fallahazad, J. Xue, D. C. Dillen, K. Kim, T. Taniguchi, K. Watanabe, and E. Tutuc, “Chemical potential

and quantum Hall ferromagnetism in bilayer graphene,” Science 345, 58 (2014).[106] J. Velasco, Y. Lee, Z. Zhao, L. Jing, P. Kratz, M. Bockrath, and C. N. Lau, “Transport Measurement of Landau Level

Gaps in Bilayer Graphene with Layer Polarization Control,” Nano Lett. 14, 1324 (2014).[107] Y.-H. Hyun, Y. Kim, C. Sochichiu, and M.-Y. Choi, “Landau level spectrum for bilayer graphene in a tilted magnetic

field,” J. Phys.: Condens. Matter 24, 045501 (2012).[108] T. Kawarabayashi, Y. Hatsugai, and H. Aoki, “Topologically protected Landau levels in bilayer graphene in finite electric

fields,” Phys. Rev. B 85, 165410 (2012).[109] M. Koshino and T. Ando, “Magneto-optical properties of multilayer graphene,” Phys. Rev. B 77, 115313 (2008).[110] Y.-H. Ho, Y.-H. Chiu, D.-H. Lin, C.-P. Chang, and M.-F. Lin, “Magneto-optical Selection Rules in Bilayer Bernal

Graphene,” ACS Nano 4, 1465 (2010).[111] K. S. Novoselov, E. McCann, S. V. Morozov, V. I. Fal’ko, M. I. Katsnelson, U. Zeitler, D. Jiang, F. Schedin, and A. K.

Geim, “Unconventional quantum Hall effect and Berry’s phase of 2π in bilayer graphene,” Nat. Phys. 2, 177 (2006).[112] M. Nakamura, L. Hirasawa, and K.-I. Imura, “Quantum Hall effect in bilayer and multilayer graphene with finite Fermi

energy,” Phys. Rev. B 78, 033403 (2008).[113] X. Du, I. Skachko, F. Duerr, A. Luican, and E. Y. Andrei, “Fractional quantum Hall effect and insulating phase of Dirac

electrons in graphene,” Nature 462, 192 (2009).[114] K. I. Bolotin, F. Ghahari, M. D. Shulman, H. L. Stormer, and P. Kim, “Observation of the fractional quantum Hall effect

in graphene,” Nature 462, 196 (2009).[115] C. R. Dean, A. F. Young, P. Cadden-Zimansky, L. Wang, H. Ren, K. Watanabe, T. Taniguchi, P. Kim, J. Hone, and

K. L. Shepard, “Multicomponent fractional quantum Hall effect in graphene,” Nat. Phys. 7, 693 (2011).[116] W. Bao, Z. Zhao, H. Zhang, G. Liu, P. Kratz, L. Jing, J. Velasco, D. Smirnov, and C. N. Lau, “Magnetoconductance

Oscillations and Evidence for Fractional Quantum Hall States in Suspended Bilayer and Trilayer Graphene,” Phys. Rev.Lett. 105, 246601 (2010).

[117] A. Kou, B. E. Feldman, A. J. Levin, B. I. Halperin, K. Watanabe, T. Taniguchi, and A. Yacoby, “Electron-hole asymmetricinteger and fractional quantum Hall effect in bilayer graphene,” Science 345, 55 (2014).

[118] D.-K. Ki, V. I. Fal’ko, D. A. Abanin, and A. F. Morpurgo, “Observation of Even Denominator Fractional Quantum HallEffect in Suspended Bilayer Graphene,” Nano Lett. 14, 2135 (2014).

[119] N. Shibata and K. Nomura, “Fractional Quantum Hall Effects in Graphene and Its Bilayer,” J. Phys. Soc. Japan 78,104708 (2009).

[120] Z. Papic and D. A. Abanin, “Topological Phases in the Zeroth Landau Level of Bilayer Graphene,” Phys. Rev. Lett.112, 046602 (2014).

[121] V. M. Apalkov and T. Chakraborty, “Controllable Driven Phase Transitions in Fractional Quantum Hall States in BilayerGraphene,” Phys. Rev. Lett. 105, 036801 (2010).

[122] Z. Papic, R. Thomale, and D. A. Abanin, “Tunable Electron Interactions and Fractional Quantum Hall States inGraphene,” Phys. Rev. Lett. 107, 176602 (2011).

[123] Z. Papic, D. A. Abanin, Y. Barlas, and R. N. Bhatt, “Tunable interactions and phase transitions in Dirac materials in amagnetic field,” Phys. Rev. B 84, 241306 (2011).

[124] V. M. Apalkov and T. Chakraborty, “Stable Pfaffian State in Bilayer Graphene,” Phys. Rev. Lett. 107, 186803 (2011).[125] K. Snizhko, V. Cheianov, and S. H. Simon, “Importance of interband transitions for the fractional quantum Hall effect

in bilayer graphene,” Phys. Rev. B 85, 201415 (2012).[126] P. Maher, L. Wang, Y. Gao, C. Forsythe, T. Taniguchi, K. Watanabe, D. Abanin, Z. Papic, P. Cadden-Zimansky, J. Hone,

et al., “Tunable fractional quantum Hall phases in bilayer graphene,” Science 345, 61 (2014).[127] S. Geraedts, M. P. Zaletel, Z. Papic, and R. S. K. Mong, “Competing Abelian and non-Abelian topological orders in

ν = 1/3 + 1/3 quantum Hall bilayers,” Phys. Rev. B 91, 205139 (2015).[128] D. S. L. Abergel and T. Chakraborty, “Long-Range Coulomb Interaction in Bilayer Graphene,” Phys. Rev. Lett. 102,

056807 (2009).[129] M. Kharitonov, “Canted Antiferromagnetic Phase of the ν=0 Quantum Hall State in Bilayer Graphene,” Phys. Rev.

Lett. 109, 046803 (2012).[130] M. Kharitonov, “Antiferromagnetic state in bilayer graphene,” Phys. Rev. B 86, 195435 (2012).[131] E. V. Gorbar, V. P. Gusynin, and V. A. Miransky, “Dynamics and phase diagram of the ν = 0 quantum Hall state in

bilayer graphene,” Phys. Rev. B 81, 155451 (2010).[132] E. V. Gorbar, V. P. Gusynin, J. Jia, and V. A. Miransky, “Broken-symmetry states and phase diagram of the lowest

Landau level in bilayer graphene,” Phys. Rev. B 84, 235449 (2011).[133] C. Toke and V. I. Fal’ko, “Intra-Landau-level magnetoexcitons and the transition between quantum Hall states in undoped

bilayer graphene,” Phys. Rev. B 83, 115455 (2011).[134] F. D. M. Haldane, “Model for a Quantum Hall Effect without Landau Levels: Condensed-Matter Realization of the

122

‘Parity Anomaly’,” Phys. Rev. Lett. 61, 2015 (1988).[135] C. L. Kane and E. J. Mele, “Quantum Spin Hall Effect in Graphene,” Phys. Rev. Lett. 95, 226801 (2005).[136] C. L. Kane and E. J. Mele, “Z2 Topological Order and the Quantum Spin Hall Effect,” Phys. Rev. Lett. 95, 146802

(2005).[137] C. Weeks, J. Hu, J. Alicea, M. Franz, and R. Wu, “Engineering a Robust Quantum Spin Hall State in Graphene via

Adatom Deposition,” Phys. Rev. X 1, 021001 (2011).[138] H. Zhang, C. Lazo, S. Blugel, S. Heinze, and Y. Mokrousov, “Electrically Tunable Quantum Anomalous Hall Effect in

Graphene Decorated by 5d Transition-Metal Adatoms,” Phys. Rev. Lett. 108, 056802 (2012).[139] Z. Qiao, S. A. Yang, W. Feng, W.-K. Tse, J. Ding, Y. Yao, J. Wang, and Q. Niu, “Quantum anomalous Hall effect in

graphene from Rashba and exchange effects,” Phys. Rev. B 82, 161414 (2010).[140] J. Ding, Z. Qiao, W. Feng, Y. Yao, and Q. Niu, “Engineering quantum anomalous/valley Hall states in graphene via

metal-atom adsorption: An ab-initio study,” Phys. Rev. B 84, 195444 (2011).[141] A. Varykhalov, J. Sanchez-Barriga, A. M. Shikin, C. Biswas, E. Vescovo, A. Rybkin, D. Marchenko, and O. Rader,

“Electronic and Magnetic Properties of Quasifreestanding Graphene on Ni,” Phys. Rev. Lett. 101, 157601 (2008).[142] Y. S. Dedkov, M. Fonin, U. Rudiger, and C. Laubschat, “Rashba Effect in the Graphene/Ni(111) System,” Phys. Rev.

Lett. 100, 107602 (2008).[143] O. Rader, A. Varykhalov, J. Sanchez-Barriga, D. Marchenko, A. Rybkin, and A. M. Shikin, “Is There a Rashba Effect

in Graphene on 3d Ferromagnets?,” Phys. Rev. Lett. 102, 057602 (2009).[144] A. Varykhalov and O. Rader, “Graphene grown on Co(0001) films and islands: Electronic structure and its precise

magnetization dependence,” Phys. Rev. B 80, 035437 (2009).[145] F. Guinea, “Spin-orbit coupling in a graphene bilayer and in graphite,” New J. Phys. 12, 083063 (2010).[146] R. van Gelderen and C. M. Smith, “Rashba and intrinsic spin-orbit interactions in biased bilayer graphene,” Phys. Rev.

B 81, 125435 (2010).[147] E. Prada, P. San-Jose, L. Brey, and H. A. Fertig, “Band topology and the quantum spin Hall effect in bilayer graphene,”

Solid State Commun. 151, 1075 (2011).[148] Z. Qiao, W.-K. Tse, H. Jiang, Y. Yao, and Q. Niu, “Two-Dimensional Topological Insulator State and Topological Phase

Transition in Bilayer Graphene,” Phys. Rev. Lett. 107, 256801 (2011).[149] F. Mireles and J. Schliemann, “Energy spectrum and Landau levels in bilayer graphene with spin-orbit interaction,” New

J. Phys. 14, 093026 (2012).[150] S. Konschuh, M. Gmitra, D. Kochan, and J. Fabian, “Theory of spin-orbit coupling in bilayer graphene,” Phys. Rev. B

85, 115423 (2012).[151] Z. Qiao, X. Li, W.-K. Tse, H. Jiang, Y. Yao, and Q. Niu, “Topological phases in gated bilayer graphene: Effects of

Rashba spin-orbit coupling and exchange field,” Phys. Rev. B 87, 125405 (2013).[152] X. Zhai and G. Jin, “Reversing Berry phase and modulating Andreev reflection by Rashba spin-orbit coupling in graphene

mono- and bilayers,” Phys. Rev. B 89, 085430 (2014).[153] A. Dyrda l and J. Barnas, “Spin Hall effect in AA-stacked bilayer graphene,” Solid State Commun. 188, 27 (2014).[154] W. Landgraf, S. Shallcross, K. Turschmann, D. Weckbecker, and O. Pankratov, “Electronic structure of twisted graphene

flakes,” Phys. Rev. B 87, 075433 (2013).[155] E. Suarez Morell, R. Vergara, M. Pacheco, L. Brey, and L. Chico, “Electronic properties of twisted bilayer nanoribbons,”

Phys. Rev. B 89, 205405 (2014).[156] Z. J. Qi, C. Daniels, S. J. Hong, Y. W. Park, V. Meunier, M. Drndic, and A. T. C. Johnson, “Electronic Transport of

Recrystallized Freestanding Graphene Nanoribbons,” ACS Nano 9, 3510 (2015).[157] B. Sahu, H. Min, and S. K. Banerjee, “Effects of magnetism and electric field on the energy gap of bilayer graphene

nanoflakes,” Phys. Rev. B 81, 045414 (2010).[158] B. Sahu, H. Min, A. H. MacDonald, and S. K. Banerjee, “Energy gaps, magnetism, and electric-field effects in bilayer

graphene nanoribbons,” Phys. Rev. B 78, 045404 (2008).[159] A. Matulis and F. M. Peeters, “Quasibound states of quantum dots in single and bilayer graphene,” Phys. Rev. B 77,

115423 (2008).[160] J. Pereira, J. Milton, P. Vasilopoulos, and F. M. Peeters, “Tunable quantum dots in bilayer graphene,” Nano Lett. 7,

946 (2007).[161] G. Giavaras and F. Nori, “Dirac gap-induced graphene quantum dot in an electrostatic potential,” Phys. Rev. B 83,

165427 (2011).[162] M. T. Allen, J. Martin, and A. Yacoby, “Gate-defined quantum confinement in suspended bilayer graphene,” Nat.

Commun. 3, 934 (2012).[163] A. S. M. Goossens, S. C. M. Driessen, T. A. Baart, K. Watanabe, T. Taniguchi, and L. M. K. Vandersypen, “Gate-Defined

Confinement in Bilayer Graphene-Hexagonal Boron Nitride Hybrid Devices,” Nano Lett. 12, 4656 (2012).[164] A. Muller, B. Kaestner, F. Hohls, T. Weimann, K. Pierz, and H. W. Schumacher, “Bilayer graphene quantum dot defined

by topgates,” J. Appl. Phys. 115, 233710 (2014).[165] A. De Martino, L. Dell’Anna, and R. Egger, “Magnetic Confinement of Massless Dirac Fermions in Graphene,” Phys.

Rev. Lett. 98, 066802 (2007).[166] G. Giavaras, P. A. Maksym, and M. Roy, “Magnetic field induced confinement-deconfinement transition in graphene

quantum dots,” J. Phys.: Condens. Matter 21, 102201 (2009).[167] G. Giavaras and F. Nori, “Tunable quantum dots in monolayer graphene,” Phys. Rev. B 85, 165446 (2012).[168] M. Zarenia, J. M. Pereira, F. M. Peeters, and G. A. Farias, “Electrostatically Confined Quantum Rings in Bilayer

Graphene,” Nano Lett. 9, 4088 (2009).

123

[169] L. J. P. Xavier, J. M. Pereira Jr., A. Chaves, G. A. Farias, and F. M. Peeters, “Topological confinement in graphenebilayer quantum rings,” Appl. Phys. Lett. 96, 212108 (2010).

[170] I. Martin, Y. M. Blanter, and A. F. Morpurgo, “Topological confinement in bilayer graphene,” Phys. Rev. Lett. 100,036804 (2008).

[171] S.-J. Sun and C. Chang, “Ballistic transport in bilayer nano-graphite ribbons under gate and magnetic fields,” Eur. Phys.J. B 64, 249 (2008).

[172] N. Xu, B. Wang, D. Shi, and C. Zhang, “Transport properties of AA-stacking bilayer graphene nanoribbons,” Solid StateCommun. 152, 994 (2012).

[173] J. W. Gonzalez, H. Santos, M. Pacheco, L. Chico, and L. Brey, “Electronic transport through bilayer graphene flakes,”Phys. Rev. B 81, 195406 (2010).

[174] M. M. Benameur, F. Gargiulo, S. Manzeli, G. Autes, M. Tosun, O. V. Yazyev, and A. Kis, “Electromechanical oscillationsin bilayer graphene,” Nat. Commun. 6 (2015).

[175] K. M. M. Habib, F. Zahid, and R. K. Lake, “Negative differential resistance in bilayer graphene nanoribbons,” Appl.Phys. Lett. 98, 192112 (2011).

[176] P. A. Maksimov, A. V. Rozhkov, and A. O. Sboychakov, “Localized electron states near the armchair edge of graphene,”Phys. Rev. B 88, 245421 (2013).

[177] E. V. Castro, N. M. R. Peres, J. M. B. Lopes dos Santos, A. H. Castro Neto, and F. Guinea, “Localized States at ZigzagEdges of Bilayer Graphene,” Phys. Rev. Lett. 100, 026802 (2008).

[178] A. Cortijo, L. Oroszlany, and H. Schomerus, “Fast and slow edges in bilayer graphene nanoribbons: Tuning the transitionfrom band to Mott insulator,” Phys. Rev. B 81, 235422 (2010).

[179] Z. Zhang, C. Chen, X. C. Zeng, and W. Guo, “Tuning the magnetic and electronic properties of bilayer graphenenanoribbons on Si(001) by bias voltage,” Phys. Rev. B 81, 155428 (2010).

[180] M. P. Lima, A. Fazzio, and A. J. R. da Silva, “Edge effects in bilayer graphene nanoribbons: Ab initio total-energydensity functional theory calculations,” Phys. Rev. B 79, 153401 (2009).

[181] A. R. Wright, J. C. Cao, and C. Zhang, “Enhanced Optical Conductivity of Bilayer Graphene Nanoribbons in theTerahertz Regime,” Phys. Rev. Lett. 103, 207401 (2009).

[182] X. Li, X. Wang, L. Zhang, S. Lee, and H. Dai, “Chemically Derived, Ultrasmooth Graphene Nanoribbon Semiconductors,”Science 319, 1229 (2008).

[183] H. Xu, T. Heinzel, and I. V. Zozoulenko, “Edge disorder and localization regimes in bilayer graphene nanoribbons,”Phys. Rev. B 80, 045308 (2009).

[184] M. Fujita, M. Igami, and K. Nakada, “Lattice distortion in nanographite ribbons,” J. Phys. Soc. Japan 66, 1864 (1997).[185] M. Zarea and N. Sandler, “Electron-electron and spin-orbit interactions in armchair graphene ribbons,” Phys. Rev. Lett.

99, 256804 (2007).[186] A. V. Rozhkov, S. Savel’ev, and F. Nori, “Electronic properties of armchair graphene nanoribbons,” Phys. Rev. B 79,

125420 (2009).[187] T. Li, C. Hsieh, S. Yang, and S. Chang, “Ballistic transport of bilayer graphene nanoribbons in a spatially modulated

magnetic field,” Solid State Commun. 206, 6 (2015).[188] M. Zarenia, J. Pereira, J. M., G. A. Farias, and F. M. Peeters, “Chiral states in bilayer graphene: Magnetic field

dependence and gap opening,” Phys. Rev. B 84, 125451 (2011).[189] A. Schroer, P. G. Silvestrov, and P. Recher, “Valley-based Cooper pair splitting via topologically confined channels in

bilayer graphene,” Phys. Rev. B 92, 241404 (2015).[190] Z. Qiao, J. Jung, Q. Niu, and A. H. MacDonald, “Electronic Highways in Bilayer Graphene,” Nano Lett. 11, 3453 (2011).[191] M. Killi, T.-C. Wei, I. Affleck, and A. Paramekanti, “Tunable Luttinger Liquid Physics in Biased Bilayer Graphene,”

Phys. Rev. Lett. 104, 216406 (2010).[192] F. Zhang, A. H. MacDonald, and E. J. Mele, “Valley Chern numbers and boundary modes in gapped bilayer graphene,”

PNAS 110, 10546 (2013).[193] A. Vaezi, Y. Liang, D. H. Ngai, L. Yang, and E.-A. Kim, “Topological Edge States at a Tilt Boundary in Gated Multilayer

Graphene,” Phys. Rev. X 3, 021018 (2013).[194] J. S. Alden, A. W. Tsen, P. Y. Huang, R. Hovden, L. Brown, J. Park, D. A. Muller, and P. L. McEuen, “Strain solitons

and topological defects in bilayer graphene,” PNAS 110, 11256 (2013).[195] L. Ju, Z. Shi, N. Nair, Y. Lv, C. Jin, J. Velasco Jr, C. Ojeda-Aristizabal, H. A. Bechtel, M. C. Martin, A. Zettl, et al.,

“Topological valley transport at bilayer graphene domain walls,” Nature 520, 650 (2015).[196] J. Li, I. Martin, M. Buttiker, and A. F. Morpurgo, “Topological origin of subgap conductance in insulating bilayer

graphene,” Nat. Phys. 7, 38 (2011).[197] R. Nandkishore and L. Levitov, “Common-path interference and oscillatory Zener tunneling in bilayer graphene p-n

junctions,” PNAS 108, 14021 (2011).[198] D. A. Gradinar, H. Schomerus, and V. I. Fal’ko, “Conductance anomaly near the Lifshitz transition in strained bilayer

graphene,” Phys. Rev. B 85, 165429 (2012).[199] B. Van Duppen and F. M. Peeters, “Four-band tunneling in bilayer graphene,” Phys. Rev. B 87, 205427 (2013).[200] V. Kleptsyn, A. Okunev, I. Schurov, D. Zubov, and M. I. Katsnelson, “Chiral tunneling through generic one-dimensional

potential barriers in bilayer graphene,” Phys. Rev. B 92, 165407 (2015).[201] C.-S. Park, “Two-dimensional transmission through modified Poschl-Teller potential in bilayer graphene,” Phys. Rev. B

92, 165422 (2015).[202] V. Ryzhii and M. Ryzhii, “Graphene bilayer field-effect phototransistor for terahertz and infrared detection,” Phys. Rev.

B 79, 245311 (2009).

124

[203] D. Spirito, D. Coquillat, S. L. De Bonis, A. Lombardo, M. Bruna, A. C. Ferrari, V. Pellegrini, A. Tredicucci, W. Knap,and M. S. Vitiello, “High performance bilayer-graphene terahertz detectors,” Appl. Phys. Lett. 104, 061111 (2014).

[204] B. Chakraborty, A. Das, and A. K. Sood, “The formation of a p-n junction in a polymer electrolyte top-gated bilayergraphene transistor,” Nanotechnology 20, 365203 (2009).

[205] B. N. Szafranek, D. Schall, M. Otto, D. Neumaier, and H. Kurz, “Electrical observation of a tunable band gap in bilayergraphene nanoribbons at room temperature,” Appl. Phys. Lett. 96, 112103 (2010).

[206] B. N. Szafranek, D. Schall, M. Otto, D. Neumaier, and H. Kurz, “High On/Off Ratios in Bilayer Graphene Field EffectTransistors Realized by Surface Dopants,” Nano Lett. 11, 2640 (2011).

[207] B. N. Szafranek, G. Fiori, D. Schall, D. Neumaier, and H. Kurz, “Current Saturation and Voltage Gain in BilayerGraphene Field Effect Transistors,” Nano Lett. 12, 1324 (2012).

[208] G. Alymov, V. Vyurkov, V. Ryzhii, and D. Svintsov, “Abrupt current switching in graphene bilayer tunnel transistorsenabled by van Hove singularities,” Sci. Rep. 6, 24654 (2016).

[209] H. Miyazaki, S.-L. Li, S. Nakaharai, and K. Tsukagoshi, “Unipolar transport in bilayer graphene controlled by multiplep-n interfaces,” Appl. Phys. Lett. 100, 163115 (2012).

[210] K. Kanayama and K. Nagashio, “Gap state analysis in electric-field-induced band gap for bilayer graphene,” Sci. Rep.5, 15789 (2015).

[211] M. Koshino and T. Ando, “Transport in bilayer graphene: Calculations within a self-consistent Born approximation,”Phys. Rev. B 73, 245403 (2006).

[212] M. Koshino, “Electronic transport in bilayer graphene,” New J. Phys. 11, 095010 (2009).[213] T. Ando, “Bilayer Graphene with Long-range Scatterers Studied in a Self-Consistent Born Approximation,” J. Phys.

Soc. Japan 80, 014707 (2011).[214] M. Trushin, J. Kailasvuori, J. Schliemann, and A. H. MacDonald, “Finite conductivity minimum in bilayer graphene

without charge inhomogeneities,” Phys. Rev. B 82, 155308 (2010).[215] M. Trushin and J. Schliemann, “Minimum Electrical and Thermal Conductivity of Graphene: A Quasiclassical Ap-

proach,” Phys. Rev. Lett. 99, 216602 (2007).[216] M. Auslender and M. I. Katsnelson, “Generalized kinetic equations for charge carriers in graphene,” Phys. Rev. B 76,

235425 (2007).[217] J. Nilsson, A. H. Castro Neto, F. Guinea, and N. M. R. Peres, “Electronic Properties of Graphene Multilayers,” Phys.

Rev. Lett. 97, 266801 (2006).[218] S. Adam and S. Das Sarma, “Boltzmann transport and residual conductivity in bilayer graphene,” Phys. Rev. B 77,

115436 (2008).[219] S. Das Sarma, E. H. Hwang, and E. Rossi, “Theory of carrier transport in bilayer graphene,” Phys. Rev. B 81, 161407

(2010).[220] S. Xiao, J.-H. Chen, S. Adam, E. D. Williams, and M. S. Fuhrer, “Charged impurity scattering in bilayer graphene,”

Phys. Rev. B 82, 041406 (2010).[221] M. Lv and S. Wan, “Screening-induced transport at finite temperature in bilayer graphene,” Phys. Rev. B 81, 195409

(2010).[222] A. Ferreira, J. Viana-Gomes, J. Nilsson, E. R. Mucciolo, N. M. R. Peres, and A. H. Castro Neto, “Unified description

of the dc conductivity of monolayer and bilayer graphene at finite densities based on resonant scatterers,” Phys. Rev. B83, 165402 (2011).

[223] Z. H. Ni, L. A. Ponomarenko, R. R. Nair, R. Yang, S. Anissimova, I. V. Grigorieva, F. Schedin, P. Blake, Z. X. Shen,E. H. Hill, et al., “On Resonant Scatterers As a Factor Limiting Carrier Mobility in Graphene,” Nano Lett. 10, 3868(2010).

[224] J. Katoch, J.-H. Chen, R. Tsuchikawa, C. Smith, E. Mucciolo, and M. Ishigami, “Uncovering the dominant scatterer ingraphene sheets on SiO2,” Phys. Rev. B 82, 081417 (2010).

[225] M. Monteverde, C. Ojeda-Aristizabal, R. Weil, K. Bennaceur, M. Ferrier, S. Gueron, C. Glattli, H. Bouchiat, J. N.Fuchs, and D. L. Maslov, “Transport and Elastic Scattering Times as Probes of the Nature of Impurity Scattering inSingle-Layer and Bilayer Graphene,” Phys. Rev. Lett. 104, 126801 (2010).

[226] S. Yuan, H. De Raedt, and M. I. Katsnelson, “Electronic transport in disordered bilayer and trilayer graphene,” Phys.Rev. B 82, 235409 (2010).

[227] S. Yuan, H. De Raedt, and M. Katsnelson, “Modeling electronic structure and transport properties of graphene withresonant scattering centers,” Phys. Rev. B 82, 115448 (2010).

[228] W. Zhu, V. Perebeinos, M. Freitag, and P. Avouris, “Carrier scattering, mobilities, and electrostatic potential in mono-layer, bilayer, and trilayer graphene,” Phys. Rev. B 80, 235402 (2009).

[229] F. Kisslinger, C. Ott, C. Heide, E. Kampert, B. Butz, E. Spiecker, S. Shallcross, and H. B. Weber, “Linear magnetore-sistance in mosaic-like bilayer graphene,” Nat. Phys. 11, 650 (2015).

[230] E. Hwang, S. Adam, and S. Das Sarma, “Carrier Transport in Two-Dimensional Graphene Layers,” Phys. Rev. Lett. 98,186806 (2007).

[231] J. Martin, N. Akerman, G. Ulbricht, T. Lohmann, J. H. Smet, K. von Klitzing, and A. Yacoby, “Observation of electron-hole puddles in graphene using a scanning single-electron transistor,” Nat. Phys. 4, 144 (2008).

[232] S. Adam and M. D. Stiles, “Temperature dependence of the diffusive conductivity of bilayer graphene,” Phys. Rev. B82, 075423 (2010).

[233] E. H. Hwang and S. Das Sarma, “Insulating behavior in metallic bilayer graphene: Interplay between density inhomo-geneity and temperature,” Phys. Rev. B 82, 081409 (2010).

[234] M. I. Katsnelson, “Minimal conductivity in bilayer graphene,” Eur. Phys. J. B 52, 151 (2006).

125

[235] J. Cserti, “Minimal longitudinal dc conductivity of perfect bilayer graphene,” Phys. Rev. B 75, 033405 (2007).[236] I. Snyman and C. W. J. Beenakker, “Ballistic transmission through a graphene bilayer,” Phys. Rev. B 75, 045322 (2007).[237] J. Cserti, A. Csordas, and G. David, “Role of the trigonal warping on the minimal conductivity of bilayer graphene,”

Phys. Rev. Lett. 99, 066802 (2007).[238] P. San-Jose, R. Gorbachev, A. Geim, K. Novoselov, and F. Guinea, “Stacking boundaries and transport in bilayer

graphene,” Nano Lett. 14, 2052 (2014).[239] J. Nilsson and A. H. Castro Neto, “Impurities in a biased graphene bilayer,” Phys. Rev. Lett. 98, 126801 (2007).[240] K. Zou and J. Zhu, “Transport in gapped bilayer graphene: The role of potential fluctuations,” Phys. Rev. B 82, 081407

(2010).[241] T. Taychatanapat and P. Jarillo-Herrero, “Electronic Transport in Dual-Gated Bilayer Graphene at Large Displacement

Fields,” Phys. Rev. Lett. 105, 166601 (2010).[242] E. Rossi and S. Das Sarma, “Inhomogenous Electronic Structure, Transport Gap, and Percolation Threshold in Disordered

Bilayer Graphene,” Phys. Rev. Lett. 107, 155502 (2011).[243] M. Trushin, “Thermally activated conductivity in gapped bilayer graphene,” EPL 98, 47007 (2012).[244] C. Park, J. Ryou, S. Hong, B. G. Sumpter, G. Kim, and M. Yoon, “Electronic Properties of Bilayer Graphene Strongly

Coupled to Interlayer Stacking and an External Electric Field,” Phys. Rev. Lett. 115, 015502 (2015).[245] Y.-B. Zhou, L. Zhang, D.-P. Yu, and Z.-M. Liao, “Magnetic field induced insulating state in bilayer graphene at charge

neutral point,” Appl. Phys. Lett. 104, 153103 (2014).[246] T. Ando, Y. Zheng, and H. Suzuura, “Dynamical Conductivity and Zero-Mode Anomaly in Honeycomb Lattices,” J.

Phys. Soc. Japan 71, 1318 (2002).[247] V. P. Gusynin and S. G. Sharapov, “Transport of Dirac quasiparticles in graphene: Hall and optical conductivities,”

Phys. Rev. B 73, 245411 (2006).[248] V. P. Gusynin, S. G. Sharapov, and J. P. Carbotte, “Unusual Microwave Response of Dirac Quasiparticles in Graphene,”

Phys. Rev. Lett. 96, 256802 (2006).[249] L. A. Falkovsky and A. A. Varlamov, “Space-time dispersion of graphene conductivity,” Eur. Phys. J. B 56, 281 (2007).[250] N. M. R. Peres, F. Guinea, and A. H. Castro Neto, “Electronic properties of disordered two-dimensional carbon,” Phys.

Rev. B 73, 125411 (2006).[251] Z. Li, E. A. Henriksen, Z. Jiang, Z. Hao, M. C. Martin, P. Kim, H. Stormer, and D. N. Basov, “Dirac charge dynamics

in graphene by infrared spectroscopy,” Nat. Phys. 4, 532 (2008).[252] A. B. Kuzmenko, E. van Heumen, F. Carbone, and D. van der Marel, “Universal Optical Conductance of Graphite,”

Phys. Rev. Lett. 100, 117401 (2008).[253] R. R. Nair, P. Blake, A. N. Grigorenko, K. S. Novoselov, T. J. Booth, T. Stauber, N. M. R. Peres, and A. K. Geim,

“Fine Structure Constant Defines Visual Transparency of Graphene,” Science 320, 1308 (2008).[254] K. F. Mak, M. Y. Sfeir, Y. Wu, C. H. Lui, J. A. Misewich, and T. F. Heinz, “Measurement of the Optical Conductivity

of Graphene,” Phys. Rev. Lett. 101, 196405 (2008).[255] C. J. Tabert and E. J. Nicol, “Dynamical conductivity of AA-stacked bilayer graphene,” Phys. Rev. B 86, 075439 (2012).[256] E. J. Nicol and J. P. Carbotte, “Optical conductivity of bilayer graphene with and without an asymmetry gap,” Phys.

Rev. B 77, 155409 (2008).[257] E. McCann, D. S. L. Abergel, and V. I. Fal’ko, “Electrons in bilayer graphene,” Solid State Commun. 143, 110 (2007).[258] J. Nilsson, A. H. Castro Neto, F. Guinea, and N. M. R. Peres, “Electronic properties of bilayer and multilayer graphene,”

Phys. Rev. B 78, 045405 (2008).[259] D. S. L. Abergel and V. I. Fal’ko, “Optical and magneto-optical far-infrared properties of bilayer graphene,” Phys. Rev.

B 75, 155430 (2007).[260] L. Benfatto, S. G. Sharapov, and J. P. Carbotte, “Robustness of the optical conductivity sum rule in bilayer graphene,”

Phys. Rev. B 77, 125422 (2008).[261] D. S. L. Abergel and M. Mucha-Kruczynski, “Infrared absorption of closely aligned heterostructures of monolayer and

bilayer graphene with hexagonal boron nitride,” Phys. Rev. B 92, 115430 (2015).[262] J. E. Drut and T. A. Lahde, “Is Graphene in Vacuum an Insulator?,” Phys. Rev. Lett. 102, 026802 (2009).[263] M. V. Ulybyshev, P. V. Buividovich, M. I. Katsnelson, and M. I. Polikarpov, “Monte Carlo Study of the Semimetal-

Insulator Phase Transition in Monolayer Graphene with a Realistic Interelectron Interaction Potential,” Phys. Rev. Lett.111, 056801 (2013).

[264] T. O. Wehling, E. Sasıoglu, C. Friedrich, A. I. Lichtenstein, M. I. Katsnelson, and S. Blugel, “Strength of EffectiveCoulomb Interactions in Graphene and Graphite,” Phys. Rev. Lett. 106, 236805 (2011).

[265] A. O. Sboychakov, A. L. Rakhmanov, A. V. Rozhkov, and F. Nori, “Metal-insulator transition and phase separation indoped AA-stacked graphene bilayer,” Phys. Rev. B 87, 121401 (2013).

[266] M. Schuler, M. Rosner, T. O. Wehling, A. I. Lichtenstein, and M. I. Katsnelson, “Optimal Hubbard Models for Materialswith Nonlocal Coulomb Interactions: Graphene, Silicene, and Benzene,” Phys. Rev. Lett. 111, 036601 (2013).

[267] T. M. Rice, “Band-Structure Effects in Itinerant Antiferromagnetism,” Phys. Rev. B 2, 3619 (1970).[268] P. Fulde and R. A. Ferrell, “Superconductivity in a Strong Spin-Exchange Field,” Phys. Rev. 135, A550 (1964).[269] A. I. Larkin and Y. N. Ovchinnikov, “Nonuniform state of superconductors,” Sov. Phys. JETP 20, 762 (1965).[270] L. Aslamazov, “Influence of impurities on the existence of an inhomogeneous state in a ferromagnetic superconduuctor,”

Sov. Phys. JETP 28, 773 (1969).[271] D. E. Sheehy and L. Radzihovsky, “BEC-BCS crossover, phase transitions and phase separation in polarized resonantly-

paired superfluids,” Ann. Phys. 322, 1790 (2007).[272] S. Takada, “Superconductivity in a Molecular Field. II: Stability of Fulde-Ferrel Phase,” Progr. Theoret. Phys. Suppl.

126

43, 27 (1970).[273] M. Le Bellac, F. Mortessagne, and G. G. Batrouni, Equilibrium and Non-Equilibrium Statistical Thermodynamics (Cam-

bridge University Press, Cambridge, 2004).[274] J. Lorenzana, C. Castellani, and C. Di Castro, “Phase separation frustrated by the long-range Coulomb interaction. I.

Theory,” Phys. Rev. B 64, 235127 (2001).[275] J. Lorenzana, C. Castellani, and C. Di Castro, “Phase separation frustrated by the long-range Coulomb interaction. II.

Applications,” Phys. Rev. B 64, 235128 (2001).[276] R. Jamei, S. Kivelson, and B. Spivak, “Universal Aspects of Coulomb-Frustrated Phase Separation,” Phys. Rev. Lett.

94, 056805 (2005).[277] K. I. Kugel, A. L. Rakhmanov, and A. O. Sboychakov, “Phase Separation in Jahn-Teller Systems with Localized and

Itinerant Electrons,” Phys. Rev. Lett. 95, 267210 (2005).[278] J.-J. Su and A. H. MacDonald, “How to make a bilayer exciton condensate flow,” Nat. Phys. 4, 799 (2008).[279] E. H. Hwang, R. Sensarma, and S. Das Sarma, “Coulomb drag in monolayer and bilayer graphene,” Phys. Rev. B 84,

245441 (2011).[280] D. Nandi, A. D. K. Finck, J. P. Eisenstein, L. N. Pfeiffer, and K. W. West, “Exciton condensation and perfect Coulomb

drag,” Nature 488, 481 (2012).[281] R. V. Gorbachev, A. K. Geim, M. I. Katsnelson, R. S. Novoselov, T. Tudorovskiy, I. V. Grigorieva, A. H. MacDonald,

S. Morozov, K. Watanabe, T. Taniguchi, et al., “Strong Coulomb drag and broken symmetry in double-layer graphene,”Nat. Phys. 8, 896 (2012).

[282] D. S. de la Pena, M. M. Scherer, and C. Honerkamp, “Electronic instabilities of the AA-honeycomb bilayer,” Ann. Phys.(Leipzig) 526, 366 (2014).

[283] L. Brey and H. A. Fertig, “Gapped phase in AA-stacked bilayer graphene,” Phys. Rev. B 87, 115411 (2013).[284] A. Nikolaev and M. Ulybyshev, “Monte-Carlo study of the phase transition in the AA-stacked bilayer graphene,” arXiv

preprint arXiv:1412.1359 (2014).[285] A. Nikolaev and M. Ulybyshev, in PoS LAT2014 (2014), vol. 054.[286] R. T. Weitz, M. T. Allen, B. E. Feldman, J. Martin, and A. Yacoby, “Broken-Symmetry States in Doubly Gated

Suspended Bilayer Graphene,” Science 330, 812 (2010).[287] F. Freitag, J. Trbovic, M. Weiss, and C. Schonenberger, “Spontaneously Gapped Ground State in Suspended Bilayer

Graphene,” Phys. Rev. Lett. 108, 076602 (2012).[288] F. Freitag, M. Weiss, R. Maurand, J. Trbovic, and C. Schnenberger, “Homogeneity of bilayer graphene,” Solid State

Communications 152, 2053 (2012).[289] A. Veligura, H. J. van Elferen, N. Tombros, J. C. Maan, U. Zeitler, and B. J. van Wees, “Transport gap in suspended

bilayer graphene at zero magnetic field,” Phys. Rev. B 85, 155412 (2012).[290] F. Freitag, M. Weiss, R. Maurand, J. Trbovic, and C. Schonenberger, “Spin symmetry of the bilayer graphene ground

state,” Phys. Rev. B 87, 161402 (2013).[291] J. Nilsson, A. H. Castro Neto, N. M. R. Peres, and F. Guinea, “Electron-electron interactions and the phase diagram of

a graphene bilayer,” Phys. Rev. B 73, 214418 (2006).[292] F. Bloch, “Bemerkung zur Elektronentheorie des Ferromagnetismus und der elektrischen Leitfahigkeit,” Z. Physik 57,

545 (1929).[293] E. V. Castro, N. M. R. Peres, T. Stauber, and N. A. P. Silva, “Low-density ferromagnetism in biased bilayer graphene,”

Phys. Rev. Lett. 100, 186803 (2008).[294] T. Stauber, N. M. R. Peres, F. Guinea, and A. H. Castro Neto, “Fermi liquid theory of a Fermi ring,” Phys. Rev. B 75,

115425 (2007).[295] H. Min, G. Borghi, M. Polini, and A. H. MacDonald, “Pseudospin magnetism in graphene,” Phys. Rev. B 77, 041407

(2008).[296] F. Zhang, H. Min, M. Polini, and A. H. MacDonald, “Spontaneous inversion symmetry breaking in graphene bilayers,”

Phys. Rev. B 81, 041402 (2010).[297] F. Zhang, H. Min, and A. H. MacDonald, “Competing ordered states in bilayer graphene,” Phys. Rev. B 86, 155128

(2012).[298] R. Nandkishore and L. Levitov, “Dynamical Screening and Excitonic Instability in Bilayer Graphene,” Phys. Rev. Lett.

104, 156803 (2010).[299] R. Nandkishore and L. Levitov, “Quantum anomalous Hall state in bilayer graphene,” Phys. Rev. B 82, 115124 (2010).[300] J. Jung, F. Zhang, and A. H. MacDonald, “Lattice theory of pseudospin ferromagnetism in bilayer graphene: Competing

interaction-induced quantum Hall states,” Phys. Rev. B 83, 115408 (2011).[301] R. Nandkishore and L. Levitov, “Polar Kerr Effect and Time Reversal Symmetry Breaking in Bilayer Graphene,” Phys.

Rev. Lett. 107, 097402 (2011).[302] F. Zhang and A. H. MacDonald, “Distinguishing Spontaneous Quantum Hall States in Bilayer Graphene,” Phys. Rev.

Lett. 108, 186804 (2012).[303] Y. Wang, H. Wang, J.-H. Gao, and F.-C. Zhang, “Layer antiferromagnetic state in bilayer graphene: A first-principles

investigation,” Phys. Rev. B 87, 195413 (2013).[304] O. Vafek, “Interacting fermions on the honeycomb bilayer: From weak to strong coupling,” Phys. Rev. B 82, 205106

(2010).[305] T. C. Lang, Z. Y. Meng, M. M. Scherer, S. Uebelacker, F. F. Assaad, A. Muramatsu, C. Honerkamp, and S. Wessel,

“Antiferromagnetism in the Hubbard Model on the Bernal-Stacked Honeycomb Bilayer,” Phys. Rev. Lett. 109, 126402(2012).

127

[306] J. Yuan, D.-H. Xu, H. Wang, Y. Zhou, J.-H. Gao, and F.-C. Zhang, “Possible half-metallic phase in bilayer graphene:Calculations based on mean-field theory applied to a two-layer Hubbard model,” Phys. Rev. B 88, 201109 (2013).

[307] J. Sun, D.-H. Xu, Y. Zhou, and F.-C. Zhang, “Electrically controllable magnetic order in the bilayer Hubbard model onhoneycomb lattice: A determinant quantum Monte Carlo study,” Phys. Rev. B 90, 125429 (2014).

[308] M. M. Scherer, S. Uebelacker, and C. Honerkamp, “Instabilities of interacting electrons on the honeycomb bilayer,” Phys.Rev. B 85, 235408 (2012).

[309] O. Vafek and K. Yang, “Many-body instability of Coulomb interacting bilayer graphene: Renormalization group ap-proach,” Phys. Rev. B 81, 041401 (2010).

[310] Y. Lemonik, I. Aleiner, and V. I. Fal’ko, “Competing nematic, antiferromagnetic, and spin-flux orders in the groundstate of bilayer graphene,” Phys. Rev. B 85, 245451 (2012).

[311] R. E. Throckmorton and O. Vafek, “Fermions on bilayer graphene: Symmetry breaking for B=0 and ν=0,” Phys. Rev.B 86, 115447 (2012).

[312] V. Cvetkovic, R. E. Throckmorton, and O. Vafek, “Electronic multicriticality in bilayer graphene,” Phys. Rev. B 86,075467 (2012).

[313] Y. Lemonik, I. L. Aleiner, C. Toke, and V. I. Fal’ko, “Spontaneous symmetry breaking and Lifshitz transition in bilayergraphene,” Phys. Rev. B 82, 201408 (2010).

[314] E. V. Gorbar, V. P. Gusynin, V. A. Miransky, and I. A. Shovkovy, “Coexistence and competition of nematic and gappedstates in bilayer graphene,” Phys. Rev. B 86, 125439 (2012).

[315] S. Ulstrup, J. C. Johannsen, F. Cilento, J. A. Miwa, A. Crepaldi, M. Zacchigna, C. Cacho, R. Chapman, E. Springate,S. Mammadov, et al., “Ultrafast dynamics of massive Dirac fermions in bilayer graphene,” Phys. Rev. Lett. 112, 257401(2014).

[316] J. Zhang, R. Nandkishore, and E. Rossi, “Disorder-tuned selection of order in bilayer graphene,” Phys. Rev. B 91, 205425(2015).

[317] R. Dillenschneider and J. H. Han, “Exciton formation in graphene bilayer,” Phys. Rev. B 78, 045401 (2008).[318] H. P. Dahal, T. O. Wehling, K. S. Bedell, J.-X. Zhu, and A. Balatsky, “Charge inhomogeneity in a single and bilayer

graphene,” Physica B 405, 2241 (2010).[319] L. Zhu, V. Aji, and C. M. Varma, “Ordered loop current states in bilayer graphene,” Phys. Rev. B 87, 035427 (2013).[320] Y. Barlas and K. Yang, “Non-Fermi-liquid behavior in neutral bilayer graphene,” Phys. Rev. B 80, 161408 (2009).[321] R. Nandkishore and L. Levitov, “Electron interactions in bilayer graphene: Marginal Fermi liquid and zero-bias anomaly,”

Phys. Rev. B 82, 115431 (2010).[322] S. V. Kusminskiy, J. Nilsson, D. K. Campbell, and A. H. Castro Neto, “Electronic compressibility of a graphene bilayer,”

Phys. Rev. Lett. 100, 106805 (2008).[323] G. Borghi, M. Polini, R. Asgari, and A. H. MacDonald, “Fermi velocity enhancement in monolayer and bilayer graphene,”

Solid State Commun. 149, 1117 (2009).[324] R. Sensarma, E. H. Hwang, and S. Das Sarma, “Quasiparticles, plasmarons, and quantum spectral function in bilayer

graphene,” Phys. Rev. B 84, 041408 (2011).[325] K. Shizuya, “Many-body corrections to cyclotron resonance in monolayer and bilayer graphene,” Phys. Rev. B 81, 075407

(2010).[326] C.-M. Cheng, L. F. Xie, A. Pachoud, H. O. Moser, W. Chen, A. T. S. Wee, A. H. Castro Neto, K.-D. Tsuei, and

B. Ozyilmaz, “Anomalous Spectral Features of a Neutral Bilayer Graphene,” Scientific reports 5 (2015).[327] E. H. Hwang and S. Das Sarma, “Screening, Kohn Anomaly, Friedel Oscillation, and RKKY Interaction in Bilayer

Graphene,” Phys. Rev. Lett. 101, 156802 (2008).[328] R. Sensarma, E. H. Hwang, and S. Das Sarma, “Dynamic screening and low-energy collective modes in bilayer graphene,”

Phys. Rev. B 82, 195428 (2010).[329] O. V. Gamayun, “Dynamical screening in bilayer graphene,” Phys. Rev. B 84, 085112 (2011).[330] C. Triola and E. Rossi, “Screening and collective modes in gapped bilayer graphene,” Phys. Rev. B 86, 161408 (2012).[331] X.-F. Wang and T. Chakraborty, “Coulomb screening and collective excitations in a graphene bilayer,” Phys. Rev. B 75,

041404 (2007).[332] X.-F. Wang and T. Chakraborty, “Coulomb screening and collective excitations in biased bilayer graphene,” Phys. Rev.

B 81, 081402 (2010).[333] M. Pisarra, A. Sindona, M. Gravina, V. M. Silkin, and J. M. Pitarke, “Dielectric screening and plasmon resonances in

bilayer graphene,” Phys. Rev. B 93, 035440 (2016).[334] N. Klier, S. Shallcross, S. Sharma, and O. Pankratov, “Ruderman-Kittel-Kasuya-Yosida interaction at finite temperature:

Graphene and bilayer graphene,” Phys. Rev. B 92, 205414 (2015).[335] Y. Mohammadi, “Charge screening and carrier transport in AA-stacked bilayer graphene: tuning via a perpendicular

electric field,” Solid State Commun. 202, 14 (2015).[336] J. H. Ho, C. L. Lu, C. C. Hwang, C. P. Chang, and M. F. Lin, “Coulomb excitations in AA- and AB-stacked bilayer

graphites,” Phys. Rev. B 74, 085406 (2006).[337] M.-F. Lin, Y.-C. Chuang, and J.-Y. Wu, “Electrically tunable plasma excitations in AA-stacked multilayer graphene,”

Phys. Rev. B 86, 125434 (2012).[338] R. Roldan and L. Brey, “Dielectric screening and plasmons in AA-stacked bilayer graphene,” Phys. Rev. B 88, 115420

(2013).[339] W. Wang, S. Xiao, and N. A. Mortensen, “Localized plasmons in bilayer graphene nanodisks,” Phys. Rev. B 93, 165407

(2016).[340] M. Tahir and K. Sabeeh, “Inter-band magnetoplasmons in mono- and bilayer graphene,” J. Phys.: Condens. Matter 20,

128

425202 (2008).[341] S. A. Mikhailov and K. Ziegler, “New Electromagnetic Mode in Graphene,” Phys. Rev. Lett. 99, 016803 (2007).[342] V. I. Fal’ko and D. E. Khmel’nitskii, “What if a film conductivity exceeds the speed of light?,” Sov. Phys. JETP 68,

1150 (1989).[343] M. Jablan, H. Buljan, and M. Soljacic, “Transverse electric plasmons in bilayer graphene,” Opt. Express 19, 11236

(2011).[344] T. Stauber, P. San-Jose, and L. Brey, “Optical conductivity, Drude weight and plasmons in twisted graphene bilayers,”

New J. Phys. 15, 113050 (2013).[345] T. Low, F. Guinea, H. Yan, F. Xia, and P. Avouris, “Novel midinfrared plasmonic properties of bilayer graphene,” Phys.

Rev. Lett. 112, 116801 (2014).[346] Z. Fei, E. Iwinski, G. Ni, L. Zhang, W. Bao, A. Rodin, Y. Lee, M. Wagner, M. Liu, S. Dai, et al., “Tunneling plasmonics

in bilayer graphene,” Nano Lett. 15, 4973 (2015).[347] H. Yan, T. Low, F. Guinea, F. Xia, and P. Avouris, “Tunable phonon-induced transparency in bilayer graphene nanorib-

bons,” Nano Lett. 14, 4581 (2014).[348] J. Hass, F. Varchon, J. E. Millan-Otoya, M. Sprinkle, N. Sharma, W. A. de Heer, C. Berger, P. N. First, L. Magaud,

and E. H. Conrad, “Why Multilayer Graphene on 4H-SiC(0001) Behaves Like a Single Sheet of Graphene,” Phys. Rev.Lett. 100, 125504 (2008).

[349] L. Meng, Y. Zhang, W. Yan, L. Feng, L. He, R.-F. Dou, and J.-C. Nie, “Single-layer behavior and slow carrier densitydynamic of twisted graphene bilayer,” Appl. Phys. Lett. 100, 091601 (2012).

[350] J. Hicks, M. Sprinkle, K. Shepperd, F. Wang, A. Tejeda, A. Taleb-Ibrahimi, F. Bertran, P. Le Fevre, W. A. de Heer,C. Berger, et al., “Symmetry breaking in commensurate graphene rotational stacking: Comparison of theory and exper-iment,” Phys. Rev. B 83, 205403 (2011).

[351] A. Luican, G. Li, A. Reina, J. Kong, R. R. Nair, K. S. Novoselov, A. K. Geim, and E. Y. Andrei, “Single-Layer Behaviorand Its Breakdown in Twisted Graphene Layers,” Phys. Rev. Lett. 106, 126802 (2011).

[352] W. Yan, M. Liu, R.-F. Dou, L. Meng, L. Feng, Z.-D. Chu, Y. Zhang, Z. Liu, J.-C. Nie, and L. He, “Angle-Dependentvan Hove Singularities in a Slightly Twisted Graphene Bilayer,” Phys. Rev. Lett. 109, 126801 (2012).

[353] L. Brown, R. Hovden, P. Huang, M. Wojcik, D. A. Muller, and J. Park, “Twinning and Twisting of Tri- and BilayerGraphene,” Nano Lett. 12, 1609 (2012).

[354] R. W. Havener, H. Zhuang, L. Brown, R. G. Hennig, and J. Park, “Angle-Resolved Raman Imaging of Interlayer Rotationsand Interactions in Twisted Bilayer Graphene,” Nano Lett. 12, 3162 (2012).

[355] A. Righi, S. D. Costa, H. Chacham, C. Fantini, P. Venezuela, C. Magnuson, L. Colombo, W. S. Bacsa, R. S. Ruoff, andM. A. Pimenta, “Graphene Moire patterns observed by umklapp double-resonance Raman scattering,” Phys. Rev. B 84,241409 (2011).

[356] A. Righi, P. Venezuela, H. Chacham, S. Costa, C. Fantini, R. Ruoff, L. Colombo, W. Bacsa, and M. Pimenta, “ResonanceRaman spectroscopy in twisted bilayer graphene,” Solid State Commun. 175176, 13 (2013), special Issue: Graphene V:Recent Advances in Studies of Graphene and Graphene analogues.

[357] J. T. Robinson, S. W. Schmucker, C. B. Diaconescu, J. P. Long, J. C. Culbertson, T. Ohta, A. L. Friedman, and T. E.Beechem, “Electronic Hybridization of Large-Area Stacked Graphene Films,” ACS Nano 7, 637 (2013).

[358] J.-B. Liu, P.-J. Li, Y.-F. Chen, Z.-G. Wang, F. Qi, J.-R. He, B.-J. Zheng, J.-H. Zhou, W.-L. Zhang, L. Gu, et al., “Ob-servation of tunable electrical bandgap in large-area twisted bilayer graphene synthesized by chemical vapor deposition,”Sci. Rep. 5, 15285 (2015).

[359] P. Poncharal, A. Ayari, T. Michel, and J.-L. Sauvajol, “Raman spectra of misoriented bilayer graphene,” Phys. Rev. B78, 113407 (2008).

[360] Z. Ni, Y. Wang, T. Yu, Y. You, and Z. Shen, “Reduction of Fermi velocity in folded graphene observed by resonanceRaman spectroscopy,” Phys. Rev. B 77, 235403 (2008).

[361] V. Carozo, C. M. Almeida, B. Fragneaud, P. M. Bede, M. V. O. Moutinho, J. Ribeiro-Soares, N. F. Andrade, A. G.Souza Filho, M. J. S. Matos, B. Wang, et al., “Resonance effects on the Raman spectra of graphene superlattices,” Phys.Rev. B 88, 085401 (2013).

[362] T. Ohta, T. E. Beechem, J. T. Robinson, and G. L. Kellogg, “Long-range atomic ordering and variable interlayerinteractions in two overlapping graphene lattices with stacking misorientations,” Phys. Rev. B 85, 075415 (2012).

[363] R. Othmen, H. Arezki, H. Ajlani, A. Cavanna, M. Boutchich, M. Oueslati, and A. Madouri, “Direct transfer and Ramancharacterization of twisted graphene bilayer,” Appl. Phys. Lett. 106, 103107 (2015).

[364] Z. Y. Rong and P. Kuiper, “Electronic effects in scanning tunneling microscopy: Moire pattern on a graphite surface,”Phys. Rev. B 48, 17427 (1993).

[365] G. Li, A. Luican, J. M. B. Lopes dos Santos, A. H. Castro Neto, A. Reina, J. Kong, and E. Y. Andrei, “Observation ofVan Hove singularities in twisted graphene layers,” Nat. Phys. 6, 109 (2010).

[366] E. Cisternas and J. Correa, “Theoretical reproduction of superstructures revealed by STM on bilayer graphene,” Chem.Phys. 409, 74 (2012).

[367] J. M. B. Lopes dos Santos, N. M. R. Peres, and A. H. Castro Neto, “Continuum model of the twisted graphene bilayer,”Phys. Rev. B 86, 155449 (2012).

[368] S. Shallcross, S. Sharma, E. Kandelaki, and O. A. Pankratov, “Electronic structure of turbostratic graphene,” Phys. Rev.B 81, 165105 (2010).

[369] S. Shallcross, S. Sharma, and O. A. Pankratov, “Quantum Interference at the Twist Boundary in Graphene,” Phys. Rev.Lett. 101, 056803 (2008).

[370] E. J. Mele, “Commensuration and interlayer coherence in twisted bilayer graphene,” Phys. Rev. B 81, 161405 (2010).

129

[371] E. J. Mele, “Band symmetries and singularities in twisted multilayer graphene,” Phys. Rev. B 84, 235439 (2011).[372] R. Bistritzer and A. H. MacDonald, “Moire bands in twisted double-layer graphene,” PNAS 108, 12233 (2011).[373] S. Shallcross, S. Sharma, and O. A. Pankratov, “Twist boundary in graphene: energetics and electric field effect,” J.

Phys.: Condens. Matter 20, 454224 (2008).[374] G. Trambly de Laissardiere, D. Mayou, and L. Magaud, “Localization of Dirac Electrons in Rotated Graphene Bilayers,”

Nano Lett. 10, 804 (2010).[375] G. Trambly de Laissardiere, D. Mayou, and L. Magaud, “Numerical studies of confined states in rotated bilayers of

graphene,” Phys. Rev. B 86, 125413 (2012).[376] E. Suarez Morell, J. D. Correa, P. Vargas, M. Pacheco, and Z. Barticevic, “Flat bands in slightly twisted bilayer graphene:

Tight-binding calculations,” Phys. Rev. B 82, 121407 (2010).[377] E. Suarez Morell, P. Vargas, L. Chico, and L. Brey, “Charge redistribution and interlayer coupling in twisted bilayer

graphene under electric fields,” Phys. Rev. B 84, 195421 (2011).[378] S. Shallcross, S. Sharma, and O. Pankratov, “Emergent momentum scale, localization, and van Hove singularities in the

graphene twist bilayer,” Phys. Rev. B 87, 245403 (2013).[379] S. Latil, V. Meunier, and L. Henrard, “Massless fermions in multilayer graphitic systems with misoriented layers: Ab

initio calculations and experimental fingerprints,” Phys. Rev. B 76, 201402 (2007).[380] L. Xian, S. Barraza-Lopez, and M. Y. Chou, “Effects of electrostatic fields and charge doping on the linear bands in

twisted graphene bilayers,” Phys. Rev. B 84, 075425 (2011).[381] K. Sato, R. Saito, C. Cong, T. Yu, and M. S. Dresselhaus, “Zone folding effect in Raman G-band intensity of twisted

bilayer graphene,” Phys. Rev. B 86, 125414 (2012).[382] K. Uchida, S. Furuya, J.-I. Iwata, and A. Oshiyama, “Atomic corrugation and electron localization due to Moire patterns

in twisted bilayer graphenes,” Phys. Rev. B 90, 155451 (2014).[383] A. Oshiyama, J.-I. Iwata, K. Uchida, and Y.-I. Matsushita, “Large-scale real-space density-functional calculations: Moire-

induced electron localization in graphene,” J. Appl. Phys. 117, 112811 (2015).[384] M. Kindermann and P. N. First, “Effective theory of rotationally faulted multilayer graphene - the local limit,” J. Phys.

D: Appl. Phys. 45, 154005 (2012).[385] R. de Gail, M. O. Goerbig, F. Guinea, G. Montambaux, and A. H. Castro Neto, “Topologically protected zero modes in

twisted bilayer graphene,” Phys. Rev. B 84, 045436 (2011).[386] M.-Y. Choi, Y.-H. Hyun, and Y. Kim, “Angle dependence of the Landau level spectrum in twisted bilayer graphene,”

Phys. Rev. B 84, 195437 (2011).[387] P. San-Jose, J. Gonzalez, and F. Guinea, “Non-Abelian Gauge Potentials in Graphene Bilayers,” Phys. Rev. Lett. 108,

216802 (2012).[388] Z.-D. Chu, W.-Y. He, and L. He, “Coexistence of van Hove singularities and superlattice Dirac points in a slightly twisted

graphene bilayer,” Phys. Rev. B 87, 155419 (2013).[389] L. Xian, Z. F. Wang, and M. Y. Chou, “Coupled Dirac Fermions and Neutrino-like Oscillations in Twisted Bilayer

Graphene,” Nano Lett. 13, 5159 (2013).[390] D. Weckbecker, S. Shallcross, M. Fleischmann, N. Ray, S. Sharma, and O. Pankratov, “Low-energy theory for the

graphene twist bilayer,” Phys. Rev. B 93, 035452 (2016).[391] M. S. Tang, C. Z. Wang, C. T. Chan, and K. M. Ho, “Environment-dependent tight-binding potential model,” Phys.

Rev. B 53, 979 (1996).[392] W.-Y. He, Y. Su, M. Yang, and L. He, “Creating in-plane pseudomagnetic fields in excess of 1000 T by misoriented

stacking in a graphene bilayer,” Phys. Rev. B 89, 125418 (2014).[393] E. Mendez, A. Misu, and M. S. Dresselhaus, “Magnetoreflection study of graphite under pressure,” Phys. Rev. B 21, 827

(1980).[394] M. Mucha-Kruczynski, O. Tsyplyatyev, A. Grishin, E. McCann, V. I. Fal’ko, A. Bostwick, and E. Rotenberg, “Charac-

terization of graphene through anisotropy of constant-energy maps in angle-resolved photoemission,” Phys. Rev. B 77,195403 (2008).

[395] D. L. Miller, K. D. Kubista, G. M. Rutter, M. Ruan, W. A. de Heer, P. N. First, and J. A. Stroscio, “Observing theQuantization of Zero Mass Carriers in Graphene,” Science 324, 924 (2009).

[396] M. Sprinkle, D. Siegel, Y. Hu, J. Hicks, A. Tejeda, A. Taleb-Ibrahimi, P. Le Fevre, F. Bertran, S. Vizzini, H. Enriquez,et al., “First Direct Observation of a Nearly Ideal Graphene Band Structure,” Phys. Rev. Lett. 103, 226803 (2009).

[397] I. Razado-Colambo, J. Avila, J.-P. Nys, C. Chen, X. Wallart, M.-C. Asensio, and D. Vignaud, “NanoARPES of twistedbilayer graphene on SiC: absence of velocity renormalization for small angles,” Sci. Rep. 6, 27261 (2016).

[398] Y. J. Song, A. F. Otte, Y. Kuk, Y. Hu, D. B. Torrance, P. N. First, W. A. de Heer, H. Min, S. Adam, M. D. Stiles, et al.,“High-resolution tunnelling spectroscopy of a graphene quartet,” Nature 467, 185 (2010).

[399] J. D. Sanchez-Yamagishi, T. Taychatanapat, K. Watanabe, T. Taniguchi, A. Yacoby, and P. Jarillo-Herrero, “QuantumHall Effect, Screening, and Layer-Polarized Insulating States in Twisted Bilayer Graphene,” Phys. Rev. Lett. 108, 076601(2012).

[400] W. Yan, L. Meng, M. Liu, J.-B. Qiao, Z.-D. Chu, R.-F. Dou, Z. Liu, J.-C. Nie, D. G. Naugle, and L. He, “Angle-dependentvan Hove singularities and their breakdown in twisted graphene bilayers,” Phys. Rev. B 90, 115402 (2014).

[401] V. Cherkez, G. Trambly de Laissardiere, P. Mallet, and J.-Y. Veuillen, “Van Hove singularities in doped twisted graphenebilayers studied by scanning tunneling spectroscopy,” Phys. Rev. B 91, 155428 (2015).

[402] L.-J. Yin, J.-B. Qiao, W.-X. Wang, W.-J. Zuo, W. Yan, R. Xu, R.-F. Dou, J.-C. Nie, and L. He, “Landau quantizationand Fermi velocity renormalization in twisted graphene bilayers,” Phys. Rev. B 92, 201408 (2015).

[403] T. Ohta, J. T. Robinson, P. J. Feibelman, A. Bostwick, E. Rotenberg, and T. E. Beechem, “Evidence for Interlayer

130

Coupling and Moire Periodic Potentials in Twisted Bilayer Graphene,” Phys. Rev. Lett. 109, 186807 (2012).[404] Z. Ni, L. Liu, Y. Wang, Z. Zheng, L.-J. Li, T. Yu, and Z. Shen, “G-band Raman double resonance in twisted bilayer

graphene: Evidence of band splitting and folding,” Phys. Rev. B 80, 125404 (2009).[405] R. He, T.-F. Chung, C. Delaney, C. Keiser, L. A. Jauregui, P. M. Shand, C. C. Chancey, Y. Wang, J. Bao, and Y. P.

Chen, “Observation of Low Energy Raman Modes in Twisted Bilayer Graphene,” Nano Lett. 13, 3594 (2013).[406] A. Jorio and L. G. Cancado, “Raman spectroscopy of twisted bilayer graphene,” Solid State Commun. 175176, 3 (2013),

special Issue: Graphene V: Recent Advances in Studies of Graphene and Graphene analogues.[407] T. E. Beechem, T. Ohta, B. Diaconescu, and J. T. Robinson, “Rotational Disorder in Twisted Bilayer Graphene,” ACS

Nano 8, 1655 (2014).[408] J.-B. Wu, X. Zhang, M. Ijas, W.-P. Han, X.-F. Qiao, X.-L. Li, D.-S. Jiang, A. C. Ferrari, and P.-H. Tan, “Resonant

Raman spectroscopy of twisted multilayer graphene,” Nat. Commun. 5 (2014).[409] D. Wong, Y. Wang, J. Jung, S. Pezzini, A. M. DaSilva, H.-Z. Tsai, H. S. Jung, R. Khajeh, Y. Kim, J. Lee, et al., “Local

spectroscopy of Moire-induced electronic structure in gate-tunable twisted bilayer graphene,” Phys. Rev. B 92, 155409(2015).

[410] A. O. Sboychakov, A. L. Rakhmanov, A. V. Rozhkov, and F. Nori, “Electronic spectrum of twisted bilayer graphene,”Phys. Rev. B 92, 075402 (2015).

[411] L.-J. Yin, J.-B. Qiao, W.-J. Zuo, W.-T. Li, and L. He, “Experimental evidence for non-Abelian gauge potentials intwisted graphene bilayers,” Phys. Rev. B 92, 081406 (2015).

[412] J. Park, W. C. Mitchel, S. Elhamri, L. Grazulis, J. Hoelscher, K. Mahalingam, C. Hwang, S.-K. Mo, and J. Lee,“Observation of the intrinsic bandgap behaviour in as-grown epitaxial twisted graphene,” Nat. Commun. 6, 5677 (2015).

[413] J. C. Slater and G. F. Koster, “Simplified LCAO Method for the Periodic Potential Problem,” Phys. Rev. 94, 1498(1954).

[414] P. San-Jose and E. Prada, “Helical networks in twisted bilayer graphene under interlayer bias,” Phys. Rev. B 88, 121408(2013).

[415] P. Moon, Y.-W. Son, and M. Koshino, “Optical absorption of twisted bilayer graphene with interlayer potential asym-metry,” Phys. Rev. B 90, 155427 (2014).

[416] A. R. Muniz and D. Maroudas, “Opening and tuning of band gap by the formation of diamond superlattices in twistedbilayer graphene,” Phys. Rev. B 86, 075404 (2012).

[417] A. R. Muniz and D. Maroudas, “Formation of fullerene superlattices by interlayer bonding in twisted bilayer graphene,”J. Appl. Phys. 111, 043513 (2012).

[418] F. Symalla, S. Shallcross, I. Beljakov, K. Fink, W. Wenzel, and V. Meded, “Band-gap engineering with a twist: Formationof intercalant superlattices in twisted graphene bilayers,” Phys. Rev. B 91, 205412 (2015).

[419] K. Ulman and S. Narasimhan, “Point defects in twisted bilayer graphene: A density functional theory study,” Phys. Rev.B 89, 245429 (2014).

[420] L. D. Landau and L. M. Lifshitz, Quantum Mechanics Non-Relativistic Theory, Third Edition: Volume 3 (Butterworth-Heinemann, 1981), 3rd ed.

[421] D. S. Lee, C. Riedl, T. Beringer, A. H. Castro Neto, K. von Klitzing, U. Starke, and J. H. Smet, “Quantum Hall Effectin Twisted Bilayer Graphene,” Phys. Rev. Lett. 107, 216602 (2011).

[422] B. Fallahazad, Y. Hao, K. Lee, S. Kim, R. S. Ruoff, and E. Tutuc, “Quantum Hall effect in Bernal stacked and twistedbilayer graphene grown on Cu by chemical vapor deposition,” Phys. Rev. B 85, 201408 (2012).

[423] D. L. Miller, K. D. Kubista, G. M. Rutter, M. Ruan, W. A. de Heer, M. Kindermann, P. N. First, and J. A. Stroscio,“Real-space mapping of magnetically quantized graphene states,” Nat. Phys. 6, 811 (2010).

[424] M. Kindermann and E. J. Mele, “Landau quantization in twisted bilayer graphene: The Dirac comb,” Phys. Rev. B 84,161406 (2011).

[425] H. K. Pal, E. J. Mele, and M. Kindermann, “Landau level splitting in rotationally faulted multilayer graphene,” Phys.Rev. B 89, 081403 (2014).

[426] V. M. Apalkov and T. Chakraborty, “Optical transitions at commensurate angles in a misoriented bilayer graphene inan external magnetic field,” Phys. Rev. B 84, 033408 (2011).

[427] M. Kindermann and P. N. First, “Local sublattice-symmetry breaking in rotationally faulted multilayer graphene,” Phys.Rev. B 83, 045425 (2011).

[428] D. R. Hofstadter, “Energy levels and wave functions of Bloch electrons in rational and irrational magnetic fields,” Phys.Rev. B 14, 2239 (1976).

[429] P. Moon and M. Koshino, “Energy spectrum and quantum Hall effect in twisted bilayer graphene,” Phys. Rev. B 85,195458 (2012).

[430] B. Hunt, J. D. Sanchez-Yamagishi, A. F. Young, M. Yankowitz, B. J. LeRoy, K. Watanabe, T. Taniguchi, P. Moon,M. Koshino, P. Jarillo-Herrero, et al., “Massive Dirac Fermions and Hofstadter Butterfly in a van der Waals Heterostruc-ture,” Science 340, 1427 (2013).

[431] L. A. Ponomarenko, R. V. Gorbachev, G. L. Yu, D. C. Elias, R. Jalil, A. A. Patel, A. Mishchenko, A. S. Mayorov, C. R.Woods, J. R. Wallbank, et al., “Cloning of Dirac fermions in graphene superlattices,” Nature 497, 594 (2013).

[432] C. R. Dean, L. Wang, P. Maher, C. Forsythe, F. Ghahari, Y. Gao, J. Katoch, M. Ishigami, P. Moon, M. Koshino, et al.,“Hofstadter’s butterfly and the fractal quantum Hall effect in moire superlattices,” Nature 497, 598 (2013).

[433] H. Schmidt, J. C. Rode, D. Smirnov, and R. J. Haug, “Superlattice structures in twisted bilayers of folded graphene,”Nat. Commun. 5, 5742 (2014).

[434] R. Bistritzer and A. H. MacDonald, “Moire butterflies in twisted bilayer graphene,” Phys. Rev. B 84, 035440 (2011).[435] Z. F. Wang, F. Liu, and M. Y. Chou, “Fractal Landau-Level Spectra in Twisted Bilayer Graphene,” Nano Lett. 12, 3833

131

(2012).[436] Y. Hasegawa and M. Kohmoto, “Periodic Landau gauge and quantum Hall effect in twisted bilayer graphene,” Phys.

Rev. B 88, 125426 (2013).[437] C.-K. Lu and H. A. Fertig, “Probing layer localization in twisted graphene bilayers via cyclotron resonance,” Phys. Rev.

B 90, 115436 (2014).[438] M. Stone, Quantum Hall Effect (World Scientific, 1992).[439] C.-K. Lu and H. A. Fertig, “Magnetic breakdown in twisted bilayer graphene,” Phys. Rev. B 89, 085408 (2014).[440] C. J. Tabert and E. J. Nicol, “Optical conductivity of twisted bilayer graphene,” Phys. Rev. B 87, 121402 (2013).[441] Y. Wang, Z. Ni, L. Liu, Y. Liu, C. Cong, T. Yu, X. Wang, D. Shen, and Z. Shen, “Stacking-Dependent Optical

Conductivity of Bilayer Graphene,” ACS Nano 4, 4074 (2010).[442] X. Zou, J. Shang, J. Leaw, Z. Luo, L. Luo, C. La-o-vorakiat, L. Cheng, S. A. Cheong, H. Su, J.-X. Zhu, et al., “Terahertz

Conductivity of Twisted Bilayer Graphene,” Phys. Rev. Lett. 110, 067401 (2013).[443] Y. Kim, H. Yun, S.-G. Nam, M. Son, D. S. Lee, D. C. Kim, S. Seo, H. C. Choi, H.-J. Lee, S. W. Lee, et al., “Breakdown

of the Interlayer Coherence in Twisted Bilayer Graphene,” Phys. Rev. Lett. 110, 096602 (2013).[444] R. Bistritzer and A. H. MacDonald, “Transport between twisted graphene layers,” Phys. Rev. B 81, 245412 (2010).[445] P. Moon and M. Koshino, “Optical absorption in twisted bilayer graphene,” Phys. Rev. B 87, 205404 (2013).[446] R. W. Havener, Y. Liang, L. Brown, L. Yang, and J. Park, “Van Hove Singularities and Excitonic Effects in the Optical

Conductivity of Twisted Bilayer Graphene,” Nano Lett. 14, 3353 (2014).[447] Y. Liang, R. Soklaski, S. Huang, M. W. Graham, R. Havener, J. Park, and L. Yang, “Strongly bound excitons in gapless

two-dimensional structures,” Phys. Rev. B 90, 115418 (2014).[448] H. Patel, R. W. Havener, L. Brown, Y. Liang, L. Yang, J. Park, and M. W. Graham, “Tunable Optical Excitations in

Twisted Bilayer Graphene Form Strongly Bound Excitons,” Nano Lett. 15, 5932 (2015).[449] E. Koren, I. Leven, E. Lortscher, A. Knoll, O. Hod, and U. Duerig, “Coherent commensurate electronic states at the

interface between misoriented graphene layers,” Nat. Nano. advance online publication, (2016).[450] W.-Y. He, Z.-D. Chu, and L. He, “Chiral Tunneling in a Twisted Graphene Bilayer,” Phys. Rev. Lett. 111, 066803

(2013).

132

Recommended